# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Cs2W7O22
_database_code_depnum_ccdc_archive 'CCDC 2211340'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_Cs2W7O22            
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form


_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs2 O22 W7'
_chemical_formula_weight         1904.77

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 21'
_space_group_name_Hall           'P 2yb'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   3.8497(3)
_cell_length_b                   7.3502(5)
_cell_length_c                   32.611(3)
_cell_angle_alpha                90
_cell_angle_beta                 90.006(3)
_cell_angle_gamma                90
_cell_volume                     922.76(12)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    1309
_cell_measurement_theta_min      3.04
_cell_measurement_theta_max      26.97

_exptl_crystal_description       plate
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    6.855
_exptl_crystal_F_000             1608
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.057
_exptl_crystal_size_mid          0.041
_exptl_crystal_size_min          0.020
_exptl_absorpt_coefficient_mu    47.439
_shelx_estimated_absorpt_T_min   0.173
_shelx_estimated_absorpt_T_max   0.450
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.2835
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.0968 before and 0.0546 after correction.
The Ratio of minimum to maximum transmission is 0.3802.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_diffrn_reflns_number            10850
_diffrn_reflns_av_unetI/netI     0.1504
_diffrn_reflns_av_R_equivalents  0.1026
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -43
_diffrn_reflns_limit_l_max       42
_diffrn_reflns_theta_min         1.249
_diffrn_reflns_theta_max         28.287
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             4291
_reflns_number_gt                2648
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.856
_reflns_Friedel_fraction_max     1.000
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1008P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_chemical_absolute_configuration ?
_refine_ls_number_reflns         4291
_refine_ls_number_parameters     184
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.1420
_refine_ls_R_factor_gt           0.0980
_refine_ls_wR_factor_ref         0.2376
_refine_ls_wR_factor_gt          0.2070
_refine_ls_goodness_of_fit_ref   0.998
_refine_ls_restrained_S_all      1.003
_refine_ls_shift/su_max          3.565
_refine_ls_shift/su_mean         0.146

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
W1 W 0.4784(10) 0.245(2) 0.1023(2) 0.0155(12) Uani 1 1
W2 W 0.503(2) 0.758(2) 0.1036(2) 0.050(3) Uani 1 1
W3 W 0.504(2) 0.504(2) 0.20395(10) 0.0305(13) Uani 1 1
W4 W 0.4624(9) 0.257(3) 0.30555(18) 0.0110(10) Uani 1 1
W5 W 0.5783(11) 0.749(3) 0.30495(19) 0.0171(11) Uani 1 1
W6 W 0.501(2) 0.003(3) 0.40213(10) 0.0357(14) Uani 1 1
W7 W 0.510(2) 0.251(3) 0.5000(3) 0.0388(15) Uani 1 1
Cs1 Cs -0.027(3) 0.000000 0.2041(2) 0.030(2) Uani 0.808(4) 1
Cs2 Cs -0.030(4) 0.506(3) 0.4032(3) 0.023(3) Uani 0.588(4) 1
Cs3 Cs 0.046(4) 0.486(4) 0.0069(4) 0.060(5) Uani 0.604(4) 1
O1 O 0.043(11) 0.255(12) 0.108(2) 0.020(16) Uiso 1 1
O2 O 0.540(13) 0.213(7) 0.0517(13) 0.014(13) Uiso 1 1
O3 O 0.506(13) 0.489(10) 0.1003(12) 0.009(10) Uiso 1 1
O4 O 0.503(18) 0.009(12) 0.1246(12) 0.012(9) Uiso 1 1
O5 O 0.474(17) 0.308(10) 0.170(3) 0.04(2) Uiso 1 1
O6 O 0.551(15) 0.810(7) 0.0500(18) 0.012(13) Uiso 1 1
O7 O 0.980(14) 0.761(10) 0.113(2) 0.009(14) Uiso 1 1
O8 O 0.488(12) 0.688(7) 0.1683(19) -0.001(11) Uiso 1 1
O9 O 0.093(10) 0.463(5) 0.2110(14) -0.001(11) Uiso 1 1
O10 O 0.564(14) 0.672(7) 0.2510(18) 0.004(10) Uiso 1 1
O11 O 0.556(13) 0.313(6) 0.2527(18) 0.003(10) Uiso 1 1
O12 O 0.024(15) 0.246(14) 0.309(2) 0.016(14) Uiso 1 1
O13 O 0.506(18) 0.501(12) 0.3237(12) 0.012(9) Uiso 1 1
O14 O 0.541(17) -0.002(12) 0.2915(14) 0.021(11) Uiso 1 1
O15 O 0.486(14) 0.183(8) 0.365(2) 0.012(14) Uiso 1 1
O16 O 1.060(16) 0.746(16) 0.309(3) 0.034(19) Uiso 1 1
O17 O 0.462(15) 0.821(9) 0.360(2) 0.020(17) Uiso 1 1
O18 O 0.065(11) -0.012(9) 0.4057(12) 0.000(12) Uiso 1 1
O19 O 0.536(14) 0.176(7) 0.445(2) 0.005(11) Uiso 1 1
O20 O 0.564(16) -0.180(8) 0.445(2) 0.017(14) Uiso 1 1
O21 O 0.922(9) 0.227(6) 0.4960(17) -0.001(10) Uiso 1 1
O22 O 0.51(2) 0.503(15) 0.4847(14) 0.024(10) Uiso 1 1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.69(4) . ?
W1 O2 1.69(4) . ?
W1 O3 1.80(7) . ?
W1 O4 1.89(8) . ?
W1 O1 2.18(5) 1_655 ?
W1 O5 2.25(9) . ?
W1 Cs3 3.946(15) . ?
W1 Cs3 4.19(2) 1_655 ?
W1 Cs1 4.229(14) 1_655 ?
W1 Cs1 4.248(12) . ?
W1 Cs3 4.44(2) 2_645 ?
W1 Cs3 4.517(16) 2_545 ?
W2 O6 1.80(6) . ?
W2 O7 1.87(6) . ?
W2 O3 1.98(7) . ?
W2 O4 1.97(9) 1_565 ?
W2 O7 2.04(6) 1_455 ?
W2 O8 2.17(6) . ?
W2 Cs3 4.13(2) . ?
W2 Cs1 4.143(11) 1_665 ?
W2 Cs1 4.249(13) 1_565 ?
W2 Cs3 4.280(18) 1_655 ?
W2 Cs3 4.338(17) 2_655 ?
W2 Cs3 4.501(19) 2 ?
W3 O9 1.63(4) . ?
W3 O8 1.78(5) . ?
W3 O5 1.82(8) . ?
W3 O10 1.98(5) . ?
W3 O11 2.13(5) . ?
W3 O9 2.30(4) 1_655 ?
W3 Cs1 4.067(15) 1_665 ?
W3 Cs1 4.123(17) 1_655 ?
W3 Cs1 4.178(17) 1_565 ?
W3 Cs1 4.233(15) . ?
W4 O12 1.69(6) . ?
W4 O11 1.81(6) . ?
W4 O13 1.90(8) . ?
W4 O14 1.98(8) . ?
W4 O15 2.02(7) . ?
W4 O12 2.17(6) 1_655 ?
W4 Cs2 4.135(15) . ?
W4 Cs2 4.162(16) 1_655 ?
W4 Cs1 4.250(11) . ?
W4 Cs1 4.287(13) 1_655 ?
W5 O10 1.85(6) . ?
W5 O16 1.86(6) . ?
W5 O14 1.89(8) 1_565 ?
W5 O17 1.93(8) . ?
W5 O13 1.94(8) . ?
W5 O16 2.00(6) 1_455 ?
W5 Cs2 3.966(16) 1_655 ?
W5 Cs1 4.066(12) 1_665 ?
W5 Cs2 4.352(14) . ?
W5 Cs1 4.433(15) 1_565 ?
W6 O18 1.69(4) . ?
W6 O15 1.80(6) . ?
W6 O19 1.90(6) . ?
W6 O17 1.92(7) 1_545 ?
W6 O20 1.96(7) . ?
W6 O18 2.18(4) 1_655 ?
W6 Cs2 4.07(2) 1_645 ?
W6 Cs2 4.12(2) 1_655 ?
W6 Cs2 4.18(2) 1_545 ?
W6 Cs2 4.23(2) . ?
W7 O21 1.60(4) . ?
W7 O19 1.88(7) . ?
W7 O20 1.89(8) 2_656 ?
W7 O22 1.90(11) 2_646 ?
W7 O22 1.91(11) . ?
W7 O21 2.27(4) 1_455 ?
W7 Cs2 4.075(16) 1_655 ?
W7 Cs2 4.077(17) 2_546 ?
W7 Cs2 4.150(19) 2_646 ?
W7 Cs2 4.217(18) . ?
Cs1 O4 3.16(5) 1_455 ?
Cs1 O5 3.17(7) . ?
Cs1 O5 3.17(7) 1_455 ?
Cs1 O8 3.18(5) 1_445 ?
Cs1 O11 3.22(5) 1_455 ?
Cs1 O8 3.25(5) 1_545 ?
Cs1 O10 3.26(5) 1_445 ?
Cs1 O4 3.30(5) . ?
Cs1 O14 3.30(5) 1_455 ?
Cs1 O7 3.43(7) 1_445 ?
Cs1 O9 3.44(4) . ?
Cs1 O11 3.58(5) . ?
Cs1 O14 3.59(6) . ?
Cs1 O10 3.65(5) 1_545 ?
Cs1 O1 3.68(8) . ?
Cs1 Cs1 3.8497(3) 1_455 ?
Cs1 Cs1 3.8497(3) 1_655 ?
Cs1 O12 3.87(8) . ?
Cs1 O16 3.91(9) 1_445 ?
Cs1 O9 3.98(4) 1_545 ?
Cs2 O20 3.10(7) 1_465 ?
Cs2 O13 3.15(5) 1_455 ?
Cs2 O22 3.18(6) 1_455 ?
Cs2 O19 3.24(6) 1_455 ?
Cs2 O15 3.27(6) 1_455 ?
Cs2 O13 3.32(5) . ?
Cs2 O17 3.30(7) . ?
Cs2 O15 3.34(6) . ?
Cs2 O17 3.34(7) 1_455 ?
Cs2 O22 3.38(7) . ?
Cs2 O20 3.52(6) 1_565 ?
Cs2 O19 3.53(6) . ?
Cs2 O18 3.56(7) 1_565 ?
Cs2 O16 3.57(9) 1_455 ?
Cs2 O12 3.63(8) . ?
Cs2 O21 3.66(5) 1_455 ?
Cs2 O21 3.69(6) 2_656 ?
Cs2 Cs2 3.8497(4) 1_655 ?
Cs2 Cs2 3.8497(4) 1_455 ?
Cs2 O18 3.83(7) . ?
Cs3 O6 2.74(6) 2_645 ?
Cs3 O2 3.00(5) 2_655 ?
Cs3 O2 3.12(6) . ?
Cs3 O2 3.15(6) 1_455 ?
Cs3 O6 3.22(6) 2_545 ?
Cs3 O6 3.36(6) 1_455 ?
Cs3 O6 3.38(6) . ?
Cs3 O2 3.40(5) 2 ?
Cs3 O3 3.52(4) . ?
Cs3 O1 3.69(8) . ?
Cs3 O3 3.68(5) 1_455 ?
Cs3 Cs3 3.720(4) 2 ?
Cs3 Cs3 3.720(4) 2_545 ?
Cs3 Cs3 3.8497(3) 1_455 ?
Cs3 Cs3 3.8497(3) 1_655 ?
Cs3 O7 4.03(7) 1_455 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 104(3) . . ?
O1 W1 O3 91(3) . . ?
O2 W1 O3 95(2) . . ?
O1 W1 O4 93(4) . . ?
O2 W1 O4 104(2) . . ?
O3 W1 O4 158(2) . . ?
O1 W1 O1 169(5) . 1_655 ?
O2 W1 O1 87(3) . 1_655 ?
O3 W1 O1 85(3) . 1_655 ?
O4 W1 O1 87(3) . 1_655 ?
O1 W1 O5 83(3) . . ?
O2 W1 O5 171(2) . . ?
O3 W1 O5 80(2) . . ?
O4 W1 O5 79(2) . . ?
O1 W1 O5 86(3) 1_655 . ?
O1 W1 Cs3 69(3) . . ?
O2 W1 Cs3 49.4(19) . . ?
O3 W1 Cs3 63.2(14) . . ?
O4 W1 Cs3 137.6(19) . . ?
O1 W1 Cs3 118(2) 1_655 . ?
O5 W1 Cs3 132.6(18) . . ?
O1 W1 Cs3 125(3) . 1_655 ?
O2 W1 Cs3 42.1(18) . 1_655 ?
O3 W1 Cs3 61.4(14) . 1_655 ?
O4 W1 Cs3 130.4(18) . 1_655 ?
O1 W1 Cs3 62(2) 1_655 1_655 ?
O5 W1 Cs3 130.1(18) . 1_655 ?
Cs3 W1 Cs3 56.4(3) . 1_655 ?
O1 W1 Cs1 113(3) . 1_655 ?
O2 W1 Cs1 130.3(19) . 1_655 ?
O3 W1 Cs1 115.3(14) . 1_655 ?
O4 W1 Cs1 44.1(18) . 1_655 ?
O1 W1 Cs1 60(2) 1_655 1_655 ?
O5 W1 Cs1 47.3(18) . 1_655 ?
Cs3 W1 Cs1 178.0(5) . 1_655 ?
Cs3 W1 Cs1 121.8(3) 1_655 1_655 ?
O1 W1 Cs1 59(3) . . ?
O2 W1 Cs1 140.5(18) . . ?
O3 W1 Cs1 118.7(14) . . ?
O4 W1 Cs1 48.0(18) . . ?
O1 W1 Cs1 114(2) 1_655 . ?
O5 W1 Cs1 47.0(18) . . ?
Cs3 W1 Cs1 127.8(4) . . ?
Cs3 W1 Cs1 175.7(3) 1_655 . ?
Cs1 W1 Cs1 54.02(16) 1_655 . ?
O1 W1 Cs3 121(3) . 2_645 ?
O2 W1 Cs3 25.2(19) . 2_645 ?
O3 W1 Cs3 112.0(14) . 2_645 ?
O4 W1 Cs3 83.9(16) . 2_645 ?
O1 W1 Cs3 70(2) 1_655 2_645 ?
O5 W1 Cs3 151.2(17) . 2_645 ?
Cs3 W1 Cs3 74.6(3) . 2_645 ?
Cs3 W1 Cs3 50.97(9) 1_655 2_645 ?
Cs1 W1 Cs3 105.1(4) 1_655 2_645 ?
Cs1 W1 Cs3 129.3(4) . 2_645 ?
O1 W1 Cs3 70(3) . 2_545 ?
O2 W1 Cs3 39.7(18) . 2_545 ?
O3 W1 Cs3 114.8(14) . 2_545 ?
O4 W1 Cs3 86.5(18) . 2_545 ?
O1 W1 Cs3 121(2) 1_655 2_545 ?
O5 W1 Cs3 148.8(18) . 2_545 ?
Cs3 W1 Cs3 51.61(9) . 2_545 ?
Cs3 W1 Cs3 80.0(3) 1_655 2_545 ?
Cs1 W1 Cs3 129.8(5) 1_655 2_545 ?
Cs1 W1 Cs3 103.4(3) . 2_545 ?
Cs3 W1 Cs3 50.9(2) 2_645 2_545 ?
O6 W2 O7 94(3) . . ?
O6 W2 O3 99(2) . . ?
O7 W2 O3 91(3) . . ?
O6 W2 O4 98(2) . 1_565 ?
O7 W2 O4 86(3) . 1_565 ?
O3 W2 O4 162.8(19) . 1_565 ?
O6 W2 O7 105(3) . 1_455 ?
O7 W2 O7 161(4) . 1_455 ?
O3 W2 O7 92(2) . 1_455 ?
O4 W2 O7 86(3) 1_565 1_455 ?
O6 W2 O8 175(2) . . ?
O7 W2 O8 82(2) . . ?
O3 W2 O8 79.5(17) . . ?
O4 W2 O8 83.3(19) 1_565 . ?
O7 W2 O8 80(2) 1_455 . ?
O6 W2 Cs3 53.5(18) . . ?
O7 W2 Cs3 124(2) . . ?
O3 W2 Cs3 58.4(13) . . ?
O4 W2 Cs3 136.1(17) 1_565 . ?
O7 W2 Cs3 73(2) 1_455 . ?
O8 W2 Cs3 128.0(13) . . ?
O6 W2 Cs1 129.1(18) . 1_665 ?
O7 W2 Cs1 55(2) . 1_665 ?
O3 W2 Cs1 118.0(13) . 1_665 ?
O4 W2 Cs1 47.3(17) 1_565 1_665 ?
O7 W2 Cs1 108(2) 1_455 1_665 ?
O8 W2 Cs1 49.1(13) . 1_665 ?
Cs3 W2 Cs1 176.4(5) . 1_665 ?
O6 W2 Cs1 135.2(17) . 1_565 ?
O7 W2 Cs1 110(2) . 1_565 ?
O3 W2 Cs1 117.6(13) . 1_565 ?
O4 W2 Cs1 48.6(17) 1_565 1_565 ?
O7 W2 Cs1 53(2) 1_455 1_565 ?
O8 W2 Cs1 48.5(12) . 1_565 ?
Cs3 W2 Cs1 125.9(4) . 1_565 ?
Cs1 W2 Cs1 54.59(14) 1_665 1_565 ?
O6 W2 Cs3 48.2(17) . 1_655 ?
O7 W2 Cs3 70(2) . 1_655 ?
O3 W2 Cs3 59.3(13) . 1_655 ?
O4 W2 Cs3 134.0(18) 1_565 1_655 ?
O7 W2 Cs3 127(2) 1_455 1_655 ?
O8 W2 Cs3 128.1(13) . 1_655 ?
Cs3 W2 Cs3 54.5(2) . 1_655 ?
Cs1 W2 Cs3 124.7(4) 1_665 1_655 ?
Cs1 W2 Cs3 176.5(4) 1_565 1_655 ?
O6 W2 Cs3 21.4(18) . 2_655 ?
O7 W2 Cs3 75(2) . 2_655 ?
O3 W2 Cs3 109.7(13) . 2_655 ?
O4 W2 Cs3 85.9(16) 1_565 2_655 ?
O7 W2 Cs3 121.5(19) 1_455 2_655 ?
O8 W2 Cs3 155.4(13) . 2_655 ?
Cs3 W2 Cs3 73.9(3) . 2_655 ?
Cs1 W2 Cs3 108.5(3) 1_665 2_655 ?
Cs1 W2 Cs3 132.2(5) 1_565 2_655 ?
Cs3 W2 Cs3 51.13(11) 1_655 2_655 ?
O6 W2 Cs3 36.0(18) . 2 ?
O7 W2 Cs3 127(2) . 2 ?
O3 W2 Cs3 109.3(13) . 2 ?
O4 W2 Cs3 86.0(16) 1_565 2 ?
O7 W2 Cs3 70.0(19) 1_455 2 ?
O8 W2 Cs3 148.6(12) . 2 ?
Cs3 W2 Cs3 50.84(8) . 2 ?
Cs1 W2 Cs3 132.7(5) 1_665 2 ?
Cs1 W2 Cs3 103.7(4) 1_565 2 ?
Cs3 W2 Cs3 79.2(3) 1_655 2 ?
Cs3 W2 Cs3 51.6(2) 2_655 2 ?
O9 W3 O8 102(2) . . ?
O9 W3 O5 83(3) . . ?
O8 W3 O5 101.6(19) . . ?
O9 W3 O10 97(2) . . ?
O8 W3 O10 92(2) . . ?
O5 W3 O10 166(3) . . ?
O9 W3 O11 82(2) . . ?
O8 W3 O11 172(2) . . ?
O5 W3 O11 86(3) . . ?
O10 W3 O11 79.7(13) . . ?
O9 W3 O9 157(2) . 1_655 ?
O8 W3 O9 101.4(18) . 1_655 ?
O5 W3 O9 91(2) . 1_655 ?
O10 W3 O9 83.6(19) . 1_655 ?
O11 W3 O9 75.3(18) . 1_655 ?
O9 W3 Cs1 126.7(14) . 1_665 ?
O8 W3 Cs1 48.5(17) . 1_665 ?
O5 W3 Cs1 138(3) . 1_665 ?
O10 W3 Cs1 52.5(15) . 1_665 ?
O11 W3 Cs1 123.3(13) . 1_665 ?
O9 W3 Cs1 71.3(10) 1_655 1_665 ?
O9 W3 Cs1 105.0(14) . 1_655 ?
O8 W3 Cs1 134.1(17) . 1_655 ?
O5 W3 Cs1 47(2) . 1_655 ?
O10 W3 Cs1 120.4(15) . 1_655 ?
O11 W3 Cs1 50.6(14) . 1_655 ?
O9 W3 Cs1 56.7(10) 1_655 1_655 ?
Cs1 W3 Cs1 127.7(4) 1_665 1_655 ?
O9 W3 Cs1 71.7(14) . 1_565 ?
O8 W3 Cs1 47.4(17) . 1_565 ?
O5 W3 Cs1 131(2) . 1_565 ?
O10 W3 Cs1 61.0(15) . 1_565 ?
O11 W3 Cs1 128.4(14) . 1_565 ?
O9 W3 Cs1 126.6(10) 1_655 1_565 ?
Cs1 W3 Cs1 55.6(2) 1_665 1_565 ?
Cs1 W3 Cs1 176.7(4) 1_655 1_565 ?
O9 W3 Cs1 50.8(14) . . ?
O8 W3 Cs1 130.3(17) . . ?
O5 W3 Cs1 44(3) . . ?
O10 W3 Cs1 126.8(15) . . ?
O11 W3 Cs1 57.8(13) . . ?
O9 W3 Cs1 111.2(10) 1_655 . ?
Cs1 W3 Cs1 177.5(5) 1_665 . ?
Cs1 W3 Cs1 54.9(2) 1_655 . ?
Cs1 W3 Cs1 121.8(4) 1_565 . ?
O12 W4 O11 106(3) . . ?
O12 W4 O13 97(4) . . ?
O11 W4 O13 94(2) . . ?
O12 W4 O14 97(4) . . ?
O11 W4 O14 88(2) . . ?
O13 W4 O14 165(2) . . ?
O12 W4 O15 88(3) . . ?
O11 W4 O15 166(2) . . ?
O13 W4 O15 87(2) . . ?
O14 W4 O15 88(2) . . ?
O12 W4 O12 172(5) . 1_655 ?
O11 W4 O12 82(2) . 1_655 ?
O13 W4 O12 86(3) . 1_655 ?
O14 W4 O12 80(3) . 1_655 ?
O15 W4 O12 84(2) . 1_655 ?
O12 W4 Cs2 61(3) . . ?
O11 W4 Cs2 136.5(15) . . ?
O13 W4 Cs2 51.8(17) . . ?
O14 W4 Cs2 132.4(15) . . ?
O15 W4 Cs2 53.0(16) . . ?
O12 W4 Cs2 116(2) 1_655 . ?
O12 W4 Cs2 116(3) . 1_655 ?
O11 W4 Cs2 122.4(15) . 1_655 ?
O13 W4 Cs2 45.8(18) . 1_655 ?
O14 W4 Cs2 121.9(17) . 1_655 ?
O15 W4 Cs2 50.3(17) . 1_655 ?
O12 W4 Cs2 61(2) 1_655 1_655 ?
Cs2 W4 Cs2 55.3(2) . 1_655 ?
O12 W4 Cs1 66(3) . . ?
O11 W4 Cs1 56.5(15) . . ?
O13 W4 Cs1 134.6(17) . . ?
O14 W4 Cs1 57.4(17) . . ?
O15 W4 Cs1 130.5(17) . . ?
O12 W4 Cs1 118(2) 1_655 . ?
Cs2 W4 Cs1 126.4(3) . . ?
Cs2 W4 Cs1 178.3(3) 1_655 . ?
O12 W4 Cs1 119(3) . 1_655 ?
O11 W4 Cs1 43.3(14) . 1_655 ?
O13 W4 Cs1 128.0(17) . 1_655 ?
O14 W4 Cs1 47.8(15) . 1_655 ?
O15 W4 Cs1 127.2(16) . 1_655 ?
O12 W4 Cs1 64(2) 1_655 1_655 ?
Cs2 W4 Cs1 179.8(5) . 1_655 ?
Cs2 W4 Cs1 124.7(3) 1_655 1_655 ?
Cs1 W4 Cs1 53.60(14) . 1_655 ?
O10 W5 O16 95(3) . . ?
O10 W5 O14 94(2) . 1_565 ?
O16 W5 O14 96(4) . 1_565 ?
O10 W5 O17 165(2) . . ?
O16 W5 O17 100(3) . . ?
O14 W5 O17 86(2) 1_565 . ?
O10 W5 O13 90(2) . . ?
O16 W5 O13 96(4) . . ?
O14 W5 O13 167(2) 1_565 . ?
O17 W5 O13 86(2) . . ?
O10 W5 O16 91(3) . 1_455 ?
O16 W5 O16 172(5) . 1_455 ?
O14 W5 O16 87(4) 1_565 1_455 ?
O17 W5 O16 73(3) . 1_455 ?
O13 W5 O16 80(4) . 1_455 ?
O10 W5 Cs2 129.9(16) . 1_655 ?
O16 W5 Cs2 64(3) . 1_655 ?
O14 W5 Cs2 130.8(17) 1_565 1_655 ?
O17 W5 Cs2 57.1(19) . 1_655 ?
O13 W5 Cs2 51.5(17) . 1_655 ?
O16 W5 Cs2 109(3) 1_455 1_655 ?
O10 W5 Cs1 51.8(15) . 1_665 ?
O16 W5 Cs1 72(3) . 1_665 ?
O14 W5 Cs1 53.1(17) 1_565 1_665 ?
O17 W5 Cs1 136(2) . 1_665 ?
O13 W5 Cs1 137.1(15) . 1_665 ?
O16 W5 Cs1 115(3) 1_455 1_665 ?
Cs2 W5 Cs1 135.7(3) 1_655 1_665 ?
O10 W5 Cs2 123.9(16) . . ?
O16 W5 Cs2 119(3) . . ?
O14 W5 Cs2 121.9(18) 1_565 . ?
O17 W5 Cs2 45.5(19) . . ?
O13 W5 Cs2 46.1(17) . . ?
O16 W5 Cs2 54(3) 1_455 . ?
Cs2 W5 Cs2 54.9(2) 1_655 . ?
Cs1 W5 Cs2 169.4(3) 1_665 . ?
O10 W5 Cs1 53.6(16) . 1_565 ?
O16 W5 Cs1 125(3) . 1_565 ?
O14 W5 Cs1 52.0(18) 1_565 1_565 ?
O17 W5 Cs1 117.2(19) . 1_565 ?
O13 W5 Cs1 123.3(18) . 1_565 ?
O16 W5 Cs1 62(3) 1_455 1_565 ?
Cs2 W5 Cs1 170.6(3) 1_655 1_565 ?
Cs1 W5 Cs1 53.65(17) 1_665 1_565 ?
Cs2 W5 Cs1 115.7(2) . 1_565 ?
O18 W6 O15 94(3) . . ?
O18 W6 O19 94(2) . . ?
O15 W6 O19 90(3) . . ?
O18 W6 O17 86(3) . 1_545 ?
O15 W6 O17 91.8(18) . 1_545 ?
O19 W6 O17 178(3) . 1_545 ?
O18 W6 O20 92(3) . . ?
O15 W6 O20 173(3) . . ?
O19 W6 O20 85.7(16) . . ?
O17 W6 O20 92(3) 1_545 . ?
O18 W6 O18 170(3) . 1_655 ?
O15 W6 O18 96(2) . 1_655 ?
O19 W6 O18 86(2) . 1_655 ?
O17 W6 O18 95(2) 1_545 1_655 ?
O20 W6 O18 79(2) . 1_655 ?
O18 W6 Cs2 112(2) . 1_645 ?
O15 W6 Cs2 133(2) . 1_645 ?
O19 W6 Cs2 124.3(18) . 1_645 ?
O17 W6 Cs2 54(2) 1_545 1_645 ?
O20 W6 Cs2 47(2) . 1_645 ?
O18 W6 Cs2 60.7(17) 1_655 1_645 ?
O18 W6 Cs2 120(2) . 1_655 ?
O15 W6 Cs2 50(2) . 1_655 ?
O19 W6 Cs2 50.1(18) . 1_655 ?
O17 W6 Cs2 132(2) 1_545 1_655 ?
O20 W6 Cs2 123.8(19) . 1_655 ?
O18 W6 Cs2 66.9(19) 1_655 1_655 ?
Cs2 W6 Cs2 127.6(4) 1_645 1_655 ?
O18 W6 Cs2 57(2) . 1_545 ?
O15 W6 Cs2 129(2) . 1_545 ?
O19 W6 Cs2 128.0(17) . 1_545 ?
O17 W6 Cs2 50(2) 1_545 1_545 ?
O20 W6 Cs2 57.0(19) . 1_545 ?
O18 W6 Cs2 116.2(18) 1_655 1_545 ?
Cs2 W6 Cs2 55.6(3) 1_645 1_545 ?
Cs2 W6 Cs2 176.7(5) 1_655 1_545 ?
O18 W6 Cs2 65(2) . . ?
O15 W6 Cs2 49(2) . . ?
O19 W6 Cs2 56.0(18) . . ?
O17 W6 Cs2 125(2) 1_545 . ?
O20 W6 Cs2 131(2) . . ?
O18 W6 Cs2 121.7(19) 1_655 . ?
Cs2 W6 Cs2 177.3(5) 1_645 . ?
Cs2 W6 Cs2 54.9(3) 1_655 . ?
Cs2 W6 Cs2 121.9(4) 1_545 . ?
O21 W7 O19 81(3) . . ?
O21 W7 O20 105(3) . 2_656 ?
O19 W7 O20 174(3) . 2_656 ?
O21 W7 O22 88(3) . 2_646 ?
O19 W7 O22 88(2) . 2_646 ?
O20 W7 O22 90(3) 2_656 2_646 ?
O21 W7 O22 94(3) . . ?
O19 W7 O22 92(2) . . ?
O20 W7 O22 89(2) 2_656 . ?
O22 W7 O22 177.7(6) 2_646 . ?
O21 W7 O21 167(3) . 1_455 ?
O19 W7 O21 89(2) . 1_455 ?
O20 W7 O21 86(2) 2_656 1_455 ?
O22 W7 O21 84(3) 2_646 1_455 ?
O22 W7 O21 94(3) . 1_455 ?
O21 W7 Cs2 64(2) . 1_655 ?
O19 W7 Cs2 51.1(16) . 1_655 ?
O20 W7 Cs2 132.7(19) 2_656 1_655 ?
O22 W7 Cs2 132(2) 2_646 1_655 ?
O22 W7 Cs2 49.5(19) . 1_655 ?
O21 W7 Cs2 115.2(15) 1_455 1_655 ?
O21 W7 Cs2 117(2) . 2_546 ?
O19 W7 Cs2 129.4(16) . 2_546 ?
O20 W7 Cs2 46.6(19) 2_656 2_546 ?
O22 W7 Cs2 49.3(19) 2_646 2_546 ?
O22 W7 Cs2 129(2) . 2_546 ?
O21 W7 Cs2 63.8(14) 1_455 2_546 ?
Cs2 W7 Cs2 178.5(6) 1_655 2_546 ?
O21 W7 Cs2 62(2) . 2_646 ?
O19 W7 Cs2 124.9(18) . 2_646 ?
O20 W7 Cs2 57.7(19) 2_656 2_646 ?
O22 W7 Cs2 53(2) 2_646 2_646 ?
O22 W7 Cs2 128(2) . 2_646 ?
O21 W7 Cs2 119.3(15) 1_455 2_646 ?
Cs2 W7 Cs2 125.4(2) 1_655 2_646 ?
Cs2 W7 Cs2 55.8(2) 2_546 2_646 ?
O21 W7 Cs2 119(2) . . ?
O19 W7 Cs2 56.2(17) . . ?
O20 W7 Cs2 121.2(19) 2_656 . ?
O22 W7 Cs2 127(2) 2_646 . ?
O22 W7 Cs2 52(2) . . ?
O21 W7 Cs2 60.2(14) 1_455 . ?
Cs2 W7 Cs2 55.3(2) 1_655 . ?
Cs2 W7 Cs2 123.5(2) 2_546 . ?
Cs2 W7 Cs2 178.9(5) 2_646 . ?
O4 Cs1 O5 93(2) 1_455 . ?
O4 Cs1 O5 50(2) 1_455 1_455 ?
O5 Cs1 O5 74.7(17) . 1_455 ?
O4 Cs1 O8 51.5(18) 1_455 1_445 ?
O5 Cs1 O8 137.9(12) . 1_445 ?
O5 Cs1 O8 91.7(13) 1_455 1_445 ?
O4 Cs1 O11 96.0(17) 1_455 1_455 ?
O5 Cs1 O11 88.1(17) . 1_455 ?
O5 Cs1 O11 50(2) 1_455 1_455 ?
O8 Cs1 O11 113.8(13) 1_445 1_455 ?
O4 Cs1 O8 94.0(17) 1_455 1_545 ?
O5 Cs1 O8 90.3(12) . 1_545 ?
O5 Cs1 O8 138.4(12) 1_455 1_545 ?
O8 Cs1 O8 73.6(11) 1_445 1_545 ?
O11 Cs1 O8 170.0(15) 1_455 1_545 ?
O4 Cs1 O10 97.1(18) 1_455 1_445 ?
O5 Cs1 O10 170.0(19) . 1_445 ?
O5 Cs1 O10 113.6(17) 1_455 1_445 ?
O8 Cs1 O10 49.9(15) 1_445 1_445 ?
O11 Cs1 O10 93.2(10) 1_455 1_445 ?
O8 Cs1 O10 86.7(13) 1_545 1_445 ?
O4 Cs1 O4 73.2(8) 1_455 . ?
O5 Cs1 O4 48(2) . . ?
O5 Cs1 O4 95(2) 1_455 . ?
O8 Cs1 O4 95.1(17) 1_445 . ?
O11 Cs1 O4 132.9(18) 1_455 . ?
O8 Cs1 O4 49.8(18) 1_545 . ?
O10 Cs1 O4 133.0(18) 1_445 . ?
O4 Cs1 O14 114.8(15) 1_455 1_455 ?
O5 Cs1 O14 128(2) . 1_455 ?
O5 Cs1 O14 90(2) 1_455 1_455 ?
O8 Cs1 O14 91.1(17) 1_445 1_455 ?
O11 Cs1 O14 47.7(18) 1_455 1_455 ?
O8 Cs1 O14 127.9(18) 1_545 1_455 ?
O10 Cs1 O14 49.3(17) 1_445 1_455 ?
O4 Cs1 O14 171.9(14) . 1_455 ?
O4 Cs1 O7 46.4(17) 1_455 1_445 ?
O5 Cs1 O7 93.3(19) . 1_445 ?
O5 Cs1 O7 94(2) 1_455 1_445 ?
O8 Cs1 O7 47.2(14) 1_445 1_445 ?
O11 Cs1 O7 142.4(14) 1_455 1_445 ?
O8 Cs1 O7 47.6(14) 1_545 1_445 ?
O10 Cs1 O7 91.7(15) 1_445 1_445 ?
O4 Cs1 O7 47.9(16) . 1_445 ?
O14 Cs1 O7 138.2(17) 1_455 1_445 ?
O4 Cs1 O9 96.4(19) 1_455 . ?
O5 Cs1 O9 40.2(16) . . ?
O5 Cs1 O9 53.0(16) 1_455 . ?
O8 Cs1 O9 144.7(12) 1_445 . ?
O11 Cs1 O9 47.8(11) 1_455 . ?
O8 Cs1 O9 129.7(11) 1_545 . ?
O10 Cs1 O9 139.9(13) 1_445 . ?
O4 Cs1 O9 87.1(17) . . ?
O14 Cs1 O9 90.9(17) 1_455 . ?
O7 Cs1 O9 124.1(14) 1_445 . ?
O4 Cs1 O11 135.1(18) 1_455 . ?
O5 Cs1 O11 46.9(19) . . ?
O5 Cs1 O11 94.4(17) 1_455 . ?
O8 Cs1 O11 173.3(14) 1_445 . ?
O11 Cs1 O11 68.7(10) 1_455 . ?
O8 Cs1 O11 103.3(13) 1_545 . ?
O10 Cs1 O11 124.7(9) 1_445 . ?
O4 Cs1 O11 87.0(16) . . ?
O14 Cs1 O11 86.3(15) 1_455 . ?
O7 Cs1 O11 134.6(13) 1_445 . ?
O9 Cs1 O11 41.6(11) . . ?
O4 Cs1 O14 177.3(15) 1_455 . ?
O5 Cs1 O14 84.9(19) . . ?
O5 Cs1 O14 131(2) 1_455 . ?
O8 Cs1 O14 130.2(16) 1_445 . ?
O11 Cs1 O14 85.1(16) 1_455 . ?
O8 Cs1 O14 84.9(16) 1_545 . ?
O10 Cs1 O14 85.3(15) 1_445 . ?
O4 Cs1 O14 104.3(13) . . ?
O14 Cs1 O14 67.7(9) 1_455 . ?
O7 Cs1 O14 132.4(16) 1_445 . ?
O9 Cs1 O14 82.5(16) . . ?
O11 Cs1 O14 43.1(15) . . ?
O4 Cs1 O10 135.5(18) 1_455 1_545 ?
O5 Cs1 O10 103.9(16) . 1_545 ?
O5 Cs1 O10 174.9(19) 1_455 1_545 ?
O8 Cs1 O10 92.5(13) 1_445 1_545 ?
O11 Cs1 O10 125.1(10) 1_455 1_545 ?
O8 Cs1 O10 45.9(14) 1_545 1_545 ?
O10 Cs1 O10 67.4(10) 1_445 1_545 ?
O4 Cs1 O10 87.5(16) . 1_545 ?
O14 Cs1 O10 87.0(16) 1_455 1_545 ?
O7 Cs1 O10 91.0(14) 1_445 1_545 ?
O9 Cs1 O10 122.8(11) . 1_545 ?
O11 Cs1 O10 81.3(8) . 1_545 ?
O14 Cs1 O10 44.4(16) . 1_545 ?
O4 Cs1 O1 47.9(17) 1_455 . ?
O5 Cs1 O1 44.9(19) . . ?
O5 Cs1 O1 51.6(18) 1_455 . ?
O8 Cs1 O1 95.5(16) 1_445 . ?
O11 Cs1 O1 95.4(16) 1_455 . ?
O8 Cs1 O1 90.5(15) 1_545 . ?
O10 Cs1 O1 144.6(15) 1_445 . ?
O4 Cs1 O1 43.3(16) . . ?
O14 Cs1 O1 141.2(18) 1_455 . ?
O7 Cs1 O1 61.6(9) 1_445 . ?
O9 Cs1 O1 62.7(15) . . ?
O11 Cs1 O1 90.3(15) . . ?
O14 Cs1 O1 129.6(14) . . ?
O10 Cs1 O1 130.6(12) 1_545 . ?
O4 Cs1 Cs1 55.1(11) 1_455 1_455 ?
O5 Cs1 Cs1 127.4(13) . 1_455 ?
O5 Cs1 Cs1 52.7(13) 1_455 1_455 ?
O8 Cs1 Cs1 54.0(9) 1_445 1_455 ?
O11 Cs1 Cs1 60.1(9) 1_455 1_455 ?
O8 Cs1 Cs1 127.6(9) 1_545 1_455 ?
O10 Cs1 Cs1 61.1(10) 1_445 1_455 ?
O4 Cs1 Cs1 128.2(11) . 1_455 ?
O14 Cs1 Cs1 59.8(11) 1_455 1_455 ?
O7 Cs1 Cs1 90.5(9) 1_445 1_455 ?
O9 Cs1 Cs1 97.7(7) . 1_455 ?
O11 Cs1 Cs1 128.8(8) . 1_455 ?
O14 Cs1 Cs1 127.5(10) . 1_455 ?
O10 Cs1 Cs1 128.5(8) 1_545 1_455 ?
O1 Cs1 Cs1 94.2(7) . 1_455 ?
O4 Cs1 Cs1 124.9(11) 1_455 1_655 ?
O5 Cs1 Cs1 52.6(13) . 1_655 ?
O5 Cs1 Cs1 127.3(13) 1_455 1_655 ?
O8 Cs1 Cs1 126.0(9) 1_445 1_655 ?
O11 Cs1 Cs1 119.9(9) 1_455 1_655 ?
O8 Cs1 Cs1 52.4(9) 1_545 1_655 ?
O10 Cs1 Cs1 118.9(10) 1_445 1_655 ?
O4 Cs1 Cs1 51.8(11) . 1_655 ?
O14 Cs1 Cs1 120.2(11) 1_455 1_655 ?
O7 Cs1 Cs1 89.5(9) 1_445 1_655 ?
O9 Cs1 Cs1 82.3(7) . 1_655 ?
O11 Cs1 Cs1 51.2(8) . 1_655 ?
O14 Cs1 Cs1 52.5(10) . 1_655 ?
O10 Cs1 Cs1 51.5(8) 1_545 1_655 ?
O1 Cs1 Cs1 85.8(7) . 1_655 ?
Cs1 Cs1 Cs1 180.0 1_455 1_655 ?
O4 Cs1 O12 138.0(19) 1_455 . ?
O5 Cs1 O12 87(2) . . ?
O5 Cs1 O12 90(2) 1_455 . ?
O8 Cs1 O12 133.7(16) 1_445 . ?
O11 Cs1 O12 42.1(15) 1_455 . ?
O8 Cs1 O12 128.0(16) 1_545 . ?
O10 Cs1 O12 87.4(16) 1_445 . ?
O4 Cs1 O12 130.8(17) . . ?
O14 Cs1 O12 42.6(16) 1_455 . ?
O7 Cs1 O12 175.6(18) 1_445 . ?
O9 Cs1 O12 58.3(16) . . ?
O11 Cs1 O12 43.8(14) . . ?
O14 Cs1 O12 43.1(16) . . ?
O10 Cs1 O12 84.6(15) 1_545 . ?
O1 Cs1 O12 121(2) . . ?
Cs1 Cs1 O12 92.9(9) 1_455 . ?
Cs1 Cs1 O12 87.1(9) 1_655 . ?
O4 Cs1 O16 141(2) 1_455 1_445 ?
O5 Cs1 O16 126(2) . 1_445 ?
O5 Cs1 O16 134(2) 1_455 1_445 ?
O8 Cs1 O16 91.6(18) 1_445 1_445 ?
O11 Cs1 O16 87.3(17) 1_455 1_445 ?
O8 Cs1 O16 85.7(18) 1_545 1_445 ?
O10 Cs1 O16 43.8(16) 1_445 1_445 ?
O4 Cs1 O16 130.0(18) . 1_445 ?
O14 Cs1 O16 44.4(18) 1_455 1_445 ?
O7 Cs1 O16 120(2) 1_445 1_445 ?
O9 Cs1 O16 113.8(18) . 1_445 ?
O11 Cs1 O16 82.3(16) . 1_445 ?
O14 Cs1 O16 41.6(16) . 1_445 ?
O10 Cs1 O16 42.6(15) 1_545 1_445 ?
O1 Cs1 O16 170.6(14) . 1_445 ?
Cs1 Cs1 O16 94.9(10) 1_455 1_445 ?
Cs1 Cs1 O16 85.1(10) 1_655 1_445 ?
O12 Cs1 O16 56.3(10) . 1_445 ?
O4 Cs1 O9 97.7(18) 1_455 1_545 ?
O5 Cs1 O9 131.0(15) . 1_545 ?
O5 Cs1 O9 143.0(15) 1_455 1_545 ?
O8 Cs1 O9 51.3(11) 1_445 1_545 ?
O11 Cs1 O9 137.5(11) 1_455 1_545 ?
O8 Cs1 O9 41.4(11) 1_545 1_545 ?
O10 Cs1 O9 45.3(11) 1_445 1_545 ?
O4 Cs1 O9 89.6(17) . 1_545 ?
O14 Cs1 O9 90.3(16) 1_455 1_545 ?
O7 Cs1 O9 62.7(14) 1_445 1_545 ?
O9 Cs1 O9 163.9(14) . 1_545 ?
O11 Cs1 O9 122.5(11) . 1_545 ?
O14 Cs1 O9 83.1(15) . 1_545 ?
O10 Cs1 O9 41.3(10) 1_545 1_545 ?
O1 Cs1 O9 123.2(15) . 1_545 ?
Cs1 Cs1 O9 96.7(6) 1_455 1_545 ?
Cs1 Cs1 O9 83.3(6) 1_655 1_545 ?
O12 Cs1 O9 113.9(17) . 1_545 ?
O16 Cs1 O9 57.8(18) 1_445 1_545 ?
O20 Cs2 O13 95(2) 1_465 1_455 ?
O20 Cs2 O22 50(2) 1_465 1_455 ?
O13 Cs2 O22 112.0(15) 1_455 1_455 ?
O20 Cs2 O19 96.4(11) 1_465 1_455 ?
O13 Cs2 O19 92.6(18) 1_455 1_455 ?
O22 Cs2 O19 50(2) 1_455 1_455 ?
O20 Cs2 O15 114.9(16) 1_465 1_455 ?
O13 Cs2 O15 49.7(18) 1_455 1_455 ?
O22 Cs2 O15 90(2) 1_455 1_455 ?
O19 Cs2 O15 47.4(17) 1_455 1_455 ?
O20 Cs2 O13 132(2) 1_465 . ?
O13 Cs2 O13 73.0(8) 1_455 . ?
O22 Cs2 O13 174.8(15) 1_455 . ?
O19 Cs2 O13 129.8(19) 1_455 . ?
O15 Cs2 O13 92.8(17) 1_455 . ?
O20 Cs2 O17 87.5(19) 1_465 . ?
O13 Cs2 O17 89.0(19) 1_455 . ?
O22 Cs2 O17 133(2) 1_455 . ?
O19 Cs2 O17 175.7(17) 1_455 . ?
O15 Cs2 O17 132.3(12) 1_455 . ?
O13 Cs2 O17 47.0(19) . . ?
O20 Cs2 O15 173.3(18) 1_465 . ?
O13 Cs2 O15 91.2(18) 1_455 . ?
O22 Cs2 O15 129(2) 1_455 . ?
O19 Cs2 O15 86.1(17) 1_455 . ?
O15 Cs2 O15 71.3(13) 1_455 . ?
O13 Cs2 O15 47.9(18) . . ?
O17 Cs2 O15 89.9(11) . . ?
O20 Cs2 O17 51(2) 1_465 1_455 ?
O13 Cs2 O17 47.9(19) 1_455 1_455 ?
O22 Cs2 O17 92(2) 1_455 1_455 ?
O19 Cs2 O17 113.1(15) 1_455 1_455 ?
O15 Cs2 O17 90.4(12) 1_455 1_455 ?
O13 Cs2 O17 92.5(18) . 1_455 ?
O17 Cs2 O17 70.8(14) . 1_455 ?
O15 Cs2 O17 133.1(11) . 1_455 ?
O20 Cs2 O22 88(2) 1_465 . ?
O13 Cs2 O22 176.1(15) 1_455 . ?
O22 Cs2 O22 71.7(10) 1_455 . ?
O19 Cs2 O22 89(2) 1_455 . ?
O15 Cs2 O22 130(2) 1_455 . ?
O13 Cs2 O22 103.2(13) . . ?
O17 Cs2 O22 89(2) . . ?
O15 Cs2 O22 85(2) . . ?
O17 Cs2 O22 134(2) 1_455 . ?
O20 Cs2 O20 70.7(14) 1_465 1_565 ?
O13 Cs2 O20 134(2) 1_455 1_565 ?
O22 Cs2 O20 92(2) 1_455 1_565 ?
O19 Cs2 O20 131.3(10) 1_455 1_565 ?
O15 Cs2 O20 173.9(15) 1_455 1_565 ?
O13 Cs2 O20 84.6(18) . 1_565 ?
O17 Cs2 O20 48.3(19) . 1_565 ?
O15 Cs2 O20 103.0(15) . 1_565 ?
O17 Cs2 O20 95.2(18) 1_455 1_565 ?
O22 Cs2 O20 46(2) . 1_565 ?
O20 Cs2 O19 130.6(11) 1_465 . ?
O13 Cs2 O19 131.2(19) 1_455 . ?
O22 Cs2 O19 91(2) 1_455 . ?
O19 Cs2 O19 69.1(12) 1_455 . ?
O15 Cs2 O19 90.0(15) 1_455 . ?
O13 Cs2 O19 84.8(17) . . ?
O17 Cs2 O19 106.9(14) . . ?
O15 Cs2 O19 44.7(17) . . ?
O17 Cs2 O19 177.3(17) 1_455 . ?
O22 Cs2 O19 46(2) . . ?
O20 Cs2 O19 84.2(10) 1_565 . ?
O20 Cs2 O18 45.7(14) 1_465 1_565 ?
O13 Cs2 O18 95.1(18) 1_455 1_565 ?
O22 Cs2 O18 93(2) 1_455 1_565 ?
O19 Cs2 O18 141.8(13) 1_455 1_565 ?
O15 Cs2 O18 142.2(14) 1_455 1_565 ?
O13 Cs2 O18 88.0(17) . 1_565 ?
O17 Cs2 O18 41.8(13) . 1_565 ?
O15 Cs2 O18 130.9(13) . 1_565 ?
O17 Cs2 O18 51.8(13) 1_455 1_565 ?
O22 Cs2 O18 86(2) . 1_565 ?
O20 Cs2 O18 43.4(12) 1_565 1_565 ?
O19 Cs2 O18 127.6(12) . 1_565 ?
O20 Cs2 O16 93(2) 1_465 1_455 ?
O13 Cs2 O16 49.4(18) 1_455 1_455 ?
O22 Cs2 O16 141(2) 1_455 1_455 ?
O19 Cs2 O16 141.5(18) 1_455 1_455 ?
O15 Cs2 O16 95(2) 1_455 1_455 ?
O13 Cs2 O16 43.1(19) . 1_455 ?
O17 Cs2 O16 39.6(18) . 1_455 ?
O15 Cs2 O16 88(2) . 1_455 ?
O17 Cs2 O16 49.5(18) 1_455 1_455 ?
O22 Cs2 O16 128(2) . 1_455 ?
O20 Cs2 O16 87.0(19) 1_565 1_455 ?
O19 Cs2 O16 127.8(17) . 1_455 ?
O18 Cs2 O16 61.1(19) 1_565 1_455 ?
O20 Cs2 O12 142.6(18) 1_465 . ?
O13 Cs2 O12 47.8(18) 1_455 . ?
O22 Cs2 O12 137(2) 1_455 . ?
O19 Cs2 O12 89.5(18) 1_455 . ?
O15 Cs2 O12 47.6(16) 1_455 . ?
O13 Cs2 O12 45.2(17) . . ?
O17 Cs2 O12 88.6(18) . . ?
O15 Cs2 O12 43.4(16) . . ?
O17 Cs2 O12 92.4(18) 1_455 . ?
O22 Cs2 O12 129(2) . . ?
O20 Cs2 O12 129.5(16) 1_565 . ?
O19 Cs2 O12 86.0(17) . . ?
O18 Cs2 O12 122.6(16) 1_565 . ?
O16 Cs2 O12 61.6(11) 1_455 . ?
O20 Cs2 O21 91.6(15) 1_465 1_455 ?
O13 Cs2 O21 130.2(16) 1_455 1_455 ?
O22 Cs2 O21 43.7(19) 1_455 1_455 ?
O19 Cs2 O21 37.6(13) 1_455 1_455 ?
O15 Cs2 O21 83.1(14) 1_455 1_455 ?
O13 Cs2 O21 132.2(16) . 1_455 ?
O17 Cs2 O21 140.7(14) . 1_455 ?
O15 Cs2 O21 86.6(14) . 1_455 ?
O17 Cs2 O21 135.0(14) 1_455 1_455 ?
O22 Cs2 O21 51.5(17) . 1_455 ?
O20 Cs2 O21 94.6(13) 1_565 1_455 ?
O19 Cs2 O21 47.7(12) . 1_455 ?
O18 Cs2 O21 123.0(10) 1_565 1_455 ?
O16 Cs2 O21 174.9(19) 1_455 1_455 ?
O12 Cs2 O21 114.0(17) . 1_455 ?
O20 Cs2 O21 48.5(15) 1_465 2_656 ?
O13 Cs2 O21 143.4(17) 1_455 2_656 ?
O22 Cs2 O21 47.3(18) 1_455 2_656 ?
O19 Cs2 O21 90.7(13) 1_455 2_656 ?
O15 Cs2 O21 136.4(14) 1_455 2_656 ?
O13 Cs2 O21 129.2(14) . 2_656 ?
O17 Cs2 O21 90.4(15) . 2_656 ?
O15 Cs2 O21 125.4(14) . 2_656 ?
O17 Cs2 O21 97.9(15) 1_455 2_656 ?
O22 Cs2 O21 40.0(17) . 2_656 ?
O20 Cs2 O21 45.1(14) 1_565 2_656 ?
O19 Cs2 O21 83.6(12) . 2_656 ?
O18 Cs2 O21 62.0(10) 1_565 2_656 ?
O16 Cs2 O21 122.7(19) 1_455 2_656 ?
O12 Cs2 O21 168.7(14) . 2_656 ?
O21 Cs2 O21 61.0(2) 1_455 2_656 ?
O20 Cs2 Cs2 120.2(12) 1_465 1_655 ?
O13 Cs2 Cs2 124.5(11) 1_455 1_655 ?
O22 Cs2 Cs2 123.4(15) 1_455 1_655 ?
O19 Cs2 Cs2 121.0(10) 1_455 1_655 ?
O15 Cs2 Cs2 124.8(10) 1_455 1_655 ?
O13 Cs2 Cs2 51.5(11) . 1_655 ?
O17 Cs2 Cs2 55.0(11) . 1_655 ?
O15 Cs2 Cs2 53.5(11) . 1_655 ?
O17 Cs2 Cs2 125.9(12) 1_455 1_655 ?
O22 Cs2 Cs2 51.7(12) . 1_655 ?
O20 Cs2 Cs2 49.5(11) 1_565 1_655 ?
O19 Cs2 Cs2 51.9(9) . 1_655 ?
O18 Cs2 Cs2 84.1(7) 1_565 1_655 ?
O16 Cs2 Cs2 84.4(10) 1_455 1_655 ?
O12 Cs2 Cs2 86.7(9) . 1_655 ?
O21 Cs2 Cs2 92.9(5) 1_455 1_655 ?
O21 Cs2 Cs2 83.5(6) 2_656 1_655 ?
O20 Cs2 Cs2 59.8(12) 1_465 1_455 ?
O13 Cs2 Cs2 55.5(11) 1_455 1_455 ?
O22 Cs2 Cs2 56.6(15) 1_455 1_455 ?
O19 Cs2 Cs2 59.0(10) 1_455 1_455 ?
O15 Cs2 Cs2 55.2(10) 1_455 1_455 ?
O13 Cs2 Cs2 128.5(11) . 1_455 ?
O17 Cs2 Cs2 125.0(11) . 1_455 ?
O15 Cs2 Cs2 126.5(11) . 1_455 ?
O17 Cs2 Cs2 54.1(11) 1_455 1_455 ?
O22 Cs2 Cs2 128.3(12) . 1_455 ?
O20 Cs2 Cs2 130.5(11) 1_565 1_455 ?
O19 Cs2 Cs2 128.1(9) . 1_455 ?
O18 Cs2 Cs2 95.9(7) 1_565 1_455 ?
O16 Cs2 Cs2 95.6(10) 1_455 1_455 ?
O12 Cs2 Cs2 93.3(9) . 1_455 ?
O21 Cs2 Cs2 87.1(5) 1_455 1_455 ?
O21 Cs2 Cs2 96.5(6) 2_656 1_455 ?
Cs2 Cs2 Cs2 180.00(3) 1_655 1_455 ?
O20 Cs2 O18 141.2(14) 1_465 . ?
O13 Cs2 O18 93.4(17) 1_455 . ?
O22 Cs2 O18 92(2) 1_455 . ?
O19 Cs2 O18 45.3(12) 1_455 . ?
O15 Cs2 O18 48.6(12) 1_455 . ?
O13 Cs2 O18 86.9(17) . . ?
O17 Cs2 O18 130.6(14) . . ?
O15 Cs2 O18 40.8(13) . . ?
O17 Cs2 O18 138.9(14) 1_455 . ?
O22 Cs2 O18 85(2) . . ?
O20 Cs2 O18 125.6(13) 1_565 . ?
O19 Cs2 O18 41.5(11) . . ?
O18 Cs2 O18 168.4(14) 1_565 . ?
O16 Cs2 O18 120.1(19) 1_455 . ?
O12 Cs2 O18 59.1(16) . . ?
O21 Cs2 O18 55.2(10) 1_455 . ?
O21 Cs2 O18 114.1(10) 2_656 . ?
Cs2 Cs2 O18 84.5(7) 1_655 . ?
Cs2 Cs2 O18 95.5(7) 1_455 . ?
O6 Cs3 O2 62.0(10) 2_645 2_655 ?
O6 Cs3 O2 70.8(14) 2_645 . ?
O2 Cs3 O2 109.3(8) 2_655 . ?
O6 Cs3 O2 111.4(18) 2_645 1_455 ?
O2 Cs3 O2 168.0(10) 2_655 1_455 ?
O2 Cs3 O2 75.7(13) . 1_455 ?
O6 Cs3 O6 79.9(15) 2_645 2_545 ?
O2 Cs3 O6 103.6(12) 2_655 2_545 ?
O2 Cs3 O6 116.5(17) . 2_545 ?
O2 Cs3 O6 64.7(13) 1_455 2_545 ?
O6 Cs3 O6 159.7(15) 2_645 1_455 ?
O2 Cs3 O6 99.9(16) 2_655 1_455 ?
O2 Cs3 O6 127.2(11) . 1_455 ?
O2 Cs3 O6 84.7(10) 1_455 1_455 ?
O6 Cs3 O6 97.0(10) 2_545 1_455 ?
O6 Cs3 O6 106.7(11) 2_645 . ?
O2 Cs3 O6 64.2(14) 2_655 . ?
O2 Cs3 O6 84.7(11) . . ?
O2 Cs3 O6 127.7(11) 1_455 . ?
O6 Cs3 O6 158.6(16) 2_545 . ?
O6 Cs3 O6 69.6(11) 1_455 . ?
O6 Cs3 O2 103.1(13) 2_645 2 ?
O2 Cs3 O2 73.7(11) 2_655 2 ?
O2 Cs3 O2 169.4(17) . 2 ?
O2 Cs3 O2 99.4(8) 1_455 2 ?
O6 Cs3 O2 53.1(9) 2_545 2 ?
O6 Cs3 O2 60.6(12) 1_455 2 ?
O6 Cs3 O2 105.6(16) . 2 ?
O6 Cs3 O3 107.7(16) 2_645 . ?
O2 Cs3 O3 106.2(15) 2_655 . ?
O2 Cs3 O3 45.1(14) . . ?
O2 Cs3 O3 85.2(14) 1_455 . ?
O6 Cs3 O3 149.3(17) 2_545 . ?
O6 Cs3 O3 85.3(15) 1_455 . ?
O6 Cs3 O3 49.2(15) . . ?
O2 Cs3 O3 144.8(16) 2 . ?
O6 Cs3 O1 112.9(17) 2_645 . ?
O2 Cs3 O1 145.5(14) 2_655 . ?
O2 Cs3 O1 45.0(12) . . ?
O2 Cs3 O1 45.2(13) 1_455 . ?
O6 Cs3 O1 109.0(16) 2_545 . ?
O6 Cs3 O1 87.2(15) 1_455 . ?
O6 Cs3 O1 87.5(15) . . ?
O2 Cs3 O1 136.4(11) 2 . ?
O3 Cs3 O1 40.3(14) . . ?
O6 Cs3 O3 151.8(19) 2_645 1_455 ?
O2 Cs3 O3 145.3(17) 2_655 1_455 ?
O2 Cs3 O3 87.8(13) . 1_455 ?
O2 Cs3 O3 43.4(14) 1_455 1_455 ?
O6 Cs3 O3 94.4(14) 2_545 1_455 ?
O6 Cs3 O3 47.9(15) 1_455 1_455 ?
O6 Cs3 O3 88.6(14) . 1_455 ?
O2 Cs3 O3 95.0(12) 2 1_455 ?
O3 Cs3 O3 64.5(7) . 1_455 ?
O1 Cs3 O3 42.9(13) . 1_455 ?
O6 Cs3 Cs3 115.8(14) 2_645 2 ?
O2 Cs3 Cs3 54.7(12) 2_655 2 ?
O2 Cs3 Cs3 138.4(13) . 2 ?
O2 Cs3 Cs3 128.7(12) 1_455 2 ?
O6 Cs3 Cs3 104.9(11) 2_545 2 ?
O6 Cs3 Cs3 45.2(10) 1_455 2 ?
O6 Cs3 Cs3 53.7(10) . 2 ?
O2 Cs3 Cs3 51.8(10) 2 2 ?
O3 Cs3 Cs3 98.4(14) . 2 ?
O1 Cs3 Cs3 124.1(14) . 2 ?
O3 Cs3 Cs3 92.3(13) 1_455 2 ?
O6 Cs3 Cs3 60.4(12) 2_645 2_545 ?
O2 Cs3 Cs3 121.6(12) 2_655 2_545 ?
O2 Cs3 Cs3 58.7(10) . 2_545 ?
O2 Cs3 Cs3 51.0(11) 1_455 2_545 ?
O6 Cs3 Cs3 57.8(11) 2_545 2_545 ?
O6 Cs3 Cs3 134.3(13) 1_455 2_545 ?
O6 Cs3 Cs3 143.3(11) . 2_545 ?
O2 Cs3 Cs3 110.8(12) 2 2_545 ?
O3 Cs3 Cs3 99.2(13) . 2_545 ?
O1 Cs3 Cs3 69.8(14) . 2_545 ?
O3 Cs3 Cs3 93.1(14) 1_455 2_545 ?
Cs3 Cs3 Cs3 162.3(8) 2 2_545 ?
O6 Cs3 Cs3 124.4(12) 2_645 1_455 ?
O2 Cs3 Cs3 122.1(10) 2_655 1_455 ?
O2 Cs3 Cs3 127.5(10) . 1_455 ?
O2 Cs3 Cs3 51.8(10) 1_455 1_455 ?
O6 Cs3 Cs3 44.5(10) 2_545 1_455 ?
O6 Cs3 Cs3 55.5(10) 1_455 1_455 ?
O6 Cs3 Cs3 125.1(10) . 1_455 ?
O2 Cs3 Cs3 48.4(9) 2 1_455 ?
O3 Cs3 Cs3 120.2(8) . 1_455 ?
O1 Cs3 Cs3 89.8(7) . 1_455 ?
O3 Cs3 Cs3 55.7(7) 1_455 1_455 ?
Cs3 Cs3 Cs3 84.6(5) 2 1_455 ?
Cs3 Cs3 Cs3 84.6(5) 2_545 1_455 ?
O6 Cs3 Cs3 55.6(12) 2_645 1_655 ?
O2 Cs3 Cs3 57.9(10) 2_655 1_655 ?
O2 Cs3 Cs3 52.5(10) . 1_655 ?
O2 Cs3 Cs3 128.2(10) 1_455 1_655 ?
O6 Cs3 Cs3 135.5(10) 2_545 1_655 ?
O6 Cs3 Cs3 124.5(10) 1_455 1_655 ?
O6 Cs3 Cs3 54.9(10) . 1_655 ?
O2 Cs3 Cs3 131.6(9) 2 1_655 ?
O3 Cs3 Cs3 59.8(8) . 1_655 ?
O1 Cs3 Cs3 90.2(7) . 1_655 ?
O3 Cs3 Cs3 124.3(7) 1_455 1_655 ?
Cs3 Cs3 Cs3 95.4(5) 2 1_655 ?
Cs3 Cs3 Cs3 95.4(5) 2_545 1_655 ?
Cs3 Cs3 Cs3 180.0 1_455 1_655 ?
O6 Cs3 W1 94.9(13) 2_645 . ?
O2 Cs3 W1 121.8(11) 2_655 . ?
O2 Cs3 W1 24.2(8) . . ?
O2 Cs3 W1 67.1(10) 1_455 . ?
O6 Cs3 W1 125.2(13) 2_545 . ?
O6 Cs3 W1 103.1(10) 1_455 . ?
O6 Cs3 W1 75.3(10) . . ?
O2 Cs3 W1 160.8(9) 2 . ?
O3 Cs3 W1 27.1(12) . . ?
O1 Cs3 W1 25.3(7) . . ?
O3 Cs3 W1 65.8(9) 1_455 . ?
Cs3 Cs3 W1 125.3(7) 2 . ?
Cs3 Cs3 W1 72.1(4) 2_545 . ?
Cs3 Cs3 W1 115.0(3) 1_455 . ?
Cs3 Cs3 W1 65.0(3) 1_655 . ?
O6 Cs3 O7 148.9(14) 2_645 1_455 ?
O2 Cs3 O7 107.6(15) 2_655 1_455 ?
O2 Cs3 O7 87.6(12) . 1_455 ?
O2 Cs3 O7 83.2(13) 1_455 1_455 ?
O6 Cs3 O7 130.8(13) 2_545 1_455 ?
O6 Cs3 O7 41.1(13) 1_455 1_455 ?
O6 Cs3 O7 47.4(13) . 1_455 ?
O2 Cs3 O7 101.3(13) 2 1_455 ?
O3 Cs3 O7 44.2(13) . 1_455 ?
O1 Cs3 O7 57.6(8) . 1_455 ?
O3 Cs3 O7 41.3(13) 1_455 1_455 ?
Cs3 Cs3 O7 66.5(11) 2 1_455 ?
Cs3 Cs3 O7 126.6(12) 2_545 1_455 ?
Cs3 Cs3 O7 86.4(7) 1_455 1_455 ?
Cs3 Cs3 O7 93.6(7) 1_655 1_455 ?
W1 Cs3 O7 64.7(10) . 1_455 ?
O6 Cs3 W2 120.3(13) 2_645 . ?
O2 Cs3 W2 89.4(12) 2_655 . ?
O2 Cs3 W2 72.2(9) . . ?
O2 Cs3 W2 102.6(9) 1_455 . ?
O6 Cs3 W2 159.7(11) 2_545 . ?
O6 Cs3 W2 65.0(11) 1_455 . ?
O6 Cs3 W2 25.3(10) . . ?
O2 Cs3 W2 118.3(11) 2 . ?
O3 Cs3 W2 28.6(12) . . ?
O1 Cs3 W2 62.9(12) . . ?
O3 Cs3 W2 66.8(9) 1_455 . ?
Cs3 Cs3 W2 69.8(5) 2 . ?
Cs3 Cs3 W2 127.8(5) 2_545 . ?
Cs3 Cs3 W2 115.2(3) 1_455 . ?
Cs3 Cs3 W2 64.8(3) 1_655 . ?
W1 Cs3 W2 55.62(19) . . ?
O7 Cs3 W2 28.9(8) 1_455 . ?
O6 Cs3 W1 126.8(14) 2_645 1_455 ?
O2 Cs3 W1 170.1(12) 2_655 1_455 ?
O2 Cs3 W1 72.6(10) . 1_455 ?
O2 Cs3 W1 21.0(8) 1_455 1_455 ?
O6 Cs3 W1 83.5(12) 2_545 1_455 ?
O6 Cs3 W1 72.2(10) 1_455 1_455 ?
O6 Cs3 W1 106.8(10) . 1_455 ?
O2 Cs3 W1 106.2(9) 2 1_455 ?
O3 Cs3 W1 67.9(9) . 1_455 ?
O1 Cs3 W1 31.3(7) . 1_455 ?
O3 Cs3 W1 25.3(12) 1_455 1_455 ?
Cs3 Cs3 W1 117.2(6) 2 1_455 ?
Cs3 Cs3 W1 67.9(6) 2_545 1_455 ?
Cs3 Cs3 W1 58.59(19) 1_455 1_455 ?
Cs3 Cs3 W1 121.41(19) 1_655 1_455 ?
W1 Cs3 W1 56.4(3) . 1_455 ?
O7 Cs3 W1 62.6(9) 1_455 1_455 ?
W2 Cs3 W1 81.9(3) . 1_455 ?
O6 Cs3 W2 174.4(13) 2_645 1_455 ?
O2 Cs3 W2 117.9(12) 2_655 1_455 ?
O2 Cs3 W2 104.7(9) . 1_455 ?
O2 Cs3 W2 69.8(9) 1_455 1_455 ?
O6 Cs3 W2 105.3(11) 2_545 1_455 ?
O6 Cs3 W2 23.5(10) 1_455 1_455 ?
O6 Cs3 W2 69.2(10) . 1_455 ?
O2 Cs3 W2 81.9(9) 2 1_455 ?
O3 Cs3 W2 66.8(10) . 1_455 ?
O1 Cs3 W2 63.8(11) . 1_455 ?
O3 Cs3 W2 27.5(11) 1_455 1_455 ?
Cs3 Cs3 W2 65.2(4) 2 1_455 ?
Cs3 Cs3 W2 120.4(8) 2_545 1_455 ?
Cs3 Cs3 W2 60.8(3) 1_455 1_455 ?
Cs3 Cs3 W2 119.2(3) 1_655 1_455 ?
W1 Cs3 W2 80.5(3) . 1_455 ?
O7 Cs3 W2 25.7(8) 1_455 1_455 ?
W2 Cs3 W2 54.5(2) . 1_455 ?
W1 Cs3 W2 52.85(19) 1_455 1_455 ?
W1 O1 W1 169(5) . 1_455 ?
W1 O1 Cs3 86(3) . . ?
W1 O1 Cs3 87(2) 1_455 . ?
W1 O1 Cs1 98(3) . . ?
W1 O1 Cs1 89(2) 1_455 . ?
Cs3 O1 Cs1 175(2) . . ?
W1 O2 Cs3 141(3) . 2_645 ?
W1 O2 Cs3 106(2) . . ?
Cs3 O2 Cs3 112.6(14) 2_645 . ?
W1 O2 Cs3 117(2) . 1_655 ?
Cs3 O2 Cs3 74.4(10) 2_645 1_655 ?
Cs3 O2 Cs3 75.7(13) . 1_655 ?
W1 O2 Cs3 122(2) . 2_545 ?
Cs3 O2 Cs3 73.7(11) 2_645 2_545 ?
Cs3 O2 Cs3 69.4(10) . 2_545 ?
Cs3 O2 Cs3 117.6(14) 1_655 2_545 ?
W1 O3 W2 173(3) . . ?
W1 O3 Cs3 89.7(19) . . ?
W2 O3 Cs3 92.9(19) . . ?
W1 O3 Cs3 93(2) . 1_655 ?
W2 O3 Cs3 93.2(18) . 1_655 ?
Cs3 O3 Cs3 64.5(7) . 1_655 ?
W1 O4 W2 137(2) . 1_545 ?
W1 O4 Cs1 111(3) . 1_655 ?
W2 O4 Cs1 105(3) 1_545 1_655 ?
W1 O4 Cs1 107(3) . . ?
W2 O4 Cs1 105(3) 1_545 . ?
Cs1 O4 Cs1 73.2(8) 1_655 . ?
W3 O5 W1 139(4) . . ?
W3 O5 Cs1 113(4) . . ?
W1 O5 Cs1 102(2) . . ?
W3 O5 Cs1 108(3) . 1_655 ?
W1 O5 Cs1 101(2) . 1_655 ?
Cs1 O5 Cs1 74.7(17) . 1_655 ?
W2 O6 Cs3 145(3) . 2_655 ?
W2 O6 Cs3 125(3) . 2 ?
Cs3 O6 Cs3 79.9(15) 2_655 2 ?
W2 O6 Cs3 108(2) . 1_655 ?
Cs3 O6 Cs3 74.3(13) 2_655 1_655 ?
Cs3 O6 Cs3 116.5(18) 2 1_655 ?
W2 O6 Cs3 101(2) . . ?
Cs3 O6 Cs3 112.0(19) 2_655 . ?
Cs3 O6 Cs3 68.4(11) 2 . ?
Cs3 O6 Cs3 69.6(11) 1_655 . ?
W2 O7 W2 161(4) . 1_655 ?
W2 O7 Cs1 98(2) . 1_665 ?
W2 O7 Cs1 99(2) 1_655 1_665 ?
W2 O7 Cs3 85(2) . 1_655 ?
W2 O7 Cs3 78.2(19) 1_655 1_655 ?
Cs1 O7 Cs3 176.9(16) 1_665 1_655 ?
W3 O8 W2 144(3) . . ?
W3 O8 Cs1 107(2) . 1_665 ?
W2 O8 Cs1 99.8(17) . 1_665 ?
W3 O8 Cs1 109(2) . 1_565 ?
W2 O8 Cs1 101.4(16) . 1_565 ?
Cs1 O8 Cs1 73.6(11) 1_665 1_565 ?
W3 O9 W3 157(2) . 1_455 ?
W3 O9 Cs1 107.7(17) . . ?
W3 O9 Cs1 89.4(12) 1_455 . ?
W3 O9 Cs1 85.5(14) . 1_565 ?
W3 O9 Cs1 75.5(10) 1_455 1_565 ?
Cs1 O9 Cs1 163.9(14) . 1_565 ?
W5 O10 W3 159(3) . . ?
W5 O10 Cs1 101.8(19) . 1_665 ?
W3 O10 Cs1 99(2) . 1_665 ?
W5 O10 Cs1 102.4(19) . 1_565 ?
W3 O10 Cs1 90.7(19) . 1_565 ?
Cs1 O10 Cs1 67.4(10) 1_665 1_565 ?
W4 O11 W3 147(3) . . ?
W4 O11 Cs1 114.0(19) . 1_655 ?
W3 O11 Cs1 99(2) . 1_655 ?
W4 O11 Cs1 98.7(18) . . ?
W3 O11 Cs1 91.9(17) . . ?
Cs1 O11 Cs1 68.7(10) 1_655 . ?
W4 O12 W4 172(5) . 1_455 ?
W4 O12 Cs2 95(3) . . ?
W4 O12 Cs2 88(2) 1_455 . ?
W4 O12 Cs1 91(3) . . ?
W4 O12 Cs1 86(2) 1_455 . ?
Cs2 O12 Cs1 173(2) . . ?
W4 O13 W5 143(2) . . ?
W4 O13 Cs2 109(3) . 1_655 ?
W5 O13 Cs2 100(3) . 1_655 ?
W4 O13 Cs2 101(3) . . ?
W5 O13 Cs2 109(3) . . ?
Cs2 O13 Cs2 73.0(8) 1_655 . ?
W5 O14 W4 153(3) 1_545 . ?
W5 O14 Cs1 100(3) 1_545 1_655 ?
W4 O14 Cs1 106(2) . 1_655 ?
W5 O14 Cs1 104(3) 1_545 . ?
W4 O14 Cs1 95(2) . . ?
Cs1 O14 Cs1 67.7(9) 1_655 . ?
W6 O15 W4 148(4) . . ?
W6 O15 Cs2 105(3) . 1_655 ?
W4 O15 Cs2 101(2) . 1_655 ?
W6 O15 Cs2 107(3) . . ?
W4 O15 Cs2 98(2) . . ?
Cs2 O15 Cs2 71.3(13) 1_655 . ?
W5 O16 W5 172(5) . 1_655 ?
W5 O16 Cs2 88(3) . 1_655 ?
W5 O16 Cs2 99(3) 1_655 1_655 ?
W5 O16 Cs1 81(3) . 1_665 ?
W5 O16 Cs1 91(3) 1_655 1_665 ?
Cs2 O16 Cs1 169.4(19) 1_655 1_665 ?
W5 O17 W6 147(4) . 1_565 ?
W5 O17 Cs2 110(3) . . ?
W6 O17 Cs2 103(3) 1_565 . ?
W5 O17 Cs2 94(2) . 1_655 ?
W6 O17 Cs2 98(3) 1_565 1_655 ?
Cs2 O17 Cs2 70.8(14) . 1_655 ?
W6 O18 W6 170(3) . 1_455 ?
W6 O18 Cs2 100(3) . 1_545 ?
W6 O18 Cs2 87.0(18) 1_455 1_545 ?
W6 O18 Cs2 92(2) . . ?
W6 O18 Cs2 81.6(19) 1_455 . ?
Cs2 O18 Cs2 168.4(14) 1_545 . ?
W7 O19 W6 154(3) . . ?
W7 O19 Cs2 102.2(19) . 1_655 ?
W6 O19 Cs2 103(2) . 1_655 ?
W7 O19 Cs2 98(2) . . ?
W6 O19 Cs2 98(2) . . ?
Cs2 O19 Cs2 69.1(12) 1_655 . ?
W7 O20 W6 148(4) 2_646 . ?
W7 O20 Cs2 107(2) 2_646 1_645 ?
W6 O20 Cs2 105(3) . 1_645 ?
W7 O20 Cs2 95(2) 2_646 1_545 ?
W6 O20 Cs2 95(2) . 1_545 ?
Cs2 O20 Cs2 70.7(14) 1_645 1_545 ?
W7 O21 W7 167(3) . 1_655 ?
W7 O21 Cs2 93(2) . 1_655 ?
W7 O21 Cs2 87.3(15) 1_655 1_655 ?
W7 O21 Cs2 95(2) . 2_646 ?
W7 O21 Cs2 82.7(15) 1_655 2_646 ?
Cs2 O21 Cs2 167.8(13) 1_655 2_646 ?
W7 O22 W7 149(3) 2_656 . ?
W7 O22 Cs2 104(3) 2_656 1_655 ?
W7 O22 Cs2 103(3) . 1_655 ?
W7 O22 Cs2 100(3) 2_656 . ?
W7 O22 Cs2 102(3) . . ?
Cs2 O22 Cs2 71.7(10) 1_655 . ?

_refine_diff_density_max         8.990
_refine_diff_density_min         -11.986
_refine_diff_density_rms         1.062


_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Rb2W7O22
_database_code_depnum_ccdc_archive 'CCDC 2211341'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_Rb2W7O22            
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form


_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'O22 Rb2 W7'
_chemical_formula_weight         1809.89

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 21'
_space_group_name_Hall           'P 2yb'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   3.8318(5)
_cell_length_b                   7.3295(12)
_cell_length_c                   32.060(4)
_cell_angle_alpha                90
_cell_angle_beta                 90.051(6)
_cell_angle_gamma                90
_cell_volume                     900.4(2)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    782
_cell_measurement_theta_min      3.18
_cell_measurement_theta_max      30.55

_exptl_crystal_description       plate
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    6.676
_exptl_crystal_F_000             1536
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.171
_exptl_crystal_size_mid          0.062
_exptl_crystal_size_min          0.023
_exptl_absorpt_coefficient_mu    50.002
_shelx_estimated_absorpt_T_min   0.043
_shelx_estimated_absorpt_T_max   0.393
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.1641
_exptl_absorpt_correction_T_max  0.4330
_exptl_absorpt_process_details   
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.1640 before and 0.0679 after correction.
The Ratio of minimum to maximum transmission is 0.3790.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_diffrn_reflns_number            7716
_diffrn_reflns_av_unetI/netI     0.1126
_diffrn_reflns_av_R_equivalents  0.0524
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -45
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_theta_min         1.270
_diffrn_reflns_theta_max         30.539
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             5245
_reflns_number_gt                4238
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.867
_reflns_Friedel_fraction_max     0.998
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0935P)²+52.5455P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_chemical_absolute_configuration ?
_refine_ls_number_reflns         5245
_refine_ls_number_parameters     184
_refine_ls_number_restraints     4
_refine_ls_R_factor_all          0.1040
_refine_ls_R_factor_gt           0.0863
_refine_ls_wR_factor_ref         0.2295
_refine_ls_wR_factor_gt          0.2131
_refine_ls_goodness_of_fit_ref   1.074
_refine_ls_restrained_S_all      1.074
_refine_ls_shift/su_max          2.277
_refine_ls_shift/su_mean         0.123

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.5007(9) 0.248(3) 0.09935(10) 0.0195(10) Uani 1 1 d D . . . .
W2 W 0.4851(15) 0.761(3) 0.09960(9) 0.043(2) Uani 1 1 d . . . . .
W3 W 0.4987(14) 0.509(3) 0.20056(6) 0.0251(9) Uani 1 1 d D . . . .
W4 W 0.4623(5) 0.264(3) 0.30354(11) 0.0116(7) Uani 1 1 d D . . . .
W5 W 0.5802(6) 0.756(3) 0.30261(12) 0.0134(6) Uani 1 1 d . . . . .
W6 W 0.485(2) 0.007(3) 0.40110(6) 0.0440(15) Uani 1 1 d . . . . .
W7 W 0.4840(13) 0.259(3) 0.5006(2) 0.0397(9) Uani 1 1 d . . . . .
Rb1 Rb -0.011(6) 0.000000 0.1986(2) 0.051(4) Uani 0.756(4) 1 d . . P . .
Rb2 Rb 0.018(8) 0.493(3) 0.4016(3) 0.046(5) Uani 0.574(4) 1 d . . P . .
Rb3 Rb 0.049(3) 0.501(5) 0.0064(3) 0.081(6) Uani 0.670(4) 1 d . . P . .
O1 O 0.547(14) 0.204(8) 0.0485(17) 0.031(12) Uiso 1 1 d . . . . .
O2 O 0.048(11) 0.243(10) 0.1012(15) 0.037(13) Uiso 1 1 d D . . . .
O3 O 0.472(15) 0.008(10) 0.1205(9) 0.021(7) Uiso 1 1 d . . . . .
O4 O 0.507(13) 0.511(9) 0.0938(8) 0.014(6) Uiso 1 1 d . . . . .
O5 O 0.465(10) 0.318(6) 0.1659(12) 0.009(7) Uiso 1 1 d . . . . .
O6 O 0.527(13) 0.812(7) 0.0465(15) 0.022(10) Uiso 1 1 d . . . . .
O7 O 0.976(10) 0.742(7) 0.1137(13) 0.019(8) Uiso 1 1 d . . . . .
O8 O 0.445(11) 0.694(6) 0.1661(13) 0.015(8) Uiso 1 1 d . . . . .
O9 O 0.968(14) 0.47(3) 0.206(3) 0.15(4) Uiso 1 1 d D . . . .
O10 O 0.524(11) 0.326(6) 0.2485(12) 0.009(7) Uiso 1 1 d . . . . .
O11 O 0.548(12) 0.691(6) 0.2511(14) 0.014(8) Uiso 1 1 d . . . . .
O12 O 0.888(10) 0.276(8) 0.3158(15) 0.033(11) Uiso 1 1 d D . . . .
O13 O 0.472(12) 0.514(7) 0.3212(8) 0.012(6) Uiso 1 1 d . . . . .
O14 O 0.541(12) 0.009(10) 0.2907(10) 0.021(7) Uiso 1 1 d . . . . .
O15 O 0.451(13) 0.189(7) 0.3619(16) 0.024(11) Uiso 1 1 d . . . . .
O16 O 0.123(8) 0.778(5) 0.2995(9) -0.001(5) Uiso 1 1 d . . . . .
O17 O 0.469(11) 0.827(6) 0.3625(14) 0.016(9) Uiso 1 1 d . . . . .
O18 O 0.049(18) 0.065(7) 0.4058(14) 0.031(13) Uiso 1 1 d . . . . .
O19 O 0.533(11) -0.172(6) 0.4430(13) 0.014(8) Uiso 1 1 d . . . . .
O20 O 0.548(14) 0.183(7) 0.4451(17) 0.025(11) Uiso 1 1 d . . . . .
O21 O 0.971(13) 0.276(9) 0.4939(17) 0.035(13) Uiso 1 1 d . . . . .
O22 O 0.483(17) 0.510(11) 0.4838(10) 0.024(7) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.67(6) . ?
W1 O2 1.74(4) . ?
W1 O3 1.89(7) . ?
W1 O4 1.93(6) . ?
W1 O2 2.10(4) 1_655 ?
W1 O5 2.20(4) . ?
W1 Rb3 3.911(15) . ?
W1 Rb3 4.09(2) 1_655 ?
W1 Rb1 4.113(13) 1_655 ?
W1 Rb1 4.158(15) . ?
W1 Rb3 4.216(18) 2_645 ?
W1 Rb3 4.382(14) 2_545 ?
W2 O6 1.75(5) . ?
W2 O4 1.85(6) . ?
W2 O7 1.94(4) . ?
W2 O3 1.93(7) 1_565 ?
W2 O7 2.01(4) 1_455 ?
W2 O8 2.19(4) . ?
W2 Rb3 3.92(2) . ?
W2 Rb1 4.093(17) 1_565 ?
W2 Rb1 4.103(15) 1_665 ?
W2 Rb3 4.153(18) 1_655 ?
W2 Rb3 4.223(17) 2_655 ?
W2 Rb3 4.336(19) 2 ?
W3 O8 1.76(4) . ?
W3 O5 1.79(4) . ?
W3 O9 1.82(7) . ?
W3 O10 2.04(4) . ?
W3 O9 2.06(6) 1_455 ?
W3 O11 2.11(4) . ?
W3 Rb1 4.06(2) 1_665 ?
W3 Rb1 4.10(2) 1_565 ?
W3 Rb1 4.18(2) 1_655 ?
W3 Rb1 4.21(2) . ?
W4 O12 1.68(4) . ?
W4 O10 1.84(4) . ?
W4 O13 1.92(5) . ?
W4 O14 1.93(7) . ?
W4 O15 1.95(5) . ?
W4 O12 2.24(4) 1_455 ?
W4 Rb2 3.951(18) . ?
W4 Rb2 4.151(19) 1_655 ?
W4 Rb1 4.284(14) . ?
W4 Rb1 4.376(16) 1_655 ?
W5 O11 1.72(4) . ?
W5 O16 1.76(3) . ?
W5 O14 1.90(7) 1_565 ?
W5 O13 1.91(5) . ?
W5 O17 2.03(4) . ?
W5 O16 2.09(3) 1_655 ?
W5 Rb2 4.073(16) 1_655 ?
W5 Rb1 4.098(14) 1_665 ?
W5 Rb2 4.29(2) . ?
W5 Rb1 4.411(14) 1_565 ?
W6 O18 1.73(7) . ?
W6 O17 1.81(4) 1_545 ?
W6 O15 1.84(5) . ?
W6 O19 1.89(4) . ?
W6 O20 1.93(5) . ?
W6 O18 2.21(7) 1_655 ?
W6 Rb2 3.99(2) . ?
W6 Rb2 4.11(3) 1_655 ?
W6 Rb2 4.17(3) 1_545 ?
W6 Rb2 4.29(2) 1_645 ?
W7 O21 1.88(5) . ?
W7 O19 1.88(4) 2_656 ?
W7 O20 1.88(5) . ?
W7 O22 1.89(8) 2_646 ?
W7 O22 1.92(8) . ?
W7 O21 1.98(5) 1_455 ?
W7 Rb2 4.023(17) . ?
W7 Rb2 4.15(2) 1_655 ?
W7 Rb2 4.155(18) 2_646 ?
W7 Rb2 4.17(2) 2_546 ?
Rb1 O8 3.03(5) 1_545 ?
Rb1 O3 3.12(5) . ?
Rb1 O5 3.14(4) . ?
Rb1 O3 3.19(4) 1_455 ?
Rb1 O8 3.23(5) 1_445 ?
Rb1 O5 3.25(4) 1_455 ?
Rb1 O11 3.29(5) 1_445 ?
Rb1 O7 3.31(5) 1_445 ?
Rb1 O10 3.38(4) 1_455 ?
Rb1 O14 3.42(4) 1_455 ?
Rb1 O10 3.53(4) . ?
Rb1 O11 3.54(5) 1_545 ?
Rb1 O2 3.60(5) . ?
Rb1 O14 3.63(4) . ?
Rb1 O16 3.66(3) 1_545 ?
Rb1 O9 3.5(2) 1_455 ?
Rb1 O9 3.9(2) 1_445 ?
Rb1 Rb1 3.8318(5) 1_655 ?
Rb1 Rb1 3.8318(5) 1_455 ?
Rb2 O15 3.05(5) . ?
Rb2 O13 3.12(4) . ?
Rb2 O18 3.14(5) . ?
Rb2 O22 3.18(5) . ?
Rb2 O20 3.22(6) 1_455 ?
Rb2 O17 3.25(5) . ?
Rb2 O12 3.21(5) 1_455 ?
Rb2 O13 3.32(4) 1_455 ?
Rb2 O22 3.34(5) 1_455 ?
Rb2 O20 3.35(6) . ?
Rb2 O19 3.35(5) 1_465 ?
Rb2 O15 3.36(5) 1_455 ?
Rb2 O21 3.37(6) 1_455 ?
Rb2 O19 3.42(5) 1_565 ?
Rb2 O17 3.46(5) 1_455 ?
Rb2 Rb2 3.8318(7) 1_455 ?
Rb2 Rb2 3.8318(7) 1_655 ?
Rb2 O16 3.90(3) . ?
Rb2 O21 3.94(6) 2_656 ?
Rb3 O6 2.73(5) 2_645 ?
Rb3 O1 2.78(6) 2_655 ?
Rb3 O6 3.11(5) 2_545 ?
Rb3 O1 3.19(6) . ?
Rb3 O6 3.19(6) . ?
Rb3 O1 3.21(6) 1_455 ?
Rb3 O1 3.24(6) 2 ?
Rb3 O6 3.29(5) 1_455 ?
Rb3 O4 3.31(4) . ?
Rb3 O4 3.49(4) 1_455 ?
Rb3 O2 3.58(6) . ?
Rb3 Rb3 3.706(3) 2 ?
Rb3 Rb3 3.706(3) 2_545 ?
Rb3 Rb3 3.8318(5) 1_655 ?
Rb3 Rb3 3.8318(5) 1_455 ?
Rb3 O7 3.88(5) 1_455 ?
Rb3 O2 3.90(6) 2 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 98(3) . . ?
O1 W1 O3 100(2) . . ?
O2 W1 O3 85(3) . . ?
O1 W1 O4 96(2) . . ?
O2 W1 O4 92(3) . . ?
O3 W1 O4 164.0(15) . . ?
O1 W1 O2 85(2) . 1_655 ?
O2 W1 O2 176(3) . 1_655 ?
O3 W1 O2 92(2) . 1_655 ?
O4 W1 O2 90(2) . 1_655 ?
O1 W1 O5 177(2) . . ?
O2 W1 O5 84.7(19) . . ?
O3 W1 O5 82.1(16) . . ?
O4 W1 O5 81.9(13) . . ?
O2 W1 O5 92.3(17) 1_655 . ?
O1 W1 Rb3 52.9(19) . . ?
O2 W1 Rb3 66.1(18) . . ?
O3 W1 Rb3 133.5(14) . . ?
O4 W1 Rb3 57.6(11) . . ?
O2 W1 Rb3 118.2(15) 1_655 . ?
O5 W1 Rb3 127.0(10) . . ?
O1 W1 Rb3 47.5(19) . 1_655 ?
O2 W1 Rb3 123.3(18) . 1_655 ?
O3 W1 Rb3 135.5(16) . 1_655 ?
O4 W1 Rb3 58.4(12) . 1_655 ?
O2 W1 Rb3 61.0(15) 1_655 1_655 ?
O5 W1 Rb3 129.5(10) . 1_655 ?
Rb3 W1 Rb3 57.2(3) . 1_655 ?
O1 W1 Rb1 128.2(19) . 1_655 ?
O2 W1 Rb1 114.6(18) . 1_655 ?
O3 W1 Rb1 48.4(14) . 1_655 ?
O4 W1 Rb1 120.4(11) . 1_655 ?
O2 W1 Rb1 61.1(15) 1_655 1_655 ?
O5 W1 Rb1 51.7(10) . 1_655 ?
Rb3 W1 Rb1 178.0(6) . 1_655 ?
Rb3 W1 Rb1 122.0(3) 1_655 1_655 ?
O1 W1 Rb1 135.2(19) . . ?
O2 W1 Rb1 59.5(18) . . ?
O3 W1 Rb1 44.8(15) . . ?
O4 W1 Rb1 120.8(11) . . ?
O2 W1 Rb1 116.3(15) 1_655 . ?
O5 W1 Rb1 47.8(10) . . ?
Rb3 W1 Rb1 125.5(4) . . ?
Rb3 W1 Rb1 176.7(3) 1_655 . ?
Rb1 W1 Rb1 55.20(15) 1_655 . ?
O1 W1 Rb3 24.3(19) . 2_645 ?
O2 W1 Rb3 115.3(18) . 2_645 ?
O3 W1 Rb3 84.9(14) . 2_645 ?
O4 W1 Rb3 110.4(11) . 2_645 ?
O2 W1 Rb3 66.7(15) 1_655 2_645 ?
O5 W1 Rb3 155.0(10) . 2_645 ?
Rb3 W1 Rb3 76.84(19) . 2_645 ?
Rb3 W1 Rb3 52.98(6) 1_655 2_645 ?
Rb1 W1 Rb3 104.2(4) 1_655 2_645 ?
Rb1 W1 Rb3 128.4(5) . 2_645 ?
O1 W1 Rb3 38.3(18) . 2_545 ?
O2 W1 Rb3 62.5(18) . 2_545 ?
O3 W1 Rb3 82.2(13) . 2_545 ?
O4 W1 Rb3 110.3(11) . 2_545 ?
O2 W1 Rb3 119.6(15) 1_655 2_545 ?
O5 W1 Rb3 144.7(10) . 2_545 ?
Rb3 W1 Rb3 52.72(6) . 2_545 ?
Rb3 W1 Rb3 82.54(19) 1_655 2_545 ?
Rb1 W1 Rb3 129.3(5) 1_655 2_545 ?
Rb1 W1 Rb3 100.6(3) . 2_545 ?
Rb3 W1 Rb3 52.9(2) 2_645 2_545 ?
O6 W2 O4 96.2(18) . . ?
O6 W2 O7 99(2) . . ?
O4 W2 O7 85(2) . . ?
O6 W2 O3 98(2) . 1_565 ?
O4 W2 O3 165.4(15) . 1_565 ?
O7 W2 O3 91(2) . 1_565 ?
O6 W2 O7 109(2) . 1_455 ?
O4 W2 O7 90(2) . 1_455 ?
O7 W2 O7 152(2) . 1_455 ?
O3 W2 O7 88(2) 1_565 1_455 ?
O6 W2 O8 178.5(19) . . ?
O4 W2 O8 82.9(14) . . ?
O7 W2 O8 79.9(17) . . ?
O3 W2 O8 82.6(16) 1_565 . ?
O7 W2 O8 72.4(16) 1_455 . ?
O6 W2 Rb3 53.2(16) . . ?
O4 W2 Rb3 57.3(11) . . ?
O7 W2 Rb3 123.7(14) . . ?
O3 W2 Rb3 135.3(14) 1_565 . ?
O7 W2 Rb3 73.9(13) 1_455 . ?
O8 W2 Rb3 127.0(12) . . ?
O6 W2 Rb1 135.0(16) . 1_565 ?
O4 W2 Rb1 121.6(12) . 1_565 ?
O7 W2 Rb1 107.6(13) . 1_565 ?
O3 W2 Rb1 47.0(15) 1_565 1_565 ?
O7 W2 Rb1 53.4(13) 1_455 1_565 ?
O8 W2 Rb1 46.4(11) . 1_565 ?
Rb3 W2 Rb1 126.9(3) . 1_565 ?
O6 W2 Rb1 128.2(16) . 1_665 ?
O4 W2 Rb1 118.7(11) . 1_665 ?
O7 W2 Rb1 52.8(14) . 1_665 ?
O3 W2 Rb1 49.0(14) 1_565 1_665 ?
O7 W2 Rb1 108.2(13) 1_455 1_665 ?
O8 W2 Rb1 51.5(11) . 1_665 ?
Rb3 W2 Rb1 175.7(5) . 1_665 ?
Rb1 W2 Rb1 55.74(18) 1_565 1_665 ?
O6 W2 Rb3 49.4(16) . 1_655 ?
O4 W2 Rb3 56.4(13) . 1_655 ?
O7 W2 Rb3 68.2(13) . 1_655 ?
O3 W2 Rb3 134.0(16) 1_565 1_655 ?
O7 W2 Rb3 129.4(13) 1_455 1_655 ?
O8 W2 Rb3 129.2(11) . 1_655 ?
Rb3 W2 Rb3 56.6(3) . 1_655 ?
Rb1 W2 Rb3 175.1(3) 1_565 1_655 ?
Rb1 W2 Rb3 120.5(4) 1_665 1_655 ?
O6 W2 Rb3 24.5(16) . 2_655 ?
O4 W2 Rb3 108.3(12) . 2_655 ?
O7 W2 Rb3 78.9(13) . 2_655 ?
O3 W2 Rb3 84.3(14) 1_565 2_655 ?
O7 W2 Rb3 128.5(13) 1_455 2_655 ?
O8 W2 Rb3 154.9(11) . 2_655 ?
Rb3 W2 Rb3 76.68(19) . 2_655 ?
Rb1 W2 Rb3 130.0(5) 1_565 2_655 ?
Rb1 W2 Rb3 104.2(4) 1_665 2_655 ?
Rb3 W2 Rb3 52.52(6) 1_655 2_655 ?
O6 W2 Rb3 36.4(16) . 2 ?
O4 W2 Rb3 110.2(11) . 2 ?
O7 W2 Rb3 132.0(13) . 2 ?
O3 W2 Rb3 83.1(13) 1_565 2 ?
O7 W2 Rb3 75.4(13) 1_455 2 ?
O8 W2 Rb3 145.1(12) . 2 ?
Rb3 W2 Rb3 53.06(5) . 2 ?
Rb1 W2 Rb3 102.4(4) 1_565 2 ?
Rb1 W2 Rb3 130.9(5) 1_665 2 ?
Rb3 W2 Rb3 82.38(19) 1_655 2 ?
Rb3 W2 Rb3 53.2(2) 2_655 2 ?
O8 W3 O5 101.8(13) . . ?
O8 W3 O9 106(6) . . ?
O5 W3 O9 91(6) . . ?
O8 W3 O10 169.6(18) . . ?
O5 W3 O10 87.4(16) . . ?
O9 W3 O10 78(5) . . ?
O8 W3 O9 92(6) . 1_455 ?
O5 W3 O9 83(6) . 1_455 ?
O9 W3 O9 162(10) . 1_455 ?
O10 W3 O9 84(5) . 1_455 ?
O8 W3 O11 90.3(18) . . ?
O5 W3 O11 167.9(17) . . ?
O9 W3 O11 86(5) . . ?
O10 W3 O11 80.5(10) . . ?
O9 W3 O11 96(5) 1_455 . ?
O8 W3 Rb1 50.3(14) . 1_665 ?
O5 W3 Rb1 135.8(12) . 1_665 ?
O9 W3 Rb1 71(8) . 1_665 ?
O10 W3 Rb1 125.0(11) . 1_665 ?
O9 W3 Rb1 125(7) 1_455 1_665 ?
O11 W3 Rb1 53.7(11) . 1_665 ?
O8 W3 Rb1 42.2(14) . 1_565 ?
O5 W3 Rb1 130.0(12) . 1_565 ?
O9 W3 Rb1 126(8) . 1_565 ?
O10 W3 Rb1 127.7(11) . 1_565 ?
O9 W3 Rb1 69(7) 1_455 1_565 ?
O11 W3 Rb1 59.8(12) . 1_565 ?
Rb1 W3 Rb1 56.0(3) 1_665 1_565 ?
O8 W3 Rb1 136.9(14) . 1_655 ?
O5 W3 Rb1 47.5(12) . 1_655 ?
O9 W3 Rb1 55(7) . 1_655 ?
O10 W3 Rb1 53.4(11) . 1_655 ?
O9 W3 Rb1 110(7) 1_455 1_655 ?
O11 W3 Rb1 122.5(12) . 1_655 ?
Rb1 W3 Rb1 125.7(6) 1_665 1_655 ?
Rb1 W3 Rb1 177.5(5) 1_565 1_655 ?
O8 W3 Rb1 128.2(14) . . ?
O5 W3 Rb1 42.7(12) . . ?
O9 W3 Rb1 110(7) . . ?
O10 W3 Rb1 56.7(11) . . ?
O9 W3 Rb1 55(7) 1_455 . ?
O11 W3 Rb1 128.0(11) . . ?
Rb1 W3 Rb1 178.2(2) 1_665 . ?
Rb1 W3 Rb1 123.8(6) 1_565 . ?
Rb1 W3 Rb1 54.4(2) 1_655 . ?
O12 W4 O10 95(2) . . ?
O12 W4 O13 82(2) . . ?
O10 W4 O13 92.5(14) . . ?
O12 W4 O14 87(2) . . ?
O10 W4 O14 90.8(15) . . ?
O13 W4 O14 168.8(15) . . ?
O12 W4 O15 79(2) . . ?
O10 W4 O15 174(2) . . ?
O13 W4 O15 89.2(16) . . ?
O14 W4 O15 86.4(17) . . ?
O12 W4 O12 156(3) . 1_455 ?
O10 W4 O12 106.6(18) . 1_455 ?
O13 W4 O12 85.9(19) . 1_455 ?
O14 W4 O12 103(2) . 1_455 ?
O15 W4 O12 79.7(19) . 1_455 ?
O12 W4 Rb2 102.1(19) . . ?
O10 W4 Rb2 135.7(12) . . ?
O13 W4 Rb2 50.8(12) . . ?
O14 W4 Rb2 130.3(12) . . ?
O15 W4 Rb2 49.2(14) . . ?
O12 W4 Rb2 54.4(13) 1_455 . ?
O12 W4 Rb2 45.8(19) . 1_655 ?
O10 W4 Rb2 124.1(13) . 1_655 ?
O13 W4 Rb2 51.7(11) . 1_655 ?
O14 W4 Rb2 118.1(12) . 1_655 ?
O15 W4 Rb2 53.0(15) . 1_655 ?
O12 W4 Rb2 110.8(13) 1_455 1_655 ?
Rb2 W4 Rb2 56.39(19) . 1_655 ?
O12 W4 Rb1 128.3(18) . . ?
O10 W4 Rb1 54.0(12) . . ?
O13 W4 Rb1 132.1(10) . . ?
O14 W4 Rb1 57.6(11) . . ?
O15 W4 Rb1 128.1(14) . . ?
O12 W4 Rb1 75.0(13) 1_455 . ?
Rb2 W4 Rb1 129.4(4) . . ?
Rb2 W4 Rb1 174.0(4) 1_655 . ?
O12 W4 Rb1 75.9(18) . 1_655 ?
O10 W4 Rb1 46.4(12) . 1_655 ?
O13 W4 Rb1 129.8(12) . 1_655 ?
O14 W4 Rb1 48.6(12) . 1_655 ?
O15 W4 Rb1 128.6(14) . 1_655 ?
O12 W4 Rb1 127.4(13) 1_455 1_655 ?
Rb2 W4 Rb1 177.5(4) . 1_655 ?
Rb2 W4 Rb1 121.7(4) 1_655 1_655 ?
Rb1 W4 Rb1 52.51(16) . 1_655 ?
O11 W5 O16 84.3(18) . . ?
O11 W5 O14 94.0(17) . 1_565 ?
O16 W5 O14 79.7(17) . 1_565 ?
O11 W5 O13 91.7(16) . . ?
O16 W5 O13 83.5(17) . . ?
O14 W5 O13 161.6(17) 1_565 . ?
O11 W5 O17 163.9(18) . . ?
O16 W5 O17 79.7(15) . . ?
O14 W5 O17 85.6(16) 1_565 . ?
O13 W5 O17 84.1(15) . . ?
O11 W5 O16 92.6(17) . 1_655 ?
O16 W5 O16 168.6(19) . 1_655 ?
O14 W5 O16 89.6(16) 1_565 1_655 ?
O13 W5 O16 107.6(16) . 1_655 ?
O17 W5 O16 103.6(15) . 1_655 ?
O11 W5 Rb2 130.3(14) . 1_655 ?
O16 W5 Rb2 119.8(11) . 1_655 ?
O14 W5 Rb2 130.5(11) 1_565 1_655 ?
O13 W5 Rb2 53.8(11) . 1_655 ?
O17 W5 Rb2 58.1(12) . 1_655 ?
O16 W5 Rb2 70.4(9) 1_655 1_655 ?
O11 W5 Rb1 50.6(14) . 1_665 ?
O16 W5 Rb1 107.1(11) . 1_665 ?
O14 W5 Rb1 56.0(12) 1_565 1_665 ?
O13 W5 Rb1 137.8(10) . 1_665 ?
O17 W5 Rb1 137.5(12) . 1_665 ?
O16 W5 Rb1 63.0(8) 1_655 1_665 ?
Rb2 W5 Rb1 133.1(5) 1_655 1_665 ?
O11 W5 Rb2 123.5(14) . . ?
O16 W5 Rb2 65.4(11) . . ?
O14 W5 Rb2 123.1(12) 1_565 . ?
O13 W5 Rb2 41.1(11) . . ?
O17 W5 Rb2 46.5(12) . . ?
O16 W5 Rb2 124.8(9) 1_655 . ?
Rb2 W5 Rb2 54.4(2) 1_655 . ?
Rb1 W5 Rb2 171.9(4) 1_665 . ?
O11 W5 Rb1 49.4(14) . 1_565 ?
O16 W5 Rb1 53.8(10) . 1_565 ?
O14 W5 Rb1 54.0(12) 1_565 1_565 ?
O13 W5 Rb1 120.0(11) . 1_565 ?
O17 W5 Rb1 120.2(12) . 1_565 ?
O16 W5 Rb1 116.3(9) 1_655 1_565 ?
Rb2 W5 Rb1 172.9(5) 1_655 1_565 ?
Rb1 W5 Rb1 53.37(15) 1_665 1_565 ?
Rb2 W5 Rb1 118.9(4) . 1_565 ?
O18 W6 O17 102(2) . 1_545 ?
O18 W6 O15 79(2) . . ?
O17 W6 O15 93.5(13) 1_545 . ?
O18 W6 O19 102(2) . . ?
O17 W6 O19 89(2) 1_545 . ?
O15 W6 O19 177(2) . . ?
O18 W6 O20 84(2) . . ?
O17 W6 O20 173(2) 1_545 . ?
O15 W6 O20 91(2) . . ?
O19 W6 O20 86.0(13) . . ?
O18 W6 O18 153(3) . 1_655 ?
O17 W6 O18 102.7(19) 1_545 1_655 ?
O15 W6 O18 89(2) . 1_655 ?
O19 W6 O18 89.5(18) . 1_655 ?
O20 W6 O18 72(2) . 1_655 ?
O18 W6 Rb2 49.2(17) . . ?
O17 W6 Rb2 129.8(14) 1_545 . ?
O15 W6 Rb2 47.3(16) . . ?
O19 W6 Rb2 131.5(13) . . ?
O20 W6 Rb2 57.0(16) . . ?
O18 W6 Rb2 105.5(14) 1_655 . ?
O18 W6 Rb2 105.5(17) . 1_655 ?
O17 W6 Rb2 130.7(14) 1_545 1_655 ?
O15 W6 Rb2 53.7(16) . 1_655 ?
O19 W6 Rb2 123.5(14) . 1_655 ?
O20 W6 Rb2 49.8(15) . 1_655 ?
O18 W6 Rb2 49.1(14) 1_655 1_655 ?
Rb2 W6 Rb2 56.5(3) . 1_655 ?
O18 W6 Rb2 78.9(17) . 1_545 ?
O17 W6 Rb2 47.9(14) 1_545 1_545 ?
O15 W6 Rb2 129.0(16) . 1_545 ?
O19 W6 Rb2 53.9(13) . 1_545 ?
O20 W6 Rb2 130.9(15) . 1_545 ?
O18 W6 Rb2 126.4(13) 1_655 1_545 ?
Rb2 W6 Rb2 127.9(8) . 1_545 ?
Rb2 W6 Rb2 175.6(8) 1_655 1_545 ?
O18 W6 Rb2 132.5(16) . 1_645 ?
O17 W6 Rb2 51.5(14) 1_545 1_645 ?
O15 W6 Rb2 132.4(16) . 1_645 ?
O19 W6 Rb2 48.7(13) . 1_645 ?
O20 W6 Rb2 121.7(16) . 1_645 ?
O18 W6 Rb2 72.7(13) 1_655 1_645 ?
Rb2 W6 Rb2 178.2(8) . 1_645 ?
Rb2 W6 Rb2 121.7(8) 1_655 1_645 ?
Rb2 W6 Rb2 53.9(3) 1_545 1_645 ?
O21 W7 O19 97(2) . 2_656 ?
O21 W7 O20 77(2) . . ?
O19 W7 O20 174(2) 2_656 . ?
O21 W7 O22 92(3) . 2_646 ?
O19 W7 O22 90.4(17) 2_656 2_646 ?
O20 W7 O22 87(2) . 2_646 ?
O21 W7 O22 85(3) . . ?
O19 W7 O22 90.6(18) 2_656 . ?
O20 W7 O22 91(2) . . ?
O22 W7 O22 176.2(4) 2_646 . ?
O21 W7 O21 165(3) . 1_455 ?
O19 W7 O21 93(2) 2_656 1_455 ?
O20 W7 O21 93(2) . 1_455 ?
O22 W7 O21 99(3) 2_646 1_455 ?
O22 W7 O21 85(3) . 1_455 ?
O21 W7 Rb2 108.8(17) . . ?
O19 W7 Rb2 128.9(13) 2_656 . ?
O20 W7 Rb2 55.9(16) . . ?
O22 W7 Rb2 130.4(14) 2_646 . ?
O22 W7 Rb2 50.9(14) . . ?
O21 W7 Rb2 56.6(16) 1_455 . ?
O21 W7 Rb2 52.9(17) . 1_655 ?
O19 W7 Rb2 129.9(14) 2_656 1_655 ?
O20 W7 Rb2 48.3(16) . 1_655 ?
O22 W7 Rb2 124.6(16) 2_646 1_655 ?
O22 W7 Rb2 52.4(16) . 1_655 ?
O21 W7 Rb2 112.5(16) 1_455 1_655 ?
Rb2 W7 Rb2 55.9(2) . 1_655 ?
O21 W7 Rb2 70.2(17) . 2_646 ?
O19 W7 Rb2 54.3(13) 2_656 2_646 ?
O20 W7 Rb2 120.9(16) . 2_646 ?
O22 W7 Rb2 47.1(15) 2_646 2_646 ?
O22 W7 Rb2 131.4(15) . 2_646 ?
O21 W7 Rb2 124.4(17) 1_455 2_646 ?
Rb2 W7 Rb2 176.8(5) . 2_646 ?
Rb2 W7 Rb2 123.01(17) 1_655 2_646 ?
O21 W7 Rb2 125.1(17) . 2_546 ?
O19 W7 Rb2 52.0(14) 2_656 2_546 ?
O20 W7 Rb2 129.4(16) . 2_546 ?
O22 W7 Rb2 51.8(16) 2_646 2_546 ?
O22 W7 Rb2 131.2(16) . 2_546 ?
O21 W7 Rb2 69.6(16) 1_455 2_546 ?
Rb2 W7 Rb2 126.05(17) . 2_546 ?
Rb2 W7 Rb2 176.4(5) 1_655 2_546 ?
Rb2 W7 Rb2 54.84(19) 2_646 2_546 ?
O8 Rb1 O3 52.7(16) 1_545 . ?
O8 Rb1 O5 95.6(10) 1_545 . ?
O3 Rb1 O5 51.1(15) . . ?
O8 Rb1 O3 95.9(14) 1_545 1_455 ?
O3 Rb1 O3 74.9(7) . 1_455 ?
O5 Rb1 O3 94.9(14) . 1_455 ?
O8 Rb1 O8 75.4(10) 1_545 1_445 ?
O3 Rb1 O8 97.9(14) . 1_445 ?
O5 Rb1 O8 141.4(8) . 1_445 ?
O3 Rb1 O8 50.3(15) 1_455 1_445 ?
O8 Rb1 O5 141.0(8) 1_545 1_455 ?
O3 Rb1 O5 95.5(14) . 1_455 ?
O5 Rb1 O5 73.7(9) . 1_455 ?
O3 Rb1 O5 49.5(15) 1_455 1_455 ?
O8 Rb1 O5 89.8(9) 1_445 1_455 ?
O8 Rb1 O11 87.9(12) 1_545 1_445 ?
O3 Rb1 O11 137.0(16) . 1_445 ?
O5 Rb1 O11 168.6(11) . 1_445 ?
O3 Rb1 O11 95.5(15) 1_455 1_445 ?
O8 Rb1 O11 50.0(11) 1_445 1_445 ?
O5 Rb1 O11 109.9(12) 1_455 1_445 ?
O8 Rb1 O7 45.8(11) 1_545 1_445 ?
O3 Rb1 O7 50.2(14) . 1_445 ?
O5 Rb1 O7 99.1(11) . 1_445 ?
O3 Rb1 O7 50.1(14) 1_455 1_445 ?
O8 Rb1 O7 48.0(11) 1_445 1_445 ?
O5 Rb1 O7 97.8(11) 1_455 1_445 ?
O11 Rb1 O7 91.2(12) 1_445 1_445 ?
O8 Rb1 O10 171.8(11) 1_545 1_455 ?
O3 Rb1 O10 132.9(16) . 1_455 ?
O5 Rb1 O10 86.6(11) . 1_455 ?
O3 Rb1 O10 91.8(14) 1_455 1_455 ?
O8 Rb1 O10 107.7(12) 1_445 1_455 ?
O5 Rb1 O10 47.2(10) 1_455 1_455 ?
O11 Rb1 O10 88.4(9) 1_445 1_455 ?
O7 Rb1 O10 141.6(11) 1_445 1_455 ?
O8 Rb1 O14 127.1(14) 1_545 1_455 ?
O3 Rb1 O14 173.2(14) . 1_455 ?
O5 Rb1 O14 124.4(14) . 1_455 ?
O3 Rb1 O14 111.5(12) 1_455 1_455 ?
O8 Rb1 O14 88.2(13) 1_445 1_455 ?
O5 Rb1 O14 87.3(13) 1_455 1_455 ?
O11 Rb1 O14 46.6(14) 1_445 1_455 ?
O7 Rb1 O14 135.6(14) 1_445 1_455 ?
O10 Rb1 O14 46.5(13) 1_455 1_455 ?
O8 Rb1 O10 108.7(12) 1_545 . ?
O3 Rb1 O10 90.3(14) . . ?
O5 Rb1 O10 46.5(10) . . ?
O3 Rb1 O10 134.7(15) 1_455 . ?
O8 Rb1 O10 171.6(11) 1_445 . ?
O5 Rb1 O10 91.2(11) 1_455 . ?
O11 Rb1 O10 122.1(8) 1_445 . ?
O7 Rb1 O10 140.0(11) 1_445 . ?
O10 Rb1 O10 67.3(8) 1_455 . ?
O14 Rb1 O10 83.4(12) 1_455 . ?
O8 Rb1 O11 48.8(11) 1_545 1_545 ?
O3 Rb1 O11 91.9(14) . 1_545 ?
O5 Rb1 O11 106.3(11) . 1_545 ?
O3 Rb1 O11 139.5(16) 1_455 1_545 ?
O8 Rb1 O11 95.7(12) 1_445 1_545 ?
O5 Rb1 O11 170.1(11) 1_455 1_545 ?
O11 Rb1 O11 68.2(8) 1_445 1_545 ?
O7 Rb1 O11 92.0(11) 1_445 1_545 ?
O10 Rb1 O11 123.0(7) 1_455 1_545 ?
O14 Rb1 O11 84.6(12) 1_455 1_545 ?
O10 Rb1 O11 82.2(8) . 1_545 ?
O8 Rb1 O2 91.8(13) 1_545 . ?
O3 Rb1 O2 42.0(14) . . ?
O5 Rb1 O2 46.1(11) . . ?
O3 Rb1 O2 49.5(13) 1_455 . ?
O8 Rb1 O2 96.0(11) 1_445 . ?
O5 Rb1 O2 53.5(11) 1_455 . ?
O11 Rb1 O2 144.8(12) 1_445 . ?
O7 Rb1 O2 64.6(12) 1_445 . ?
O10 Rb1 O2 95.4(13) 1_455 . ?
O14 Rb1 O2 140.5(16) 1_455 . ?
O10 Rb1 O2 91.2(12) . . ?
O11 Rb1 O2 133.6(12) 1_545 . ?
O8 Rb1 O14 87.6(13) 1_545 . ?
O3 Rb1 O14 107.8(12) . . ?
O5 Rb1 O14 85.3(12) . . ?
O3 Rb1 O14 176.5(16) 1_455 . ?
O8 Rb1 O14 130.5(13) 1_445 . ?
O5 Rb1 O14 127.4(13) 1_455 . ?
O11 Rb1 O14 84.0(12) 1_445 . ?
O7 Rb1 O14 133.4(14) 1_445 . ?
O10 Rb1 O14 84.7(12) 1_455 . ?
O14 Rb1 O14 65.7(6) 1_455 . ?
O10 Rb1 O14 44.0(12) . . ?
O11 Rb1 O14 43.4(13) 1_545 . ?
O2 Rb1 O14 131.2(13) . . ?
O8 Rb1 O16 83.9(10) 1_545 1_545 ?
O3 Rb1 O16 129.5(14) . 1_545 ?
O5 Rb1 O16 123.0(10) . 1_545 ?
O3 Rb1 O16 142.1(14) 1_455 1_545 ?
O8 Rb1 O16 93.8(10) 1_445 1_545 ?
O5 Rb1 O16 133.7(10) 1_455 1_545 ?
O11 Rb1 O16 46.5(9) 1_445 1_545 ?
O7 Rb1 O16 118.3(10) 1_445 1_545 ?
O10 Rb1 O16 88.2(9) 1_455 1_545 ?
O14 Rb1 O16 46.7(10) 1_455 1_545 ?
O10 Rb1 O16 79.6(8) . 1_545 ?
O11 Rb1 O16 37.9(8) 1_545 1_545 ?
O2 Rb1 O16 168.0(11) . 1_545 ?
O14 Rb1 O16 37.6(11) . 1_545 ?
O8 Rb1 O9 140.8(16) 1_545 1_455 ?
O3 Rb1 O9 92.8(19) . 1_455 ?
O5 Rb1 O9 45.2(14) . 1_455 ?
O3 Rb1 O9 91.2(18) 1_455 1_455 ?
O8 Rb1 O9 134.4(14) 1_445 1_455 ?
O5 Rb1 O9 45.0(12) 1_455 1_455 ?
O11 Rb1 O9 129.8(16) 1_445 1_455 ?
O7 Rb1 O9 128.7(17) 1_445 1_455 ?
O10 Rb1 O9 41.6(14) 1_455 1_455 ?
O14 Rb1 O9 84.8(19) 1_455 1_455 ?
O10 Rb1 O9 46.2(13) . 1_455 ?
O11 Rb1 O9 128.2(15) 1_545 1_455 ?
O2 Rb1 O9 64.3(18) . 1_455 ?
O14 Rb1 O9 86.5(17) . 1_455 ?
O16 Rb1 O9 112.8(15) 1_545 1_455 ?
O8 Rb1 O9 45.1(14) 1_545 1_445 ?
O3 Rb1 O9 94.6(19) . 1_445 ?
O5 Rb1 O9 140.6(15) . 1_445 ?
O3 Rb1 O9 93.1(18) 1_455 1_445 ?
O8 Rb1 O9 46.7(12) 1_445 1_445 ?
O5 Rb1 O9 136.3(13) 1_455 1_445 ?
O11 Rb1 O9 43.2(14) 1_445 1_445 ?
O7 Rb1 O9 58.7(15) 1_445 1_445 ?
O10 Rb1 O9 131.6(15) 1_455 1_445 ?
O14 Rb1 O9 87.5(18) 1_455 1_445 ?
O10 Rb1 O9 131.2(13) . 1_445 ?
O11 Rb1 O9 49.2(12) 1_545 1_445 ?
O2 Rb1 O9 123.2(17) . 1_445 ?
O14 Rb1 O9 88.9(15) . 1_445 ?
O16 Rb1 O9 60.3(13) 1_545 1_445 ?
O9 Rb1 O9 172(3) 1_455 1_445 ?
O8 Rb1 Rb1 54.7(9) 1_545 1_655 ?
O3 Rb1 Rb1 53.4(9) . 1_655 ?
O5 Rb1 Rb1 54.4(8) . 1_655 ?
O3 Rb1 Rb1 128.3(10) 1_455 1_655 ?
O8 Rb1 Rb1 130.1(8) 1_445 1_655 ?
O5 Rb1 Rb1 128.2(7) 1_455 1_655 ?
O11 Rb1 Rb1 120.9(9) 1_445 1_655 ?
O7 Rb1 Rb1 90.8(8) 1_445 1_655 ?
O10 Rb1 Rb1 121.8(8) 1_455 1_655 ?
O14 Rb1 Rb1 120.2(8) 1_455 1_655 ?
O10 Rb1 Rb1 54.5(7) . 1_655 ?
O11 Rb1 Rb1 52.8(8) 1_545 1_655 ?
O2 Rb1 Rb1 86.4(8) . 1_655 ?
O14 Rb1 Rb1 54.4(7) . 1_655 ?
O16 Rb1 Rb1 82.0(6) 1_545 1_655 ?
O9 Rb1 Rb1 91.3(11) 1_455 1_655 ?
O9 Rb1 Rb1 91.2(10) 1_445 1_655 ?
O8 Rb1 Rb1 125.3(9) 1_545 1_455 ?
O3 Rb1 Rb1 126.6(9) . 1_455 ?
O5 Rb1 Rb1 125.6(8) . 1_455 ?
O3 Rb1 Rb1 51.7(10) 1_455 1_455 ?
O8 Rb1 Rb1 49.9(8) 1_445 1_455 ?
O5 Rb1 Rb1 51.8(7) 1_455 1_455 ?
O11 Rb1 Rb1 59.1(9) 1_445 1_455 ?
O7 Rb1 Rb1 89.2(8) 1_445 1_455 ?
O10 Rb1 Rb1 58.2(8) 1_455 1_455 ?
O14 Rb1 Rb1 59.8(8) 1_455 1_455 ?
O10 Rb1 Rb1 125.5(7) . 1_455 ?
O11 Rb1 Rb1 127.2(8) 1_545 1_455 ?
O2 Rb1 Rb1 93.6(8) . 1_455 ?
O14 Rb1 Rb1 125.6(7) . 1_455 ?
O16 Rb1 Rb1 98.0(6) 1_545 1_455 ?
O9 Rb1 Rb1 88.7(11) 1_455 1_455 ?
O9 Rb1 Rb1 88.8(10) 1_445 1_455 ?
Rb1 Rb1 Rb1 180.0 1_655 1_455 ?
O8 Rb1 W3 67.5(9) 1_545 1_445 ?
O3 Rb1 W3 107.8(14) . 1_445 ?
O5 Rb1 W3 158.7(8) . 1_445 ?
O3 Rb1 W3 75.1(13) 1_455 1_445 ?
O8 Rb1 W3 24.8(8) 1_445 1_445 ?
O5 Rb1 W3 110.8(9) 1_455 1_445 ?
O11 Rb1 W3 31.2(8) 1_445 1_445 ?
O7 Rb1 W3 60.0(8) 1_445 1_445 ?
O10 Rb1 W3 112.0(8) 1_455 1_445 ?
O14 Rb1 W3 76.8(11) 1_455 1_445 ?
O10 Rb1 W3 149.4(7) . 1_445 ?
O11 Rb1 W3 72.9(8) 1_545 1_445 ?
O2 Rb1 W3 118.8(10) . 1_445 ?
O14 Rb1 W3 105.9(11) . 1_445 ?
O16 Rb1 W3 69.9(6) 1_545 1_445 ?
O9 Rb1 W3 150.8(13) 1_455 1_445 ?
O9 Rb1 W3 26.5(9) 1_445 1_445 ?
Rb1 Rb1 W3 117.5(3) 1_655 1_445 ?
Rb1 Rb1 W3 62.5(3) 1_455 1_445 ?
O15 Rb2 O13 52.3(13) . . ?
O15 Rb2 O18 43.1(15) . . ?
O13 Rb2 O18 93.7(15) . . ?
O15 Rb2 O22 94.0(18) . . ?
O13 Rb2 O22 111.7(15) . . ?
O18 Rb2 O22 89.0(18) . . ?
O15 Rb2 O20 88.2(15) . 1_455 ?
O13 Rb2 O20 135.0(14) . 1_455 ?
O18 Rb2 O20 45.3(16) . 1_455 ?
O22 Rb2 O20 89.0(17) . 1_455 ?
O15 Rb2 O17 95.7(12) . . ?
O13 Rb2 O17 49.1(12) . . ?
O18 Rb2 O17 138.5(19) . . ?
O22 Rb2 O17 89.5(16) . . ?
O20 Rb2 O17 175.9(14) 1_455 . ?
O15 Rb2 O12 50.8(12) . 1_455 ?
O13 Rb2 O12 53.4(12) . 1_455 ?
O18 Rb2 O12 63.2(13) . 1_455 ?
O22 Rb2 O12 144.6(18) . 1_455 ?
O20 Rb2 O12 86.3(15) 1_455 1_455 ?
O17 Rb2 O12 97.1(13) . 1_455 ?
O15 Rb2 O13 93.1(13) . 1_455 ?
O13 Rb2 O13 73.0(6) . 1_455 ?
O18 Rb2 O13 96.0(15) . 1_455 ?
O22 Rb2 O13 172.9(17) . 1_455 ?
O20 Rb2 O13 91.0(15) 1_455 1_455 ?
O17 Rb2 O13 90.0(12) . 1_455 ?
O12 Rb2 O13 42.4(12) 1_455 1_455 ?
O15 Rb2 O22 133.6(18) . 1_455 ?
O13 Rb2 O22 173.6(17) . 1_455 ?
O18 Rb2 O22 91.5(19) . 1_455 ?
O22 Rb2 O22 71.9(7) . 1_455 ?
O20 Rb2 O22 48.8(17) 1_455 1_455 ?
O17 Rb2 O22 127.1(17) . 1_455 ?
O12 Rb2 O22 126.8(17) 1_455 1_455 ?
O13 Rb2 O22 103.0(13) 1_455 1_455 ?
O15 Rb2 O20 49.4(15) . . ?
O13 Rb2 O20 92.3(14) . . ?
O18 Rb2 O20 44.1(15) . . ?
O22 Rb2 O20 49.0(17) . . ?
O20 Rb2 O20 71.3(11) 1_455 . ?
O17 Rb2 O20 110.4(14) . . ?
O12 Rb2 O20 96.6(14) 1_455 . ?
O13 Rb2 O20 137.4(14) 1_455 . ?
O22 Rb2 O20 94.0(15) 1_455 . ?
O15 Rb2 O19 178.7(14) . 1_465 ?
O13 Rb2 O19 126.9(13) . 1_465 ?
O18 Rb2 O19 137.2(18) . 1_465 ?
O22 Rb2 O19 87.3(15) . 1_465 ?
O20 Rb2 O19 92.0(11) 1_455 1_465 ?
O17 Rb2 O19 84.1(12) . 1_465 ?
O12 Rb2 O19 127.9(13) 1_455 1_465 ?
O13 Rb2 O19 85.6(12) 1_455 1_465 ?
O22 Rb2 O19 47.1(15) 1_455 1_465 ?
O20 Rb2 O19 131.9(8) . 1_465 ?
O15 Rb2 O15 73.2(11) . 1_455 ?
O13 Rb2 O15 94.7(12) . 1_455 ?
O18 Rb2 O15 51.6(15) . 1_455 ?
O22 Rb2 O15 134.5(17) . 1_455 ?
O20 Rb2 O15 48.3(14) 1_455 1_455 ?
O17 Rb2 O15 134.2(8) . 1_455 ?
O12 Rb2 O15 41.3(12) 1_455 1_455 ?
O13 Rb2 O15 48.0(12) 1_455 1_455 ?
O22 Rb2 O15 85.8(16) 1_455 1_455 ?
O20 Rb2 O15 95.7(15) . 1_455 ?
O19 Rb2 O15 106.1(14) 1_465 1_455 ?
O15 Rb2 O21 92.9(15) . 1_455 ?
O13 Rb2 O21 141.4(15) . 1_455 ?
O18 Rb2 O21 59.5(15) . 1_455 ?
O22 Rb2 O21 47.3(15) . 1_455 ?
O20 Rb2 O21 41.8(14) 1_455 1_455 ?
O17 Rb2 O21 136.4(14) . 1_455 ?
O12 Rb2 O21 120.7(16) 1_455 1_455 ?
O13 Rb2 O21 132.1(15) 1_455 1_455 ?
O22 Rb2 O21 44.8(15) 1_455 1_455 ?
O20 Rb2 O21 49.2(13) . 1_455 ?
O19 Rb2 O21 88.2(13) 1_465 1_455 ?
O15 Rb2 O21 89.1(14) 1_455 1_455 ?
O15 Rb2 O19 111.8(15) . 1_565 ?
O13 Rb2 O19 87.9(13) . 1_565 ?
O18 Rb2 O19 132.8(17) . 1_565 ?
O22 Rb2 O19 47.7(16) . 1_565 ?
O20 Rb2 O19 131.4(9) 1_455 1_565 ?
O17 Rb2 O19 45.7(12) . 1_565 ?
O12 Rb2 O19 140.9(14) 1_455 1_565 ?
O13 Rb2 O19 129.1(13) 1_455 1_565 ?
O22 Rb2 O19 91.2(14) 1_455 1_565 ?
O20 Rb2 O19 88.6(10) . 1_565 ?
O19 Rb2 O19 68.9(9) 1_465 1_565 ?
O15 Rb2 O19 174.9(14) 1_455 1_565 ?
O21 Rb2 O19 91.7(12) 1_455 1_565 ?
O15 Rb2 O17 134.0(9) . 1_455 ?
O13 Rb2 O17 90.2(11) . 1_455 ?
O18 Rb2 O17 138.1(18) . 1_455 ?
O22 Rb2 O17 127.7(17) . 1_455 ?
O20 Rb2 O17 108.5(14) 1_455 1_455 ?
O17 Rb2 O17 69.6(9) . 1_455 ?
O12 Rb2 O17 86.8(12) 1_455 1_455 ?
O13 Rb2 O17 45.9(11) 1_455 1_455 ?
O22 Rb2 O17 83.5(15) 1_455 1_455 ?
O20 Rb2 O17 176.5(13) . 1_455 ?
O19 Rb2 O17 44.7(11) 1_465 1_455 ?
O15 Rb2 O17 86.5(10) 1_455 1_455 ?
O21 Rb2 O17 128.3(14) 1_455 1_455 ?
O19 Rb2 O17 89.0(12) 1_565 1_455 ?
O15 Rb2 Rb2 122.9(10) . 1_455 ?
O13 Rb2 Rb2 124.0(8) . 1_455 ?
O18 Rb2 Rb2 92.1(16) . 1_455 ?
O22 Rb2 Rb2 124.0(12) . 1_455 ?
O20 Rb2 Rb2 56.0(11) 1_455 1_455 ?
O17 Rb2 Rb2 122.2(9) . 1_455 ?
O12 Rb2 Rb2 81.1(10) 1_455 1_455 ?
O13 Rb2 Rb2 51.0(8) 1_455 1_455 ?
O22 Rb2 Rb2 52.1(10) 1_455 1_455 ?
O20 Rb2 Rb2 127.3(10) . 1_455 ?
O19 Rb2 Rb2 56.3(9) 1_465 1_455 ?
O15 Rb2 Rb2 49.7(9) 1_455 1_455 ?
O21 Rb2 Rb2 86.9(9) 1_455 1_455 ?
O19 Rb2 Rb2 125.2(8) 1_565 1_455 ?
O17 Rb2 Rb2 52.6(8) 1_455 1_455 ?
O15 Rb2 Rb2 57.1(11) . 1_655 ?
O13 Rb2 Rb2 56.0(8) . 1_655 ?
O18 Rb2 Rb2 87.9(16) . 1_655 ?
O22 Rb2 Rb2 56.0(12) . 1_655 ?
O20 Rb2 Rb2 124.0(11) 1_455 1_655 ?
O17 Rb2 Rb2 57.8(9) . 1_655 ?
O12 Rb2 Rb2 98.9(10) 1_455 1_655 ?
O13 Rb2 Rb2 129.0(8) 1_455 1_655 ?
O22 Rb2 Rb2 127.9(10) 1_455 1_655 ?
O20 Rb2 Rb2 52.7(10) . 1_655 ?
O19 Rb2 Rb2 123.7(9) 1_465 1_655 ?
O15 Rb2 Rb2 130.3(9) 1_455 1_655 ?
O21 Rb2 Rb2 93.1(10) 1_455 1_655 ?
O19 Rb2 Rb2 54.8(8) 1_565 1_655 ?
O17 Rb2 Rb2 127.4(8) 1_455 1_655 ?
Rb2 Rb2 Rb2 179.998(11) 1_455 1_655 ?
O15 Rb2 O16 89.1(11) . . ?
O13 Rb2 O16 38.9(9) . . ?
O18 Rb2 O16 124.5(11) . . ?
O22 Rb2 O16 128.0(16) . . ?
O20 Rb2 O16 143.1(13) 1_455 . ?
O17 Rb2 O16 38.6(9) . . ?
O12 Rb2 O16 64.0(10) 1_455 . ?
O13 Rb2 O16 52.3(9) 1_455 . ?
O22 Rb2 O16 134.8(14) 1_455 . ?
O20 Rb2 O16 130.5(12) . . ?
O19 Rb2 O16 89.9(10) 1_465 . ?
O15 Rb2 O16 96.0(10) 1_455 . ?
O21 Rb2 O16 174.9(13) 1_455 . ?
O19 Rb2 O16 83.2(10) 1_565 . ?
O17 Rb2 O16 51.7(9) 1_455 . ?
Rb2 Rb2 O16 95.9(5) 1_455 . ?
Rb2 Rb2 O16 84.1(5) 1_655 . ?
O15 Rb2 O21 137.1(14) . 2_656 ?
O13 Rb2 O21 132.2(15) . 2_656 ?
O18 Rb2 O21 119.2(14) . 2_656 ?
O22 Rb2 O21 43.1(15) . 2_656 ?
O20 Rb2 O21 90.5(14) 1_455 2_656 ?
O17 Rb2 O21 85.8(13) . 2_656 ?
O12 Rb2 O21 171.5(14) 1_455 2_656 ?
O13 Rb2 O21 129.9(13) 1_455 2_656 ?
O22 Rb2 O21 46.8(15) 1_455 2_656 ?
O20 Rb2 O21 89.8(13) . 2_656 ?
O19 Rb2 O21 44.3(11) 1_465 2_656 ?
O15 Rb2 O21 132.6(14) 1_455 2_656 ?
O21 Rb2 O21 60.1(3) 1_455 2_656 ?
O19 Rb2 O21 44.4(11) 1_565 2_656 ?
O17 Rb2 O21 86.7(12) 1_455 2_656 ?
Rb2 Rb2 O21 90.6(9) 1_455 2_656 ?
Rb2 Rb2 O21 89.4(9) 1_655 2_656 ?
O16 Rb2 O21 115.5(12) . 2_656 ?
O15 Rb2 W4 28.9(10) . . ?
O13 Rb2 W4 28.6(9) . . ?
O18 Rb2 W4 66.0(11) . . ?
O22 Rb2 W4 115.8(14) . . ?
O20 Rb2 W4 106.6(11) 1_455 . ?
O17 Rb2 W4 77.5(9) . . ?
O12 Rb2 W4 34.5(8) 1_455 . ?
O13 Rb2 W4 71.0(7) 1_455 . ?
O22 Rb2 W4 155.3(16) 1_455 . ?
O20 Rb2 W4 77.4(10) . . ?
O19 Rb2 W4 149.9(9) 1_465 . ?
O15 Rb2 W4 72.3(9) 1_455 . ?
O21 Rb2 W4 121.5(12) 1_455 . ?
O19 Rb2 W4 111.4(10) 1_565 . ?
O17 Rb2 W4 105.9(8) 1_455 . ?
Rb2 Rb2 W4 115.6(4) 1_455 . ?
Rb2 Rb2 W4 64.4(4) 1_655 . ?
O16 Rb2 W4 61.0(5) . . ?
O21 Rb2 W4 153.6(12) 2_656 . ?
O6 Rb3 O1 62.9(11) 2_645 2_655 ?
O6 Rb3 O6 81.8(14) 2_645 2_545 ?
O1 Rb3 O6 106.8(12) 2_655 2_545 ?
O6 Rb3 O1 63.9(12) 2_645 . ?
O1 Rb3 O1 107.4(9) 2_655 . ?
O6 Rb3 O1 110.5(18) 2_545 . ?
O6 Rb3 O6 105.7(9) 2_645 . ?
O1 Rb3 O6 63.5(14) 2_655 . ?
O6 Rb3 O6 160.9(17) 2_545 . ?
O1 Rb3 O6 88.5(10) . . ?
O6 Rb3 O1 106.0(19) 2_645 1_455 ?
O1 Rb3 O1 165.0(15) 2_655 1_455 ?
O6 Rb3 O1 60.1(12) 2_545 1_455 ?
O1 Rb3 O1 73.5(13) . 1_455 ?
O6 Rb3 O1 131.3(10) . 1_455 ?
O6 Rb3 O1 108.3(11) 2_645 2 ?
O1 Rb3 O1 78.6(15) 2_655 2 ?
O6 Rb3 O1 53.8(9) 2_545 2 ?
O1 Rb3 O1 164.2(19) . 2 ?
O6 Rb3 O1 107.1(17) . 2 ?
O1 Rb3 O1 96.8(10) 1_455 2 ?
O6 Rb3 O6 163.0(14) 2_645 1_455 ?
O1 Rb3 O6 102.5(18) 2_655 1_455 ?
O6 Rb3 O6 95.2(8) 2_545 1_455 ?
O1 Rb3 O6 132.0(9) . 1_455 ?
O6 Rb3 O6 72.4(12) . 1_455 ?
O1 Rb3 O6 86.6(10) 1_455 1_455 ?
O1 Rb3 O6 57.8(10) 2 1_455 ?
O6 Rb3 O4 102.8(14) 2_645 . ?
O1 Rb3 O4 103.3(16) 2_655 . ?
O6 Rb3 O4 148.0(16) 2_545 . ?
O1 Rb3 O4 48.7(14) . . ?
O6 Rb3 O4 48.7(14) . . ?
O1 Rb3 O4 88.6(15) 1_455 . ?
O1 Rb3 O4 145.5(16) 2 . ?
O6 Rb3 O4 88.7(13) 1_455 . ?
O6 Rb3 O4 149.8(18) 2_645 1_455 ?
O1 Rb3 O4 146.2(18) 2_655 1_455 ?
O6 Rb3 O4 91.4(13) 2_545 1_455 ?
O1 Rb3 O4 91.7(13) . 1_455 ?
O6 Rb3 O4 90.2(13) . 1_455 ?
O1 Rb3 O4 47.0(14) 1_455 1_455 ?
O1 Rb3 O4 90.5(12) 2 1_455 ?
O6 Rb3 O4 46.4(13) 1_455 1_455 ?
O4 Rb3 O4 68.6(5) . 1_455 ?
O6 Rb3 O2 105.1(16) 2_645 . ?
O1 Rb3 O2 145.3(14) 2_655 . ?
O6 Rb3 O2 103.1(14) 2_545 . ?
O1 Rb3 O2 44.1(13) . . ?
O6 Rb3 O2 92.1(13) . . ?
O1 Rb3 O2 44.1(13) 1_455 . ?
O1 Rb3 O2 134.6(12) 2 . ?
O6 Rb3 O2 91.9(13) 1_455 . ?
O4 Rb3 O2 45.0(13) . . ?
O4 Rb3 O2 47.7(12) 1_455 . ?
O6 Rb3 Rb3 119.6(13) 2_645 2 ?
O1 Rb3 Rb3 57.1(13) 2_655 2 ?
O6 Rb3 Rb3 108.0(10) 2_545 2 ?
O1 Rb3 Rb3 141.4(12) . 2 ?
O6 Rb3 Rb3 52.9(10) . 2 ?
O1 Rb3 Rb3 131.2(11) 1_455 2 ?
O1 Rb3 Rb3 54.3(11) 2 2 ?
O6 Rb3 Rb3 45.4(9) 1_455 2 ?
O4 Rb3 Rb3 97.2(13) . 2 ?
O4 Rb3 Rb3 90.5(11) 1_455 2 ?
O2 Rb3 Rb3 128.0(12) . 2 ?
O6 Rb3 Rb3 59.3(12) 2_645 2_545 ?
O1 Rb3 Rb3 121.0(13) 2_655 2_545 ?
O6 Rb3 Rb3 55.0(11) 2_545 2_545 ?
O1 Rb3 Rb3 55.4(11) . 2_545 ?
O6 Rb3 Rb3 143.9(10) . 2_545 ?
O1 Rb3 Rb3 46.7(11) 1_455 2_545 ?
O1 Rb3 Rb3 108.8(12) 2 2_545 ?
O6 Rb3 Rb3 131.8(11) 1_455 2_545 ?
O4 Rb3 Rb3 99.7(12) . 2_545 ?
O4 Rb3 Rb3 92.8(12) 1_455 2_545 ?
O2 Rb3 Rb3 64.6(11) . 2_545 ?
Rb3 Rb3 Rb3 162.8(6) 2 2_545 ?
O6 Rb3 Rb3 53.4(11) 2_645 1_655 ?
O1 Rb3 Rb3 56.0(12) 2_655 1_655 ?
O6 Rb3 Rb3 135.2(9) 2_545 1_655 ?
O1 Rb3 Rb3 53.4(10) . 1_655 ?
O6 Rb3 Rb3 55.0(9) . 1_655 ?
O1 Rb3 Rb3 126.9(10) 1_455 1_655 ?
O1 Rb3 Rb3 134.7(10) 2 1_655 ?
O6 Rb3 Rb3 127.4(9) 1_455 1_655 ?
O4 Rb3 Rb3 58.0(8) . 1_655 ?
O4 Rb3 Rb3 126.5(7) 1_455 1_655 ?
O2 Rb3 Rb3 90.1(7) . 1_655 ?
Rb3 Rb3 Rb3 95.8(4) 2 1_655 ?
Rb3 Rb3 Rb3 95.8(4) 2_545 1_655 ?
O6 Rb3 Rb3 126.6(11) 2_645 1_455 ?
O1 Rb3 Rb3 124.0(12) 2_655 1_455 ?
O6 Rb3 Rb3 44.8(9) 2_545 1_455 ?
O1 Rb3 Rb3 126.6(10) . 1_455 ?
O6 Rb3 Rb3 125.0(9) . 1_455 ?
O1 Rb3 Rb3 53.1(10) 1_455 1_455 ?
O1 Rb3 Rb3 45.3(10) 2 1_455 ?
O6 Rb3 Rb3 52.6(9) 1_455 1_455 ?
O4 Rb3 Rb3 122.0(8) . 1_455 ?
O4 Rb3 Rb3 53.5(7) 1_455 1_455 ?
O2 Rb3 Rb3 89.9(7) . 1_455 ?
Rb3 Rb3 Rb3 84.2(4) 2 1_455 ?
Rb3 Rb3 Rb3 84.2(4) 2_545 1_455 ?
Rb3 Rb3 Rb3 180.0 1_655 1_455 ?
O6 Rb3 O7 145.7(12) 2_645 1_455 ?
O1 Rb3 O7 111.1(17) 2_655 1_455 ?
O6 Rb3 O7 129.5(11) 2_545 1_455 ?
O1 Rb3 O7 88.8(12) . 1_455 ?
O6 Rb3 O7 50.2(11) . 1_455 ?
O1 Rb3 O7 83.8(12) 1_455 1_455 ?
O1 Rb3 O7 102.8(13) 2 1_455 ?
O6 Rb3 O7 45.1(11) 1_455 1_455 ?
O4 Rb3 O7 43.7(11) . 1_455 ?
O4 Rb3 O7 40.1(11) 1_455 1_455 ?
O2 Rb3 O7 59.1(11) . 1_455 ?
Rb3 Rb3 O7 68.9(9) 2 1_455 ?
Rb3 Rb3 O7 122.8(10) 2_545 1_455 ?
Rb3 Rb3 O7 94.2(6) 1_655 1_455 ?
Rb3 Rb3 O7 85.8(6) 1_455 1_455 ?
O6 Rb3 O2 74.8(13) 2_645 2 ?
O1 Rb3 O2 41.2(14) 2_655 2 ?
O6 Rb3 O2 69.7(12) 2_545 2 ?
O1 Rb3 O2 137.8(13) . 2 ?
O6 Rb3 O2 94.9(15) . 2 ?
O1 Rb3 O2 128.8(13) 1_455 2 ?
O1 Rb3 O2 40.9(11) 2 2 ?
O6 Rb3 O2 88.5(13) 1_455 2 ?
O4 Rb3 O2 142.2(16) . 2 ?
O4 Rb3 O2 130.2(12) 1_455 2 ?
O2 Rb3 O2 172.8(14) . 2 ?
Rb3 Rb3 O2 56.1(11) 2 2 ?
Rb3 Rb3 O2 110.0(11) 2_545 2 ?
Rb3 Rb3 O2 95.4(7) 1_655 2 ?
Rb3 Rb3 O2 84.6(7) 1_455 2 ?
O7 Rb3 O2 124.8(16) 1_455 2 ?
O6 Rb3 W1 88.2(11) 2_645 . ?
O1 Rb3 W1 119.3(12) 2_655 . ?
O6 Rb3 W1 121.2(13) 2_545 . ?
O1 Rb3 W1 24.7(10) . . ?
O6 Rb3 W1 77.1(9) . . ?
O1 Rb3 W1 67.8(11) 1_455 . ?
O1 Rb3 W1 160.4(10) 2 . ?
O6 Rb3 W1 107.4(9) 1_455 . ?
O4 Rb3 W1 29.5(11) . . ?
O4 Rb3 W1 70.2(8) 1_455 . ?
O2 Rb3 W1 26.3(7) . . ?
Rb3 Rb3 W1 126.6(6) 2 . ?
Rb3 Rb3 W1 70.2(4) 2_545 . ?
Rb3 Rb3 W1 63.8(2) 1_655 . ?
Rb3 Rb3 W1 116.2(2) 1_455 . ?
O7 Rb3 W1 64.7(7) 1_455 . ?
O2 Rb3 W1 158.7(7) 2 . ?
O6 Rb3 W2 117.8(11) 2_645 . ?
O1 Rb3 W2 89.1(13) 2_655 . ?
O6 Rb3 W2 159.3(10) 2_545 . ?
O1 Rb3 W2 75.8(10) . . ?
O6 Rb3 W2 26.0(9) . . ?
O1 Rb3 W2 105.4(10) 1_455 . ?
O1 Rb3 W2 119.4(13) 2 . ?
O6 Rb3 W2 67.9(10) 1_455 . ?
O4 Rb3 W2 28.1(11) . . ?
O4 Rb3 W2 68.4(9) 1_455 . ?
O2 Rb3 W2 67.1(9) . . ?
Rb3 Rb3 W2 69.2(5) 2 . ?
Rb3 Rb3 W2 127.5(5) 2_545 . ?
Rb3 Rb3 W2 64.78(19) 1_655 . ?
Rb3 Rb3 W2 115.22(19) 1_455 . ?
O7 Rb3 W2 29.8(7) 1_455 . ?
O2 Rb3 W2 119.5(13) 2 . ?
W1 Rb3 W2 57.40(15) . . ?
O6 Rb3 W1 122.0(14) 2_645 1_455 ?
O1 Rb3 W1 172.4(14) 2_655 1_455 ?
O6 Rb3 W1 80.3(10) 2_545 1_455 ?
O1 Rb3 W1 71.9(10) . 1_455 ?
O6 Rb3 W1 108.9(9) . 1_455 ?
O1 Rb3 W1 22.6(10) 1_455 1_455 ?
O1 Rb3 W1 104.0(10) 2 1_455 ?
O6 Rb3 W1 73.5(9) 1_455 1_455 ?
O4 Rb3 W1 70.4(9) . 1_455 ?
O4 Rb3 W1 28.1(10) 1_455 1_455 ?
O2 Rb3 W1 30.8(7) . 1_455 ?
Rb3 Rb3 W1 118.5(5) 2 1_455 ?
Rb3 Rb3 W1 65.3(5) 2_545 1_455 ?
Rb3 Rb3 W1 120.93(15) 1_655 1_455 ?
Rb3 Rb3 W1 59.07(15) 1_455 1_455 ?
O7 Rb3 W1 61.5(7) 1_455 1_455 ?
O2 Rb3 W1 143.4(7) 2 1_455 ?
W1 Rb3 W1 57.2(3) . 1_455 ?
W2 Rb3 W1 83.3(2) . 1_455 ?
W1 O1 Rb3 141(3) . 2_645 ?
W1 O1 Rb3 102(2) . . ?
Rb3 O1 Rb3 115.5(18) 2_645 . ?
W1 O1 Rb3 110(2) . 1_655 ?
Rb3 O1 Rb3 76.2(13) 2_645 1_655 ?
Rb3 O1 Rb3 73.5(13) . 1_655 ?
W1 O1 Rb3 123(2) . 2_545 ?
Rb3 O1 Rb3 78.6(15) 2_645 2_545 ?
Rb3 O1 Rb3 70.3(11) . 2_545 ?
Rb3 O1 Rb3 120.3(17) 1_655 2_545 ?
W1 O2 W1 176(3) . 1_455 ?
W1 O2 Rb3 87.5(19) . . ?
W1 O2 Rb3 88.2(16) 1_455 . ?
W1 O2 Rb1 96(2) . . ?
W1 O2 Rb1 88.3(16) 1_455 . ?
Rb3 O2 Rb1 175.9(17) . . ?
W1 O2 Rb3 94(2) . 2_545 ?
W1 O2 Rb3 83.6(15) 1_455 2_545 ?
Rb3 O2 Rb3 59.3(7) . 2_545 ?
Rb1 O2 Rb3 122.4(19) . 2_545 ?
W1 O3 W2 138.3(18) . 1_545 ?
W1 O3 Rb1 110(3) . . ?
W2 O3 Rb1 106(2) 1_545 . ?
W1 O3 Rb1 105(2) . 1_655 ?
W2 O3 Rb1 104(2) 1_545 1_655 ?
Rb1 O3 Rb1 74.9(7) . 1_655 ?
W2 O4 W1 168.5(18) . . ?
W2 O4 Rb3 94.7(17) . . ?
W1 O4 Rb3 92.8(17) . . ?
W2 O4 Rb3 97.3(18) . 1_655 ?
W1 O4 Rb3 93.5(17) . 1_655 ?
Rb3 O4 Rb3 68.6(5) . 1_655 ?
W3 O5 W1 141(2) . . ?
W3 O5 Rb1 114.5(17) . . ?
W1 O5 Rb1 100.9(13) . . ?
W3 O5 Rb1 108.4(16) . 1_655 ?
W1 O5 Rb1 96.2(12) . 1_655 ?
Rb1 O5 Rb1 73.7(9) . 1_655 ?
W2 O6 Rb3 140(2) . 2_655 ?
W2 O6 Rb3 124(2) . 2 ?
Rb3 O6 Rb3 81.8(14) 2_655 2 ?
W2 O6 Rb3 101(2) . . ?
Rb3 O6 Rb3 117.0(16) 2_655 . ?
Rb3 O6 Rb3 72.1(11) 2 . ?
W2 O6 Rb3 107(2) . 1_655 ?
Rb3 O6 Rb3 75.3(11) 2_655 1_655 ?
Rb3 O6 Rb3 121.8(16) 2 1_655 ?
Rb3 O6 Rb3 72.4(12) . 1_655 ?
W2 O7 W2 152(2) . 1_655 ?
W2 O7 Rb1 99.4(16) . 1_665 ?
W2 O7 Rb1 97.5(16) 1_655 1_665 ?
W2 O7 Rb3 84.1(14) . 1_655 ?
W2 O7 Rb3 76.2(12) 1_655 1_655 ?
Rb1 O7 Rb3 170.9(16) 1_665 1_655 ?
W3 O8 W2 141(2) . . ?
W3 O8 Rb1 114.9(19) . 1_565 ?
W2 O8 Rb1 102.0(15) . 1_565 ?
W3 O8 Rb1 104.9(17) . 1_665 ?
W2 O8 Rb1 96.4(14) . 1_665 ?
Rb1 O8 Rb1 75.4(10) 1_565 1_665 ?
W3 O9 W3 162(10) . 1_655 ?
W3 O9 Rb1 99(7) . 1_655 ?
W3 O9 Rb1 95(7) 1_655 1_655 ?
W3 O9 Rb1 83(8) . 1_665 ?
W3 O9 Rb1 81(6) 1_655 1_665 ?
Rb1 O9 Rb1 172(3) 1_655 1_665 ?
W4 O10 W3 151(2) . . ?
W4 O10 Rb1 110.4(15) . 1_655 ?
W3 O10 Rb1 97.6(14) . 1_655 ?
W4 O10 Rb1 101.2(14) . . ?
W3 O10 Rb1 94.4(14) . . ?
Rb1 O10 Rb1 67.3(8) 1_655 . ?
W5 O11 W3 156(2) . . ?
W5 O11 Rb1 105.5(18) . 1_665 ?
W3 O11 Rb1 95.1(14) . 1_665 ?
W5 O11 Rb1 108.9(17) . 1_565 ?
W3 O11 Rb1 89.2(15) . 1_565 ?
Rb1 O11 Rb1 68.2(8) 1_665 1_565 ?
W4 O12 W4 156(3) . 1_655 ?
W4 O12 Rb2 112(2) . 1_655 ?
W4 O12 Rb2 91.1(14) 1_655 1_655 ?
W5 O13 W4 142.8(17) . . ?
W5 O13 Rb2 115.2(18) . . ?
W4 O13 Rb2 100.6(17) . . ?
W5 O13 Rb2 98.6(16) . 1_655 ?
W4 O13 Rb2 101.3(16) . 1_655 ?
Rb2 O13 Rb2 73.0(6) . 1_655 ?
W5 O14 W4 155.8(19) 1_545 . ?
W5 O14 Rb1 96.5(18) 1_545 1_655 ?
W4 O14 Rb1 106(2) . 1_655 ?
W5 O14 Rb1 100.9(18) 1_545 . ?
W4 O14 Rb1 95.7(17) . . ?
Rb1 O14 Rb1 65.7(6) 1_655 . ?
W6 O15 W4 149(3) . . ?
W6 O15 Rb2 106(2) . . ?
W4 O15 Rb2 101.9(18) . . ?
W6 O15 Rb2 100.2(19) . 1_655 ?
W4 O15 Rb2 99.3(18) . 1_655 ?
Rb2 O15 Rb2 73.2(11) . 1_655 ?
W5 O16 W5 168.6(19) . 1_455 ?
W5 O16 Rb1 103.3(13) . 1_565 ?
W5 O16 Rb1 86.5(10) 1_455 1_565 ?
W5 O16 Rb2 90.3(11) . . ?
W5 O16 Rb2 79.4(9) 1_455 . ?
Rb1 O16 Rb2 164.9(10) 1_565 . ?
W6 O17 W5 146(2) 1_565 . ?
W6 O17 Rb2 107.6(18) 1_565 . ?
W5 O17 Rb2 106.5(16) . . ?
W6 O17 Rb2 104.4(17) 1_565 1_655 ?
W5 O17 Rb2 91.9(14) . 1_655 ?
Rb2 O17 Rb2 69.6(9) . 1_655 ?
W6 O18 W6 153(3) . 1_455 ?
W6 O18 Rb2 106(3) . . ?
W6 O18 Rb2 99(2) 1_455 . ?
W7 O19 W6 150(2) 2_646 . ?
W7 O19 Rb2 101.7(16) 2_646 1_645 ?
W6 O19 Rb2 106.3(17) . 1_645 ?
W7 O19 Rb2 99.2(16) 2_646 1_545 ?
W6 O19 Rb2 99.6(17) . 1_545 ?
Rb2 O19 Rb2 68.9(9) 1_645 1_545 ?
W7 O20 W6 151(3) . . ?
W7 O20 Rb2 106(2) . 1_655 ?
W6 O20 Rb2 103(2) . 1_655 ?
W7 O20 Rb2 96.4(19) . . ?
W6 O20 Rb2 94(2) . . ?
Rb2 O20 Rb2 71.3(11) 1_655 . ?
W7 O21 W7 165(3) . 1_655 ?
W7 O21 Rb2 101(2) . 1_655 ?
W7 O21 Rb2 94.0(19) 1_655 1_655 ?
W7 O21 Rb2 83.1(19) . 2_646 ?
W7 O21 Rb2 82.3(17) 1_655 2_646 ?
Rb2 O21 Rb2 175(2) 1_655 2_646 ?
W7 O22 W7 148.2(19) 2_656 . ?
W7 O22 Rb2 107(2) 2_656 . ?
W7 O22 Rb2 101(2) . . ?
W7 O22 Rb2 102(2) 2_656 1_655 ?
W7 O22 Rb2 101(2) . 1_655 ?
Rb2 O22 Rb2 71.9(7) . 1_655 ?

_refine_diff_density_max         6.597
_refine_diff_density_min         -11.961
_refine_diff_density_rms         1.018



_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_K4W11O35
_database_code_depnum_ccdc_archive 'CCDC 2211342'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_K4W11O35            
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form

_audit_creation_date             2022-07-13
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
_shelx_SHELXL_version_number     2017/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'K4.002 O35 W11'
_chemical_formula_sum            'K4 O35 W11'
_chemical_formula_weight         2738.75
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           3
_space_group_name_H-M_alt        'P 1 2 1'
_space_group_name_Hall           'P 2y'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'

_cell_length_a                   3.8184(5)
_cell_length_b                   7.2998(9)
_cell_length_c                   25.440(3)
_cell_angle_alpha                90
_cell_angle_beta                 90.026(7)
_cell_angle_gamma                90
_cell_volume                     709.11(15)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    928
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      29.92
_cell_measurement_theta_min      2.79
_shelx_estimated_absorpt_T_max   0.466
_shelx_estimated_absorpt_T_min   0.061
_exptl_absorpt_coefficient_mu    45.118
_exptl_absorpt_correction_T_max  0.7461
_exptl_absorpt_correction_T_min  0.4428
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.0916 before and 0.0531 after correction.
The Ratio of minimum to maximum transmission is 0.5935.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    6.413
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       needle
_exptl_crystal_F_000             1170
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0850
_diffrn_reflns_av_unetI/netI     0.0662
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       36
_diffrn_reflns_limit_l_min       -36
_diffrn_reflns_number            17089
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.608
_diffrn_reflns_theta_min         1.601
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.997
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_reflns_Friedel_coverage         0.868
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.998
_reflns_number_gt                4221
_reflns_number_total             4367
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         5.923
_refine_diff_density_min         -11.028
_refine_diff_density_rms         0.931
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_refine_ls_extinction_coef       0.00079(19)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_goodness_of_fit_ref   1.082
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     179
_refine_ls_number_reflns         4367
_refine_ls_number_restraints     2
_refine_ls_R_factor_all          0.0652
_refine_ls_R_factor_gt           0.0632
_refine_ls_restrained_S_all      1.091
_refine_ls_shift/su_max          4.592
_refine_ls_shift/su_mean         0.166
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0882P)²+17.0568P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1577
_refine_ls_wR_factor_ref         0.1599
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.23947
 0.26214 0.25936 0.23903
2. Restrained distances
 W2-O4
 1.7 with sigma of 0.01
3. Others
 1*[Sof(K1)]+1*[Sof(K2)]+1*[Sof(K4)]=1.5 with esd of 0
 Sof(W6B)=Sof(O18B)=1-FVAR(1)
 Sof(W6A)=Sof(O18A)=FVAR(1)
 Fixed Sof: W1(0.5) O1(0.5)
 Fixed Y: W1(0)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.5933(14) 0.000000 -0.0001(3) 0.0186(10) Uani 0.5 1 d . . P . .
W2 W 0.4818(12) 0.7523(10) 0.12348(12) 0.0341(7) Uani 1 1 d D . . . .
W3 W 0.5447(4) 0.2569(11) 0.12404(14) 0.0187(6) Uani 1 1 d . . . . .
W4 W 0.4586(10) 0.5038(9) 0.25099(5) 0.0292(7) Uani 1 1 d . . . . .
W5 W 0.5023(5) 0.2446(8) 0.37661(10) 0.0054(3) Uani 1 1 d . . . . .
W6A W 0.6098(12) 0.7535(12) 0.37874(19) 0.0211(11) Uani 0.576(9) 1 d . . P . .
W6B W 0.3693(14) 0.7539(14) 0.3744(3) 0.0210(15) Uani 0.424(9) 1 d . . P . .
K1 K 0.104(4) -0.004(5) 0.2539(4) 0.032(3) Uani 0.834(4) 1 d . . P . .
K2 K 0.107(6) 0.494(5) -0.0023(9) 0.018(4) Uani 0.409(4) 1 d . . P . .
K3 K 0.000000 0.007(6) 0.500000 0.056(5) Uani 1 2 d S T P . .
K4 K 0.647(8) 0.495(6) 0.5049(15) 0.006(6) Uani 0.258(4) 1 d . . P . .
O1 O 1.05(3) -0.063(7) 0.003(6) 0.041(19) Uiso 0.5 1 d . . P . .
O2 O 0.568(8) 0.181(4) 0.0510(13) 0.018(6) Uiso 1 1 d . . . . .
O3 O 0.575(9) -0.181(4) 0.0511(15) 0.025(7) Uiso 1 1 d . . . . .
O4 O 0.062(3) 0.777(3) 0.1247(8) -0.001(4) Uiso 1 1 d D . . . .
O5 O 0.431(9) 0.683(4) 0.1930(13) 0.021(6) Uiso 1 1 d . . . . .
O6 O 0.558(7) 1.002(5) 0.1420(7) 0.021(4) Uiso 1 1 d . . . . .
O7 O 0.473(8) 0.501(5) 0.1006(8) 0.024(4) Uiso 1 1 d . . . . .
O8 O 0.114(5) 0.280(3) 0.1214(8) 0.000(4) Uiso 1 1 d . . . . .
O9 O 0.440(8) 0.323(4) 0.1924(13) 0.019(6) Uiso 1 1 d . . . . .
O10 O 0.88(3) 0.49(3) 0.237(2) 0.14(3) Uiso 1 1 d . . . . .
O11 O 0.550(10) 0.687(5) 0.2948(15) 0.028(7) Uiso 1 1 d . . . . .
O12 O 0.572(8) 0.309(4) 0.2968(13) 0.021(6) Uiso 1 1 d . . . . .
O13 O 0.95(2) 0.237(9) 0.363(2) 0.09(2) Uiso 1 1 d . . . . .
O14 O 0.427(10) 0.193(5) 0.4422(16) 0.030(7) Uiso 1 1 d . . . . .
O15 O 0.546(8) 0.500(5) 0.3855(8) 0.024(4) Uiso 1 1 d . . . . .
O16 O 0.457(7) 0.001(5) 0.3501(7) 0.017(4) Uiso 1 1 d . . . . .
O17 O 0.432(9) 0.810(4) 0.4424(13) 0.019(6) Uiso 1 1 d . . . . .
O18A O 1.081(10) 0.776(5) 0.3806(13) -0.001(7) Uiso 0.576(9) 1 d . . P . .
O18B O 0.881(12) 0.769(8) 0.367(2) -0.001(9) Uiso 0.424(9) 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 W1 0.712(11) 2_655 ?
W1 W1 3.106(11) 2_755 ?
W1 K2 3.87(4) 2_645 ?
W1 K2 4.06(3) . ?
W1 K2 3.78(3) 2_655 ?
W1 O1 1.82(11) . ?
W1 O1 1.43(11) 2_755 ?
W1 O1 2.11(11) 1_455 ?
W1 O2 1.95(3) 2_655 ?
W1 O2 1.86(3) . ?
W1 O3 1.86(4) . ?
W1 O3 1.96(4) 2_655 ?
W2 K1 4.029(18) 1_565 ?
W2 K2 3.98(3) . ?
W2 K2 4.25(2) 2 ?
W2 K2 3.94(3) 2_655 ?
W2 O3 1.94(4) 1_565 ?
W2 O4 1.615(12) . ?
W2 O4 2.221(12) 1_655 ?
W2 O5 1.85(3) . ?
W2 O6 1.90(4) . ?
W2 O7 1.93(4) . ?
W3 K1 4.169(19) . ?
W3 K1 4.37(2) 1_655 ?
W3 K2 4.24(3) 1_655 ?
W3 K2 4.33(3) 2 ?
W3 K2 4.02(2) . ?
W3 K2 3.79(3) 2_655 ?
W3 O2 1.94(3) . ?
W3 O6 1.92(4) 1_545 ?
W3 O7 1.90(4) . ?
W3 O8 1.66(2) . ?
W3 O8 2.18(2) 1_655 ?
W3 O9 1.85(3) . ?
W4 K1 3.95(3) . ?
W4 K1 3.84(3) 1_565 ?
W4 O5 1.97(3) . ?
W4 O9 1.99(3) . ?
W4 O10 1.66(10) . ?
W4 O10 2.23(10) 1_455 ?
W4 O11 1.78(3) . ?
W4 O12 1.89(3) . ?
W5 K1 4.283(18) 1_655 ?
W5 K1 3.919(17) . ?
W5 K3 4.068(19) . ?
W5 K3 4.058(19) 1_655 ?
W5 K4 3.57(4) 2_656 ?
W5 K4 3.78(4) . ?
W5 O12 2.10(3) . ?
W5 O13 2.15(8) 1_455 ?
W5 O13 1.73(8) . ?
W5 O14 1.74(4) . ?
W5 O15 1.89(4) . ?
W5 O16 1.91(3) . ?
W6A W6B 2.902(7) 1_655 ?
W6A W6B 0.924(7) . ?
W6A K3 3.89(2) 1_665 ?
W6A K4 3.65(4) 2_656 ?
W6A K4 3.73(4) . ?
W6A O11 2.20(4) . ?
W6A O15 1.87(4) . ?
W6A O16 2.04(3) 1_565 ?
W6A O17 1.80(3) . ?
W6A O18A 2.03(4) 1_455 ?
W6A O18A 1.81(4) . ?
W6A O18B 1.09(5) . ?
W6B K1 3.68(2) 1_565 ?
W6B K3 3.95(2) 1_565 ?
W6B K4 3.61(4) 2_656 ?
W6B O11 2.20(4) . ?
W6B O15 1.99(4) . ?
W6B O16 1.94(3) 1_565 ?
W6B O17 1.79(3) . ?
W6B O18A 1.12(4) 1_455 ?
W6B O18B 1.97(5) . ?
W6B O18B 1.88(5) 1_455 ?
K1 K1 3.8184(5) 1_455 ?
K1 K1 3.8184(5) 1_655 ?
K1 O5 3.03(4) 1_545 ?
K1 O6 3.53(3) 1_445 ?
K1 O6 3.33(2) 1_545 ?
K1 O9 3.13(4) . ?
K1 O11 3.26(4) 1_445 ?
K1 O11 3.01(5) 1_545 ?
K1 O12 3.25(4) 1_455 ?
K1 O12 3.10(4) . ?
K1 O13 3.35(7) 1_455 ?
K1 O16 2.79(2) . ?
K1 O16 3.48(3) 1_455 ?
K1 O18A 3.60(4) 1_445 ?
K1 O18B 3.42(6) 1_445 ?
K2 K2 3.00(4) 2_655 ?
K2 K2 3.8184(5) 1_455 ?
K2 K2 0.83(4) 2 ?
K2 O1 3.24(6) 1_465 ?
K2 O1 3.29(7) 2_665 ?
K2 O2 2.88(4) 2_655 ?
K2 O2 3.18(4) . ?
K2 O2 3.36(4) 1_455 ?
K2 O2 3.66(5) 2 ?
K2 O3 3.40(4) 1_465 ?
K2 O3 2.94(5) 2_665 ?
K2 O3 3.26(5) 1_565 ?
K2 O7 2.97(3) . ?
K2 O7 2.97(3) 2_655 ?
K2 O7 3.34(3) 2 ?
K2 O7 3.57(3) 1_455 ?
K2 O8 3.52(3) . ?
K2 O8 3.51(4) 2 ?
K3 K3 3.8184(6) 1_655 ?
K3 K3 3.8184(6) 1_455 ?
K3 K4 3.81(6) 2_656 ?
K3 K4 3.98(6) 2_646 ?
K3 K4 3.98(6) 1_445 ?
K3 K4 3.81(6) 1_455 ?
K3 O14 2.58(5) 2_556 ?
K3 O14 2.96(4) 2_656 ?
K3 O14 2.96(4) 1_455 ?
K3 O14 2.58(5) . ?
K3 O17 2.64(4) 2_546 ?
K3 O17 2.99(4) 2_646 ?
K3 O17 2.99(4) 1_445 ?
K3 O17 2.64(4) 1_545 ?
K3 O18A 3.49(4) 2_646 ?
K3 O18A 3.49(4) 1_445 ?
K4 K4 3.8184(8) 1_655 ?
K4 K4 1.15(6) 2_656 ?
K4 K4 3.8184(8) 1_455 ?
K4 K4 2.71(6) 2_756 ?
K4 O14 2.85(6) . ?
K4 O14 2.60(6) 2_656 ?
K4 O15 2.88(4) 2_656 ?
K4 O15 3.06(4) . ?
K4 O17 2.91(6) . ?
K4 O17 2.68(5) 2_656 ?
K4 O18A 3.71(5) 2_756 ?
O1 O1 0.4(2) 2_755 ?
O18A O18B 0.84(6) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W1 W1 W1 179.4(13) 2_655 2_755 ?
W1 W1 K2 72.8(3) 2_755 2_645 ?
W1 W1 K2 107.2(3) 2_655 2_645 ?
W1 W1 K2 107.6(4) 2_655 2_655 ?
W1 W1 K2 62.8(4) 2_655 . ?
W1 W1 K2 72.4(4) 2_755 2_655 ?
W1 W1 K2 117.2(4) 2_755 . ?
W1 W1 O1 12.7(16) 2_655 1_455 ?
W1 W1 O1 161(3) 2_655 2_755 ?
W1 W1 O1 165(2) 2_655 . ?
W1 W1 O2 86.6(13) 2_655 . ?
W1 W1 O2 72.0(11) 2_655 2_655 ?
W1 W1 O3 71.3(12) 2_655 2_655 ?
W1 W1 O3 87.5(13) 2_655 . ?
K2 W1 K2 145.1(7) 2_655 2_645 ?
K2 W1 K2 170.0(4) 2_645 . ?
K2 W1 K2 44.9(8) 2_655 . ?
O1 W1 W1 14.9(19) . 2_755 ?
O1 W1 W1 167.2(16) 1_455 2_755 ?
O1 W1 W1 19(3) 2_755 2_755 ?
O1 W1 K2 136(3) 2_755 . ?
O1 W1 K2 94.5(15) 1_455 2_645 ?
O1 W1 K2 120.2(16) 1_455 2_655 ?
O1 W1 K2 58.0(18) . 2_645 ?
O1 W1 K2 132.0(17) . . ?
O1 W1 K2 75.4(15) 1_455 . ?
O1 W1 K2 54(3) 2_755 2_645 ?
O1 W1 K2 87.1(19) . 2_655 ?
O1 W1 K2 91(2) 2_755 2_655 ?
O1 W1 O1 6(9) 2_755 . ?
O1 W1 O1 148(4) 2_755 1_455 ?
O1 W1 O1 152(3) . 1_455 ?
O1 W1 O2 119(5) 2_755 2_655 ?
O1 W1 O2 120(4) . 2_655 ?
O1 W1 O2 108(5) 2_755 . ?
O1 W1 O2 102(4) . . ?
O1 W1 O3 100(4) . 2_655 ?
O1 W1 O3 80(4) . . ?
O1 W1 O3 81(5) 2_755 . ?
O1 W1 O3 94(5) 2_755 2_655 ?
O2 W1 W1 93.0(10) . 2_755 ?
O2 W1 W1 108.4(10) 2_655 2_755 ?
O2 W1 K2 57.2(10) 2_655 2_655 ?
O2 W1 K2 40.8(10) 2_655 . ?
O2 W1 K2 138.8(10) 2_655 2_645 ?
O2 W1 K2 47.6(10) . 2_655 ?
O2 W1 K2 133.2(11) . 2_645 ?
O2 W1 K2 49.6(11) . . ?
O2 W1 O1 95(3) . 1_455 ?
O2 W1 O1 82(3) 2_655 1_455 ?
O2 W1 O2 87.9(19) . 2_655 ?
O2 W1 O3 90.8(9) . . ?
O2 W1 O3 85.2(9) 2_655 2_655 ?
O2 W1 O3 157.9(17) . 2_655 ?
O3 W1 W1 109.2(10) 2_655 2_755 ?
O3 W1 W1 92.1(11) . 2_755 ?
O3 W1 K2 116.2(11) 2_655 . ?
O3 W1 K2 57.5(11) 2_655 2_645 ?
O3 W1 K2 132.7(12) . 2_655 ?
O3 W1 K2 128.7(11) . . ?
O3 W1 K2 47.2(11) . 2_645 ?
O3 W1 K2 138.9(11) 2_655 2_655 ?
O3 W1 O1 78(3) . 1_455 ?
O3 W1 O1 64(3) 2_655 1_455 ?
O3 W1 O2 159.5(17) . 2_655 ?
O3 W1 O3 88(2) . 2_655 ?
K1 W2 K2 127.1(4) 1_565 2 ?
K2 W2 K1 176.0(6) 2_655 1_565 ?
K2 W2 K1 137.9(4) . 1_565 ?
K2 W2 K2 55.4(3) 2_655 2 ?
K2 W2 K2 10.9(6) . 2 ?
K2 W2 K2 44.6(6) 2_655 . ?
O3 W2 K1 137.6(11) 1_565 1_565 ?
O3 W2 K2 54.5(11) 1_565 . ?
O3 W2 K2 45.8(11) 1_565 2_655 ?
O3 W2 K2 61.3(11) 1_565 2 ?
O3 W2 O4 79.0(12) 1_565 1_655 ?
O4 W2 K1 65.1(8) . 1_565 ?
O4 W2 K1 108.0(6) 1_655 1_565 ?
O4 W2 K2 117.7(8) . 2_655 ?
O4 W2 K2 124.9(6) 1_655 2 ?
O4 W2 K2 73.3(8) . . ?
O4 W2 K2 114.1(6) 1_655 . ?
O4 W2 K2 69.7(6) 1_655 2_655 ?
O4 W2 K2 62.6(8) . 2 ?
O4 W2 O3 100.0(13) . 1_565 ?
O4 W2 O4 168.6(14) . 1_655 ?
O4 W2 O5 84.7(13) . . ?
O4 W2 O6 92.3(11) . . ?
O4 W2 O7 95.5(12) . . ?
O5 W2 K1 45.3(10) . 1_565 ?
O5 W2 K2 126.9(11) . . ?
O5 W2 K2 131.1(11) . 2_655 ?
O5 W2 K2 121.0(11) . 2 ?
O5 W2 O3 175.3(16) . 1_565 ?
O5 W2 O4 96.6(12) . 1_655 ?
O5 W2 O6 92.5(11) . . ?
O5 W2 O7 91.4(12) . . ?
O6 W2 K1 55.2(8) . 1_565 ?
O6 W2 K2 135.0(8) . . ?
O6 W2 K2 126.2(8) . 2_655 ?
O6 W2 K2 133.2(9) . 2 ?
O6 W2 O3 88.2(12) . 1_565 ?
O6 W2 O4 76.4(10) . 1_655 ?
O6 W2 O7 171.6(12) . . ?
O7 W2 K1 131.5(9) . 1_565 ?
O7 W2 K2 45.5(8) . . ?
O7 W2 K2 46.7(9) . 2_655 ?
O7 W2 K2 49.4(9) . 2 ?
O7 W2 O3 87.3(11) . 1_565 ?
O7 W2 O4 95.7(11) . 1_655 ?
K1 W3 K1 53.1(3) . 1_655 ?
K1 W3 K2 121.2(4) . 2 ?
K1 W3 K2 173.2(5) . 1_655 ?
K2 W3 K1 131.6(4) . . ?
K2 W3 K1 130.2(4) 2_655 1_655 ?
K2 W3 K1 175.1(3) . 1_655 ?
K2 W3 K1 174.2(4) 2 1_655 ?
K2 W3 K1 176.7(4) 2_655 . ?
K2 W3 K1 120.3(3) 1_655 1_655 ?
K2 W3 K2 45.2(7) 2_655 . ?
K2 W3 K2 55.6(4) 2_655 2 ?
K2 W3 K2 9.9(6) 2_655 1_655 ?
K2 W3 K2 65.5(5) 1_655 2 ?
K2 W3 K2 10.5(6) . 2 ?
K2 W3 K2 55.0(3) . 1_655 ?
O2 W3 K1 130.4(10) . . ?
O2 W3 K1 125.3(10) . 1_655 ?
O2 W3 K2 50.7(10) . 1_655 ?
O2 W3 K2 57.0(10) . 2 ?
O2 W3 K2 48.0(10) . 2_655 ?
O2 W3 K2 51.3(10) . . ?
O2 W3 O8 86.9(11) . 1_655 ?
O6 W3 K1 51.9(8) 1_545 1_655 ?
O6 W3 K1 51.5(8) 1_545 . ?
O6 W3 K2 129.0(8) 1_545 2_655 ?
O6 W3 K2 125.1(8) 1_545 2 ?
O6 W3 K2 128.4(8) 1_545 . ?
O6 W3 K2 124.3(8) 1_545 1_655 ?
O6 W3 O2 87.3(11) 1_545 . ?
O6 W3 O8 93.1(10) 1_545 1_655 ?
O7 W3 K1 128.3(9) . . ?
O7 W3 K1 135.8(9) . 1_655 ?
O7 W3 K2 56.7(9) . 1_655 ?
O7 W3 K2 44.2(9) . . ?
O7 W3 K2 50.6(9) . 2_655 ?
O7 W3 K2 47.0(9) . 2 ?
O7 W3 O2 88.4(11) . . ?
O7 W3 O6 171.8(11) . 1_545 ?
O7 W3 O8 93.6(11) . 1_655 ?
O8 W3 K1 124.1(8) . 1_655 ?
O8 W3 K1 71.2(7) . . ?
O8 W3 K1 64.5(6) 1_655 1_655 ?
O8 W3 K1 117.5(7) 1_655 . ?
O8 W3 K2 55.9(6) 1_655 1_655 ?
O8 W3 K2 60.7(8) . . ?
O8 W3 K2 65.8(7) 1_655 2_655 ?
O8 W3 K2 110.9(7) 1_655 . ?
O8 W3 K2 50.2(8) . 2 ?
O8 W3 K2 105.7(9) . 2_655 ?
O8 W3 K2 115.6(8) . 1_655 ?
O8 W3 K2 121.3(6) 1_655 2 ?
O8 W3 O2 92.0(12) . . ?
O8 W3 O6 97.7(12) . 1_545 ?
O8 W3 O7 75.5(12) . . ?
O8 W3 O8 169.1(14) . 1_655 ?
O8 W3 O9 78.3(13) . . ?
O9 W3 K1 44.5(10) . . ?
O9 W3 K1 60.5(10) . 1_655 ?
O9 W3 K2 116.4(11) . 2 ?
O9 W3 K2 135.8(10) . 1_655 ?
O9 W3 K2 136.5(10) . 2_655 ?
O9 W3 K2 123.5(11) . . ?
O9 W3 O2 170.1(15) . . ?
O9 W3 O6 91.9(11) . 1_545 ?
O9 W3 O7 91.2(12) . . ?
O9 W3 O8 103.0(12) . 1_655 ?
K1 W4 K1 139.3(4) 1_565 . ?
O5 W4 K1 51.4(9) . 1_565 ?
O5 W4 K1 128.1(10) . . ?
O5 W4 O9 83.0(8) . . ?
O5 W4 O10 81(4) . 1_455 ?
O9 W4 K1 128.5(10) . 1_565 ?
O9 W4 K1 51.6(9) . . ?
O9 W4 O10 80(4) . 1_455 ?
O10 W4 K1 113(8) . 1_565 ?
O10 W4 K1 107(8) . . ?
O10 W4 K1 72(6) 1_455 1_565 ?
O10 W4 K1 69(6) 1_455 . ?
O10 W4 O5 85(5) . . ?
O10 W4 O9 81(5) . . ?
O10 W4 O10 158(4) . 1_455 ?
O10 W4 O11 89(6) . . ?
O10 W4 O12 83(6) . . ?
O11 W4 K1 139.7(12) . . ?
O11 W4 K1 49.6(12) . 1_565 ?
O11 W4 O5 89.0(15) . . ?
O11 W4 O9 167.4(16) . . ?
O11 W4 O10 108(5) . 1_455 ?
O11 W4 O12 97.7(9) . . ?
O12 W4 K1 50.2(10) . . ?
O12 W4 K1 140.6(10) . 1_565 ?
O12 W4 O5 166.4(14) . . ?
O12 W4 O9 88.3(14) . . ?
O12 W4 O10 108(5) . 1_455 ?
K1 W5 K1 55.3(2) . 1_655 ?
K1 W5 K3 103.6(4) . . ?
K1 W5 K3 126.8(6) . 1_655 ?
K3 W5 K1 97.5(4) 1_655 1_655 ?
K3 W5 K1 129.4(6) . 1_655 ?
K3 W5 K3 56.1(3) 1_655 . ?
K4 W5 K1 139.1(5) . 1_655 ?
K4 W5 K1 148.0(6) 2_656 . ?
K4 W5 K1 156.7(6) 2_656 1_655 ?
K4 W5 K1 165.6(5) . . ?
K4 W5 K3 68.9(8) 2_656 1_655 ?
K4 W5 K3 59.4(8) 2_656 . ?
K4 W5 K3 66.9(8) . . ?
K4 W5 K3 58.0(8) . 1_655 ?
K4 W5 K4 17.7(9) 2_656 . ?
O12 W5 K1 47.4(9) . 1_655 ?
O12 W5 K1 51.9(9) . . ?
O12 W5 K3 141.7(9) . 1_655 ?
O12 W5 K3 154.3(9) . . ?
O12 W5 K4 135.0(11) . . ?
O12 W5 K4 136.1(10) . 2_656 ?
O12 W5 O13 88.7(19) . 1_455 ?
O13 W5 K1 58.6(18) 1_455 . ?
O13 W5 K1 113.8(18) 1_455 1_655 ?
O13 W5 K1 47(2) . 1_655 ?
O13 W5 K1 102(2) . . ?
O13 W5 K3 127(2) . . ?
O13 W5 K3 71(2) . 1_655 ?
O13 W5 K3 69.2(17) 1_455 . ?
O13 W5 K3 124.9(17) 1_455 1_655 ?
O13 W5 K4 89.4(18) 1_455 2_656 ?
O13 W5 K4 92(2) . . ?
O13 W5 K4 107.1(19) 1_455 . ?
O13 W5 K4 110(2) . 2_656 ?
O13 W5 O12 72(2) . . ?
O13 W5 O13 159(4) . 1_455 ?
O13 W5 O14 110(2) . . ?
O13 W5 O15 88(2) . . ?
O13 W5 O16 89(2) . . ?
O14 W5 K1 134.2(13) . 1_655 ?
O14 W5 K1 126.9(13) . . ?
O14 W5 K3 40.6(13) . 1_655 ?
O14 W5 K3 24.0(14) . . ?
O14 W5 K4 43.4(14) . 2_656 ?
O14 W5 K4 45.5(14) . . ?
O14 W5 O12 177.7(17) . . ?
O14 W5 O13 89(2) . 1_455 ?
O14 W5 O15 96.6(13) . . ?
O14 W5 O16 97.0(14) . . ?
O15 W5 K1 117.4(8) . 1_655 ?
O15 W5 K1 126.0(8) . . ?
O15 W5 K3 111.8(9) . . ?
O15 W5 K3 106.8(9) . 1_655 ?
O15 W5 K4 53.6(10) . . ?
O15 W5 K4 53.7(9) . 2_656 ?
O15 W5 O12 83.2(10) . . ?
O15 W5 O13 98(2) . 1_455 ?
O15 W5 O16 166.1(9) . . ?
O16 W5 K1 52.9(8) . 1_655 ?
O16 W5 K1 41.5(8) . . ?
O16 W5 K3 80.4(8) . . ?
O16 W5 K3 85.3(9) . 1_655 ?
O16 W5 K4 139.5(9) . 2_656 ?
O16 W5 K4 140.2(9) . . ?
O16 W5 O12 83.1(10) . . ?
O16 W5 O13 80(2) . 1_455 ?
W6B W6A W6B 171.0(8) . 1_655 ?
W6B W6A K3 118.1(7) . 1_665 ?
W6B W6A K3 69.3(2) 1_655 1_665 ?
W6B W6A K4 80.2(8) . 2_656 ?
W6B W6A K4 107.5(5) 1_655 2_656 ?
W6B W6A K4 89.7(6) 1_655 . ?
W6B W6A K4 98.1(8) . . ?
W6B W6A O11 77.5(12) . . ?
W6B W6A O15 83.4(12) . . ?
W6B W6A O16 70.7(11) . 1_565 ?
W6B W6A O17 74.4(13) . . ?
W6B W6A O18A 9.3(11) . 1_455 ?
W6B W6A O18A 172.4(14) . . ?
W6B W6A O18B 156(3) . . ?
K4 W6A K3 62.9(8) . 1_665 ?
K4 W6A K3 72.9(8) 2_656 1_665 ?
K4 W6A K4 17.9(9) 2_656 . ?
O11 W6A W6B 93.8(11) . 1_655 ?
O11 W6A K3 155.9(10) . 1_665 ?
O11 W6A K4 136.7(11) . . ?
O11 W6A K4 130.2(11) . 2_656 ?
O15 W6A W6B 97.8(10) . 1_655 ?
O15 W6A K3 116.5(9) . 1_665 ?
O15 W6A K4 55.0(9) . . ?
O15 W6A K4 51.6(10) . 2_656 ?
O15 W6A O11 81.8(11) . . ?
O15 W6A O16 150.7(11) . 1_565 ?
O15 W6A O18A 87.1(14) . 1_455 ?
O16 W6A W6B 105.8(8) 1_565 1_655 ?
O16 W6A K3 88.3(8) 1_565 1_665 ?
O16 W6A K4 140.3(9) 1_565 . ?
O16 W6A K4 132.3(9) 1_565 2_656 ?
O16 W6A O11 79.5(10) 1_565 . ?
O17 W6A W6B 114.2(11) . 1_655 ?
O17 W6A K3 47.5(11) . 1_665 ?
O17 W6A K4 44.5(12) . 2_656 ?
O17 W6A K4 49.9(12) . . ?
O17 W6A O11 151.9(16) . . ?
O17 W6A O15 95.3(11) . . ?
O17 W6A O16 90.7(11) . 1_565 ?
O17 W6A O18A 65.4(15) . 1_455 ?
O18A W6A W6B 6.4(11) . 1_655 ?
O18A W6A W6B 175.1(11) 1_455 1_655 ?
O18A W6A K3 108.8(10) 1_455 1_665 ?
O18A W6A K3 63.5(11) . 1_665 ?
O18A W6A K4 75.8(12) 1_455 2_656 ?
O18A W6A K4 89.2(13) . . ?
O18A W6A K4 107.2(12) . 2_656 ?
O18A W6A K4 93.4(11) 1_455 . ?
O18A W6A O11 98.6(15) . . ?
O18A W6A O11 86.5(14) 1_455 . ?
O18A W6A O15 102.7(15) . . ?
O18A W6A O16 69.4(13) 1_455 1_565 ?
O18A W6A O16 102.3(14) . 1_565 ?
O18A W6A O17 109.3(15) . . ?
O18A W6A O18A 170(2) . 1_455 ?
O18B W6A W6B 15(3) . 1_655 ?
O18B W6A K3 79(3) . 1_665 ?
O18B W6A K4 123(3) . 2_656 ?
O18B W6A K4 105(3) . . ?
O18B W6A O11 81(3) . . ?
O18B W6A O15 105(3) . . ?
O18B W6A O16 95(3) . 1_565 ?
O18B W6A O17 126(3) . . ?
O18B W6A O18A 18(3) . . ?
O18B W6A O18A 162(3) . 1_455 ?
W6A W6B W6A 171.0(8) . 1_455 ?
W6A W6B K1 76.0(3) 1_455 1_565 ?
W6A W6B K1 111.9(7) . 1_565 ?
W6A W6B K3 105.1(7) . 1_565 ?
W6A W6B K3 67.2(2) 1_455 1_565 ?
W6A W6B K4 87.1(5) 1_455 2_656 ?
W6A W6B K4 85.1(9) . 2_656 ?
W6A W6B O11 78.2(12) . . ?
W6A W6B O15 69.1(11) . . ?
W6A W6B O16 82.6(11) . 1_565 ?
W6A W6B O17 75.8(13) . . ?
W6A W6B O18A 163(2) . 1_455 ?
W6A W6B O18B 13.0(17) . . ?
W6A W6B O18B 177(2) . 1_455 ?
K1 W6B K3 110.6(5) 1_565 1_565 ?
K4 W6B K1 162.9(6) 2_656 1_565 ?
K4 W6B K3 63.3(9) 2_656 1_565 ?
O11 W6B W6A 110.4(11) . 1_455 ?
O11 W6B K1 54.8(10) . 1_565 ?
O11 W6B K3 164.2(11) . 1_565 ?
O11 W6B K4 132.4(12) . 2_656 ?
O15 W6B W6A 109.4(9) . 1_455 ?
O15 W6B K1 131.0(8) . 1_565 ?
O15 W6B K3 116.2(8) . 1_565 ?
O15 W6B K4 53.0(9) . 2_656 ?
O15 W6B O11 79.5(11) . . ?
O16 W6B W6A 100.7(8) 1_565 1_455 ?
O16 W6B K1 48.2(7) 1_565 1_565 ?
O16 W6B K3 83.4(9) 1_565 1_565 ?
O16 W6B K4 139.8(9) 1_565 2_656 ?
O16 W6B O11 81.8(11) 1_565 . ?
O16 W6B O15 148.6(11) 1_565 . ?
O16 W6B O18B 75.3(19) 1_565 . ?
O17 W6B W6A 95.5(11) . 1_455 ?
O17 W6B K1 137.1(11) . 1_565 ?
O17 W6B K3 33.0(11) . 1_565 ?
O17 W6B K4 45.6(13) . 2_656 ?
O17 W6B O11 154.0(15) . . ?
O17 W6B O15 91.7(12) . . ?
O17 W6B O16 94.3(12) . 1_565 ?
O17 W6B O18B 87.3(19) . . ?
O17 W6B O18B 103(2) . 1_455 ?
O18A W6B W6A 10.4(18) 1_455 1_455 ?
O18A W6B K1 77.2(19) 1_455 1_565 ?
O18A W6B K3 57.9(17) 1_455 1_565 ?
O18A W6B K4 87(2) 1_455 2_656 ?
O18A W6B O11 118(2) 1_455 . ?
O18A W6B O15 117(2) 1_455 . ?
O18A W6B O16 94(2) 1_455 1_565 ?
O18A W6B O17 88(2) 1_455 . ?
O18A W6B O18B 15(2) 1_455 1_455 ?
O18A W6B O18B 168(3) 1_455 . ?
O18B W6B W6A 175.3(17) . 1_455 ?
O18B W6B W6A 8.9(17) 1_455 1_455 ?
O18B W6B K1 67.2(18) 1_455 1_565 ?
O18B W6B K1 99.4(17) . 1_565 ?
O18B W6B K3 72.8(17) 1_455 1_565 ?
O18B W6B K3 114.2(17) . 1_565 ?
O18B W6B K4 95.8(19) 1_455 2_656 ?
O18B W6B K4 97.6(17) . 2_656 ?
O18B W6B O11 66.8(19) . . ?
O18B W6B O11 103(2) 1_455 . ?
O18B W6B O15 74(2) . . ?
O18B W6B O15 114(2) 1_455 . ?
O18B W6B O16 95(2) 1_455 1_565 ?
O18B W6B O18B 167(3) 1_455 . ?
W4 K1 W2 106.0(4) . 1_545 ?
W4 K1 W2 56.3(4) 1_545 1_545 ?
W4 K1 W4 139.3(4) 1_545 . ?
W4 K1 W5 108.2(5) 1_545 . ?
W5 K1 W2 136.2(4) . 1_545 ?
W5 K1 W4 56.4(4) . . ?
W6B K1 W2 112.1(8) 1_545 1_545 ?
W6B K1 W4 111.8(4) 1_545 . ?
W6B K1 W4 58.0(5) 1_545 1_545 ?
W6B K1 W5 56.8(2) 1_545 . ?
W6B K1 K1 105.9(3) 1_545 1_455 ?
W6B K1 K1 74.1(3) 1_545 1_655 ?
K1 K1 W2 69.0(2) 1_655 1_545 ?
K1 K1 W2 111.0(2) 1_455 1_545 ?
K1 K1 W4 110.0(3) 1_455 . ?
K1 K1 W4 110.6(3) 1_455 1_545 ?
K1 K1 W4 69.4(3) 1_655 1_545 ?
K1 K1 W4 70.0(3) 1_655 . ?
K1 K1 W5 67.2(3) 1_655 . ?
K1 K1 W5 112.8(3) 1_455 . ?
K1 K1 K1 180.00(3) 1_455 1_655 ?
O5 K1 W2 25.7(6) 1_545 1_545 ?
O5 K1 W4 123.9(8) 1_545 . ?
O5 K1 W4 30.6(7) 1_545 1_545 ?
O5 K1 W5 126.7(9) 1_545 . ?
O5 K1 W6B 87.2(10) 1_545 1_545 ?
O5 K1 K1 114.3(7) 1_545 1_455 ?
O5 K1 K1 65.7(7) 1_545 1_655 ?
O5 K1 O6 80.8(9) 1_545 1_445 ?
O5 K1 O6 50.2(9) 1_545 1_545 ?
O5 K1 O9 98.7(7) 1_545 . ?
O5 K1 O11 84.8(13) 1_545 1_445 ?
O5 K1 O12 163.8(11) 1_545 1_455 ?
O5 K1 O12 120.0(11) 1_545 . ?
O5 K1 O13 153.6(16) 1_545 1_455 ?
O5 K1 O16 131.4(13) 1_545 1_455 ?
O5 K1 O18A 97.7(13) 1_545 1_445 ?
O5 K1 O18B 99.6(14) 1_545 1_445 ?
O6 K1 W2 63.5(5) 1_445 1_545 ?
O6 K1 W2 28.0(6) 1_545 1_545 ?
O6 K1 W4 100.1(9) 1_445 . ?
O6 K1 W4 79.2(8) 1_545 1_545 ?
O6 K1 W4 101.8(8) 1_445 1_545 ?
O6 K1 W4 78.1(8) 1_545 . ?
O6 K1 W5 150.0(11) 1_445 . ?
O6 K1 W5 118.2(7) 1_545 . ?
O6 K1 W6B 125.1(9) 1_545 1_545 ?
O6 K1 W6B 147.2(10) 1_445 1_545 ?
O6 K1 K1 121.4(5) 1_545 1_455 ?
O6 K1 K1 53.8(5) 1_445 1_455 ?
O6 K1 K1 126.2(5) 1_445 1_655 ?
O6 K1 K1 58.6(5) 1_545 1_655 ?
O6 K1 O6 67.6(4) 1_545 1_445 ?
O6 K1 O13 142.8(17) 1_545 1_455 ?
O6 K1 O16 166.0(8) 1_545 1_455 ?
O6 K1 O18A 135.5(11) 1_445 1_445 ?
O6 K1 O18A 141.6(12) 1_545 1_445 ?
O6 K1 O18B 148.5(14) 1_545 1_445 ?
O9 K1 W2 77.2(6) . 1_545 ?
O9 K1 W4 124.1(7) . 1_545 ?
O9 K1 W4 29.9(7) . . ?
O9 K1 W5 83.4(9) . . ?
O9 K1 W6B 132.0(8) . 1_545 ?
O9 K1 K1 65.8(7) . 1_655 ?
O9 K1 K1 114.2(7) . 1_455 ?
O9 K1 O6 80.2(9) . 1_445 ?
O9 K1 O6 49.4(9) . 1_545 ?
O9 K1 O11 162.3(11) . 1_445 ?
O9 K1 O12 83.5(12) . 1_455 ?
O9 K1 O13 95.0(16) . 1_455 ?
O9 K1 O16 129.3(13) . 1_455 ?
O9 K1 O18A 142.8(11) . 1_445 ?
O9 K1 O18B 153.0(12) . 1_445 ?
O11 K1 W2 101.0(10) 1_445 1_545 ?
O11 K1 W2 75.7(9) 1_545 1_545 ?
O11 K1 W4 26.7(7) 1_545 1_545 ?
O11 K1 W4 151.3(9) 1_445 . ?
O11 K1 W4 65.7(9) 1_445 1_545 ?
O11 K1 W4 121.1(9) 1_545 . ?
O11 K1 W5 108.5(7) 1_445 . ?
O11 K1 W5 81.5(8) 1_545 . ?
O11 K1 W6B 36.6(8) 1_545 1_545 ?
O11 K1 W6B 65.2(8) 1_445 1_545 ?
O11 K1 K1 49.5(8) 1_445 1_455 ?
O11 K1 K1 55.6(8) 1_545 1_655 ?
O11 K1 K1 124.4(8) 1_545 1_455 ?
O11 K1 K1 130.5(8) 1_445 1_655 ?
O11 K1 O5 51.7(11) 1_545 1_545 ?
O11 K1 O6 83.3(10) 1_445 1_445 ?
O11 K1 O6 128.5(13) 1_545 1_445 ?
O11 K1 O6 128.3(12) 1_445 1_545 ?
O11 K1 O6 90.7(11) 1_545 1_545 ?
O11 K1 O9 120.8(11) 1_545 . ?
O11 K1 O11 74.9(10) 1_545 1_445 ?
O11 K1 O12 96.1(8) 1_545 . ?
O11 K1 O12 139.9(7) 1_545 1_455 ?
O11 K1 O13 88.9(14) 1_445 1_455 ?
O11 K1 O13 102.0(15) 1_545 1_455 ?
O11 K1 O16 47.3(8) 1_445 1_455 ?
O11 K1 O16 99.6(10) 1_545 1_455 ?
O11 K1 O18A 52.5(10) 1_445 1_445 ?
O11 K1 O18A 51.1(10) 1_545 1_445 ?
O11 K1 O18B 59.2(12) 1_545 1_445 ?
O11 K1 O18B 40.2(11) 1_445 1_445 ?
O12 K1 W2 144.2(8) 1_455 1_545 ?
O12 K1 W2 114.2(7) . 1_545 ?
O12 K1 W4 152.4(8) 1_455 1_545 ?
O12 K1 W4 63.8(8) 1_455 . ?
O12 K1 W4 27.9(6) . . ?
O12 K1 W4 119.7(8) . 1_545 ?
O12 K1 W5 69.4(7) 1_455 . ?
O12 K1 W5 32.2(6) . . ?
O12 K1 W6B 103.3(6) 1_455 1_545 ?
O12 K1 W6B 84.4(7) . 1_545 ?
O12 K1 K1 54.9(7) . 1_655 ?
O12 K1 K1 51.3(7) 1_455 1_455 ?
O12 K1 K1 125.1(7) . 1_455 ?
O12 K1 K1 128.7(7) 1_455 1_655 ?
O12 K1 O6 127.1(12) 1_455 1_545 ?
O12 K1 O6 89.5(10) . 1_545 ?
O12 K1 O6 127.9(13) . 1_445 ?
O12 K1 O6 83.8(9) 1_455 1_445 ?
O12 K1 O9 51.4(10) . . ?
O12 K1 O11 140.4(6) . 1_445 ?
O12 K1 O11 88.5(7) 1_455 1_445 ?
O12 K1 O12 73.8(9) . 1_455 ?
O12 K1 O13 40.4(14) 1_455 1_455 ?
O12 K1 O13 54.7(15) . 1_455 ?
O12 K1 O16 46.4(8) 1_455 1_455 ?
O12 K1 O16 98.8(9) . 1_455 ?
O12 K1 O18A 89.8(9) 1_455 1_445 ?
O12 K1 O18A 91.6(9) . 1_445 ?
O12 K1 O18B 101.9(11) . 1_445 ?
O12 K1 O18B 84.4(11) 1_455 1_445 ?
O13 K1 W2 168.7(15) 1_455 1_545 ?
O13 K1 W4 65.4(13) 1_455 . ?
O13 K1 W4 124.8(13) 1_455 1_545 ?
O13 K1 W5 33.2(14) 1_455 . ?
O13 K1 W6B 66.9(12) 1_455 1_545 ?
O13 K1 K1 79.6(14) 1_455 1_455 ?
O13 K1 K1 100.4(14) 1_455 1_655 ?
O13 K1 O6 123.9(16) 1_455 1_445 ?
O13 K1 O16 44.0(14) 1_455 1_455 ?
O13 K1 O18A 59.0(12) 1_455 1_445 ?
O13 K1 O18B 60.8(12) 1_455 1_445 ?
O16 K1 W2 123.8(9) . 1_545 ?
O16 K1 W2 147.0(9) 1_455 1_545 ?
O16 K1 W4 80.6(9) . . ?
O16 K1 W4 106.0(9) 1_455 1_545 ?
O16 K1 W4 104.2(9) 1_455 . ?
O16 K1 W4 82.0(9) . 1_545 ?
O16 K1 W5 26.9(7) . . ?
O16 K1 W5 73.1(5) 1_455 . ?
O16 K1 W6B 31.2(8) . 1_545 ?
O16 K1 W6B 67.4(5) 1_455 1_545 ?
O16 K1 K1 118.8(6) . 1_455 ?
O16 K1 K1 135.3(4) 1_455 1_655 ?
O16 K1 K1 61.2(6) . 1_655 ?
O16 K1 K1 44.7(4) 1_455 1_455 ?
O16 K1 O5 105.2(13) . 1_545 ?
O16 K1 O6 172.4(9) . 1_445 ?
O16 K1 O6 98.5(7) 1_455 1_445 ?
O16 K1 O6 119.8(8) . 1_545 ?
O16 K1 O9 103.2(12) . . ?
O16 K1 O11 55.7(10) . 1_545 ?
O16 K1 O11 92.5(10) . 1_445 ?
O16 K1 O12 89.8(10) . 1_455 ?
O16 K1 O12 53.4(9) . . ?
O16 K1 O13 49.5(14) . 1_455 ?
O16 K1 O16 74.1(5) . 1_455 ?
O16 K1 O18A 40.0(9) . 1_445 ?
O16 K1 O18A 50.0(8) 1_455 1_445 ?
O16 K1 O18B 52.6(11) . 1_445 ?
O18A K1 W2 123.4(11) 1_445 1_545 ?
O18A K1 W4 116.3(8) 1_445 . ?
O18A K1 W4 67.1(8) 1_445 1_545 ?
O18A K1 W5 60.1(6) 1_445 . ?
O18A K1 W6B 17.7(6) 1_445 1_545 ?
O18A K1 K1 88.6(7) 1_445 1_455 ?
O18A K1 K1 91.4(7) 1_445 1_655 ?
O18B K1 W2 124.5(13) 1_445 1_545 ?
O18B K1 W4 123.8(10) 1_445 . ?
O18B K1 W4 69.6(10) 1_445 1_545 ?
O18B K1 W5 69.7(9) 1_445 . ?
O18B K1 W6B 30.4(8) 1_445 1_545 ?
O18B K1 K1 104.5(8) 1_445 1_655 ?
O18B K1 K1 75.5(8) 1_445 1_455 ?
O18B K1 O6 122.4(10) 1_445 1_445 ?
O18B K1 O16 40.4(10) 1_445 1_455 ?
O18B K1 O18A 13.5(11) 1_445 1_445 ?
W1 K2 W3 58.1(5) 2_655 2_655 ?
W1 K2 K2 107.6(4) 2_655 1_455 ?
W3 K2 K2 110.6(4) 2_655 1_455 ?
K2 K2 W1 72.4(4) 2_655 2_655 ?
K2 K2 W1 107.3(4) 2 2_655 ?
K2 K2 W3 71.4(7) 2_655 2_655 ?
K2 K2 W3 118(3) 2 2_655 ?
K2 K2 K2 8(3) 2 1_455 ?
K2 K2 K2 169(4) 2 2_655 ?
K2 K2 K2 177.7(8) 2_655 1_455 ?
K2 K2 O1 86(2) 2 1_465 ?
K2 K2 O1 100.7(19) 2_655 2_665 ?
K2 K2 O1 79.4(19) 2 2_665 ?
K2 K2 O1 94(2) 2_655 1_465 ?
K2 K2 O2 119.3(17) 2 2_655 ?
K2 K2 O2 48.3(14) 2 1_455 ?
K2 K2 O2 126.6(9) 2_655 1_455 ?
K2 K2 O2 49.6(17) 2 2 ?
K2 K2 O2 119(2) 2 . ?
K2 K2 O2 135.8(8) 2_655 2 ?
K2 K2 O2 55.4(8) 2_655 . ?
K2 K2 O3 55.7(8) 2_655 1_565 ?
K2 K2 O3 119(2) 2 1_565 ?
K2 K2 O3 49.6(13) 2 1_465 ?
K2 K2 O3 125.5(10) 2_655 1_465 ?
K2 K2 O3 118.0(16) 2 2_665 ?
K2 K2 O7 133.8(12) 2_655 2 ?
K2 K2 O7 130.5(12) 2_655 1_455 ?
K2 K2 O7 131(3) 2 2_655 ?
K2 K2 O7 110(3) 2 . ?
K2 K2 O7 39(3) 2 1_455 ?
K2 K2 O7 57(3) 2 2 ?
K2 K2 O8 105.9(10) 2_655 2 ?
K2 K2 O8 83(3) 2 2 ?
K2 K2 O8 87.6(9) 2_655 . ?
K2 K2 O8 83(3) 2 . ?
O1 K2 W1 166(2) 1_465 2_655 ?
O1 K2 W1 173.1(19) 2_665 2_655 ?
O1 K2 W3 121(3) 2_665 2_655 ?
O1 K2 W3 121(3) 1_465 2_655 ?
O1 K2 K2 86(2) 1_465 1_455 ?
O1 K2 K2 79.3(19) 2_665 1_455 ?
O1 K2 O1 7(4) 1_465 2_665 ?
O1 K2 O2 124(2) 2_665 1_455 ?
O1 K2 O2 129(2) 1_465 1_455 ?
O1 K2 O2 126(2) 1_465 2 ?
O1 K2 O2 119(2) 2_665 2 ?
O1 K2 O3 42(2) 1_465 1_465 ?
O1 K2 O3 37(2) 2_665 1_465 ?
O1 K2 O3 45(3) 1_465 1_565 ?
O1 K2 O7 85(3) 1_465 1_455 ?
O1 K2 O7 82(3) 2_665 2 ?
O1 K2 O7 88(3) 1_465 2 ?
O1 K2 O7 82(3) 2_665 1_455 ?
O1 K2 O8 116(3) 2_665 . ?
O1 K2 O8 114(3) 1_465 . ?
O1 K2 O8 118(3) 1_465 2 ?
O1 K2 O8 113(3) 2_665 2 ?
O2 K2 W1 28.5(7) 2_655 2_655 ?
O2 K2 W1 67.9(8) 2 2_655 ?
O2 K2 W1 31.0(7) . 2_655 ?
O2 K2 W1 62.1(8) 1_455 2_655 ?
O2 K2 W3 30.0(7) 2_655 2_655 ?
O2 K2 W3 71.7(7) 2 2_655 ?
O2 K2 W3 103.6(11) 1_455 2_655 ?
O2 K2 W3 80.0(8) . 2_655 ?
O2 K2 K2 52.2(7) 1_455 1_455 ?
O2 K2 K2 115.6(9) 2_655 1_455 ?
O2 K2 K2 123.5(7) . 1_455 ?
O2 K2 K2 65.5(9) 2_655 2_655 ?
O2 K2 K2 45.2(6) 2 1_455 ?
O2 K2 O1 147(3) 2_655 1_465 ?
O2 K2 O1 149(3) 2_655 2_665 ?
O2 K2 O1 137(3) . 1_465 ?
O2 K2 O1 144(2) . 2_665 ?
O2 K2 O2 70.3(10) 2_655 2 ?
O2 K2 O2 51.4(13) 2_655 . ?
O2 K2 O2 94.9(14) . 2 ?
O2 K2 O2 71.3(9) . 1_455 ?
O2 K2 O2 84.3(15) 2_655 1_455 ?
O2 K2 O2 44.1(11) 1_455 2 ?
O2 K2 O3 168.9(15) 2_655 1_465 ?
O2 K2 O3 92.3(8) . 1_565 ?
O2 K2 O3 106.2(9) 2_655 2_665 ?
O2 K2 O3 86.9(7) 1_455 1_465 ?
O2 K2 O3 121.2(12) 2_655 1_565 ?
O2 K2 O3 131.1(9) . 1_465 ?
O2 K2 O7 88.6(12) 2_655 2 ?
O2 K2 O7 94.1(10) . 1_455 ?
O2 K2 O7 54.4(10) 2_655 2_655 ?
O2 K2 O7 100.9(12) 2_655 . ?
O2 K2 O7 128.3(14) 2_655 1_455 ?
O2 K2 O7 45.3(8) 1_455 1_455 ?
O2 K2 O7 134.1(15) . 2 ?
O2 K2 O8 45.2(7) . . ?
O2 K2 O8 51.6(9) 2_655 2 ?
O2 K2 O8 84.2(10) 1_455 2 ?
O2 K2 O8 48.7(8) 1_455 . ?
O2 K2 O8 100.4(11) . 2 ?
O2 K2 O8 91.7(11) 2_655 . ?
O3 K2 W1 146.8(10) 1_465 2_655 ?
O3 K2 W1 130.6(10) 2_665 2_655 ?
O3 K2 W1 121.3(9) 1_565 2_655 ?
O3 K2 W3 83.0(8) 2_665 2_655 ?
O3 K2 W3 118.7(9) 1_565 2_655 ?
O3 K2 W3 148.7(10) 1_465 2_655 ?
O3 K2 K2 53.4(8) 1_465 1_455 ?
O3 K2 K2 114.4(8) 2_665 1_455 ?
O3 K2 K2 123.2(7) 1_565 1_455 ?
O3 K2 K2 66.6(9) 2_665 2_655 ?
O3 K2 O1 52(2) 1_565 2_665 ?
O3 K2 O1 40(3) 2_665 1_465 ?
O3 K2 O1 44(2) 2_665 2_665 ?
O3 K2 O2 168.4(12) 1_565 2 ?
O3 K2 O2 130.7(9) 2_665 2 ?
O3 K2 O2 166.4(14) 2_665 1_455 ?
O3 K2 O2 98.6(9) 1_465 2 ?
O3 K2 O2 122.0(12) 2_665 . ?
O3 K2 O2 131.3(9) 1_565 1_455 ?
O3 K2 O3 69.8(9) 1_565 1_465 ?
O3 K2 O3 50.5(14) 2_665 1_565 ?
O3 K2 O3 81.7(15) 2_665 1_465 ?
O3 K2 O7 44.9(8) 1_465 1_455 ?
O3 K2 O7 86.9(11) 2_665 2 ?
O3 K2 O7 99.5(14) 2_665 . ?
O3 K2 O7 93.2(10) 1_565 1_455 ?
O3 K2 O7 125.4(14) 2_665 1_455 ?
O3 K2 O7 53.7(11) 2_665 2_655 ?
O3 K2 O7 131.6(14) 1_565 2 ?
O3 K2 O8 86.9(9) 1_565 . ?
O3 K2 O8 120.8(9) 1_465 2 ?
O3 K2 O8 144.5(11) 1_565 2 ?
O3 K2 O8 95.4(10) 2_665 2 ?
O3 K2 O8 87.5(9) 1_465 . ?
O3 K2 O8 137.3(12) 2_665 . ?
O7 K2 W1 82.3(10) 2_655 2_655 ?
O7 K2 W1 101.9(10) 1_455 2_655 ?
O7 K2 W1 103.1(11) 2 2_655 ?
O7 K2 W1 81.9(10) . 2_655 ?
O7 K2 W3 124.3(9) . 2_655 ?
O7 K2 W3 29.6(8) 2_655 2_655 ?
O7 K2 W3 68.2(7) 2 2_655 ?
O7 K2 W3 147.6(12) 1_455 2_655 ?
O7 K2 K2 59.7(9) . 2_655 ?
O7 K2 K2 122.7(7) 2_655 1_455 ?
O7 K2 K2 118.1(7) . 1_455 ?
O7 K2 K2 48.5(6) 2 1_455 ?
O7 K2 K2 59.6(9) 2_655 2_655 ?
O7 K2 K2 47.2(6) 1_455 1_455 ?
O7 K2 O1 93(3) 2_655 1_465 ?
O7 K2 O1 95(3) 2_655 2_665 ?
O7 K2 O1 89(3) . 1_465 ?
O7 K2 O1 94(3) . 2_665 ?
O7 K2 O2 44.7(8) 2 2 ?
O7 K2 O2 84.6(10) 2 1_455 ?
O7 K2 O2 129.8(13) . 2 ?
O7 K2 O2 96.1(11) 2_655 2 ?
O7 K2 O2 51.4(9) . . ?
O7 K2 O2 94.1(11) 2_655 . ?
O7 K2 O2 77.2(9) 1_455 2 ?
O7 K2 O2 86.8(10) . 1_455 ?
O7 K2 O2 133.0(15) 2_655 1_455 ?
O7 K2 O3 83.9(10) 2 1_465 ?
O7 K2 O3 130.3(14) 2_655 1_465 ?
O7 K2 O3 85.2(11) . 1_465 ?
O7 K2 O3 50.4(10) . 1_565 ?
O7 K2 O3 92.4(12) 2_655 1_565 ?
O7 K2 O7 70.8(6) . 1_455 ?
O7 K2 O7 119.2(8) . 2_655 ?
O7 K2 O7 95.7(7) 2 1_455 ?
O7 K2 O7 169.8(8) 2_655 1_455 ?
O7 K2 O7 74.2(7) 2_655 2 ?
O7 K2 O7 166.4(8) . 2 ?
O7 K2 O8 139.2(11) 2_655 . ?
O7 K2 O8 38.2(8) . . ?
O7 K2 O8 133.0(11) 2 . ?
O7 K2 O8 151.8(13) . 2 ?
O7 K2 O8 53.9(8) 2_655 2 ?
O7 K2 O8 37.1(7) 2 2 ?
O8 K2 W1 63.8(6) . 2_655 ?
O8 K2 W1 70.2(7) 2 2_655 ?
O8 K2 W3 34.5(4) 2 2_655 ?
O8 K2 W3 121.7(9) . 2_655 ?
O8 K2 K2 90.4(5) . 1_455 ?
O8 K2 K2 76.1(5) 2 1_455 ?
O8 K2 O2 42.4(7) 2 2 ?
O8 K2 O2 91.7(9) . 2 ?
O8 K2 O7 118.5(10) 2 1_455 ?
O8 K2 O7 49.7(7) . 1_455 ?
O8 K2 O8 125.1(12) . 2 ?
W6A K3 W6A 123.2(11) 1_445 2_646 ?
W6A K3 W6B 43.4(3) 2_646 2_546 ?
W6A K3 W6B 43.4(3) 1_445 1_545 ?
W6A K3 W6B 106.4(8) 2_646 1_545 ?
W6A K3 W6B 106.4(8) 1_445 2_546 ?
W6A K3 K4 56.5(7) 2_646 2_646 ?
W6A K3 K4 70.0(8) 2_646 1_445 ?
W6A K3 K4 70.0(8) 1_445 2_646 ?
W6A K3 K4 56.5(7) 1_445 1_445 ?
W6B K3 W6B 124.2(12) 1_545 2_546 ?
K3 K3 W6A 112.48(14) 1_655 1_445 ?
K3 K3 W6A 67.52(15) 1_655 2_646 ?
K3 K3 W6A 112.48(14) 1_455 2_646 ?
K3 K3 W6A 67.52(15) 1_455 1_445 ?
K3 K3 W6B 110.94(15) 1_455 1_545 ?
K3 K3 W6B 69.06(15) 1_455 2_546 ?
K3 K3 W6B 110.94(15) 1_655 2_546 ?
K3 K3 W6B 69.06(15) 1_655 1_545 ?
K3 K3 K3 179.999(13) 1_655 1_455 ?
K3 K3 K4 110.7(6) 1_655 1_455 ?
K3 K3 K4 70.2(5) 1_655 2_646 ?
K3 K3 K4 69.3(6) 1_455 1_455 ?
K3 K3 K4 70.2(5) 1_455 1_445 ?
K3 K3 K4 109.8(5) 1_655 1_445 ?
K3 K3 K4 109.8(5) 1_455 2_646 ?
K3 K3 K4 110.7(6) 1_455 2_656 ?
K3 K3 K4 69.3(6) 1_655 2_656 ?
K4 K3 W6A 123.6(8) 1_455 2_646 ?
K4 K3 W6A 109.6(7) 1_455 1_445 ?
K4 K3 W6A 123.6(8) 2_656 1_445 ?
K4 K3 W6A 109.6(7) 2_656 2_646 ?
K4 K3 W6B 106.5(7) 1_455 2_546 ?
K4 K3 W6B 54.1(7) 2_646 1_545 ?
K4 K3 W6B 126.2(8) 2_656 2_546 ?
K4 K3 W6B 73.0(9) 2_646 2_546 ?
K4 K3 W6B 54.1(7) 1_445 2_546 ?
K4 K3 W6B 126.2(8) 1_455 1_545 ?
K4 K3 W6B 73.0(9) 1_445 1_545 ?
K4 K3 W6B 106.5(7) 2_656 1_545 ?
K4 K3 K4 139.3(9) 1_455 1_445 ?
K4 K3 K4 179.1(7) 2_656 1_445 ?
K4 K3 K4 179.1(7) 1_455 2_646 ?
K4 K3 K4 39.8(10) 1_445 2_646 ?
K4 K3 K4 41.6(12) 2_656 1_455 ?
K4 K3 K4 139.3(9) 2_656 2_646 ?
O14 K3 W6A 117.3(9) . 2_646 ?
O14 K3 W6A 92.3(9) . 1_445 ?
O14 K3 W6A 117.3(9) 2_556 1_445 ?
O14 K3 W6A 153.2(8) 2_656 1_445 ?
O14 K3 W6A 62.8(7) 1_455 1_445 ?
O14 K3 W6A 62.8(7) 2_656 2_646 ?
O14 K3 W6A 153.2(8) 1_455 2_646 ?
O14 K3 W6A 92.3(9) 2_556 2_646 ?
O14 K3 W6B 110.6(8) 2_656 1_545 ?
O14 K3 W6B 110.6(8) 1_455 2_546 ?
O14 K3 W6B 63.8(9) . 1_545 ?
O14 K3 W6B 63.8(9) 2_556 2_546 ?
O14 K3 W6B 94.4(8) 1_455 1_545 ?
O14 K3 W6B 158.7(10) . 2_546 ?
O14 K3 W6B 94.4(8) 2_656 2_546 ?
O14 K3 W6B 158.7(10) 2_556 1_545 ?
O14 K3 K3 129.2(10) . 1_455 ?
O14 K3 K3 50.8(10) . 1_655 ?
O14 K3 K3 129.2(10) 2_556 1_655 ?
O14 K3 K3 137.6(9) 1_455 1_655 ?
O14 K3 K3 137.6(9) 2_656 1_455 ?
O14 K3 K3 42.4(9) 2_656 1_655 ?
O14 K3 K3 50.8(10) 2_556 1_455 ?
O14 K3 K3 42.4(9) 1_455 1_455 ?
O14 K3 K4 47.8(10) 2_656 2_656 ?
O14 K3 K4 136.5(13) . 1_445 ?
O14 K3 K4 75.6(14) 2_556 2_656 ?
O14 K3 K4 79.5(13) 1_455 2_656 ?
O14 K3 K4 101.3(11) 1_455 1_445 ?
O14 K3 K4 42.8(12) 2_556 1_455 ?
O14 K3 K4 131.6(12) 1_455 2_646 ?
O14 K3 K4 75.6(14) . 1_455 ?
O14 K3 K4 131.6(12) 2_656 1_445 ?
O14 K3 K4 79.5(13) 2_656 1_455 ?
O14 K3 K4 136.5(13) 2_556 2_646 ?
O14 K3 K4 47.8(10) 1_455 1_455 ?
O14 K3 K4 101.3(11) 2_656 2_646 ?
O14 K3 K4 42.8(12) . 2_656 ?
O14 K3 K4 105.2(12) 2_556 1_445 ?
O14 K3 K4 105.2(12) . 2_646 ?
O14 K3 O14 64.9(16) 2_556 1_455 ?
O14 K3 O14 117(2) 2_556 . ?
O14 K3 O14 64.9(16) . 2_656 ?
O14 K3 O14 86.8(14) . 1_455 ?
O14 K3 O14 126(2) 2_656 1_455 ?
O14 K3 O14 86.8(14) 2_556 2_656 ?
O14 K3 O17 178(2) 2_556 1_545 ?
O14 K3 O17 64.8(7) 2_556 2_546 ?
O14 K3 O17 178.4(19) 2_656 1_445 ?
O14 K3 O17 94.2(11) 2_556 1_445 ?
O14 K3 O17 178(2) . 2_546 ?
O14 K3 O17 94.2(11) . 2_646 ?
O14 K3 O17 115.7(8) . 1_445 ?
O14 K3 O17 56.1(6) 1_455 1_445 ?
O14 K3 O17 56.1(6) 2_656 2_646 ?
O14 K3 O17 115.7(8) 2_556 2_646 ?
O14 K3 O17 178.4(19) 1_455 2_646 ?
O14 K3 O17 64.8(7) . 1_545 ?
O14 K3 O18A 143.7(11) 2_556 1_445 ?
O14 K3 O18A 143.7(11) . 2_646 ?
O14 K3 O18A 126.0(10) 1_455 2_646 ?
O14 K3 O18A 72.6(11) . 1_445 ?
O14 K3 O18A 81.6(10) 2_656 2_646 ?
O14 K3 O18A 126.0(10) 2_656 1_445 ?
O14 K3 O18A 81.6(10) 1_455 1_445 ?
O14 K3 O18A 72.6(11) 2_556 2_646 ?
O17 K3 W6A 62.5(9) 2_546 2_646 ?
O17 K3 W6A 115.9(13) 1_445 2_646 ?
O17 K3 W6A 115.9(13) 2_646 1_445 ?
O17 K3 W6A 86.6(10) 1_545 2_646 ?
O17 K3 W6A 26.4(6) 2_646 2_646 ?
O17 K3 W6A 86.6(10) 2_546 1_445 ?
O17 K3 W6A 62.5(9) 1_545 1_445 ?
O17 K3 W6A 26.4(6) 1_445 1_445 ?
O17 K3 W6B 84.9(9) 2_646 1_545 ?
O17 K3 W6B 114.7(14) 1_545 2_546 ?
O17 K3 W6B 21.7(8) 2_546 2_546 ?
O17 K3 W6B 84.9(9) 1_445 2_546 ?
O17 K3 W6B 68.7(8) 2_646 2_546 ?
O17 K3 W6B 21.7(8) 1_545 1_545 ?
O17 K3 W6B 68.7(8) 1_445 1_545 ?
O17 K3 W6B 114.7(14) 2_546 1_545 ?
O17 K3 K3 43.5(7) 1_445 1_455 ?
O17 K3 K3 43.5(7) 2_646 1_655 ?
O17 K3 K3 128.8(8) 1_545 1_455 ?
O17 K3 K3 128.8(8) 2_546 1_655 ?
O17 K3 K3 51.2(8) 2_546 1_455 ?
O17 K3 K3 136.5(7) 2_646 1_455 ?
O17 K3 K3 136.5(7) 1_445 1_655 ?
O17 K3 K3 51.2(8) 1_545 1_655 ?
O17 K3 K4 77.1(11) 2_646 1_445 ?
O17 K3 K4 73.5(12) 1_545 1_445 ?
O17 K3 K4 105.8(10) 1_545 2_656 ?
O17 K3 K4 77.1(11) 1_445 2_646 ?
O17 K3 K4 133.7(12) 2_646 1_455 ?
O17 K3 K4 46.8(10) 2_646 2_646 ?
O17 K3 K4 41.9(11) 2_546 1_445 ?
O17 K3 K4 46.8(10) 1_445 1_445 ?
O17 K3 K4 105.8(10) 2_546 1_455 ?
O17 K3 K4 102.1(9) 1_445 1_455 ?
O17 K3 K4 138.7(13) 1_545 1_455 ?
O17 K3 K4 102.1(9) 2_646 2_656 ?
O17 K3 K4 138.7(13) 2_546 2_656 ?
O17 K3 K4 73.5(12) 2_546 2_646 ?
O17 K3 K4 41.9(11) 1_545 2_646 ?
O17 K3 K4 133.7(12) 1_445 2_656 ?
O17 K3 O14 115.9(8) 2_546 2_656 ?
O17 K3 O14 93.7(11) 2_546 1_455 ?
O17 K3 O14 93.7(11) 1_545 2_656 ?
O17 K3 O14 115.9(8) 1_545 1_455 ?
O17 K3 O17 63.5(13) 1_545 2_646 ?
O17 K3 O17 122.3(19) 1_445 2_646 ?
O17 K3 O17 85.3(12) 1_545 1_445 ?
O17 K3 O17 114(2) 2_546 1_545 ?
O17 K3 O17 85.3(12) 2_546 2_646 ?
O17 K3 O17 63.5(14) 2_546 1_445 ?
O17 K3 O18A 106.0(15) 2_546 1_445 ?
O17 K3 O18A 53.5(10) 1_445 1_445 ?
O17 K3 O18A 53.5(10) 2_646 2_646 ?
O17 K3 O18A 36.5(10) 1_545 1_445 ?
O17 K3 O18A 97.4(11) 2_646 1_445 ?
O17 K3 O18A 36.5(10) 2_546 2_646 ?
O17 K3 O18A 106.0(14) 1_545 2_646 ?
O17 K3 O18A 97.4(12) 1_445 2_646 ?
O18A K3 W6A 27.7(6) 2_646 2_646 ?
O18A K3 W6A 27.7(6) 1_445 1_445 ?
O18A K3 W6A 115.3(11) 2_646 1_445 ?
O18A K3 W6A 115.3(11) 1_445 2_646 ?
O18A K3 W6B 120.7(12) 2_646 1_545 ?
O18A K3 W6B 15.9(6) 1_445 1_545 ?
O18A K3 W6B 120.7(12) 1_445 2_546 ?
O18A K3 W6B 15.9(6) 2_646 2_546 ?
O18A K3 K3 84.9(6) 1_445 1_655 ?
O18A K3 K3 84.9(6) 2_646 1_455 ?
O18A K3 K3 95.1(6) 2_646 1_655 ?
O18A K3 K3 95.1(6) 1_445 1_455 ?
O18A K3 K4 113.0(9) 2_646 1_455 ?
O18A K3 K4 120.8(10) 2_646 2_656 ?
O18A K3 K4 66.7(10) 2_646 2_646 ?
O18A K3 K4 59.2(10) 1_445 2_646 ?
O18A K3 K4 59.2(10) 2_646 1_445 ?
O18A K3 K4 120.8(10) 1_445 1_455 ?
O18A K3 K4 113.0(10) 1_445 2_656 ?
O18A K3 K4 66.7(10) 1_445 1_445 ?
O18A K3 O18A 122.3(17) 1_445 2_646 ?
W5 K4 W5 117.3(12) 2_656 . ?
W5 K4 W6A 62.4(6) 2_656 2_656 ?
W5 K4 W6A 168.6(9) 2_656 . ?
W5 K4 W6B 155.2(9) 2_656 . ?
W5 K4 W6B 57.9(6) . . ?
W5 K4 K3 66.8(8) 2_656 1_655 ?
W5 K4 K3 124.2(10) 2_656 1_665 ?
W5 K4 K3 118.4(11) . 1_665 ?
W5 K4 K3 64.7(7) . 1_655 ?
W5 K4 K3 59.7(6) . . ?
W5 K4 K3 60.9(7) 2_656 . ?
W5 K4 K4 80.8(5) 2_656 1_455 ?
W5 K4 K4 99.2(5) 2_656 1_655 ?
W5 K4 O18A 70.5(9) 2_656 2_756 ?
W6A K4 W5 155.7(9) 2_656 . ?
W6A K4 W5 59.7(6) . . ?
W6A K4 W6A 115.2(12) 2_656 . ?
W6A K4 W6B 13.34(17) . . ?
W6A K4 W6B 111.1(11) 2_656 . ?
W6A K4 K3 107.2(9) 2_656 . ?
W6A K4 K3 127.3(12) 2_656 1_655 ?
W6A K4 K3 117.3(10) . 1_655 ?
W6A K4 K3 111.7(8) . . ?
W6A K4 K3 68.3(8) 2_656 1_665 ?
W6A K4 K3 60.6(7) . 1_665 ?
W6A K4 K4 87.8(5) . 1_455 ?
W6A K4 K4 74.4(5) 2_656 1_455 ?
W6A K4 K4 92.2(5) . 1_655 ?
W6A K4 K4 105.6(5) 2_656 1_655 ?
W6A K4 O18A 32.0(7) 2_656 2_756 ?
W6B K4 W5 170.3(10) 2_656 . ?
W6B K4 W5 63.1(6) 2_656 2_656 ?
W6B K4 W6A 14.6(2) 2_656 2_656 ?
W6B K4 W6A 117.8(12) 2_656 . ?
W6B K4 W6B 117.2(12) 2_656 . ?
W6B K4 K3 116.4(10) 2_656 . ?
W6B K4 K3 102.4(7) . . ?
W6B K4 K3 62.6(7) 2_656 1_665 ?
W6B K4 K3 121.7(11) 2_656 1_655 ?
W6B K4 K4 89.0(5) 2_656 1_455 ?
W6B K4 K4 91.0(5) 2_656 1_655 ?
W6B K4 O18A 17.6(6) 2_656 2_756 ?
K3 K4 W6B 120.9(10) 1_655 . ?
K3 K4 W6B 67.4(8) 1_665 . ?
K3 K4 K3 164.6(10) 1_665 . ?
K3 K4 K3 55.5(8) 1_655 . ?
K3 K4 K3 139.3(9) 1_655 1_665 ?
K4 K4 W5 93.7(16) 2_756 . ?
K4 K4 W5 71(3) 2_656 . ?
K4 K4 W5 81.6(5) 1_455 . ?
K4 K4 W5 98.4(5) 1_655 . ?
K4 K4 W5 92(3) 2_656 2_656 ?
K4 K4 W5 103.8(15) 2_756 2_656 ?
K4 K4 W6A 87.6(15) 2_756 . ?
K4 K4 W6A 85(3) 2_656 2_656 ?
K4 K4 W6A 110.1(15) 2_756 2_656 ?
K4 K4 W6A 77(3) 2_656 . ?
K4 K4 W6B 100(3) 2_656 2_656 ?
K4 K4 W6B 105.5(5) 1_655 . ?
K4 K4 W6B 64(3) 2_656 . ?
K4 K4 W6B 74.5(5) 1_455 . ?
K4 K4 W6B 100.9(16) 2_756 . ?
K4 K4 W6B 95.6(14) 2_756 2_656 ?
K4 K4 K3 110.7(6) 1_455 1_655 ?
K4 K4 K3 55.2(5) 1_455 . ?
K4 K4 K3 70.1(5) 2_756 1_665 ?
K4 K4 K3 55.8(7) 2_656 . ?
K4 K4 K3 109.8(5) 1_455 1_665 ?
K4 K4 K3 124.4(6) 2_756 . ?
K4 K4 K3 124.8(5) 1_655 . ?
K4 K4 K3 69.3(6) 1_655 1_655 ?
K4 K4 K3 70.2(5) 1_655 1_665 ?
K4 K4 K3 108.9(7) 2_656 1_665 ?
K4 K4 K3 69.2(6) 2_756 1_655 ?
K4 K4 K3 109.8(7) 2_656 1_655 ?
K4 K4 K4 180.00(6) 1_655 1_455 ?
K4 K4 K4 174.7(16) 2_756 1_455 ?
K4 K4 K4 167(4) 2_656 1_655 ?
K4 K4 K4 5.3(16) 2_756 1_655 ?
K4 K4 K4 162(5) 2_656 2_756 ?
K4 K4 K4 13(4) 2_656 1_455 ?
K4 K4 O14 66(2) 2_656 . ?
K4 K4 O14 90(2) 2_656 2_656 ?
K4 K4 O14 104.0(15) 2_756 . ?
K4 K4 O15 91.9(19) 2_756 . ?
K4 K4 O15 70(4) 2_656 . ?
K4 K4 O15 88(4) 2_656 2_656 ?
K4 K4 O15 110.1(19) 2_756 2_656 ?
K4 K4 O17 103.3(15) 2_756 . ?
K4 K4 O17 67(2) 2_656 . ?
K4 K4 O17 90(2) 2_656 2_656 ?
K4 K4 O18A 116(3) 2_656 2_756 ?
K4 K4 O18A 78.2(14) 2_756 2_756 ?
O14 K4 W5 27.3(10) 2_656 2_656 ?
O14 K4 W5 25.8(9) . . ?
O14 K4 W5 91.2(15) 2_656 . ?
O14 K4 W5 91.7(15) . 2_656 ?
O14 K4 W6A 150.6(17) 2_656 . ?
O14 K4 W6A 89.4(14) 2_656 2_656 ?
O14 K4 W6A 84.2(12) . . ?
O14 K4 W6A 140.9(15) . 2_656 ?
O14 K4 W6B 144.0(16) 2_656 . ?
O14 K4 W6B 90.2(14) 2_656 2_656 ?
O14 K4 W6B 79.7(11) . . ?
O14 K4 W6B 151.4(17) . 2_656 ?
O14 K4 K3 42.5(11) 2_656 1_655 ?
O14 K4 K3 34.9(10) . . ?
O14 K4 K3 41.9(11) 2_656 . ?
O14 K4 K3 144.1(16) . 1_665 ?
O14 K4 K3 50.4(11) . 1_655 ?
O14 K4 K3 148.4(15) 2_656 1_665 ?
O14 K4 K4 99.0(14) 2_656 2_756 ?
O14 K4 K4 83.7(11) 2_656 1_455 ?
O14 K4 K4 96.3(11) 2_656 1_655 ?
O14 K4 K4 72.9(10) . 1_455 ?
O14 K4 K4 107.1(10) . 1_655 ?
O14 K4 O14 66(2) 2_656 . ?
O14 K4 O15 58.9(14) 2_656 2_656 ?
O14 K4 O15 54.4(12) . . ?
O14 K4 O15 120.7(19) 2_656 . ?
O14 K4 O17 102.8(13) . . ?
O14 K4 O17 157.1(19) 2_656 . ?
O14 K4 O17 117.2(16) 2_656 2_656 ?
O14 K4 O18A 161.9(19) . 2_756 ?
O14 K4 O18A 95.5(15) 2_656 2_756 ?
O15 K4 W5 29.7(8) . . ?
O15 K4 W5 31.8(9) 2_656 2_656 ?
O15 K4 W5 145.5(16) . 2_656 ?
O15 K4 W5 143.5(16) 2_656 . ?
O15 K4 W6A 30.6(8) 2_656 2_656 ?
O15 K4 W6A 30.0(8) . . ?
O15 K4 W6A 144.6(16) 2_656 . ?
O15 K4 W6A 139.8(15) . 2_656 ?
O15 K4 W6B 137.2(14) 2_656 . ?
O15 K4 W6B 146.6(17) . 2_656 ?
O15 K4 W6B 29.5(8) . . ?
O15 K4 W6B 33.4(9) 2_656 2_656 ?
O15 K4 K3 96.0(13) 2_656 1_665 ?
O15 K4 K3 89.9(13) . 1_665 ?
O15 K4 K3 84.9(11) . . ?
O15 K4 K3 97.8(14) 2_656 1_655 ?
O15 K4 K3 83.9(12) 2_656 . ?
O15 K4 K3 91.4(12) . 1_655 ?
O15 K4 K4 75.2(8) 2_656 1_455 ?
O15 K4 K4 82.8(8) . 1_455 ?
O15 K4 K4 97.2(8) . 1_655 ?
O15 K4 K4 104.8(8) 2_656 1_655 ?
O15 K4 O14 118.5(19) 2_656 . ?
O15 K4 O15 157.9(12) 2_656 . ?
O15 K4 O17 116.4(17) 2_656 . ?
O15 K4 O18A 143.7(18) . 2_756 ?
O15 K4 O18A 46.0(11) 2_656 2_756 ?
O17 K4 W5 89.9(12) 2_656 2_656 ?
O17 K4 W5 146.1(16) 2_656 . ?
O17 K4 W5 145.0(13) . 2_656 ?
O17 K4 W5 82.4(11) . . ?
O17 K4 W6A 28.2(8) 2_656 2_656 ?
O17 K4 W6A 89.5(14) 2_656 . ?
O17 K4 W6A 87.6(12) . 2_656 ?
O17 K4 W6A 28.3(7) . . ?
O17 K4 W6B 92.6(13) . 2_656 ?
O17 K4 W6B 28.6(8) 2_656 2_656 ?
O17 K4 W6B 24.6(7) . . ?
O17 K4 W6B 88.8(13) 2_656 . ?
O17 K4 K3 149.2(14) 2_656 1_655 ?
O17 K4 K3 48.4(10) . 1_665 ?
O17 K4 K3 145.0(14) . 1_655 ?
O17 K4 K3 130.9(13) 2_656 . ?
O17 K4 K3 118.1(11) . . ?
O17 K4 K3 41.1(10) 2_656 1_665 ?
O17 K4 K4 99.1(12) 2_656 2_756 ?
O17 K4 K4 96.5(10) 2_656 1_655 ?
O17 K4 K4 73.6(9) . 1_455 ?
O17 K4 K4 106.4(9) . 1_655 ?
O17 K4 K4 83.5(10) 2_656 1_455 ?
O17 K4 O14 155.7(18) 2_656 . ?
O17 K4 O15 54.0(11) . . ?
O17 K4 O15 58.4(12) 2_656 2_656 ?
O17 K4 O15 118.1(19) 2_656 . ?
O17 K4 O17 64.1(16) 2_656 . ?
O17 K4 O18A 33.2(10) 2_656 2_756 ?
O17 K4 O18A 94.0(14) . 2_756 ?
O18A K4 W5 170.2(13) 2_756 . ?
O18A K4 W6A 113.9(14) 2_756 . ?
O18A K4 W6B 117.8(13) 2_756 . ?
O18A K4 K3 116.4(11) 2_756 1_655 ?
O18A K4 K3 129.6(12) 2_756 . ?
O18A K4 K3 53.8(8) 2_756 1_665 ?
O18A K4 K4 106.2(8) 2_756 1_455 ?
O18A K4 K4 73.8(8) 2_756 1_655 ?
W1 O1 W1 6.3(10) 2_755 1_655 ?
W1 O1 W1 146(4) 2_755 . ?
W1 O1 W1 152(3) . 1_655 ?
W1 O1 K2 105(4) 2_755 1_645 ?
W1 O1 K2 94(3) . 2_645 ?
W1 O1 K2 120(4) 2_755 2_645 ?
W1 O1 K2 108(3) . 1_645 ?
W1 O1 K2 113(3) 1_655 2_645 ?
W1 O1 K2 99(3) 1_655 1_645 ?
K2 O1 K2 14.5(9) 1_645 2_645 ?
O1 O1 W1 21(10) 2_755 . ?
O1 O1 W1 157(10) 2_755 1_655 ?
O1 O1 W1 153(10) 2_755 2_755 ?
O1 O1 K2 80(3) 2_755 2_645 ?
O1 O1 K2 93(3) 2_755 1_645 ?
W1 O2 W1 21.4(5) . 2_655 ?
W1 O2 W3 151.0(18) . . ?
W1 O2 K2 91.7(13) 2_655 . ?
W1 O2 K2 104.2(13) . 2 ?
W1 O2 K2 99.7(13) . 1_655 ?
W1 O2 K2 112.7(13) 2_655 1_655 ?
W1 O2 K2 104.0(14) . . ?
W1 O2 K2 88.7(12) 2_655 2 ?
W1 O2 K2 103.9(14) . 2_655 ?
W1 O2 K2 112.9(14) 2_655 2_655 ?
W3 O2 W1 144.5(17) . 2_655 ?
W3 O2 K2 102.8(12) . 1_655 ?
W3 O2 K2 101.9(13) . 2_655 ?
W3 O2 K2 100.4(12) . . ?
W3 O2 K2 96.6(12) . 2 ?
K2 O2 K2 71.3(9) . 1_655 ?
K2 O2 K2 82.6(10) 1_655 2 ?
K2 O2 K2 11.4(6) . 2 ?
K2 O2 K2 59.1(12) 2_655 . ?
K2 O2 K2 12.4(7) 2_655 1_655 ?
K2 O2 K2 70.3(10) 2_655 2 ?
W1 O3 W1 21.3(5) . 2_655 ?
W1 O3 W2 148.4(19) . 1_545 ?
W1 O3 K2 113.6(16) 2_655 2_645 ?
W1 O3 K2 105.2(16) . 2_645 ?
W1 O3 K2 101.1(14) . 1_645 ?
W1 O3 K2 113.6(15) 2_655 1_645 ?
W1 O3 K2 92.0(14) 2_655 1_545 ?
W1 O3 K2 104.2(15) . 1_545 ?
W2 O3 W1 137.5(18) 1_545 2_655 ?
W2 O3 K2 106.0(14) 1_545 2_645 ?
W2 O3 K2 96.5(13) 1_545 1_545 ?
W2 O3 K2 108.4(13) 1_545 1_645 ?
K2 O3 K2 12.4(7) 2_645 1_645 ?
K2 O3 K2 57.7(10) 2_645 1_545 ?
K2 O3 K2 69.8(9) 1_545 1_645 ?
W2 O4 W2 168.6(14) . 1_455 ?
W2 O5 W4 153.0(18) . . ?
W2 O5 K1 108.9(13) . 1_565 ?
W4 O5 K1 98.0(13) . 1_565 ?
W2 O6 W3 149.9(12) . 1_565 ?
W2 O6 K1 106.2(13) . 1_665 ?
W2 O6 K1 96.8(12) . 1_565 ?
W3 O6 K1 102.8(12) 1_565 1_665 ?
W3 O6 K1 101.7(12) 1_565 1_565 ?
K1 O6 K1 67.6(4) 1_565 1_665 ?
W2 O7 K2 105.1(14) . 2_655 ?
W2 O7 K2 104.6(13) . 2 ?
W2 O7 K2 102.9(13) . 1_655 ?
W2 O7 K2 106.9(14) . . ?
W3 O7 W2 142.8(12) . . ?
W3 O7 K2 109.2(15) . . ?
W3 O7 K2 96.9(12) . 1_655 ?
W3 O7 K2 99.8(14) . 2_655 ?
W3 O7 K2 108.5(14) . 2 ?
K2 O7 K2 60.8(8) . 2_655 ?
K2 O7 K2 74.2(7) 2_655 2 ?
K2 O7 K2 84.3(7) 2 1_655 ?
K2 O7 K2 13.4(8) . 2 ?
K2 O7 K2 10.1(8) 2_655 1_655 ?
K2 O7 K2 70.8(6) . 1_655 ?
W3 O8 W3 169.0(14) . 1_455 ?
W3 O8 K2 108.5(10) . 2 ?
W3 O8 K2 95.1(9) . . ?
W3 O8 K2 93.1(8) 1_455 . ?
W3 O8 K2 79.7(7) 1_455 2 ?
K2 O8 K2 13.5(7) . 2 ?
W3 O9 W4 150.3(17) . . ?
W3 O9 K1 111.1(12) . . ?
W4 O9 K1 98.5(13) . . ?
W4 O10 W4 158(4) . 1_655 ?
W4 O11 W6A 142.6(19) . . ?
W4 O11 W6B 133.2(19) . . ?
W4 O11 K1 103.6(16) . 1_565 ?
W4 O11 K1 116.6(17) . 1_665 ?
W6A O11 K1 103.3(13) . 1_565 ?
W6A O11 K1 95.2(12) . 1_665 ?
W6B O11 W6A 24.3(4) . . ?
W6B O11 K1 110.2(13) . 1_665 ?
W6B O11 K1 88.6(12) . 1_565 ?
K1 O11 K1 74.9(10) 1_565 1_665 ?
W4 O12 W5 137.5(17) . . ?
W4 O12 K1 101.9(13) . . ?
W4 O12 K1 117.7(14) . 1_655 ?
W5 O12 K1 104.2(11) . 1_655 ?
W5 O12 K1 95.8(11) . . ?
K1 O12 K1 73.8(9) . 1_655 ?
W5 O13 W5 159(4) . 1_655 ?
W5 O13 K1 111(3) . 1_655 ?
W5 O13 K1 88(2) 1_655 1_655 ?
W5 O14 K3 140(2) . . ?
W5 O14 K3 117.1(18) . 1_655 ?
W5 O14 K4 109.3(18) . 2_656 ?
W5 O14 K4 108.7(18) . . ?
K3 O14 K3 86.8(14) . 1_655 ?
K3 O14 K4 105.9(17) . . ?
K3 O14 K4 94.7(16) . 2_656 ?
K4 O14 K3 81.9(15) . 1_655 ?
K4 O14 K3 102.3(17) 2_656 1_655 ?
K4 O14 K4 23.9(13) 2_656 . ?
W5 O15 W6B 150.9(16) . . ?
W5 O15 K4 96.7(14) . . ?
W5 O15 K4 94.5(14) . 2_656 ?
W6A O15 W5 167.6(12) . . ?
W6A O15 W6B 27.5(5) . . ?
W6A O15 K4 95.0(13) . . ?
W6A O15 K4 97.8(14) . 2_656 ?
W6B O15 K4 93.6(13) . 2_656 ?
W6B O15 K4 101.2(13) . . ?
K4 O15 K4 22.1(12) 2_656 . ?
W5 O16 W6A 132.4(10) . 1_545 ?
W5 O16 W6B 140.3(10) . 1_545 ?
W5 O16 K1 101.2(11) . 1_655 ?
W5 O16 K1 111.6(14) . . ?
W6A O16 K1 116.0(14) 1_545 . ?
W6A O16 K1 92.1(10) 1_545 1_655 ?
W6B O16 W6A 26.7(5) 1_545 1_545 ?
W6B O16 K1 109.6(12) 1_545 1_655 ?
W6B O16 K1 100.6(13) 1_545 . ?
K1 O16 K1 74.1(5) . 1_655 ?
W6A O17 K3 106.0(14) . 1_665 ?
W6A O17 K3 149.3(17) . 1_565 ?
W6A O17 K4 101.8(14) . . ?
W6A O17 K4 107.3(15) . 2_656 ?
W6B O17 W6A 29.8(6) . . ?
W6B O17 K3 125.3(16) . 1_565 ?
W6B O17 K3 132.7(16) . 1_665 ?
W6B O17 K4 105.9(16) . 2_656 ?
W6B O17 K4 112.7(15) . . ?
K3 O17 K3 85.3(12) 1_565 1_665 ?
K3 O17 K4 107.7(14) 1_565 . ?
K4 O17 K3 104.5(14) 2_656 1_665 ?
K4 O17 K3 96.9(16) 2_656 1_565 ?
K4 O17 K3 84.7(14) . 1_665 ?
K4 O17 K4 23.3(13) 2_656 . ?
W6A O18A W6A 170(2) . 1_655 ?
W6A O18A K1 92.4(14) . 1_665 ?
W6A O18A K1 89.5(12) 1_655 1_665 ?
W6A O18A K3 88.8(12) . 1_665 ?
W6A O18A K3 98.6(12) 1_655 1_665 ?
W6A O18A K4 104.3(15) . 2_756 ?
W6A O18A K4 72.2(12) 1_655 2_756 ?
W6B O18A W6A 163(3) 1_655 . ?
W6B O18A W6A 7.7(9) 1_655 1_655 ?
W6B O18A K1 85.1(19) 1_655 1_665 ?
W6B O18A K3 106(2) 1_655 1_665 ?
W6B O18A K4 76(2) 1_655 2_756 ?
K1 O18A K4 160.3(14) 1_665 2_756 ?
K3 O18A K1 124.6(13) 1_665 1_665 ?
K3 O18A K4 67.0(11) 1_665 2_756 ?
O18B O18A W6A 152(5) . 1_655 ?
O18B O18A W6A 23(4) . . ?
O18B O18A W6B 145(5) . 1_655 ?
O18B O18A K1 71(5) . 1_665 ?
O18B O18A K3 109(4) . 1_665 ?
O18B O18A K4 123(5) . 2_756 ?
W6A O18B W6B 156(5) . 1_655 ?
W6A O18B W6B 11.0(14) . . ?
W6A O18B K1 122(3) . 1_665 ?
W6B O18B W6B 167(3) 1_655 . ?
W6B O18B K1 82.4(18) 1_655 1_665 ?
W6B O18B K1 111(2) . 1_665 ?
O18A O18B W6A 139(7) . . ?
O18A O18B W6B 20(3) . 1_655 ?
O18A O18B W6B 149(6) . . ?
O18A O18B K1 95(5) . 1_665 ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.23947
2 0.26214
3 0.25936
4 0.23903
_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_K2W7O22
_database_code_depnum_ccdc_archive 'CCDC 2211344'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_K2W7O22             
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form

_audit_creation_date             2022-07-10
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
_shelx_SHELXL_version_number     2017/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'K2.001 O22 W7'
_chemical_formula_sum            'K2 O22 W7'
_chemical_formula_weight         1717.15
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           3
_space_group_name_H-M_alt        'P 1 2 1'
_space_group_name_Hall           'P 2y'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'

_cell_length_a                   7.3142(5)
_cell_length_b                   3.8123(3)
_cell_length_c                   31.947(2)
_cell_angle_alpha                90
_cell_angle_beta                 96.472(3)
_cell_angle_gamma                90
_cell_volume                     885.13(11)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9092
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      33.17
_cell_measurement_theta_min      2.57
_shelx_estimated_absorpt_T_max   0.657
_shelx_estimated_absorpt_T_min   0.208
_exptl_absorpt_coefficient_mu    45.872
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.4111
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1251 before and 0.0631 after correction.
The Ratio of minimum to maximum transmission is 0.5507.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    6.443
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             1464
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.01
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0584
_diffrn_reflns_av_unetI/netI     0.0522
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       49
_diffrn_reflns_limit_l_min       -49
_diffrn_reflns_number            23831
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.256
_diffrn_reflns_theta_min         1.925
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.997
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_reflns_Friedel_coverage         0.774
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.998
_reflns_number_gt                6519
_reflns_number_total             6698
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         5.484
_refine_diff_density_min         -9.143
_refine_diff_density_rms         0.758
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_refine_ls_extinction_coef       0.00016(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_goodness_of_fit_ref   1.087
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     197
_refine_ls_number_reflns         6698
_refine_ls_number_restraints     2
_refine_ls_R_factor_all          0.0567
_refine_ls_R_factor_gt           0.0548
_refine_ls_restrained_S_all      1.089
_refine_ls_shift/su_max          3.321
_refine_ls_shift/su_mean         0.079
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0289P)²+83.8331P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1346
_refine_ls_wR_factor_ref         0.1360
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.27544
 0.24568 0.22563 0.25325
2. Restrained distances
 K1-O6_$1
 2.7 with sigma of 0.03
3. Others
 0.5*[Sof(K2)]+1*[Sof(K3A)]+1*[Sof(K3B)]+1*[Sof(K4A)]+1*[Sof(K4B)]=1.5 with
 esd of 0
 Sof(W4B)=Sof(O12B)=1-FVAR(1)
 Sof(W4A)=Sof(O12A)=FVAR(1)
 Fixed Sof: O21(0.5)
 Fixed Y: K1(0)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.2828(3) 0.556(5) 0.09889(6) 0.0182(5) Uani 1 1 d . . . . .
W2 W 0.7975(3) 0.530(5) 0.09770(6) 0.0254(8) Uani 1 1 d . . . . .
W3 W 0.5985(3) 0.447(5) 0.19904(4) 0.0135(3) Uani 1 1 d . . . . .
W4A W 0.8882(6) 0.580(5) 0.30147(10) 0.0083(9) Uani 0.67(3) 1 d . . P . .
W4B W 0.8941(15) 0.441(8) 0.3036(2) 0.018(3) Uani 0.33(3) 1 d . . P . .
W5 W 0.3960(3) 0.483(5) 0.30134(7) 0.0321(12) Uani 1 1 d . . . . .
W6 W 0.2046(4) 0.483(5) 0.40029(4) 0.0240(6) Uani 1 1 d . . . . .
W7 W 0.500000 0.428(5) 0.500000 0.0047(3) Uani 1 2 d S T P . .
W8 W 0.000000 0.565(5) 0.500000 0.0082(4) Uani 1 2 d S T P . .
K1 K 0.000000 0.000000 0.000000 0.068(7) Uiso 1 2 d DS . P . .
K2 K 0.500000 -0.013(10) 0.000000 0.012(4) Uiso 0.437(9) 2 d S . P . .
K3A K 0.107(6) 0.013(11) 0.1971(7) 0.062(7) Uiso 0.572(5) 1 d . . P . .
K3B K 0.066(4) 0.407(11) 0.1974(9) -0.001(5) Uiso 0.191(4) 1 d . . P . .
K4A K 0.330(4) 0.011(10) 0.5977(7) 0.022(5) Uiso 0.350(5) 1 d . . P . .
K4B K 0.295(4) 0.204(10) 0.5982(8) -0.001(4) Uiso 0.169(5) 1 d . . P . .
O1 O 0.293(2) 0.992(6) 0.0937(6) -0.001(3) Uiso 1 1 d . . . . .
O2 O 0.209(4) 0.456(10) 0.0444(9) 0.022(5) Uiso 1 1 d . . . . .
O3 O 0.055(6) 0.529(9) 0.1193(7) 0.025(5) Uiso 1 1 d . . . . .
O4 O 0.542(5) 0.530(9) 0.0924(7) 0.025(5) Uiso 1 1 d . . . . .
O5 O 0.389(4) 0.461(9) 0.1646(8) 0.021(5) Uiso 1 1 d . . . . .
O6 O 0.828(4) 0.593(9) 0.0464(9) 0.027(6) Uiso 1 1 d . . . . .
O7 O 0.797(3) 0.009(7) 0.1074(8) 0.011(5) Uiso 1 1 d . . . . .
O8 O 0.761(4) 0.591(9) 0.1610(8) 0.020(5) Uiso 1 1 d . . . . .
O9 O 0.584(6) -0.013(12) 0.2070(9) 0.032(8) Uiso 1 1 d . . . . .
O10 O 0.803(3) 0.455(9) 0.2467(8) 0.017(5) Uiso 1 1 d . . . . .
O11 O 0.438(4) 0.573(10) 0.2471(9) 0.022(5) Uiso 1 1 d . . . . .
O12A O 0.881(4) 0.105(10) 0.3066(9) 0.004(5) Uiso 0.67(3) 1 d . . P . .
O12B O 0.939(7) -0.030(16) 0.2935(16) -0.001(9) Uiso 0.33(3) 1 d . . P . .
O13 O 0.660(6) 0.529(9) 0.3203(7) 0.027(5) Uiso 1 1 d . . . . .
O14 O 1.144(6) 0.517(9) 0.2881(7) 0.025(5) Uiso 1 1 d . . . . .
O15 O 0.991(3) 0.452(10) 0.3600(8) 0.018(5) Uiso 1 1 d . . . . .
O16 O 0.400(7) 0.002(15) 0.3050(18) 0.07(2) Uiso 1 1 d . . . . .
O17 O 0.358(3) 0.579(9) 0.3597(8) 0.017(4) Uiso 1 1 d . . . . .
O18 O 0.404(3) 0.415(11) 0.4435(8) 0.018(4) Uiso 1 1 d . . . . .
O19 O 0.257(3) -0.013(9) 0.4038(6) 0.005(4) Uiso 1 1 d . . . . .
O20 O 0.039(3) 0.576(9) 0.4435(8) 0.015(4) Uiso 1 1 d . . . . .
O21 O 0.496(8) -0.022(13) 0.5146(19) 0.022(11) Uiso 0.5 1 d . . P . .
O22 O 0.257(6) 0.506(9) 0.5163(7) 0.023(5) Uiso 1 1 d . . . . .
O23 O 0.000000 0.06(2) 0.500000 0.062(19) Uiso 1 2 d S . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 K1 4.158(9) . ?
W1 K1 3.955(8) 1_565 ?
W1 K2 4.040(11) 1_565 ?
W1 K3A 3.93(3) 1_565 ?
W1 K3A 4.09(3) . ?
W1 K3B 3.73(3) . ?
W1 O1 2.161(14) 1_545 ?
W1 O1 1.671(14) . ?
W1 O2 1.81(3) . ?
W1 O3 1.86(4) . ?
W1 O4 1.93(4) . ?
W1 O5 2.18(3) . ?
W2 K1 4.130(9) 1_655 ?
W2 K1 4.025(8) 1_665 ?
W2 K2 4.151(13) . ?
W2 K2 3.998(12) 1_565 ?
W2 K3A 4.12(3) 1_665 ?
W2 K3B 3.58(3) 1_655 ?
W2 O3 1.93(4) 1_655 ?
W2 O4 1.86(4) . ?
W2 O6 1.70(3) . ?
W2 O7 2.01(2) . ?
W2 O7 1.85(2) 1_565 ?
W2 O8 2.08(3) . ?
W3 K3A 4.08(4) 1_655 ?
W3 K3A 4.18(4) 1_565 ?
W3 K3A 3.95(4) . ?
W3 K3A 4.31(4) 1_665 ?
W3 K3B 3.43(3) 1_655 ?
W3 K3B 3.90(3) . ?
W3 O5 1.78(3) . ?
W3 O8 1.88(3) . ?
W3 O9 2.08(4) 1_565 ?
W3 O9 1.77(4) . ?
W3 O10 2.01(2) . ?
W3 O11 2.09(3) . ?
W4A W4B 0.536(19) . ?
W4A K3B 3.76(3) 1_655 ?
W4A K4A 4.10(3) 2_666 ?
W4A K4B 3.88(3) 2_656 ?
W4A O10 1.85(3) . ?
W4A O12A 2.01(3) 1_565 ?
W4A O12A 1.82(3) . ?
W4A O12B 1.56(6) 1_565 ?
W4A O12B 2.37(6) . ?
W4A O13 1.85(4) . ?
W4A O14 1.98(4) . ?
W4A O15 2.00(3) . ?
W4B K3A 4.23(3) 1_655 ?
W4B K3B 3.75(3) 1_655 ?
W4B K4A 4.06(3) 2_656 ?
W4B K4B 3.68(3) 2_656 ?
W4B O10 1.87(3) . ?
W4B O12A 1.29(3) . ?
W4B O12B 2.08(7) 1_565 ?
W4B O12B 1.86(6) . ?
W4B O13 1.88(4) . ?
W4B O14 1.97(4) . ?
W4B O15 1.86(3) . ?
W5 K3A 4.25(3) 1_565 ?
W5 K3A 4.14(3) . ?
W5 K3B 3.89(3) . ?
W5 K4A 4.02(3) 2_656 ?
W5 K4A 4.12(3) 2_666 ?
W5 K4B 3.86(3) 2_656 ?
W5 O11 1.82(3) . ?
W5 O13 1.97(4) . ?
W5 O14 1.85(4) 1_455 ?
W5 O16 1.83(6) . ?
W5 O16 1.99(6) 1_565 ?
W5 O17 1.95(3) . ?
W6 K4A 4.41(3) 2_566 ?
W6 K4A 3.84(3) 2_656 ?
W6 K4A 3.95(3) 2_666 ?
W6 K4A 4.31(3) 2_556 ?
W6 K4B 3.81(3) 2_556 ?
W6 K4B 3.81(3) 2_656 ?
W6 O15 1.91(2) 1_455 ?
W6 O17 1.84(3) . ?
W6 O18 1.91(3) . ?
W6 O19 1.93(3) . ?
W6 O19 1.96(3) 1_565 ?
W6 O20 1.97(2) . ?
W7 K4A 3.83(3) 2_656 ?
W7 K4A 3.83(3) . ?
W7 K4B 3.73(3) 2_656 ?
W7 K4B 3.73(3) . ?
W7 O18 1.86(2) 2_656 ?
W7 O18 1.86(2) . ?
W7 O21 1.78(5) . ?
W7 O21 1.78(5) 2_656 ?
W7 O21 2.15(5) 2_666 ?
W7 O21 2.15(5) 1_565 ?
W7 O22 1.93(4) . ?
W7 O22 1.93(4) 2_656 ?
W8 K4A 4.28(3) . ?
W8 K4A 4.28(3) 2_556 ?
W8 K4A 4.10(3) 1_565 ?
W8 K4A 4.10(3) 2_566 ?
W8 K4B 3.86(3) 2_556 ?
W8 K4B 3.86(3) . ?
W8 O20 1.86(2) . ?
W8 O20 1.86(2) 2_556 ?
W8 O22 1.91(4) . ?
W8 O22 1.91(4) 2_556 ?
W8 O23 1.91(9) . ?
W8 O23 1.90(9) 1_565 ?
K1 K1 3.8123(3) 1_565 ?
K1 K1 3.8123(3) 1_545 ?
K1 K2 3.6575(6) 1_455 ?
K1 K2 3.6575(6) . ?
K1 O1 3.481(18) 1_545 ?
K1 O1 3.481(18) 2_545 ?
K1 O2 2.62(3) 2 ?
K1 O2 2.86(3) 1_545 ?
K1 O2 2.86(3) 2_545 ?
K1 O2 2.62(3) . ?
K1 O6 3.05(4) 1_455 ?
K1 O6 3.05(4) 2_655 ?
K1 O6 2.57(3) 1_445 ?
K1 O6 2.57(3) 2_645 ?
K1 O7 3.89(2) 2_655 ?
K1 O7 3.89(2) 1_455 ?
K2 K2 3.8123(3) 1_545 ?
K2 K2 3.8123(3) 1_565 ?
K2 O1 3.502(18) 2_645 ?
K2 O1 3.502(18) 1_545 ?
K2 O2 3.37(3) 2_645 ?
K2 O2 3.23(3) 2_655 ?
K2 O2 3.37(3) 1_545 ?
K2 O2 3.23(3) . ?
K2 O4 3.59(3) 2_655 ?
K2 O4 3.41(3) 1_545 ?
K2 O4 3.59(3) . ?
K2 O4 3.41(3) 2_645 ?
K2 O6 3.54(4) 2_655 ?
K2 O6 3.54(4) . ?
K2 O6 3.07(3) 2_645 ?
K2 O6 3.07(3) 1_545 ?
K2 O7 3.85(3) 2_655 ?
K2 O7 3.85(3) . ?
K3A K3A 3.8123(4) 1_545 ?
K3A K3A 3.8123(4) 1_565 ?
K3A K3B 1.54(6) . ?
K3A K3B 2.33(6) 1_545 ?
K3A O1 3.71(3) 1_545 ?
K3A O3 3.16(4) . ?
K3A O3 3.08(4) 1_545 ?
K3A O5 3.20(5) 1_545 ?
K3A O5 2.96(5) . ?
K3A O7 3.45(4) 1_455 ?
K3A O8 3.11(5) 1_445 ?
K3A O8 3.46(5) 1_455 ?
K3A O9 3.47(7) . ?
K3A O10 3.58(5) 1_445 ?
K3A O10 3.34(5) 1_455 ?
K3A O11 3.48(5) . ?
K3A O11 3.21(5) 1_545 ?
K3A O12B 3.45(6) 1_455 ?
K3A O14 3.47(4) 1_455 ?
K3A O14 3.45(4) 1_445 ?
K3B K3B 3.8123(4) 1_545 ?
K3B K3B 3.8123(4) 1_565 ?
K3B O3 2.53(4) . ?
K3B O5 2.70(4) . ?
K3B O7 3.63(4) 1_455 ?
K3B O8 2.49(4) 1_455 ?
K3B O9 3.91(5) 1_455 ?
K3B O10 2.63(4) 1_455 ?
K3B O11 3.06(4) . ?
K3B O12B 3.70(6) 1_455 ?
K3B O14 2.92(4) 1_455 ?
K4A K4A 3.8123(9) 1_545 ?
K4A K4B 3.09(5) 1_545 ?
K4A K4B 0.78(4) . ?
K4A O12A 3.60(4) 2_656 ?
K4A O13 3.19(4) 2_646 ?
K4A O13 3.27(4) 2_656 ?
K4A O15 3.55(4) 2_646 ?
K4A O15 3.30(4) 2_656 ?
K4A O16 3.49(6) 2_656 ?
K4A O17 3.32(4) 2_656 ?
K4A O17 3.01(4) 2_646 ?
K4A O18 2.91(4) 2_656 ?
K4A O18 3.35(4) 2_646 ?
K4A O19 3.02(3) 2_656 ?
K4A O20 3.59(4) 2_556 ?
K4A O20 3.31(4) 2_546 ?
K4A O21 3.05(6) . ?
K4A O22 3.21(4) . ?
K4A O22 3.23(4) 1_545 ?
K4A O23 3.73(2) . ?
K4B O12A 3.45(4) 2_656 ?
K4B O13 2.87(4) 2_656 ?
K4B O13 3.65(4) 2_646 ?
K4B O15 2.77(4) 2_656 ?
K4B O16 3.68(6) 2_656 ?
K4B O17 3.63(4) 2_646 ?
K4B O17 3.09(4) 2_656 ?
K4B O18 2.82(4) 2_656 ?
K4B O19 3.39(4) 2_656 ?
K4B O20 3.57(4) 2_546 ?
K4B O20 3.00(4) 2_556 ?
K4B O21 3.31(6) . ?
K4B O22 2.84(4) . ?
K4B O22 3.72(4) 1_545 ?
K4B O23 3.64(3) . ?
O12A O12B 0.81(6) . ?
O21 O21 0.94(12) 2_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
K1 W1 K1 55.99(4) 1_565 . ?
K1 W1 K2 54.43(9) 1_565 1_565 ?
K1 W1 K3A 130.5(6) 1_565 . ?
K2 W1 K1 79.6(3) 1_565 . ?
K2 W1 K3A 172.5(6) 1_565 . ?
K3A W1 K1 130.8(6) 1_565 . ?
K3A W1 K1 98.7(5) . . ?
K3A W1 K1 105.1(5) 1_565 1_565 ?
K3A W1 K2 129.6(7) 1_565 1_565 ?
K3A W1 K3A 56.8(4) 1_565 . ?
K3B W1 K1 120.4(4) . 1_565 ?
K3B W1 K1 109.9(5) . . ?
K3B W1 K2 164.8(7) . 1_565 ?
K3B W1 K3A 35.3(8) . 1_565 ?
K3B W1 K3A 22.1(8) . . ?
O1 W1 K1 61.4(7) . 1_565 ?
O1 W1 K1 56.8(5) 1_545 . ?
O1 W1 K1 117.1(7) . . ?
O1 W1 K1 112.6(5) 1_545 1_565 ?
O1 W1 K2 59.5(7) . 1_565 ?
O1 W1 K2 108.9(6) 1_545 1_565 ?
O1 W1 K3A 127.0(8) . . ?
O1 W1 K3A 121.3(8) 1_545 1_565 ?
O1 W1 K3A 64.6(7) 1_545 . ?
O1 W1 K3A 70.3(8) . 1_565 ?
O1 W1 K3B 86.3(7) 1_545 . ?
O1 W1 K3B 105.3(9) . . ?
O1 W1 O1 168.4(11) . 1_545 ?
O1 W1 O2 97.3(12) . . ?
O1 W1 O3 98.3(11) . . ?
O1 W1 O4 89.1(11) . . ?
O1 W1 O5 84.0(9) 1_545 . ?
O1 W1 O5 104.2(10) . . ?
O2 W1 K1 24.4(10) . . ?
O2 W1 K1 41.2(10) . 1_565 ?
O2 W1 K2 55.5(10) . 1_565 ?
O2 W1 K3A 123.1(11) . . ?
O2 W1 K3A 140.8(10) . 1_565 ?
O2 W1 K3B 132.2(10) . . ?
O2 W1 O1 73.9(12) . 1_545 ?
O2 W1 O3 98.2(12) . . ?
O2 W1 O4 94.4(11) . . ?
O2 W1 O5 157.9(13) . . ?
O3 W1 K1 84.0(8) . 1_565 ?
O3 W1 K1 81.3(8) . . ?
O3 W1 K2 138.1(8) . 1_565 ?
O3 W1 K3A 50.1(10) . 1_565 ?
O3 W1 K3A 47.9(10) . . ?
O3 W1 K3B 37.9(9) . . ?
O3 W1 O1 90.6(10) . 1_545 ?
O3 W1 O4 164.4(11) . . ?
O3 W1 O5 83.7(10) . . ?
O4 W1 K1 107.6(8) . . ?
O4 W1 K1 111.6(7) . 1_565 ?
O4 W1 K2 57.3(8) . 1_565 ?
O4 W1 K3A 121.5(10) . 1_565 ?
O4 W1 K3A 116.9(10) . . ?
O4 W1 K3B 126.8(8) . . ?
O4 W1 O1 84.0(10) . 1_545 ?
O4 W1 O5 81.2(10) . . ?
O5 W1 K1 159.4(8) . 1_565 ?
O5 W1 K1 137.6(8) . . ?
O5 W1 K2 133.6(7) . 1_565 ?
O5 W1 K3A 54.5(9) . 1_565 ?
O5 W1 K3A 44.5(9) . . ?
O5 W1 K3B 45.8(8) . . ?
K1 W2 K1 55.73(3) 1_665 1_655 ?
K1 W2 K2 81.2(3) 1_665 . ?
K1 W2 K3A 100.4(5) 1_665 1_665 ?
K2 W2 K1 54.25(9) 1_565 1_665 ?
K2 W2 K1 80.4(3) 1_565 1_655 ?
K2 W2 K1 52.42(9) . 1_655 ?
K2 W2 K2 55.75(4) 1_565 . ?
K2 W2 K3A 127.6(6) 1_565 1_665 ?
K3A W2 K1 126.0(6) 1_665 1_655 ?
K3A W2 K2 176.6(6) 1_665 . ?
K3B W2 K1 122.4(5) 1_655 1_665 ?
K3B W2 K1 113.7(5) 1_655 1_655 ?
K3B W2 K2 161.3(7) 1_655 1_565 ?
K3B W2 K2 142.4(7) 1_655 . ?
K3B W2 K3A 34.3(8) 1_655 1_665 ?
O3 W2 K1 81.4(8) 1_655 1_655 ?
O3 W2 K1 81.3(8) 1_655 1_665 ?
O3 W2 K2 132.5(8) 1_655 . ?
O3 W2 K2 134.7(8) 1_655 1_565 ?
O3 W2 K3A 45.2(10) 1_655 1_665 ?
O3 W2 K3B 42.9(9) 1_655 1_655 ?
O3 W2 O7 87.7(11) 1_655 . ?
O3 W2 O8 83.1(10) 1_655 . ?
O4 W2 K1 112.0(8) . 1_655 ?
O4 W2 K1 112.5(8) . 1_665 ?
O4 W2 K2 58.3(8) . 1_565 ?
O4 W2 K2 59.7(8) . . ?
O4 W2 K3A 122.0(9) . 1_665 ?
O4 W2 K3B 121.7(8) . 1_655 ?
O4 W2 O3 164.4(10) . 1_655 ?
O4 W2 O7 89.8(12) . . ?
O4 W2 O8 81.4(10) . . ?
O6 W2 K1 40.7(11) . 1_655 ?
O6 W2 K1 24.0(10) . 1_665 ?
O6 W2 K2 57.3(10) . . ?
O6 W2 K2 45.8(10) . 1_565 ?
O6 W2 K3A 124.0(11) . 1_665 ?
O6 W2 K3B 139.4(11) . 1_655 ?
O6 W2 O3 96.6(12) . 1_655 ?
O6 W2 O4 98.8(12) . . ?
O6 W2 O7 91.4(13) . 1_565 ?
O6 W2 O7 107.1(13) . . ?
O6 W2 O8 165.3(14) . . ?
O7 W2 K1 124.6(7) . 1_665 ?
O7 W2 K1 68.9(7) . 1_655 ?
O7 W2 K1 72.4(8) 1_565 1_665 ?
O7 W2 K1 128.0(8) 1_565 1_655 ?
O7 W2 K2 67.3(8) . . ?
O7 W2 K2 122.8(8) . 1_565 ?
O7 W2 K2 127.4(9) 1_565 . ?
O7 W2 K2 72.0(9) 1_565 1_565 ?
O7 W2 K3A 109.4(9) . 1_665 ?
O7 W2 K3A 56.0(9) 1_565 1_665 ?
O7 W2 K3B 89.4(10) 1_565 1_655 ?
O7 W2 K3B 75.1(9) . 1_655 ?
O7 W2 O3 87.8(12) 1_565 1_655 ?
O7 W2 O4 89.7(12) 1_565 . ?
O7 W2 O7 161.4(14) 1_565 . ?
O7 W2 O8 87.6(11) . . ?
O7 W2 O8 74.0(11) 1_565 . ?
O8 W2 K1 152.2(8) . 1_655 ?
O8 W2 K1 143.3(9) . 1_665 ?
O8 W2 K2 132.3(8) . . ?
O8 W2 K2 126.3(8) . 1_565 ?
O8 W2 K3A 47.3(9) . 1_665 ?
O8 W2 K3B 42.9(9) . 1_655 ?
K3A W3 K3A 172.7(11) 1_655 1_565 ?
K3A W3 K3A 131.2(11) . 1_655 ?
K3A W3 K3A 55.8(5) . 1_565 ?
K3A W3 K3A 118.9(9) 1_565 1_665 ?
K3A W3 K3A 174.5(11) . 1_665 ?
K3A W3 K3A 54.0(5) 1_655 1_665 ?
K3B W3 K3A 151.4(9) 1_655 1_565 ?
K3B W3 K3A 32.6(8) 1_655 1_665 ?
K3B W3 K3A 152.6(9) 1_655 . ?
K3B W3 K3A 33.2(8) . 1_565 ?
K3B W3 K3A 152.1(8) . 1_665 ?
K3B W3 K3A 21.4(9) 1_655 1_655 ?
K3B W3 K3A 153.8(8) . 1_655 ?
K3B W3 K3A 22.6(8) . . ?
K3B W3 K3B 175.0(12) 1_655 . ?
O5 W3 K3A 131.2(10) . 1_665 ?
O5 W3 K3A 45.5(10) . 1_565 ?
O5 W3 K3A 44.5(10) . . ?
O5 W3 K3A 136.4(10) . 1_655 ?
O5 W3 K3B 37.4(9) . . ?
O5 W3 K3B 141.3(10) . 1_655 ?
O5 W3 O8 98.8(10) . . ?
O5 W3 O9 89.6(15) . 1_565 ?
O5 W3 O10 168.7(11) . . ?
O5 W3 O11 86.1(11) . . ?
O8 W3 K3A 116.4(10) . 1_565 ?
O8 W3 K3A 39.8(9) . 1_665 ?
O8 W3 K3A 57.5(10) . 1_655 ?
O8 W3 K3A 139.0(9) . . ?
O8 W3 K3B 135.2(9) . . ?
O8 W3 K3B 45.3(10) . 1_655 ?
O8 W3 O9 80.4(14) . 1_565 ?
O8 W3 O10 90.9(10) . . ?
O8 W3 O11 149.0(13) . . ?
O9 W3 K3A 61.3(17) . . ?
O9 W3 K3A 70.8(16) . 1_655 ?
O9 W3 K3A 117.6(13) 1_565 1_655 ?
O9 W3 K3A 55.7(15) 1_565 1_565 ?
O9 W3 K3A 64.0(14) 1_565 1_665 ?
O9 W3 K3A 116.5(15) . 1_565 ?
O9 W3 K3A 111.0(13) 1_565 . ?
O9 W3 K3A 124.2(15) . 1_665 ?
O9 W3 K3B 92.0(16) . 1_655 ?
O9 W3 K3B 83.6(16) . . ?
O9 W3 K3B 88.6(14) 1_565 . ?
O9 W3 K3B 96.3(14) 1_565 1_655 ?
O9 W3 O5 93.3(16) . . ?
O9 W3 O8 115.7(16) . . ?
O9 W3 O9 162.9(19) . 1_565 ?
O9 W3 O10 87.6(15) . . ?
O9 W3 O11 94.3(15) . . ?
O9 W3 O11 69.0(14) 1_565 . ?
O10 W3 K3A 124.5(9) . 1_565 ?
O10 W3 K3A 55.5(9) . 1_665 ?
O10 W3 K3A 54.4(8) . 1_655 ?
O10 W3 K3A 128.0(8) . . ?
O10 W3 K3B 131.8(8) . . ?
O10 W3 K3B 49.9(8) . 1_655 ?
O10 W3 O9 86.3(14) . 1_565 ?
O10 W3 O11 82.6(8) . . ?
O11 W3 K3A 116.9(10) . 1_665 ?
O11 W3 K3A 133.9(8) . 1_655 ?
O11 W3 K3A 61.5(9) . . ?
O11 W3 K3A 48.7(9) . 1_565 ?
O11 W3 K3B 51.3(9) . . ?
O11 W3 K3B 131.7(9) . 1_655 ?
W4B W4A K3B 84.8(12) . 1_655 ?
W4B W4A K4A 109.2(12) . 2_666 ?
W4B W4A K4B 63.8(12) . 2_656 ?
W4B W4A O10 83.1(12) . . ?
W4B W4A O12A 6.4(16) . . ?
W4B W4A O12A 167.9(11) . 1_565 ?
W4B W4A O12B 161(3) . 1_565 ?
W4B W4A O12B 14.7(15) . . ?
W4B W4A O13 85.1(18) . . ?
W4B W4A O14 81.0(17) . . ?
W4B W4A O15 67.7(13) . . ?
K3B W4A K4A 165.7(8) 1_655 2_666 ?
K3B W4A K4B 148.2(7) 1_655 2_656 ?
K4B W4A K4A 45.4(6) 2_656 2_666 ?
O10 W4A K3B 40.0(9) . 1_655 ?
O10 W4A K4A 136.4(9) . 2_666 ?
O10 W4A K4B 124.9(10) . 2_656 ?
O10 W4A O12A 108.9(13) . 1_565 ?
O10 W4A O12B 71.8(15) . . ?
O10 W4A O13 93.3(11) . . ?
O10 W4A O14 89.5(10) . . ?
O10 W4A O15 150.8(15) . . ?
O12A W4A K3B 85.5(11) . 1_655 ?
O12A W4A K3B 105.2(10) 1_565 1_655 ?
O12A W4A K4A 61.3(10) 1_565 2_666 ?
O12A W4A K4A 108.1(11) . 2_666 ?
O12A W4A K4B 62.7(11) . 2_656 ?
O12A W4A K4B 106.6(9) 1_565 2_656 ?
O12A W4A O10 79.6(13) . . ?
O12A W4A O12A 169.3(18) . 1_565 ?
O12A W4A O12B 16.5(16) . . ?
O12A W4A O12B 172.2(16) 1_565 . ?
O12A W4A O13 80.1(14) . . ?
O12A W4A O14 86.3(13) . . ?
O12A W4A O15 71.5(13) . . ?
O12B W4A K3B 85(2) 1_565 1_655 ?
O12B W4A K3B 70.1(14) . 1_655 ?
O12B W4A K4A 123.9(14) . 2_666 ?
O12B W4A K4A 82(2) 1_565 2_666 ?
O12B W4A K4B 78.5(14) . 2_656 ?
O12B W4A K4B 126.6(19) 1_565 2_656 ?
O12B W4A O10 99(2) 1_565 . ?
O12B W4A O12A 167(2) 1_565 . ?
O12B W4A O12A 22(2) 1_565 1_565 ?
O12B W4A O12B 151(3) 1_565 . ?
O12B W4A O13 113(2) 1_565 . ?
O12B W4A O14 80(2) 1_565 . ?
O12B W4A O15 108(2) 1_565 . ?
O13 W4A K3B 133.1(9) . 1_655 ?
O13 W4A K4A 48.7(9) . 2_666 ?
O13 W4A K4B 44.3(10) . 2_656 ?
O13 W4A O12A 92.6(13) . 1_565 ?
O13 W4A O12B 95.1(17) . . ?
O13 W4A O14 165.4(12) . . ?
O13 W4A O15 85.7(11) . . ?
O14 W4A K3B 50.1(8) . 1_655 ?
O14 W4A K4A 132.9(8) . 2_666 ?
O14 W4A K4B 123.7(9) . 2_656 ?
O14 W4A O12A 100.0(13) . 1_565 ?
O14 W4A O12B 72.2(16) . . ?
O14 W4A O15 84.8(10) . . ?
O15 W4A K3B 130.9(9) . 1_655 ?
O15 W4A K4A 60.0(9) . 2_666 ?
O15 W4A K4B 42.6(8) . 2_656 ?
O15 W4A O12A 100.3(12) . 1_565 ?
O15 W4A O12B 79.3(15) . . ?
W4A W4B K3A 108.1(11) . 1_655 ?
W4A W4B K3B 87.0(12) . 1_655 ?
W4A W4B K4A 117.7(14) . 2_656 ?
W4A W4B K4B 108.6(13) . 2_656 ?
W4A W4B O10 80.3(13) . . ?
W4A W4B O12A 171(2) . . ?
W4A W4B O12B 161.1(19) . . ?
W4A W4B O12B 14.0(19) . 1_565 ?
W4A W4B O13 78.3(19) . . ?
W4A W4B O14 83.4(18) . . ?
W4A W4B O15 96.8(16) . . ?
K3B W4B K3A 21.1(8) 1_655 1_655 ?
K3B W4B K4A 153.5(11) 1_655 2_656 ?
K4A W4B K3A 133.4(9) 2_656 1_655 ?
K4B W4B K3A 143.1(9) 2_656 1_655 ?
K4B W4B K3B 163.5(10) 2_656 1_655 ?
K4B W4B K4A 10.1(6) 2_656 2_656 ?
O10 W4B K3A 49.6(10) . 1_655 ?
O10 W4B K3B 40.5(9) . 1_655 ?
O10 W4B K4A 129.5(11) . 2_656 ?
O10 W4B K4B 135.2(10) . 2_656 ?
O10 W4B O12B 84.8(19) . . ?
O10 W4B O12B 82.3(18) . 1_565 ?
O10 W4B O13 91.9(12) . . ?
O10 W4B O14 89.5(11) . . ?
O12A W4B K3A 73.3(15) . 1_655 ?
O12A W4B K3B 93.9(16) . 1_655 ?
O12A W4B K4A 60.1(15) . 2_656 ?
O12A W4B K4B 69.8(15) . 2_656 ?
O12A W4B O10 94.6(18) . . ?
O12A W4B O12B 22(2) . . ?
O12A W4B O12B 173(2) . 1_565 ?
O12A W4B O13 94.5(18) . . ?
O12A W4B O14 104.1(19) . . ?
O12A W4B O15 88.5(17) . . ?
O12B W4B K3A 53.0(17) . 1_655 ?
O12B W4B K3A 99.8(15) 1_565 1_655 ?
O12B W4B K3B 74.1(17) . 1_655 ?
O12B W4B K3B 79.5(16) 1_565 1_655 ?
O12B W4B K4A 126.7(16) 1_565 2_656 ?
O12B W4B K4A 80.9(19) . 2_656 ?
O12B W4B K4B 116.9(15) 1_565 2_656 ?
O12B W4B K4B 90.2(18) . 2_656 ?
O12B W4B O12B 151(3) . 1_565 ?
O12B W4B O14 85(2) . . ?
O13 W4B K3A 136.7(10) . 1_655 ?
O13 W4B K3B 132.1(10) . 1_655 ?
O13 W4B K4A 52.5(10) . 2_656 ?
O13 W4B K4B 50.2(10) . 2_656 ?
O13 W4B O12B 114(2) . . ?
O13 W4B O12B 92.1(19) . 1_565 ?
O13 W4B O14 161.2(19) . . ?
O14 W4B K3A 54.3(10) . 1_655 ?
O14 W4B K3B 50.3(8) . 1_655 ?
O14 W4B K4A 136.3(10) . 2_656 ?
O14 W4B K4B 134.4(9) . 2_656 ?
O14 W4B O12B 69.5(19) . 1_565 ?
O15 W4B K3A 130.9(12) . 1_655 ?
O15 W4B K3B 138.4(9) . 1_655 ?
O15 W4B K4A 53.1(9) . 2_656 ?
O15 W4B K4B 47.0(9) . 2_656 ?
O15 W4B O10 177(2) . . ?
O15 W4B O12B 98(2) . . ?
O15 W4B O12B 94.6(18) . 1_565 ?
O15 W4B O13 88.8(11) . . ?
O15 W4B O14 88.8(11) . . ?
K3A W5 K3A 54.0(3) . 1_565 ?
K3B W5 K3A 32.9(8) . 1_565 ?
K3B W5 K3A 21.7(8) . . ?
K3B W5 K4A 154.6(8) . 2_666 ?
K3B W5 K4A 148.9(8) . 2_656 ?
K4A W5 K3A 127.8(7) 2_656 . ?
K4A W5 K3A 178.1(7) 2_656 1_565 ?
K4A W5 K3A 122.3(7) 2_666 1_565 ?
K4A W5 K3A 176.3(7) 2_666 . ?
K4A W5 K4A 55.8(3) 2_656 2_666 ?
K4B W5 K3A 138.3(7) 2_656 . ?
K4B W5 K3A 167.2(7) 2_656 1_565 ?
K4B W5 K3B 159.8(7) 2_656 . ?
K4B W5 K4A 45.4(6) 2_656 2_666 ?
K4B W5 K4A 11.1(6) 2_656 2_656 ?
O11 W5 K3A 56.2(11) . . ?
O11 W5 K3A 44.6(10) . 1_565 ?
O11 W5 K3B 50.1(10) . . ?
O11 W5 K4A 122.1(11) . 2_666 ?
O11 W5 K4A 136.4(10) . 2_656 ?
O11 W5 K4B 134.1(10) . 2_656 ?
O11 W5 O13 90.7(12) . . ?
O11 W5 O14 92.2(11) . 1_455 ?
O11 W5 O16 82(2) . 1_565 ?
O11 W5 O16 104(2) . . ?
O11 W5 O17 158.2(14) . . ?
O13 W5 K3A 125.7(10) . 1_565 ?
O13 W5 K3A 132.8(10) . . ?
O13 W5 K3B 139.8(8) . . ?
O13 W5 K4A 48.9(9) . 2_666 ?
O13 W5 K4A 53.8(9) . 2_656 ?
O13 W5 K4B 46.0(9) . 2_656 ?
O14 W5 K3A 52.6(9) 1_455 1_565 ?
O14 W5 K3A 56.0(9) 1_455 . ?
O14 W5 K3B 45.7(8) 1_455 . ?
O14 W5 K4A 121.9(9) 1_455 2_666 ?
O14 W5 K4A 127.5(9) 1_455 2_656 ?
O14 W5 K4B 133.3(9) 1_455 2_656 ?
O14 W5 O13 169.7(11) 1_455 . ?
O14 W5 O16 87.2(18) 1_455 1_565 ?
O14 W5 O16 95(2) 1_455 . ?
O14 W5 O17 87.7(10) 1_455 . ?
O16 W5 K3A 121.8(19) . 1_565 ?
O16 W5 K3A 67.9(18) . . ?
O16 W5 K3A 64.8(18) 1_565 1_565 ?
O16 W5 K3A 118.8(18) 1_565 . ?
O16 W5 K3B 97.3(17) 1_565 . ?
O16 W5 K3B 89.1(19) . . ?
O16 W5 K4A 115.8(19) . 2_666 ?
O16 W5 K4A 57.5(17) 1_565 2_666 ?
O16 W5 K4A 113.3(18) 1_565 2_656 ?
O16 W5 K4A 60.0(18) . 2_656 ?
O16 W5 K4B 70.7(18) . 2_656 ?
O16 W5 K4B 102.8(18) 1_565 2_656 ?
O16 W5 O13 83.4(18) 1_565 . ?
O16 W5 O13 93.5(19) . . ?
O16 W5 O16 173(3) . 1_565 ?
O16 W5 O17 76.0(19) 1_565 . ?
O16 W5 O17 97(2) . . ?
O17 W5 K3A 137.3(9) . . ?
O17 W5 K3A 123.2(10) . 1_565 ?
O17 W5 K3B 133.4(8) . . ?
O17 W5 K4A 55.2(9) . 2_656 ?
O17 W5 K4A 43.1(9) . 2_666 ?
O17 W5 K4B 52.5(9) . 2_656 ?
O17 W5 O13 86.0(10) . . ?
K4A W6 K4A 51.8(3) 2_556 2_566 ?
K4A W6 K4A 127.4(10) 2_656 2_556 ?
K4A W6 K4A 173.7(10) 2_666 2_556 ?
K4A W6 K4A 178.1(7) 2_656 2_566 ?
K4A W6 K4A 122.1(9) 2_666 2_566 ?
K4A W6 K4A 58.6(4) 2_656 2_666 ?
K4B W6 K4A 135.8(8) 2_556 2_656 ?
K4B W6 K4A 139.1(7) 2_656 2_556 ?
K4B W6 K4A 168.9(7) 2_656 2_566 ?
K4B W6 K4A 11.7(6) 2_656 2_656 ?
K4B W6 K4A 43.4(6) 2_556 2_566 ?
K4B W6 K4A 165.5(8) 2_556 2_666 ?
K4B W6 K4A 8.4(6) 2_556 2_556 ?
K4B W6 K4A 46.9(7) 2_656 2_666 ?
K4B W6 K4B 147.5(9) 2_556 2_656 ?
O15 W6 K4A 51.6(9) 1_455 2_566 ?
O15 W6 K4A 132.9(9) 1_455 2_666 ?
O15 W6 K4A 46.3(9) 1_455 2_556 ?
O15 W6 K4A 129.6(9) 1_455 2_656 ?
O15 W6 K4B 43.8(8) 1_455 2_556 ?
O15 W6 K4B 134.7(9) 1_455 2_656 ?
O15 W6 O19 103.9(11) 1_455 1_565 ?
O15 W6 O19 96.9(12) 1_455 . ?
O15 W6 O20 87.7(10) 1_455 . ?
O17 W6 K4A 135.9(9) . 2_556 ?
O17 W6 K4A 59.8(10) . 2_656 ?
O17 W6 K4A 122.1(9) . 2_566 ?
O17 W6 K4A 47.1(9) . 2_666 ?
O17 W6 K4B 136.4(9) . 2_556 ?
O17 W6 K4B 53.4(9) . 2_656 ?
O17 W6 O15 93.2(9) . 1_455 ?
O17 W6 O18 93.4(11) . . ?
O17 W6 O19 73.4(11) . 1_565 ?
O17 W6 O19 95.8(11) . . ?
O17 W6 O20 158.2(13) . . ?
O18 W6 K4A 58.1(10) . 2_666 ?
O18 W6 K4A 123.5(10) . 2_556 ?
O18 W6 K4A 131.2(9) . 2_566 ?
O18 W6 K4A 47.3(9) . 2_656 ?
O18 W6 K4B 127.4(9) . 2_556 ?
O18 W6 K4B 45.4(9) . 2_656 ?
O18 W6 O15 167.7(14) . 1_455 ?
O18 W6 O19 87.9(13) . 1_565 ?
O18 W6 O19 72.2(13) . . ?
O18 W6 O20 89.9(8) . . ?
O19 W6 K4A 128.2(7) . 2_566 ?
O19 W6 K4A 73.8(7) 1_565 2_566 ?
O19 W6 K4A 106.9(8) 1_565 2_656 ?
O19 W6 K4A 48.4(9) 1_565 2_666 ?
O19 W6 K4A 50.9(9) . 2_656 ?
O19 W6 K4A 109.4(9) . 2_666 ?
O19 W6 K4A 76.4(7) . 2_556 ?
O19 W6 K4A 125.5(7) 1_565 2_556 ?
O19 W6 K4B 84.9(8) . 2_556 ?
O19 W6 K4B 62.7(8) . 2_656 ?
O19 W6 K4B 117.1(8) 1_565 2_556 ?
O19 W6 K4B 95.2(8) 1_565 2_656 ?
O19 W6 O19 156.9(12) . 1_565 ?
O19 W6 O20 105.7(10) . . ?
O19 W6 O20 85.2(10) 1_565 . ?
O20 W6 K4A 119.6(9) . 2_666 ?
O20 W6 K4A 133.4(8) . 2_656 ?
O20 W6 K4A 55.5(9) . 2_556 ?
O20 W6 K4A 44.8(8) . 2_566 ?
O20 W6 K4B 135.1(8) . 2_656 ?
O20 W6 K4B 51.3(9) . 2_556 ?
K4A W7 K4A 131.0(11) 2_656 . ?
K4B W7 K4A 11.8(6) 2_656 2_656 ?
K4B W7 K4A 142.1(8) . 2_656 ?
K4B W7 K4A 142.1(8) 2_656 . ?
K4B W7 K4A 11.8(6) . . ?
K4B W7 K4B 153.5(10) 2_656 . ?
O18 W7 K4A 131.1(10) . . ?
O18 W7 K4A 47.2(10) 2_656 . ?
O18 W7 K4A 47.2(10) . 2_656 ?
O18 W7 K4A 131.1(10) 2_656 2_656 ?
O18 W7 K4B 47.3(9) . 2_656 ?
O18 W7 K4B 131.8(9) 2_656 2_656 ?
O18 W7 K4B 47.3(9) 2_656 . ?
O18 W7 K4B 131.8(10) . . ?
O18 W7 O18 177(2) 2_656 . ?
O18 W7 O21 80.1(19) 2_656 1_565 ?
O18 W7 O21 102.9(19) . 1_565 ?
O18 W7 O21 80.1(19) . 2_666 ?
O18 W7 O21 102.9(19) 2_656 2_666 ?
O18 W7 O22 90.4(10) . . ?
O18 W7 O22 90.1(10) . 2_656 ?
O18 W7 O22 90.4(10) 2_656 2_656 ?
O18 W7 O22 90.1(10) 2_656 . ?
O21 W7 K4A 51.0(19) 2_656 2_656 ?
O21 W7 K4A 51.0(19) . . ?
O21 W7 K4A 126.5(16) 2_666 . ?
O21 W7 K4A 126.5(17) 1_565 2_656 ?
O21 W7 K4A 102.4(17) 1_565 . ?
O21 W7 K4A 102.4(17) 2_666 2_656 ?
O21 W7 K4A 80.2(19) 2_656 . ?
O21 W7 K4A 80.2(19) . 2_656 ?
O21 W7 K4B 91.4(16) 1_565 . ?
O21 W7 K4B 114.9(16) 1_565 2_656 ?
O21 W7 K4B 91.1(19) 2_656 . ?
O21 W7 K4B 114.9(16) 2_666 . ?
O21 W7 K4B 91.4(16) 2_666 2_656 ?
O21 W7 K4B 62.6(19) 2_656 2_656 ?
O21 W7 K4B 62.6(19) . . ?
O21 W7 K4B 91.1(19) . 2_656 ?
O21 W7 O18 102(2) 2_656 2_656 ?
O21 W7 O18 75(2) 2_656 . ?
O21 W7 O18 102(2) . . ?
O21 W7 O18 75(2) . 2_656 ?
O21 W7 O21 152(3) . 1_565 ?
O21 W7 O21 152(3) 2_656 2_666 ?
O21 W7 O21 177.3(8) 2_656 1_565 ?
O21 W7 O21 25(3) 1_565 2_666 ?
O21 W7 O21 177.3(8) . 2_666 ?
O21 W7 O21 31(4) 2_656 . ?
O21 W7 O22 105(2) 2_656 . ?
O21 W7 O22 105(2) . 2_656 ?
O21 W7 O22 92(2) . . ?
O21 W7 O22 92(2) 2_656 2_656 ?
O22 W7 K4A 56.7(8) . . ?
O22 W7 K4A 132.5(8) . 2_656 ?
O22 W7 K4A 56.7(8) 2_656 2_656 ?
O22 W7 K4A 132.5(8) 2_656 . ?
O22 W7 K4B 48.5(8) 2_656 2_656 ?
O22 W7 K4B 137.1(8) 2_656 . ?
O22 W7 K4B 137.1(8) . 2_656 ?
O22 W7 K4B 48.5(8) . . ?
O22 W7 O21 86.8(17) . 2_666 ?
O22 W7 O21 86.8(17) 2_656 1_565 ?
O22 W7 O21 76.0(17) 2_656 2_666 ?
O22 W7 O21 76.0(17) . 1_565 ?
O22 W7 O22 162.4(17) . 2_656 ?
K4A W8 K4A 175.0(10) 2_566 . ?
K4A W8 K4A 54.1(3) 2_566 2_556 ?
K4A W8 K4A 54.1(3) 1_565 . ?
K4A W8 K4A 121.0(10) 2_556 . ?
K4A W8 K4A 175.0(9) 1_565 2_556 ?
K4A W8 K4A 130.9(10) 1_565 2_566 ?
K4B W8 K4A 45.6(6) . 1_565 ?
K4B W8 K4A 175.0(7) 2_556 1_565 ?
K4B W8 K4A 129.5(7) . 2_556 ?
K4B W8 K4A 45.6(6) 2_556 2_566 ?
K4B W8 K4A 9.2(6) 2_556 2_556 ?
K4B W8 K4A 129.5(7) 2_556 . ?
K4B W8 K4A 9.2(6) . . ?
K4B W8 K4A 175.0(6) . 2_566 ?
K4B W8 K4B 138.2(10) 2_556 . ?
O20 W8 K4A 126.1(9) 2_556 2_566 ?
O20 W8 K4A 125.8(9) . . ?
O20 W8 K4A 126.1(9) . 1_565 ?
O20 W8 K4A 125.8(9) 2_556 2_556 ?
O20 W8 K4A 52.5(9) 2_556 1_565 ?
O20 W8 K4A 55.9(9) 2_556 . ?
O20 W8 K4A 52.5(9) . 2_566 ?
O20 W8 K4A 55.9(9) . 2_556 ?
O20 W8 K4B 49.5(9) 2_556 . ?
O20 W8 K4B 131.8(9) . . ?
O20 W8 K4B 49.5(9) . 2_556 ?
O20 W8 K4B 131.8(9) 2_556 2_556 ?
O20 W8 O20 177.3(19) . 2_556 ?
O20 W8 O22 89.5(10) 2_556 . ?
O20 W8 O22 90.8(10) 2_556 2_556 ?
O20 W8 O22 89.5(10) . 2_556 ?
O20 W8 O22 90.8(10) . . ?
O20 W8 O23 91.4(9) 2_556 . ?
O20 W8 O23 91.4(9) . . ?
O22 W8 K4A 137.4(8) 2_556 1_565 ?
O22 W8 K4A 137.4(8) . 2_566 ?
O22 W8 K4A 126.8(9) 2_556 . ?
O22 W8 K4A 44.3(9) 2_556 2_556 ?
O22 W8 K4A 126.8(9) . 2_556 ?
O22 W8 K4A 50.4(8) . 1_565 ?
O22 W8 K4A 44.3(9) . . ?
O22 W8 K4A 50.4(8) 2_556 2_566 ?
O22 W8 K4B 128.6(9) . 2_556 ?
O22 W8 K4B 44.9(9) . . ?
O22 W8 K4B 128.6(9) 2_556 . ?
O22 W8 K4B 44.9(9) 2_556 2_556 ?
O22 W8 O22 166.4(17) . 2_556 ?
O22 W8 O23 83.2(9) 2_556 . ?
O22 W8 O23 83.2(9) . . ?
O23 W8 K4A 114.6(5) . 1_565 ?
O23 W8 K4A 119.5(5) 1_565 2_556 ?
O23 W8 K4A 60.5(5) . 2_556 ?
O23 W8 K4A 119.5(5) 1_565 . ?
O23 W8 K4A 114.6(5) . 2_566 ?
O23 W8 K4A 65.4(5) 1_565 1_565 ?
O23 W8 K4A 60.5(5) . . ?
O23 W8 K4A 65.4(5) 1_565 2_566 ?
O23 W8 K4B 69.1(5) . . ?
O23 W8 K4B 69.1(5) . 2_556 ?
O23 W8 K4B 110.9(5) 1_565 . ?
O23 W8 K4B 110.9(5) 1_565 2_556 ?
O23 W8 O20 88.6(9) 1_565 2_556 ?
O23 W8 O20 88.6(9) 1_565 . ?
O23 W8 O22 96.8(9) 1_565 . ?
O23 W8 O22 96.8(8) 1_565 2_556 ?
O23 W8 O23 180.00(15) 1_565 . ?
W1 K1 W1 129.4(5) 2_545 1_545 ?
W1 K1 W2 102.9(3) 2_545 1_445 ?
W1 K1 W2 102.9(3) 1_545 2_645 ?
W1 K1 W2 52.78(12) 1_545 1_445 ?
W1 K1 W2 52.78(12) 2_545 2_645 ?
W2 K1 W2 127.1(5) 2_645 1_445 ?
K1 K1 W1 115.3(2) 1_565 2_545 ?
K1 K1 W1 115.3(2) 1_565 1_545 ?
K1 K1 W1 64.7(2) 1_545 2_545 ?
K1 K1 W1 64.7(2) 1_545 1_545 ?
K1 K1 W2 116.5(2) 1_565 2_645 ?
K1 K1 W2 63.5(2) 1_545 1_445 ?
K1 K1 W2 116.5(2) 1_565 1_445 ?
K1 K1 W2 63.5(2) 1_545 2_645 ?
K1 K1 K1 180.0 1_565 1_545 ?
K1 K1 O7 90.5(4) 1_545 2_655 ?
K1 K1 O7 89.5(4) 1_565 2_655 ?
K1 K1 O7 89.5(4) 1_565 1_455 ?
K1 K1 O7 90.5(4) 1_545 1_455 ?
K2 K1 W1 64.0(2) 1_455 2_545 ?
K2 K1 W1 115.3(3) 1_455 1_545 ?
K2 K1 W1 115.3(3) . 2_545 ?
K2 K1 W1 64.0(2) . 1_545 ?
K2 K1 W2 62.5(2) . 2_645 ?
K2 K1 W2 116.7(3) . 1_445 ?
K2 K1 W2 62.5(2) 1_455 1_445 ?
K2 K1 W2 116.7(3) 1_455 2_645 ?
K2 K1 K1 89.2(6) 1_455 1_545 ?
K2 K1 K1 90.8(6) . 1_565 ?
K2 K1 K1 89.2(6) . 1_545 ?
K2 K1 K1 90.8(6) 1_455 1_565 ?
K2 K1 K2 178.4(12) . 1_455 ?
K2 K1 O7 118.7(4) . 1_455 ?
K2 K1 O7 61.3(4) . 2_655 ?
K2 K1 O7 118.7(4) 1_455 2_655 ?
K2 K1 O7 61.3(4) 1_455 1_455 ?
O1 K1 W1 24.9(2) 1_545 1_545 ?
O1 K1 W1 154.1(6) 2_545 1_545 ?
O1 K1 W1 24.9(2) 2_545 2_545 ?
O1 K1 W1 154.1(6) 1_545 2_545 ?
O1 K1 W2 64.8(3) 1_545 1_445 ?
O1 K1 W2 114.7(3) 1_545 2_645 ?
O1 K1 W2 114.7(3) 2_545 1_445 ?
O1 K1 W2 64.8(3) 2_545 2_645 ?
O1 K1 K1 90.5(4) 2_545 1_565 ?
O1 K1 K1 89.5(4) 2_545 1_545 ?
O1 K1 K1 90.5(4) 1_545 1_565 ?
O1 K1 K1 89.5(4) 1_545 1_545 ?
O1 K1 K2 121.3(3) 2_545 . ?
O1 K1 K2 121.3(3) 1_545 1_455 ?
O1 K1 K2 58.7(3) 2_545 1_455 ?
O1 K1 K2 58.7(3) 1_545 . ?
O1 K1 O1 179.0(7) 2_545 1_545 ?
O1 K1 O7 120.0(5) 1_545 2_655 ?
O1 K1 O7 60.0(5) 1_545 1_455 ?
O1 K1 O7 60.0(5) 2_545 2_655 ?
O1 K1 O7 120.0(5) 2_545 1_455 ?
O2 K1 W1 159.3(8) . 2_545 ?
O2 K1 W1 68.4(7) . 1_545 ?
O2 K1 W1 24.6(6) 1_545 1_545 ?
O2 K1 W1 24.6(6) 2_545 2_545 ?
O2 K1 W1 106.7(7) 2_545 1_545 ?
O2 K1 W1 106.7(7) 1_545 2_545 ?
O2 K1 W1 159.3(8) 2 1_545 ?
O2 K1 W1 68.4(7) 2 2_545 ?
O2 K1 W2 96.8(6) 2 2_645 ?
O2 K1 W2 96.8(6) . 1_445 ?
O2 K1 W2 60.9(6) 1_545 1_445 ?
O2 K1 W2 118.2(6) . 2_645 ?
O2 K1 W2 80.7(6) 2_545 1_445 ?
O2 K1 W2 80.7(6) 1_545 2_645 ?
O2 K1 W2 118.2(6) 2 1_445 ?
O2 K1 W2 60.9(6) 2_545 2_645 ?
O2 K1 K1 136.6(6) 1_545 1_565 ?
O2 K1 K1 131.5(7) . 1_545 ?
O2 K1 K1 43.4(6) 1_545 1_545 ?
O2 K1 K1 48.5(7) 2 1_565 ?
O2 K1 K1 43.4(6) 2_545 1_545 ?
O2 K1 K1 48.5(7) . 1_565 ?
O2 K1 K1 131.5(7) 2 1_545 ?
O2 K1 K1 136.6(6) 2_545 1_565 ?
O2 K1 K2 60.8(7) 1_545 . ?
O2 K1 K2 60.8(7) 2_545 1_455 ?
O2 K1 K2 59.2(7) 2 1_455 ?
O2 K1 K2 122.0(8) . 1_455 ?
O2 K1 K2 117.9(8) 1_545 1_455 ?
O2 K1 K2 122.0(8) 2 . ?
O2 K1 K2 59.2(7) . . ?
O2 K1 K2 117.9(8) 2_545 . ?
O2 K1 O1 131.6(8) 2_545 1_545 ?
O2 K1 O1 43.6(7) 2 2_545 ?
O2 K1 O1 137.4(9) . 2_545 ?
O2 K1 O1 47.4(6) 1_545 1_545 ?
O2 K1 O1 131.6(8) 1_545 2_545 ?
O2 K1 O1 137.4(9) 2 1_545 ?
O2 K1 O1 47.4(6) 2_545 2_545 ?
O2 K1 O1 43.6(7) . 1_545 ?
O2 K1 O2 174.9(11) . 2_545 ?
O2 K1 O2 174.9(11) 2 1_545 ?
O2 K1 O2 88.1(8) 2 2_545 ?
O2 K1 O2 88.1(8) . 1_545 ?
O2 K1 O2 97.0(15) 2 . ?
O2 K1 O2 86.8(13) 2_545 1_545 ?
O2 K1 O6 61.6(8) . 2_655 ?
O2 K1 O6 59.5(8) 2 2_655 ?
O2 K1 O6 121.6(6) 2_545 2_655 ?
O2 K1 O6 123.6(7) 1_545 2_655 ?
O2 K1 O6 61.6(8) 2 1_455 ?
O2 K1 O6 121.6(6) 1_545 1_455 ?
O2 K1 O6 59.5(8) . 1_455 ?
O2 K1 O6 123.6(7) 2_545 1_455 ?
O2 K1 O7 76.9(7) 2 2_655 ?
O2 K1 O7 102.0(7) 1_545 2_655 ?
O2 K1 O7 76.9(7) . 1_455 ?
O2 K1 O7 102.4(7) . 2_655 ?
O2 K1 O7 102.0(7) 2_545 1_455 ?
O2 K1 O7 78.7(7) 2_545 2_655 ?
O2 K1 O7 78.7(7) 1_545 1_455 ?
O2 K1 O7 102.4(7) 2 1_455 ?
O6 K1 W1 61.8(7) 1_445 1_545 ?
O6 K1 W1 87.5(8) 1_445 2_545 ?
O6 K1 W1 119.9(6) 2_655 1_545 ?
O6 K1 W1 87.5(8) 2_645 1_545 ?
O6 K1 W1 97.8(6) 2_655 2_545 ?
O6 K1 W1 97.8(6) 1_455 1_545 ?
O6 K1 W1 61.8(7) 2_645 2_545 ?
O6 K1 W1 119.9(6) 1_455 2_545 ?
O6 K1 W2 115.2(9) 1_445 2_645 ?
O6 K1 W2 15.6(7) 1_445 1_445 ?
O6 K1 W2 156.2(6) 2_655 1_445 ?
O6 K1 W2 15.6(7) 2_645 2_645 ?
O6 K1 W2 75.3(5) 1_455 1_445 ?
O6 K1 W2 156.2(6) 1_455 2_645 ?
O6 K1 W2 75.3(5) 2_655 2_645 ?
O6 K1 W2 115.2(9) 2_645 1_445 ?
O6 K1 K1 127.1(8) 1_445 1_565 ?
O6 K1 K1 52.9(8) 1_445 1_545 ?
O6 K1 K1 137.8(5) 2_655 1_545 ?
O6 K1 K1 42.2(5) 1_455 1_565 ?
O6 K1 K1 137.8(5) 1_455 1_545 ?
O6 K1 K1 52.9(8) 2_645 1_545 ?
O6 K1 K1 127.1(8) 2_645 1_565 ?
O6 K1 K1 42.2(5) 2_655 1_565 ?
O6 K1 K2 62.9(7) 1_455 1_455 ?
O6 K1 K2 55.8(7) 1_445 1_455 ?
O6 K1 K2 55.8(7) 2_645 . ?
O6 K1 K2 62.9(7) 2_655 . ?
O6 K1 K2 118.5(8) 1_455 . ?
O6 K1 K2 123.0(9) 1_445 . ?
O6 K1 K2 123.0(9) 2_645 1_455 ?
O6 K1 K2 118.5(8) 2_655 1_455 ?
O6 K1 O1 100.2(7) 1_455 2_545 ?
O6 K1 O1 78.0(7) 1_445 1_545 ?
O6 K1 O1 78.0(7) 2_645 2_545 ?
O6 K1 O1 80.6(6) 2_655 2_545 ?
O6 K1 O1 101.4(8) 2_645 1_545 ?
O6 K1 O1 101.4(8) 1_445 2_545 ?
O6 K1 O1 80.6(6) 1_455 1_545 ?
O6 K1 O1 100.2(7) 2_655 1_545 ?
O6 K1 O2 65.1(8) 1_445 2_545 ?
O6 K1 O2 112.4(7) 2_645 2 ?
O6 K1 O2 114.8(8) 2_645 . ?
O6 K1 O2 62.8(8) 2_645 2_545 ?
O6 K1 O2 65.1(8) 2_645 1_545 ?
O6 K1 O2 62.8(8) 1_445 1_545 ?
O6 K1 O2 114.8(8) 1_445 2 ?
O6 K1 O2 112.4(7) 1_445 . ?
O6 K1 O6 169.3(11) 2_645 1_455 ?
O6 K1 O6 84.3(10) 1_455 2_655 ?
O6 K1 O6 85.0(8) 2_645 2_655 ?
O6 K1 O6 105.7(16) 1_445 2_645 ?
O6 K1 O6 169.3(11) 1_445 2_655 ?
O6 K1 O6 85.0(8) 1_445 1_455 ?
O6 K1 O7 40.2(8) 2_645 2_655 ?
O6 K1 O7 140.7(10) 2_645 1_455 ?
O6 K1 O7 140.7(10) 1_445 2_655 ?
O6 K1 O7 129.9(7) 1_455 2_655 ?
O6 K1 O7 40.2(8) 1_445 1_455 ?
O6 K1 O7 49.2(6) 2_655 2_655 ?
O6 K1 O7 49.2(6) 1_455 1_455 ?
O6 K1 O7 129.9(7) 2_655 1_455 ?
O7 K1 W1 61.0(4) 1_455 1_545 ?
O7 K1 W1 61.0(4) 2_655 2_545 ?
O7 K1 W1 119.4(4) 1_455 2_545 ?
O7 K1 W1 119.4(4) 2_655 1_545 ?
O7 K1 W2 27.0(3) 2_655 2_645 ?
O7 K1 W2 154.0(6) 1_455 2_645 ?
O7 K1 W2 27.0(3) 1_455 1_445 ?
O7 K1 W2 154.0(6) 2_655 1_445 ?
O7 K1 O7 179.0(8) 2_655 1_455 ?
K1 K2 K1 178.4(12) . 1_655 ?
K1 K2 K2 90.8(6) 1_655 1_545 ?
K1 K2 K2 90.8(6) . 1_545 ?
K1 K2 K2 89.2(6) 1_655 1_565 ?
K1 K2 K2 89.2(6) . 1_565 ?
K1 K2 O7 62.3(4) 1_655 . ?
K1 K2 O7 117.6(4) 1_655 2_655 ?
K1 K2 O7 62.3(4) . 2_655 ?
K1 K2 O7 117.6(4) . . ?
K2 K2 K2 180.0 1_565 1_545 ?
K2 K2 O7 88.7(4) 1_565 . ?
K2 K2 O7 91.3(4) 1_545 2_655 ?
K2 K2 O7 91.3(4) 1_545 . ?
K2 K2 O7 88.7(4) 1_565 2_655 ?
O1 K2 K1 121.9(3) 1_545 1_655 ?
O1 K2 K1 58.1(3) 2_645 1_655 ?
O1 K2 K1 121.9(3) 2_645 . ?
O1 K2 K1 58.1(3) 1_545 . ?
O1 K2 K2 90.3(5) 2_645 1_545 ?
O1 K2 K2 89.7(5) 2_645 1_565 ?
O1 K2 K2 90.3(5) 1_545 1_545 ?
O1 K2 K2 89.7(5) 1_545 1_565 ?
O1 K2 O1 179.3(10) 2_645 1_545 ?
O1 K2 O4 45.5(6) 1_545 . ?
O1 K2 O4 45.5(6) 2_645 2_655 ?
O1 K2 O4 134.0(9) 2_645 . ?
O1 K2 O4 134.0(9) 1_545 2_655 ?
O1 K2 O6 90.9(6) 1_545 2_655 ?
O1 K2 O6 88.6(5) 2_645 2_655 ?
O1 K2 O6 88.6(5) 1_545 . ?
O1 K2 O6 90.9(6) 2_645 . ?
O1 K2 O7 120.5(5) 2_645 . ?
O1 K2 O7 120.5(5) 1_545 2_655 ?
O1 K2 O7 59.5(5) 2_645 2_655 ?
O1 K2 O7 59.5(5) 1_545 . ?
O2 K2 K1 44.2(6) . . ?
O2 K2 K1 133.6(8) 1_545 1_655 ?
O2 K2 K1 133.6(8) 2_645 . ?
O2 K2 K1 134.6(9) 2_655 . ?
O2 K2 K1 47.8(6) 1_545 . ?
O2 K2 K1 44.2(6) 2_655 1_655 ?
O2 K2 K1 134.6(9) . 1_655 ?
O2 K2 K1 47.8(6) 2_645 1_655 ?
O2 K2 K2 127.0(6) 2_645 1_565 ?
O2 K2 K2 53.0(6) 2_645 1_545 ?
O2 K2 K2 123.6(7) 2_655 1_545 ?
O2 K2 K2 53.0(6) 1_545 1_545 ?
O2 K2 K2 123.6(7) . 1_545 ?
O2 K2 K2 56.4(7) . 1_565 ?
O2 K2 K2 127.0(6) 1_545 1_565 ?
O2 K2 K2 56.4(7) 2_655 1_565 ?
O2 K2 O1 41.6(6) 2_655 2_645 ?
O2 K2 O1 41.6(6) . 1_545 ?
O2 K2 O1 135.9(9) 2_645 1_545 ?
O2 K2 O1 137.9(8) . 2_645 ?
O2 K2 O1 44.7(6) 1_545 1_545 ?
O2 K2 O1 135.9(9) 1_545 2_645 ?
O2 K2 O1 44.7(6) 2_645 2_645 ?
O2 K2 O1 137.9(8) 2_655 1_545 ?
O2 K2 O2 176.7(12) 2_655 1_545 ?
O2 K2 O2 70.6(5) . 1_545 ?
O2 K2 O2 106.1(13) 1_545 2_645 ?
O2 K2 O2 70.6(5) 2_655 2_645 ?
O2 K2 O2 112.8(14) 2_655 . ?
O2 K2 O2 176.7(12) . 2_645 ?
O2 K2 O4 92.4(9) 2_655 . ?
O2 K2 O4 47.1(8) 2_655 2_655 ?
O2 K2 O4 47.8(8) 1_545 1_545 ?
O2 K2 O4 47.1(8) . . ?
O2 K2 O4 84.4(7) 2_655 2_645 ?
O2 K2 O4 92.4(9) . 2_655 ?
O2 K2 O4 93.3(9) 2_645 1_545 ?
O2 K2 O4 131.5(8) . 2_645 ?
O2 K2 O4 84.4(7) . 1_545 ?
O2 K2 O4 90.0(7) 1_545 . ?
O2 K2 O4 133.9(7) 1_545 2_655 ?
O2 K2 O4 133.9(7) 2_645 . ?
O2 K2 O4 90.0(7) 2_645 2_655 ?
O2 K2 O4 131.5(8) 2_655 1_545 ?
O2 K2 O4 47.8(8) 2_645 2_645 ?
O2 K2 O4 93.3(9) 1_545 2_645 ?
O2 K2 O6 84.5(8) 2_655 2_655 ?
O2 K2 O6 51.1(6) 2_655 . ?
O2 K2 O6 130.5(5) 2_645 2_655 ?
O2 K2 O6 97.9(6) 2_645 . ?
O2 K2 O6 97.9(6) 1_545 2_655 ?
O2 K2 O6 130.5(5) 1_545 . ?
O2 K2 O6 51.1(6) . 2_655 ?
O2 K2 O6 84.5(8) . . ?
O2 K2 O7 93.9(6) 2_645 . ?
O2 K2 O7 92.6(6) 2_655 . ?
O2 K2 O7 87.6(6) 1_545 . ?
O2 K2 O7 92.6(6) . 2_655 ?
O2 K2 O7 86.0(6) . . ?
O2 K2 O7 93.9(6) 1_545 2_655 ?
O2 K2 O7 87.6(6) 2_645 2_655 ?
O2 K2 O7 86.0(6) 2_655 2_655 ?
O4 K2 K1 90.0(7) 1_545 . ?
O4 K2 K1 89.1(7) 2_655 1_655 ?
O4 K2 K1 90.8(7) 2_645 . ?
O4 K2 K1 90.0(7) 2_655 . ?
O4 K2 K1 90.0(7) . 1_655 ?
O4 K2 K1 89.1(7) . . ?
O4 K2 K1 90.0(7) 2_645 1_655 ?
O4 K2 K1 90.8(7) 1_545 1_655 ?
O4 K2 K2 120.7(6) 2_645 1_565 ?
O4 K2 K2 59.3(6) 2_645 1_545 ?
O4 K2 K2 125.2(6) 2_655 1_545 ?
O4 K2 K2 120.7(6) 1_545 1_565 ?
O4 K2 K2 59.3(6) 1_545 1_545 ?
O4 K2 K2 54.8(6) 2_655 1_565 ?
O4 K2 K2 54.8(6) . 1_565 ?
O4 K2 K2 125.2(6) . 1_545 ?
O4 K2 O1 43.0(6) 2_645 2_645 ?
O4 K2 O1 43.0(6) 1_545 1_545 ?
O4 K2 O1 137.5(8) 1_545 2_645 ?
O4 K2 O1 137.5(8) 2_645 1_545 ?
O4 K2 O4 118.6(12) 2_645 1_545 ?
O4 K2 O4 175.5(11) 2_645 . ?
O4 K2 O4 175.5(11) 1_545 2_655 ?
O4 K2 O4 65.9(4) 2_645 2_655 ?
O4 K2 O4 65.9(4) 1_545 . ?
O4 K2 O4 109.5(11) 2_655 . ?
O4 K2 O6 88.9(7) 1_545 . ?
O4 K2 O6 133.4(8) 2_645 . ?
O4 K2 O6 88.9(7) 2_645 2_655 ?
O4 K2 O6 133.4(7) 1_545 2_655 ?
O4 K2 O7 41.7(7) 1_545 . ?
O4 K2 O7 135.0(8) 2_655 . ?
O4 K2 O7 135.0(8) . 2_655 ?
O4 K2 O7 42.9(6) . . ?
O4 K2 O7 140.3(8) 2_645 . ?
O4 K2 O7 41.7(7) 2_645 2_655 ?
O4 K2 O7 140.3(8) 1_545 2_655 ?
O4 K2 O7 42.9(6) 2_655 2_655 ?
O6 K2 K1 128.5(9) 2_655 1_655 ?
O6 K2 K1 128.5(9) . . ?
O6 K2 K1 137.3(8) 2_645 1_655 ?
O6 K2 K1 50.2(6) . 1_655 ?
O6 K2 K1 137.3(8) 1_545 . ?
O6 K2 K1 43.8(5) 2_645 . ?
O6 K2 K1 50.1(6) 2_655 . ?
O6 K2 K1 43.8(5) 1_545 1_655 ?
O6 K2 K2 130.8(6) . 1_545 ?
O6 K2 K2 130.8(6) 2_655 1_545 ?
O6 K2 K2 60.7(7) 1_545 1_545 ?
O6 K2 K2 119.3(7) 1_545 1_565 ?
O6 K2 K2 60.7(7) 2_645 1_545 ?
O6 K2 K2 49.2(6) . 1_565 ?
O6 K2 K2 119.3(7) 2_645 1_565 ?
O6 K2 K2 49.2(6) 2_655 1_565 ?
O6 K2 O1 91.5(6) 2_645 1_545 ?
O6 K2 O1 88.8(6) 1_545 1_545 ?
O6 K2 O1 91.5(6) 1_545 2_645 ?
O6 K2 O1 88.8(6) 2_645 2_645 ?
O6 K2 O2 125.3(6) 2_645 2_655 ?
O6 K2 O2 87.9(6) 1_545 2_655 ?
O6 K2 O2 90.0(8) 2_645 2_645 ?
O6 K2 O2 53.9(7) 2_645 1_545 ?
O6 K2 O2 90.0(8) 1_545 1_545 ?
O6 K2 O2 125.3(6) 1_545 . ?
O6 K2 O2 53.9(7) 1_545 2_645 ?
O6 K2 O2 87.9(6) 2_645 . ?
O6 K2 O4 132.0(8) 2_645 . ?
O6 K2 O4 84.0(8) 2_645 2_655 ?
O6 K2 O4 99.1(10) 1_545 2_645 ?
O6 K2 O4 99.1(10) 2_645 1_545 ?
O6 K2 O4 87.6(9) 2_655 . ?
O6 K2 O4 132.0(8) 1_545 2_655 ?
O6 K2 O4 48.9(8) 2_645 2_645 ?
O6 K2 O4 44.5(8) 2_655 2_655 ?
O6 K2 O4 44.5(8) . . ?
O6 K2 O4 48.9(8) 1_545 1_545 ?
O6 K2 O4 84.0(8) 1_545 . ?
O6 K2 O4 87.6(9) . 2_655 ?
O6 K2 O6 168.4(12) 2_645 . ?
O6 K2 O6 121.5(15) 1_545 2_645 ?
O6 K2 O6 98.3(12) 2_655 . ?
O6 K2 O6 70.1(6) 2_645 2_655 ?
O6 K2 O6 70.1(6) 1_545 . ?
O6 K2 O6 168.4(12) 1_545 2_655 ?
O6 K2 O7 130.4(8) 2_655 . ?
O6 K2 O7 130.4(8) . 2_655 ?
O6 K2 O7 140.7(9) 2_645 . ?
O6 K2 O7 47.4(5) . . ?
O6 K2 O7 41.2(7) 2_645 2_655 ?
O6 K2 O7 140.7(9) 1_545 2_655 ?
O6 K2 O7 47.4(5) 2_655 2_655 ?
O6 K2 O7 41.2(7) 1_545 . ?
O7 K2 O7 177.5(9) 2_655 . ?
K3A K3A K3A 179.999(16) 1_565 1_545 ?
K3B K3A K3A 7.6(12) 1_545 1_545 ?
K3B K3A K3A 11.5(19) . 1_565 ?
K3B K3A K3A 168.5(19) . 1_545 ?
K3B K3A K3A 172.4(12) 1_545 1_565 ?
K3B K3A K3B 161(3) . 1_545 ?
K3B K3A O1 92.6(12) 1_545 1_545 ?
K3B K3A O1 96.9(17) . 1_545 ?
K3B K3A O3 128.1(14) 1_545 . ?
K3B K3A O3 52.3(15) . . ?
K3B K3A O3 125.9(18) . 1_545 ?
K3B K3A O3 53.6(11) 1_545 1_545 ?
K3B K3A O5 65.4(18) . . ?
K3B K3A O5 141(2) . 1_545 ?
K3B K3A O5 132.2(18) 1_545 . ?
K3B K3A O5 56.0(12) 1_545 1_545 ?
K3B K3A O7 84.1(17) . 1_455 ?
K3B K3A O7 85.7(12) 1_545 1_455 ?
K3B K3A O8 111(2) . 1_445 ?
K3B K3A O8 52.2(12) 1_545 1_445 ?
K3B K3A O8 40.4(15) . 1_455 ?
K3B K3A O8 122.8(17) 1_545 1_455 ?
K3B K3A O9 103(2) . . ?
K3B K3A O9 95.9(17) 1_545 . ?
K3B K3A O10 50.0(16) . 1_455 ?
K3B K3A O10 116(2) . 1_445 ?
K3B K3A O10 113.8(16) 1_545 1_455 ?
K3B K3A O10 47.2(11) 1_545 1_445 ?
K3B K3A O11 61.5(17) . . ?
K3B K3A O11 64.7(12) 1_545 1_545 ?
K3B K3A O11 133.8(16) 1_545 . ?
K3B K3A O11 130(2) . 1_545 ?
K3B K3A O12B 87.0(19) . 1_455 ?
K3B K3A O12B 83.6(16) 1_545 1_455 ?
K3B K3A O14 121.8(18) . 1_445 ?
K3B K3A O14 56.5(15) . 1_455 ?
K3B K3A O14 56.7(11) 1_545 1_445 ?
K3B K3A O14 122.9(13) 1_545 1_455 ?
O1 K3A K3A 91.2(6) 1_545 1_565 ?
O1 K3A K3A 88.8(6) 1_545 1_545 ?
O3 K3A K3A 51.5(8) . 1_565 ?
O3 K3A K3A 53.2(8) 1_545 1_545 ?
O3 K3A K3A 126.8(8) 1_545 1_565 ?
O3 K3A K3A 128.5(8) . 1_545 ?
O3 K3A O1 45.2(8) 1_545 1_545 ?
O3 K3A O1 48.5(7) . 1_545 ?
O3 K3A O3 75.3(7) 1_545 . ?
O3 K3A O5 51.0(10) 1_545 1_545 ?
O3 K3A O5 100.3(11) . 1_545 ?
O3 K3A O7 47.0(8) 1_545 1_455 ?
O3 K3A O7 48.6(8) . 1_455 ?
O3 K3A O8 47.2(9) . 1_455 ?
O3 K3A O8 51.0(10) 1_545 1_445 ?
O3 K3A O8 95.4(11) 1_545 1_455 ?
O3 K3A O9 96.9(14) . . ?
O3 K3A O9 95.1(14) 1_545 . ?
O3 K3A O10 131.0(15) 1_545 1_455 ?
O3 K3A O10 133.8(15) . 1_445 ?
O3 K3A O10 88.6(13) 1_545 1_445 ?
O3 K3A O10 91.8(13) . 1_455 ?
O3 K3A O11 96.2(14) 1_545 1_545 ?
O3 K3A O11 137.2(16) . 1_545 ?
O3 K3A O11 89.7(13) . . ?
O3 K3A O11 139.0(15) 1_545 . ?
O3 K3A O12B 131.9(17) 1_545 1_455 ?
O3 K3A O12B 135.1(16) . 1_455 ?
O3 K3A O14 173.9(14) . 1_445 ?
O3 K3A O14 175.7(15) 1_545 1_455 ?
O3 K3A O14 107.8(13) . 1_455 ?
O3 K3A O14 110.0(13) 1_545 1_445 ?
O5 K3A K3A 131.1(9) 1_545 1_565 ?
O5 K3A K3A 54.7(9) . 1_565 ?
O5 K3A K3A 125.3(9) . 1_545 ?
O5 K3A K3A 48.9(9) 1_545 1_545 ?
O5 K3A O1 50.2(7) . 1_545 ?
O5 K3A O1 51.9(7) 1_545 1_545 ?
O5 K3A O3 95.2(12) . 1_545 ?
O5 K3A O3 52.5(10) . . ?
O5 K3A O5 76.4(11) . 1_545 ?
O5 K3A O7 97.5(10) . 1_455 ?
O5 K3A O7 96.6(10) 1_545 1_455 ?
O5 K3A O8 91.6(11) . 1_455 ?
O5 K3A O8 141.8(9) 1_545 1_455 ?
O5 K3A O8 137.8(10) . 1_445 ?
O5 K3A O9 48.1(10) 1_545 . ?
O5 K3A O9 46.7(10) . . ?
O5 K3A O10 113.9(14) . 1_455 ?
O5 K3A O10 173.5(12) . 1_445 ?
O5 K3A O10 102.2(13) 1_545 1_445 ?
O5 K3A O10 167.6(13) 1_545 1_455 ?
O5 K3A O11 48.9(9) 1_545 1_545 ?
O5 K3A O11 47.9(9) . . ?
O5 K3A O11 87.8(13) . 1_545 ?
O5 K3A O11 96.5(13) 1_545 . ?
O5 K3A O12B 124.6(14) 1_545 1_455 ?
O5 K3A O12B 132.4(16) . 1_455 ?
O5 K3A O14 85.5(11) 1_545 1_445 ?
O5 K3A O14 130.1(13) 1_545 1_455 ?
O5 K3A O14 89.0(13) . 1_455 ?
O5 K3A O14 128.4(14) . 1_445 ?
O7 K3A K3A 90.2(7) 1_455 1_565 ?
O7 K3A K3A 89.8(7) 1_455 1_545 ?
O7 K3A O1 62.2(7) 1_455 1_545 ?
O7 K3A O8 48.5(8) 1_455 1_455 ?
O7 K3A O9 129.5(11) 1_455 . ?
O7 K3A O10 88.9(11) 1_455 1_445 ?
O7 K3A O11 138.0(13) 1_455 . ?
O7 K3A O12B 118.3(16) 1_455 1_455 ?
O7 K3A O14 132.7(15) 1_455 1_445 ?
O7 K3A O14 132.8(14) 1_455 1_455 ?
O8 K3A K3A 129.6(8) 1_455 1_545 ?
O8 K3A K3A 50.4(8) 1_455 1_565 ?
O8 K3A K3A 58.9(9) 1_445 1_545 ?
O8 K3A K3A 121.1(9) 1_445 1_565 ?
O8 K3A O1 91.4(9) 1_445 1_545 ?
O8 K3A O1 92.6(8) 1_455 1_545 ?
O8 K3A O3 90.5(11) 1_445 . ?
O8 K3A O5 93.9(12) 1_445 1_545 ?
O8 K3A O7 42.1(7) 1_445 1_455 ?
O8 K3A O8 70.8(9) 1_445 1_455 ?
O8 K3A O9 142.0(17) 1_445 . ?
O8 K3A O9 137.7(16) 1_455 . ?
O8 K3A O10 93.3(12) 1_455 1_445 ?
O8 K3A O10 83.0(12) 1_445 1_455 ?
O8 K3A O10 48.3(8) 1_445 1_445 ?
O8 K3A O11 116.8(15) 1_445 1_545 ?
O8 K3A O11 169.4(15) 1_445 . ?
O8 K3A O11 101.9(13) 1_455 . ?
O8 K3A O12B 87.1(14) 1_445 1_455 ?
O8 K3A O14 90.7(12) 1_445 1_445 ?
O8 K3A O14 84.9(11) 1_455 1_455 ?
O8 K3A O14 125.4(14) 1_445 1_455 ?
O9 K3A K3A 91.6(11) . 1_565 ?
O9 K3A K3A 88.4(11) . 1_545 ?
O9 K3A O1 67.3(9) . 1_545 ?
O9 K3A O10 127.9(13) . 1_445 ?
O9 K3A O11 48.4(10) . . ?
O10 K3A K3A 126.4(8) 1_445 1_565 ?
O10 K3A K3A 120.4(9) 1_455 1_545 ?
O10 K3A K3A 53.6(8) 1_445 1_545 ?
O10 K3A K3A 59.6(9) 1_455 1_565 ?
O10 K3A O1 133.7(12) 1_445 1_545 ?
O10 K3A O1 139.9(11) 1_455 1_545 ?
O10 K3A O7 89.1(12) 1_455 1_455 ?
O10 K3A O8 48.1(8) 1_455 1_455 ?
O10 K3A O9 133.6(14) 1_455 . ?
O10 K3A O10 66.8(8) 1_455 1_445 ?
O10 K3A O11 86.4(10) 1_455 . ?
O10 K3A O12B 43.4(11) 1_455 1_455 ?
O10 K3A O14 46.7(9) 1_455 1_455 ?
O10 K3A O14 82.5(10) 1_455 1_445 ?
O11 K3A K3A 58.6(9) 1_545 1_545 ?
O11 K3A K3A 127.9(8) . 1_545 ?
O11 K3A K3A 121.4(9) 1_545 1_565 ?
O11 K3A K3A 52.1(8) . 1_565 ?
O11 K3A O1 96.7(11) . 1_545 ?
O11 K3A O1 95.8(11) 1_545 1_545 ?
O11 K3A O7 143.0(14) 1_545 1_455 ?
O11 K3A O8 168.5(13) 1_545 1_455 ?
O11 K3A O9 41.3(10) 1_545 . ?
O11 K3A O10 86.6(10) 1_545 1_445 ?
O11 K3A O10 122.1(9) 1_545 1_455 ?
O11 K3A O10 126.6(8) . 1_445 ?
O11 K3A O11 69.3(9) 1_545 . ?
O11 K3A O12B 81.7(12) 1_545 1_455 ?
O11 K3A O14 46.6(9) 1_545 1_445 ?
O11 K3A O14 83.6(10) 1_545 1_455 ?
O12B K3A K3A 92.7(11) 1_455 1_565 ?
O12B K3A K3A 87.3(11) 1_455 1_545 ?
O12B K3A O1 176.1(15) 1_455 1_545 ?
O12B K3A O8 90.3(13) 1_455 1_455 ?
O12B K3A O9 112.0(12) 1_455 . ?
O12B K3A O10 43.4(11) 1_455 1_445 ?
O12B K3A O11 85.3(12) 1_455 . ?
O12B K3A O14 43.9(11) 1_455 1_455 ?
O14 K3A K3A 56.4(7) 1_455 1_565 ?
O14 K3A K3A 123.2(8) 1_445 1_565 ?
O14 K3A K3A 56.8(8) 1_445 1_545 ?
O14 K3A K3A 123.6(7) 1_455 1_545 ?
O14 K3A O1 137.4(13) 1_445 1_545 ?
O14 K3A O1 139.1(14) 1_455 1_545 ?
O14 K3A O8 127.9(13) 1_445 1_455 ?
O14 K3A O9 87.5(12) 1_455 . ?
O14 K3A O9 85.8(12) 1_445 . ?
O14 K3A O10 87.2(10) 1_455 1_445 ?
O14 K3A O10 45.2(9) 1_445 1_445 ?
O14 K3A O11 88.0(10) 1_445 . ?
O14 K3A O11 44.8(9) 1_455 . ?
O14 K3A O12B 39.1(11) 1_445 1_455 ?
O14 K3A O14 66.8(6) 1_445 1_455 ?
W1 K3B W3 58.9(4) . . ?
W1 K3B W4A 160.5(11) . 1_455 ?
W1 K3B W4B 167.7(12) . 1_455 ?
W1 K3B W5 115.2(7) . . ?
W1 K3B K3B 98.8(6) . 1_545 ?
W1 K3B K3B 81.2(6) . 1_565 ?
W1 K3B O9 127.0(9) . 1_455 ?
W2 K3B W1 58.1(4) 1_455 . ?
W2 K3B W3 117.0(7) 1_455 . ?
W2 K3B W4A 123.7(8) 1_455 1_455 ?
W2 K3B W4B 126.6(8) 1_455 1_455 ?
W2 K3B W5 167.3(11) 1_455 . ?
W2 K3B K3B 97.5(6) 1_455 1_545 ?
W2 K3B K3B 82.5(6) 1_455 1_565 ?
W2 K3B O7 32.4(4) 1_455 1_455 ?
W2 K3B O9 73.4(7) 1_455 1_455 ?
W2 K3B O12B 129.3(11) 1_455 1_455 ?
W3 K3B W1 121.8(8) 1_455 . ?
W3 K3B W2 63.9(5) 1_455 1_455 ?
W3 K3B W3 175.0(12) 1_455 . ?
W3 K3B W4A 62.3(5) 1_455 1_455 ?
W3 K3B W4B 63.2(5) 1_455 1_455 ?
W3 K3B W5 120.6(8) 1_455 . ?
W3 K3B K3B 92.5(6) 1_455 1_545 ?
W3 K3B K3B 87.5(6) 1_455 1_565 ?
W3 K3B O7 65.1(6) 1_455 1_455 ?
W3 K3B O9 157.4(12) . 1_455 ?
W3 K3B O9 27.0(7) 1_455 1_455 ?
W3 K3B O12B 70.4(10) 1_455 1_455 ?
W4A K3B W3 115.2(7) 1_455 . ?
W4A K3B W5 58.4(4) 1_455 . ?
W4A K3B K3B 100.1(6) 1_455 1_545 ?
W4A K3B K3B 79.9(6) 1_455 1_565 ?
W4A K3B O9 66.4(6) 1_455 1_455 ?
W4B K3B W3 115.0(7) 1_455 . ?
W4B K3B W4A 8.2(3) 1_455 1_455 ?
W4B K3B W5 57.6(4) 1_455 . ?
W4B K3B K3B 88.0(7) 1_455 1_565 ?
W4B K3B K3B 92.0(7) 1_455 1_545 ?
W4B K3B O9 63.1(6) 1_455 1_455 ?
W5 K3B W3 57.4(4) . . ?
W5 K3B O9 116.2(8) . 1_455 ?
K3A K3B W1 77.0(11) 1_565 . ?
K3A K3B W1 92.2(17) . . ?
K3A K3B W2 102.1(17) . 1_455 ?
K3A K3B W2 85.7(11) 1_565 1_455 ?
K3A K3B W3 95.1(14) 1_565 1_455 ?
K3A K3B W3 80.2(13) 1_565 . ?
K3A K3B W3 80.7(19) . . ?
K3A K3B W3 104(2) . 1_455 ?
K3A K3B W4A 105.5(17) . 1_455 ?
K3A K3B W4A 83.7(12) 1_565 1_455 ?
K3A K3B W4B 91.6(13) 1_565 1_455 ?
K3A K3B W4B 97.3(18) . 1_455 ?
K3A K3B W5 88.5(16) . . ?
K3A K3B W5 82.1(11) 1_565 . ?
K3A K3B K3A 161(3) . 1_565 ?
K3A K3B K3B 168.5(19) . 1_565 ?
K3A K3B K3B 7.6(12) 1_565 1_565 ?
K3A K3B K3B 172.4(12) 1_565 1_545 ?
K3A K3B K3B 11.5(19) . 1_545 ?
K3A K3B O3 78.6(14) 1_565 . ?
K3A K3B O3 98.9(19) . . ?
K3A K3B O5 78.6(15) 1_565 . ?
K3A K3B O5 84(2) . . ?
K3A K3B O7 118.1(13) 1_565 1_455 ?
K3A K3B O7 71.0(17) . 1_455 ?
K3A K3B O8 80.2(16) 1_565 1_455 ?
K3A K3B O8 116(2) . 1_455 ?
K3A K3B O9 121.7(15) 1_565 1_455 ?
K3A K3B O9 77(2) . 1_455 ?
K3A K3B O10 103(2) . 1_455 ?
K3A K3B O10 92.3(16) 1_565 1_455 ?
K3A K3B O11 92.3(19) . . ?
K3A K3B O11 71.8(14) 1_565 . ?
K3A K3B O12B 119.7(16) 1_565 1_455 ?
K3A K3B O12B 68.5(18) . 1_455 ?
K3A K3B O14 81.5(13) 1_565 1_455 ?
K3A K3B O14 97.5(17) . 1_455 ?
K3B K3B W3 92.2(6) 1_545 . ?
K3B K3B W3 87.8(6) 1_565 . ?
K3B K3B W5 94.2(6) 1_545 . ?
K3B K3B W5 85.8(5) 1_565 . ?
K3B K3B K3B 180.0(15) 1_565 1_545 ?
K3B K3B O9 114.2(8) 1_565 1_455 ?
K3B K3B O9 65.8(8) 1_545 1_455 ?
O3 K3B W1 26.8(10) . . ?
O3 K3B W2 31.3(10) . 1_455 ?
O3 K3B W3 85.7(12) . . ?
O3 K3B W3 95.0(12) . 1_455 ?
O3 K3B W4A 149.8(14) . 1_455 ?
O3 K3B W4B 155.5(14) . 1_455 ?
O3 K3B W5 140.8(14) . . ?
O3 K3B K3B 79.5(11) . 1_565 ?
O3 K3B K3B 100.5(11) . 1_545 ?
O3 K3B O5 62.2(12) . . ?
O3 K3B O7 48.8(10) . 1_455 ?
O3 K3B O9 102.9(13) . 1_455 ?
O3 K3B O10 129.5(15) . 1_455 ?
O3 K3B O11 113.6(14) . . ?
O3 K3B O12B 156.6(17) . 1_455 ?
O3 K3B O14 158.9(17) . 1_455 ?
O5 K3B W1 35.4(7) . . ?
O5 K3B W2 93.4(9) . 1_455 ?
O5 K3B W3 157.0(12) . 1_455 ?
O5 K3B W3 23.6(6) . . ?
O5 K3B W4A 137.3(11) . 1_455 ?
O5 K3B W4B 138.2(11) . 1_455 ?
O5 K3B W5 80.7(8) . . ?
O5 K3B K3B 94.4(10) . 1_545 ?
O5 K3B K3B 85.6(10) . 1_565 ?
O5 K3B O7 98.2(10) . 1_455 ?
O5 K3B O9 153.7(14) . 1_455 ?
O5 K3B O11 54.5(9) . . ?
O5 K3B O12B 131.9(14) . 1_455 ?
O5 K3B O14 106.9(13) . 1_455 ?
O7 K3B W1 68.8(6) 1_455 . ?
O7 K3B W3 118.5(8) 1_455 . ?
O7 K3B W4A 124.4(9) 1_455 1_455 ?
O7 K3B W4B 121.7(9) 1_455 1_455 ?
O7 K3B W5 159.4(11) 1_455 . ?
O7 K3B K3B 114.8(7) 1_455 1_565 ?
O7 K3B K3B 65.2(7) 1_455 1_545 ?
O7 K3B O9 58.6(7) 1_455 1_455 ?
O7 K3B O12B 107.8(12) 1_455 1_455 ?
O8 K3B W1 90.4(10) 1_455 . ?
O8 K3B W2 34.6(7) 1_455 1_455 ?
O8 K3B W3 32.3(7) 1_455 1_455 ?
O8 K3B W3 146.6(13) 1_455 . ?
O8 K3B W4A 89.1(10) 1_455 1_455 ?
O8 K3B W4B 92.3(10) 1_455 1_455 ?
O8 K3B W5 144.5(13) 1_455 . ?
O8 K3B K3B 106.3(11) 1_455 1_545 ?
O8 K3B K3B 73.7(11) 1_455 1_565 ?
O8 K3B O3 64.0(13) 1_455 . ?
O8 K3B O5 124.9(13) 1_455 . ?
O8 K3B O7 51.2(9) 1_455 1_455 ?
O8 K3B O9 52.2(10) 1_455 1_455 ?
O8 K3B O10 65.4(10) 1_455 1_455 ?
O8 K3B O11 151.6(18) 1_455 . ?
O8 K3B O12B 102.7(13) 1_455 1_455 ?
O8 K3B O14 119.3(14) 1_455 1_455 ?
O10 K3B W1 155.1(12) 1_455 . ?
O10 K3B W2 99.2(9) 1_455 1_455 ?
O10 K3B W3 142.1(11) 1_455 . ?
O10 K3B W3 35.8(6) 1_455 1_455 ?
O10 K3B W4A 27.0(6) 1_455 1_455 ?
O10 K3B W4B 27.5(6) 1_455 1_455 ?
O10 K3B W5 84.8(9) 1_455 . ?
O10 K3B K3B 86.0(11) 1_455 1_565 ?
O10 K3B K3B 94.0(11) 1_455 1_545 ?
O10 K3B O5 163.8(16) 1_455 . ?
O10 K3B O7 97.9(11) 1_455 1_455 ?
O10 K3B O9 41.8(9) 1_455 1_455 ?
O10 K3B O11 110.1(11) 1_455 . ?
O10 K3B O12B 42.7(12) 1_455 1_455 ?
O10 K3B O14 58.0(11) 1_455 1_455 ?
O11 K3B W1 88.1(8) . . ?
O11 K3B W2 143.3(11) . 1_455 ?
O11 K3B W3 144.5(11) . 1_455 ?
O11 K3B W3 32.3(6) . . ?
O11 K3B W4A 83.1(8) . 1_455 ?
O11 K3B W4B 83.8(8) . 1_455 ?
O11 K3B W5 27.2(6) . . ?
O11 K3B K3B 101.9(9) . 1_545 ?
O11 K3B K3B 78.1(9) . 1_565 ?
O11 K3B O7 150.3(12) . 1_455 ?
O11 K3B O9 143.2(11) . 1_455 ?
O11 K3B O12B 87.4(12) . 1_455 ?
O12B K3B W1 160.0(14) 1_455 . ?
O12B K3B W3 110.5(11) 1_455 . ?
O12B K3B W4A 37.1(9) 1_455 1_455 ?
O12B K3B W4B 28.9(10) 1_455 1_455 ?
O12B K3B W5 61.0(9) 1_455 . ?
O12B K3B K3B 63.2(11) 1_455 1_545 ?
O12B K3B K3B 116.8(11) 1_455 1_565 ?
O12B K3B O9 55.9(10) 1_455 1_455 ?
O14 K3B W1 139.6(12) 1_455 . ?
O14 K3B W2 153.1(13) 1_455 1_455 ?
O14 K3B W3 84.1(10) 1_455 . ?
O14 K3B W3 93.7(11) 1_455 1_455 ?
O14 K3B W4A 31.4(8) 1_455 1_455 ?
O14 K3B W4B 31.3(9) 1_455 1_455 ?
O14 K3B W5 27.0(8) 1_455 . ?
O14 K3B K3B 81.8(9) 1_455 1_565 ?
O14 K3B K3B 98.2(9) 1_455 1_545 ?
O14 K3B O7 151.1(13) 1_455 1_455 ?
O14 K3B O9 93.4(11) 1_455 1_455 ?
O14 K3B O11 52.5(11) 1_455 . ?
O14 K3B O12B 44.0(11) 1_455 1_455 ?
K4B K4A K4A 4.9(7) 1_545 1_545 ?
K4B K4A K4A 160(3) . 1_545 ?
K4B K4A K4B 155(4) . 1_545 ?
K4B K4A O12A 73(3) . 2_656 ?
K4B K4A O12A 92.9(11) 1_545 2_656 ?
K4B K4A O13 120(3) . 2_646 ?
K4B K4A O13 126.2(11) 1_545 2_656 ?
K4B K4A O13 53(3) . 2_656 ?
K4B K4A O13 54.3(9) 1_545 2_646 ?
K4B K4A O15 116.2(11) 1_545 2_656 ?
K4B K4A O15 48.6(9) 1_545 2_646 ?
K4B K4A O15 42(3) . 2_656 ?
K4B K4A O15 109(3) . 2_646 ?
K4B K4A O16 91.4(14) 1_545 2_656 ?
K4B K4A O16 98(3) . 2_656 ?
K4B K4A O17 134.5(12) 1_545 2_656 ?
K4B K4A O17 66(3) . 2_656 ?
K4B K4A O17 138(3) . 2_646 ?
K4B K4A O18 149(3) . 2_646 ?
K4B K4A O18 76(3) . 2_656 ?
K4B K4A O18 51.7(10) 1_545 2_646 ?
K4B K4A O19 111(4) . 2_656 ?
K4B K4A O20 103(3) . 2_546 ?
K4B K4A O20 122.7(11) 1_545 2_556 ?
K4B K4A O20 37(3) . 2_556 ?
K4B K4A O20 55.8(10) 1_545 2_546 ?
K4B K4A O21 103(3) . . ?
K4B K4A O21 90.3(14) 1_545 . ?
K4B K4A O22 53.4(9) 1_545 1_545 ?
K4B K4A O22 125.7(12) 1_545 . ?
K4B K4A O22 56(3) . . ?
K4B K4A O22 124(3) . 1_545 ?
K4B K4A O23 90.7(17) 1_545 . ?
K4B K4A O23 77(3) . . ?
O12A K4A K4A 95.7(8) 2_656 1_545 ?
O12A K4A O20 82.8(9) 2_656 2_556 ?
O12A K4A O23 113.9(8) 2_656 . ?
O13 K4A K4A 54.8(8) 2_646 1_545 ?
O13 K4A K4A 127.1(7) 2_656 1_545 ?
O13 K4A O12A 48.1(8) 2_646 2_656 ?
O13 K4A O12A 39.8(9) 2_656 2_656 ?
O13 K4A O13 72.2(7) 2_646 2_656 ?
O13 K4A O15 45.3(9) 2_646 2_646 ?
O13 K4A O15 84.8(10) 2_646 2_656 ?
O13 K4A O15 46.9(9) 2_656 2_656 ?
O13 K4A O15 90.8(9) 2_656 2_646 ?
O13 K4A O16 46.1(12) 2_646 2_656 ?
O13 K4A O16 48.3(12) 2_656 2_656 ?
O13 K4A O17 47.8(10) 2_656 2_656 ?
O13 K4A O17 95.1(10) 2_646 2_656 ?
O13 K4A O18 88.4(11) 2_646 2_646 ?
O13 K4A O18 139.6(12) 2_656 2_646 ?
O13 K4A O20 88.8(12) 2_646 2_546 ?
O13 K4A O20 126.4(11) 2_646 2_556 ?
O13 K4A O20 124.2(11) 2_656 2_546 ?
O13 K4A O20 83.1(10) 2_656 2_556 ?
O13 K4A O22 171.5(12) 2_646 . ?
O13 K4A O22 107.6(13) 2_646 1_545 ?
O13 K4A O23 132.0(16) 2_646 . ?
O13 K4A O23 126.2(15) 2_656 . ?
O15 K4A K4A 53.1(7) 2_646 1_545 ?
O15 K4A K4A 120.6(8) 2_656 1_545 ?
O15 K4A O12A 37.5(7) 2_656 2_656 ?
O15 K4A O12A 51.0(8) 2_646 2_656 ?
O15 K4A O15 67.6(7) 2_656 2_646 ?
O15 K4A O16 89.9(12) 2_656 2_656 ?
O15 K4A O18 167.6(14) 2_656 2_646 ?
O15 K4A O20 45.8(7) 2_656 2_556 ?
O15 K4A O20 89.9(8) 2_646 2_556 ?
O15 K4A O20 80.3(9) 2_656 2_546 ?
O15 K4A O23 87.5(12) 2_646 . ?
O15 K4A O23 83.7(10) 2_656 . ?
O16 K4A K4A 89.4(12) 2_656 1_545 ?
O16 K4A O12A 59.9(10) 2_656 2_656 ?
O16 K4A O15 89.3(11) 2_656 2_646 ?
O16 K4A O20 131.3(14) 2_656 2_556 ?
O16 K4A O23 173.6(13) 2_656 . ?
O17 K4A K4A 56.8(9) 2_646 1_545 ?
O17 K4A K4A 130.7(7) 2_656 1_545 ?
O17 K4A K4B 60.8(11) 2_646 1_545 ?
O17 K4A O12A 85.8(10) 2_656 2_656 ?
O17 K4A O12A 92.7(9) 2_646 2_656 ?
O17 K4A O13 50.9(10) 2_646 2_646 ?
O17 K4A O13 91.2(10) 2_646 2_656 ?
O17 K4A O15 133.5(8) 2_656 2_646 ?
O17 K4A O15 129.2(9) 2_646 2_656 ?
O17 K4A O15 89.9(11) 2_646 2_646 ?
O17 K4A O15 89.3(11) 2_656 2_656 ?
O17 K4A O16 43.0(11) 2_646 2_656 ?
O17 K4A O16 49.3(12) 2_656 2_656 ?
O17 K4A O17 73.9(8) 2_646 2_656 ?
O17 K4A O18 101.6(10) 2_656 2_646 ?
O17 K4A O18 50.5(8) 2_646 2_646 ?
O17 K4A O19 44.3(8) 2_646 2_656 ?
O17 K4A O20 168.5(13) 2_656 2_546 ?
O17 K4A O20 102.3(12) 2_656 2_556 ?
O17 K4A O20 116.6(14) 2_646 2_546 ?
O17 K4A O20 174.3(12) 2_646 2_556 ?
O17 K4A O21 90.9(14) 2_646 . ?
O17 K4A O22 137.5(12) 2_646 . ?
O17 K4A O22 94.9(12) 2_646 1_545 ?
O17 K4A O23 131.1(17) 2_656 . ?
O17 K4A O23 142.5(17) 2_646 . ?
O18 K4A K4A 122.0(10) 2_656 1_545 ?
O18 K4A K4A 47.3(8) 2_646 1_545 ?
O18 K4A K4B 126.2(13) 2_656 1_545 ?
O18 K4A O12A 134.9(15) 2_656 2_656 ?
O18 K4A O12A 136.5(12) 2_646 2_656 ?
O18 K4A O13 95.1(13) 2_656 2_656 ?
O18 K4A O13 136.2(13) 2_656 2_646 ?
O18 K4A O15 117.3(15) 2_656 2_656 ?
O18 K4A O15 100.3(12) 2_646 2_646 ?
O18 K4A O15 174.1(14) 2_656 2_646 ?
O18 K4A O16 92.8(12) 2_646 2_656 ?
O18 K4A O16 93.9(13) 2_656 2_656 ?
O18 K4A O17 51.5(9) 2_656 2_656 ?
O18 K4A O17 89.1(10) 2_656 2_646 ?
O18 K4A O18 74.6(8) 2_656 2_646 ?
O18 K4A O19 44.8(9) 2_656 2_656 ?
O18 K4A O20 129.9(9) 2_656 2_546 ?
O18 K4A O20 91.7(11) 2_656 2_556 ?
O18 K4A O20 135.1(8) 2_646 2_556 ?
O18 K4A O21 43.5(12) 2_656 . ?
O18 K4A O22 90.6(10) 2_656 1_545 ?
O18 K4A O22 51.8(10) 2_656 . ?
O18 K4A O23 89.7(10) 2_656 . ?
O18 K4A O23 93.3(12) 2_646 . ?
O19 K4A K4A 88.2(11) 2_656 1_545 ?
O19 K4A K4B 93.1(14) 2_656 1_545 ?
O19 K4A O12A 122.8(10) 2_656 2_656 ?
O19 K4A O13 95.8(13) 2_656 2_656 ?
O19 K4A O13 93.8(12) 2_656 2_646 ?
O19 K4A O15 133.7(15) 2_656 2_646 ?
O19 K4A O15 141.3(15) 2_656 2_656 ?
O19 K4A O16 63.2(10) 2_656 2_656 ?
O19 K4A O17 52.2(9) 2_656 2_656 ?
O19 K4A O18 49.4(9) 2_656 2_646 ?
O19 K4A O20 136.4(15) 2_656 2_556 ?
O19 K4A O20 138.4(15) 2_656 2_546 ?
O19 K4A O21 59.2(13) 2_656 . ?
O19 K4A O22 92.5(12) 2_656 1_545 ?
O19 K4A O22 94.7(12) 2_656 . ?
O19 K4A O23 122.8(8) 2_656 . ?
O20 K4A K4A 126.9(7) 2_556 1_545 ?
O20 K4A K4A 60.0(8) 2_546 1_545 ?
O20 K4A O12A 88.8(9) 2_546 2_656 ?
O20 K4A O15 46.0(7) 2_546 2_646 ?
O20 K4A O16 134.7(14) 2_546 2_656 ?
O20 K4A O18 89.3(11) 2_546 2_646 ?
O20 K4A O20 66.9(6) 2_546 2_556 ?
O20 K4A O23 43.3(12) 2_546 . ?
O20 K4A O23 43.2(12) 2_556 . ?
O21 K4A K4A 87.6(12) . 1_545 ?
O21 K4A O12A 176.1(16) . 2_656 ?
O21 K4A O13 138.5(17) . 2_656 ?
O21 K4A O13 135.8(16) . 2_646 ?
O21 K4A O15 138.6(14) . 2_656 ?
O21 K4A O15 130.7(16) . 2_646 ?
O21 K4A O16 122.4(15) . 2_656 ?
O21 K4A O17 93.6(14) . 2_656 ?
O21 K4A O18 47.5(11) . 2_646 ?
O21 K4A O20 93.6(12) . 2_556 ?
O21 K4A O20 91.1(13) . 2_546 ?
O21 K4A O22 50.5(11) . . ?
O21 K4A O22 47.1(12) . 1_545 ?
O21 K4A O23 63.7(11) . . ?
O22 K4A K4A 126.0(8) . 1_545 ?
O22 K4A K4A 53.4(7) 1_545 1_545 ?
O22 K4A O12A 125.6(13) . 2_656 ?
O22 K4A O12A 134.0(13) 1_545 2_656 ?
O22 K4A O13 171.7(12) 1_545 2_656 ?
O22 K4A O13 106.4(13) . 2_656 ?
O22 K4A O15 127.1(11) . 2_646 ?
O22 K4A O15 88.3(11) . 2_656 ?
O22 K4A O15 83.7(11) 1_545 2_646 ?
O22 K4A O15 124.8(12) 1_545 2_656 ?
O22 K4A O16 139.0(17) . 2_656 ?
O22 K4A O16 137.5(16) 1_545 2_656 ?
O22 K4A O17 89.7(12) . 2_656 ?
O22 K4A O17 139.7(11) 1_545 2_656 ?
O22 K4A O18 48.0(9) 1_545 2_646 ?
O22 K4A O18 97.5(10) . 2_646 ?
O22 K4A O20 90.7(9) 1_545 2_556 ?
O22 K4A O20 47.7(9) 1_545 2_546 ?
O22 K4A O20 85.2(10) . 2_546 ?
O22 K4A O20 45.5(9) . 2_556 ?
O22 K4A O22 72.5(7) . 1_545 ?
O22 K4A O23 41.9(13) . . ?
O22 K4A O23 47.6(13) 1_545 . ?
O23 K4A K4A 93.1(15) . 1_545 ?
W4B K4B W6 57.9(5) 2_656 2_556 ?
W4B K4B W7 152.5(10) 2_656 . ?
W4B K4B O16 65.6(10) 2_656 2_656 ?
W4B K4B O22 140.3(11) 2_656 1_545 ?
W7 K4B W6 115.1(7) . 2_556 ?
W7 K4B O22 65.0(6) . 1_545 ?
K4A K4B W4B 114(3) . 2_656 ?
K4A K4B W4B 78.5(8) 1_565 2_656 ?
K4A K4B W6 78.7(8) 1_565 2_556 ?
K4A K4B W6 126(3) . 2_556 ?
K4A K4B W7 74.1(8) 1_565 . ?
K4A K4B W7 92(3) . . ?
K4A K4B K4A 155(4) . 1_565 ?
K4A K4B O12A 94(3) . 2_656 ?
K4A K4B O12A 98.8(10) 1_565 2_656 ?
K4A K4B O13 115(3) . 2_656 ?
K4A K4B O13 134.9(11) 1_565 2_646 ?
K4A K4B O13 49(3) . 2_646 ?
K4A K4B O15 127(3) . 2_656 ?
K4A K4B O16 99.7(13) 1_565 2_656 ?
K4A K4B O16 69(3) . 2_656 ?
K4A K4B O17 58.4(10) 1_565 2_656 ?
K4A K4B O17 101(3) . 2_656 ?
K4A K4B O17 34(3) . 2_646 ?
K4A K4B O17 126.9(12) 1_565 2_646 ?
K4A K4B O18 89(3) . 2_656 ?
K4A K4B O19 99.3(11) 1_565 2_656 ?
K4A K4B O19 56(3) . 2_656 ?
K4A K4B O20 134(3) . 2_556 ?
K4A K4B O20 136.1(11) 1_565 2_546 ?
K4A K4B O20 65(3) . 2_546 ?
K4A K4B O21 64(3) . . ?
K4A K4B O21 102.1(14) 1_565 . ?
K4A K4B O22 111(3) . . ?
K4A K4B O22 135.1(11) 1_565 1_545 ?
K4A K4B O22 46(3) . 1_545 ?
K4A K4B O23 100.6(17) 1_565 . ?
K4A K4B O23 91(3) . . ?
O12A K4B W4B 20.5(6) 2_656 2_656 ?
O12A K4B W6 64.3(7) 2_656 2_556 ?
O12A K4B W7 172.7(11) 2_656 . ?
O12A K4B O13 46.2(8) 2_656 2_646 ?
O12A K4B O16 59.3(10) 2_656 2_656 ?
O12A K4B O17 85.2(9) 2_656 2_646 ?
O12A K4B O20 87.1(10) 2_656 2_546 ?
O12A K4B O22 122.4(11) 2_656 1_545 ?
O12A K4B O23 120.0(12) 2_656 . ?
O13 K4B W4B 65.0(7) 2_646 2_656 ?
O13 K4B W4B 30.3(9) 2_656 2_656 ?
O13 K4B W6 83.1(11) 2_656 2_556 ?
O13 K4B W6 101.4(10) 2_646 2_556 ?
O13 K4B W7 130.5(13) 2_656 . ?
O13 K4B W7 138.5(10) 2_646 . ?
O13 K4B K4A 64.8(10) 2_656 1_565 ?
O13 K4B O12A 42.6(10) 2_656 2_656 ?
O13 K4B O13 70.4(8) 2_656 2_646 ?
O13 K4B O16 48.1(12) 2_656 2_656 ?
O13 K4B O16 42.0(11) 2_646 2_656 ?
O13 K4B O17 86.7(11) 2_656 2_646 ?
O13 K4B O17 53.1(11) 2_656 2_656 ?
O13 K4B O19 96.4(12) 2_656 2_656 ?
O13 K4B O20 101.8(13) 2_656 2_556 ?
O13 K4B O20 129.2(13) 2_656 2_546 ?
O13 K4B O21 146.1(18) 2_656 . ?
O13 K4B O22 89.4(9) 2_646 1_545 ?
O13 K4B O22 159.9(13) 2_656 1_545 ?
O13 K4B O23 147.4(15) 2_656 . ?
O15 K4B W4B 29.4(6) 2_656 2_656 ?
O15 K4B W6 28.6(6) 2_656 2_556 ?
O15 K4B W7 136.5(12) 2_656 . ?
O15 K4B K4A 74.4(10) 2_656 1_565 ?
O15 K4B O12A 40.3(9) 2_656 2_656 ?
O15 K4B O13 84.8(11) 2_656 2_646 ?
O15 K4B O13 55.3(11) 2_656 2_656 ?
O15 K4B O16 94.9(12) 2_656 2_656 ?
O15 K4B O17 105.1(11) 2_656 2_656 ?
O15 K4B O17 125.5(11) 2_656 2_646 ?
O15 K4B O18 143.5(16) 2_656 2_656 ?
O15 K4B O19 151.3(12) 2_656 2_656 ?
O15 K4B O20 55.5(9) 2_656 2_556 ?
O15 K4B O20 83.5(11) 2_656 2_546 ?
O15 K4B O21 155.1(16) 2_656 . ?
O15 K4B O22 125.6(13) 2_656 1_545 ?
O15 K4B O22 107.8(14) 2_656 . ?
O15 K4B O23 93.4(11) 2_656 . ?
O16 K4B W6 122.6(11) 2_656 2_556 ?
O16 K4B W7 119.4(12) 2_656 . ?
O16 K4B O22 115.5(14) 2_656 1_545 ?
O17 K4B W4B 99.2(8) 2_646 2_656 ?
O17 K4B W4B 83.4(8) 2_656 2_656 ?
O17 K4B W6 127.5(10) 2_656 2_556 ?
O17 K4B W6 144.2(10) 2_646 2_556 ?
O17 K4B W7 97.5(8) 2_646 . ?
O17 K4B W7 82.6(8) 2_656 . ?
O17 K4B O12A 92.1(10) 2_656 2_656 ?
O17 K4B O13 90.7(10) 2_656 2_646 ?
O17 K4B O13 43.0(8) 2_646 2_646 ?
O17 K4B O16 38.7(11) 2_646 2_656 ?
O17 K4B O16 48.7(11) 2_656 2_656 ?
O17 K4B O17 68.6(8) 2_656 2_646 ?
O17 K4B O19 51.1(8) 2_656 2_656 ?
O17 K4B O20 165.4(13) 2_656 2_546 ?
O17 K4B O21 93.1(14) 2_656 . ?
O17 K4B O22 77.5(9) 2_646 1_545 ?
O17 K4B O22 129.1(12) 2_656 1_545 ?
O17 K4B O23 145.2(14) 2_656 . ?
O18 K4B W4B 136.3(12) 2_656 2_656 ?
O18 K4B W6 136.7(12) 2_656 2_556 ?
O18 K4B W7 29.0(6) 2_656 . ?
O18 K4B K4A 69.1(12) 2_656 1_565 ?
O18 K4B O12A 146.8(14) 2_656 2_656 ?
O18 K4B O13 106.9(14) 2_656 2_656 ?
O18 K4B O13 121.7(13) 2_656 2_646 ?
O18 K4B O16 91.4(13) 2_656 2_656 ?
O18 K4B O17 79.1(10) 2_656 2_646 ?
O18 K4B O17 54.9(9) 2_656 2_656 ?
O18 K4B O19 41.5(9) 2_656 2_656 ?
O18 K4B O20 107.1(12) 2_656 2_556 ?
O18 K4B O20 123.5(11) 2_656 2_546 ?
O18 K4B O21 41.3(12) 2_656 . ?
O18 K4B O22 56.6(11) 2_656 . ?
O18 K4B O22 82.6(11) 2_656 1_545 ?
O18 K4B O23 93.0(10) 2_656 . ?
O19 K4B W4B 122.2(9) 2_656 2_656 ?
O19 K4B W6 177.9(12) 2_656 2_556 ?
O19 K4B W7 63.8(6) 2_656 . ?
O19 K4B O12A 116.6(10) 2_656 2_656 ?
O19 K4B O13 80.3(10) 2_656 2_646 ?
O19 K4B O16 57.9(11) 2_656 2_656 ?
O19 K4B O17 37.7(7) 2_656 2_646 ?
O19 K4B O20 116.8(11) 2_656 2_546 ?
O19 K4B O22 78.9(10) 2_656 1_545 ?
O19 K4B O23 115.3(9) 2_656 . ?
O20 K4B W4B 84.1(8) 2_556 2_656 ?
O20 K4B W4B 100.1(9) 2_546 2_656 ?
O20 K4B W6 64.9(7) 2_546 2_556 ?
O20 K4B W6 30.8(6) 2_556 2_556 ?
O20 K4B W7 84.4(8) 2_556 . ?
O20 K4B W7 99.3(8) 2_546 . ?
O20 K4B K4A 65.9(9) 2_556 1_565 ?
O20 K4B O12A 94.5(11) 2_556 2_656 ?
O20 K4B O13 78.2(10) 2_546 2_646 ?
O20 K4B O13 130.8(13) 2_556 2_646 ?
O20 K4B O16 119.8(14) 2_546 2_656 ?
O20 K4B O16 149.0(14) 2_556 2_656 ?
O20 K4B O17 124.2(13) 2_556 2_656 ?
O20 K4B O17 167.1(13) 2_556 2_646 ?
O20 K4B O17 96.8(10) 2_546 2_646 ?
O20 K4B O19 147.9(11) 2_556 2_656 ?
O20 K4B O20 70.3(8) 2_556 2_546 ?
O20 K4B O21 100.2(13) 2_556 . ?
O20 K4B O22 42.6(8) 2_546 1_545 ?
O20 K4B O22 91.9(10) 2_556 1_545 ?
O20 K4B O23 42.8(12) 2_546 . ?
O20 K4B O23 46.7(13) 2_556 . ?
O21 K4B W4B 175.4(15) . 2_656 ?
O21 K4B W6 126.7(13) . 2_556 ?
O21 K4B W7 28.5(9) . . ?
O21 K4B O12A 157.9(14) . 2_656 ?
O21 K4B O13 112.3(13) . 2_646 ?
O21 K4B O16 109.9(16) . 2_656 ?
O21 K4B O17 76.8(12) . 2_646 ?
O21 K4B O19 53.2(11) . 2_656 ?
O21 K4B O20 82.6(13) . 2_546 ?
O21 K4B O22 41.4(11) . 1_545 ?
O21 K4B O23 62.6(12) . . ?
O22 K4B W4B 132.7(12) . 2_656 ?
O22 K4B W6 102.3(10) 1_545 2_556 ?
O22 K4B W6 84.5(11) . 2_556 ?
O22 K4B W7 30.6(9) . . ?
O22 K4B K4A 65.9(10) . 1_565 ?
O22 K4B O12A 147.9(14) . 2_656 ?
O22 K4B O13 130.6(14) . 2_656 ?
O22 K4B O13 158.9(13) . 2_646 ?
O22 K4B O16 147.5(16) . 2_656 ?
O22 K4B O17 101.8(13) . 2_656 ?
O22 K4B O17 126.7(12) . 2_646 ?
O22 K4B O19 94.3(11) . 2_656 ?
O22 K4B O20 86.3(11) . 2_546 ?
O22 K4B O20 53.8(11) . 2_556 ?
O22 K4B O21 50.8(12) . . ?
O22 K4B O22 69.5(7) . 1_545 ?
O22 K4B O23 43.8(13) . . ?
O23 K4B W4B 121.8(9) . 2_656 ?
O23 K4B W6 64.9(7) . 2_556 ?
O23 K4B W7 64.1(6) . . ?
O23 K4B O13 120.5(16) . 2_646 ?
O23 K4B O16 159(2) . 2_656 ?
O23 K4B O17 123.0(15) . 2_646 ?
O23 K4B O22 45.5(13) . 1_545 ?
W1 O1 W1 168.4(11) . 1_565 ?
W1 O1 K1 91.9(6) 1_565 1_565 ?
W1 O1 K1 93.6(7) . 1_565 ?
W1 O1 K2 95.4(7) 1_565 1_565 ?
W1 O1 K2 96.2(8) . 1_565 ?
W1 O1 K3A 83.7(8) 1_565 1_565 ?
W1 O1 K3A 84.7(9) . 1_565 ?
K1 O1 K2 63.2(3) 1_565 1_565 ?
K1 O1 K3A 120.9(8) 1_565 1_565 ?
K2 O1 K3A 175.9(9) 1_565 1_565 ?
W1 O2 K1 114.2(14) . 1_565 ?
W1 O2 K1 139.1(15) . . ?
W1 O2 K2 98.2(11) . 1_565 ?
W1 O2 K2 113.6(12) . . ?
K1 O2 K1 88.1(8) . 1_565 ?
K1 O2 K2 121.9(10) . 1_565 ?
K1 O2 K2 121.8(9) 1_565 . ?
K1 O2 K2 76.6(8) . . ?
K1 O2 K2 71.5(7) 1_565 1_565 ?
K2 O2 K2 70.6(5) . 1_565 ?
W1 O3 W2 138.6(12) . 1_455 ?
W1 O3 K3A 106.1(15) . . ?
W1 O3 K3A 102.4(15) . 1_565 ?
W1 O3 K3B 115.3(16) . . ?
W2 O3 K3A 108.0(15) 1_455 . ?
W2 O3 K3A 108.3(15) 1_455 1_565 ?
W2 O3 K3B 105.9(16) 1_455 . ?
K3A O3 K3A 75.3(7) 1_565 . ?
K3B O3 K3A 28.7(11) . . ?
K3B O3 K3A 47.8(11) . 1_565 ?
W1 O4 K2 97.2(11) . . ?
W1 O4 K2 94.2(10) . 1_565 ?
W2 O4 W1 168.3(14) . . ?
W2 O4 K2 93.8(10) . . ?
W2 O4 K2 94.1(11) . 1_565 ?
K2 O4 K2 65.9(4) 1_565 . ?
W1 O5 K3A 91.7(10) . 1_565 ?
W1 O5 K3A 104.3(11) . . ?
W1 O5 K3B 98.8(11) . . ?
W3 O5 W1 141.9(14) . . ?
W3 O5 K3A 110.4(13) . . ?
W3 O5 K3A 111.1(13) . 1_565 ?
W3 O5 K3B 119.1(13) . . ?
K3A O5 K3A 76.4(11) . 1_565 ?
K3B O5 K3A 31.1(12) . . ?
K3B O5 K3A 45.5(12) . 1_565 ?
W2 O6 K1 118.1(14) . 1_655 ?
W2 O6 K1 140.4(17) . 1_665 ?
W2 O6 K2 110.8(13) . 1_565 ?
W2 O6 K2 98.8(11) . . ?
K1 O6 K1 85.0(8) 1_665 1_655 ?
K1 O6 K2 80.4(8) 1_665 1_565 ?
K1 O6 K2 67.0(7) 1_655 . ?
K1 O6 K2 120.4(10) 1_665 . ?
K2 O6 K1 118.0(10) 1_565 1_655 ?
K2 O6 K2 70.1(6) 1_565 . ?
W2 O7 W2 161.4(14) 1_545 . ?
W2 O7 K1 80.5(8) 1_545 1_655 ?
W2 O7 K1 82.2(7) . 1_655 ?
W2 O7 K2 83.9(8) . . ?
W2 O7 K2 80.8(9) 1_545 . ?
W2 O7 K3A 97.5(10) 1_545 1_655 ?
W2 O7 K3A 96.5(11) . 1_655 ?
W2 O7 K3B 131.8(11) . 1_645 ?
W2 O7 K3B 122.4(12) 1_545 1_655 ?
W2 O7 K3B 72.5(9) . 1_655 ?
W2 O7 K3B 63.1(8) 1_545 1_645 ?
K1 O7 K3B 115.0(7) 1_655 1_645 ?
K2 O7 K1 56.4(3) . 1_655 ?
K2 O7 K3B 143.8(8) . 1_645 ?
K3A O7 K1 116.9(10) 1_655 1_655 ?
K3A O7 K2 173.2(11) 1_655 . ?
K3A O7 K3B 24.9(9) 1_655 1_655 ?
K3A O7 K3B 35.3(8) 1_655 1_645 ?
K3B O7 K1 118.5(8) 1_655 1_655 ?
K3B O7 K2 156.4(9) 1_655 . ?
K3B O7 K3B 59.6(6) 1_655 1_645 ?
W2 O8 K3A 103.3(11) . 1_665 ?
W2 O8 K3A 94.8(10) . 1_655 ?
W2 O8 K3B 104.3(10) . 1_665 ?
W2 O8 K3B 102.5(12) . 1_655 ?
W3 O8 W2 139.1(15) . . ?
W3 O8 K3A 117.4(12) . 1_665 ?
W3 O8 K3A 95.2(12) . 1_655 ?
W3 O8 K3B 102.3(13) . 1_655 ?
W3 O8 K3B 114.8(12) . 1_665 ?
K3A O8 K3A 70.8(9) 1_665 1_655 ?
K3A O8 K3B 92.1(10) 1_655 1_665 ?
K3A O8 K3B 21.4(9) 1_665 1_665 ?
K3B O8 K3A 47.5(12) 1_655 1_665 ?
K3B O8 K3A 23.5(11) 1_655 1_655 ?
K3B O8 K3B 68.7(9) 1_655 1_665 ?
W3 O9 W3 162.9(19) . 1_545 ?
W3 O9 K3A 92.0(19) . . ?
W3 O9 K3A 87.2(16) 1_545 1_655 ?
W3 O9 K3A 94.6(17) 1_545 . ?
W3 O9 K3A 83.6(17) . 1_655 ?
W3 O9 K3B 115.9(16) 1_545 . ?
W3 O9 K3B 61.1(13) . 1_655 ?
W3 O9 K3B 70.9(14) . . ?
W3 O9 K3B 109.7(16) 1_545 1_655 ?
K3A O9 K3A 169.7(12) . 1_655 ?
K3A O9 K3B 22.7(9) 1_655 1_655 ?
K3A O9 K3B 154.0(15) 1_655 . ?
K3A O9 K3B 152.5(16) . 1_655 ?
K3A O9 K3B 21.4(9) . . ?
K3B O9 K3B 131.9(14) 1_655 . ?
W3 O10 K3A 96.9(10) . 1_665 ?
W3 O10 K3A 96.3(11) . 1_655 ?
W3 O10 K3B 94.4(11) . 1_655 ?
W4A O10 W3 149.7(15) . . ?
W4A O10 W4B 16.6(6) . . ?
W4A O10 K3A 113.9(12) . 1_655 ?
W4A O10 K3A 96.0(12) . 1_665 ?
W4A O10 K3B 113.0(13) . 1_655 ?
W4B O10 W3 153.2(15) . . ?
W4B O10 K3A 105.2(12) . 1_655 ?
W4B O10 K3A 106.0(13) . 1_665 ?
W4B O10 K3B 112.0(13) . 1_655 ?
K3A O10 K3A 66.8(8) 1_655 1_665 ?
K3B O10 K3A 40.5(11) 1_655 1_665 ?
K3B O10 K3A 26.6(11) 1_655 1_655 ?
W3 O11 K3A 86.5(11) . . ?
W3 O11 K3A 102.0(12) . 1_565 ?
W3 O11 K3B 96.4(11) . . ?
W5 O11 W3 145.1(17) . . ?
W5 O11 K3A 112.0(13) . 1_565 ?
W5 O11 K3A 98.0(12) . . ?
W5 O11 K3B 102.7(12) . . ?
K3A O11 K3A 69.3(9) 1_565 . ?
K3B O11 K3A 26.2(10) . . ?
K3B O11 K3A 43.5(11) . 1_565 ?
W4A O12A W4A 169.3(18) . 1_545 ?
W4A O12A K3A 89.4(12) . 1_655 ?
W4A O12A K3A 80.0(11) 1_545 1_655 ?
W4A O12A K3B 101.5(12) 1_545 1_655 ?
W4A O12A K3B 67.9(10) . 1_655 ?
W4A O12A K4A 89.3(12) 1_545 2_656 ?
W4A O12A K4A 101.3(14) . 2_656 ?
W4A O12A K4B 101.3(11) 1_545 2_656 ?
W4A O12A K4B 89.3(12) . 2_656 ?
W4B O12A W4A 169(2) . 1_545 ?
W4B O12A W4A 2.7(7) . . ?
W4B O12A K3A 88.9(15) . 1_655 ?
W4B O12A K3B 67.6(14) . 1_655 ?
W4B O12A K4A 101.8(17) . 2_656 ?
W4B O12A K4B 89.7(16) . 2_656 ?
K3B O12A K3A 21.9(8) 1_655 1_655 ?
K4A O12A K3A 169.2(14) 2_656 1_655 ?
K4A O12A K3B 168.1(13) 2_656 1_655 ?
K4B O12A K3A 177.5(11) 2_656 1_655 ?
K4B O12A K3B 157.1(12) 2_656 1_655 ?
K4B O12A K4A 12.5(7) 2_656 2_656 ?
O12B O12A W4A 46(5) . 1_545 ?
O12B O12A W4A 124(5) . . ?
O12B O12A W4B 123(5) . . ?
O12B O12A K3A 38(4) . 1_655 ?
O12B O12A K3B 59(5) . 1_655 ?
O12B O12A K4A 132(5) . 2_656 ?
O12B O12A K4B 142(5) . 2_656 ?
W4A O12B W4A 151(3) 1_545 . ?
W4A O12B W4B 147(3) 1_545 . ?
W4A O12B W4B 4.8(7) 1_545 1_545 ?
W4A O12B K3A 108(2) 1_545 1_655 ?
W4A O12B K3A 97.3(18) . 1_655 ?
W4A O12B K3B 71.9(19) 1_545 1_645 ?
W4A O12B K3B 72.8(15) . 1_655 ?
W4A O12B K3B 132(2) . 1_645 ?
W4A O12B K3B 131(3) 1_545 1_655 ?
W4A O12B K4B 67.2(13) . 2_656 ?
W4A O12B K4B 87(2) 1_545 2_656 ?
W4B O12B W4A 4.2(5) . . ?
W4B O12B W4A 155(3) 1_545 . ?
W4B O12B W4B 151(3) . 1_545 ?
W4B O12B K3A 101(2) . 1_655 ?
W4B O12B K3A 105(2) 1_545 1_655 ?
W4B O12B K3B 69.3(15) 1_545 1_645 ?
W4B O12B K3B 136(2) . 1_645 ?
W4B O12B K3B 77.0(18) . 1_655 ?
W4B O12B K3B 129(2) 1_545 1_655 ?
W4B O12B K4B 63.1(15) . 2_656 ?
W4B O12B K4B 89.5(17) 1_545 2_656 ?
K3A O12B K3B 36.0(10) 1_655 1_645 ?
K3A O12B K3B 24.5(9) 1_655 1_655 ?
K3A O12B K4B 164.3(19) 1_655 2_656 ?
K3B O12B K3B 59.8(9) 1_655 1_645 ?
K3B O12B K4B 157.9(18) 1_645 2_656 ?
K3B O12B K4B 139.8(18) 1_655 2_656 ?
O12A O12B W4A 112(6) . 1_545 ?
O12A O12B W4A 39(4) . . ?
O12A O12B W4B 116(5) . 1_545 ?
O12A O12B W4B 36(4) . . ?
O12A O12B K3A 134(5) . 1_655 ?
O12A O12B K3B 110(5) . 1_655 ?
O12A O12B K3B 158(5) . 1_645 ?
O12A O12B K4B 31(4) . 2_656 ?
W4A O13 W4B 16.5(7) . . ?
W4A O13 W5 143.3(13) . . ?
W4A O13 K4A 105.6(14) . 2_666 ?
W4A O13 K4A 112.7(15) . 2_656 ?
W4A O13 K4B 98.3(13) . 2_666 ?
W4A O13 K4B 109.0(16) . 2_656 ?
W4B O13 W5 142.3(14) . . ?
W4B O13 K4A 100.5(14) . 2_656 ?
W4B O13 K4A 113.5(15) . 2_666 ?
W4B O13 K4B 108.4(15) . 2_666 ?
W4B O13 K4B 99.5(15) . 2_656 ?
W5 O13 K4A 103.5(14) . 2_666 ?
W5 O13 K4A 97.1(13) . 2_656 ?
W5 O13 K4B 104.5(14) . 2_656 ?
W5 O13 K4B 106.8(13) . 2_666 ?
K4A O13 K4A 72.2(7) 2_666 2_656 ?
K4A O13 K4B 10.7(7) 2_666 2_666 ?
K4A O13 K4B 82.1(8) 2_656 2_666 ?
K4B O13 K4A 61.0(9) 2_656 2_666 ?
K4B O13 K4A 12.5(8) 2_656 2_656 ?
K4B O13 K4B 70.4(8) 2_656 2_666 ?
W4A O14 K3A 97.4(13) . 1_665 ?
W4A O14 K3A 105.2(14) . 1_655 ?
W4A O14 K3B 98.4(13) . 1_655 ?
W4B O14 W4A 15.6(6) . . ?
W4B O14 K3A 107.8(15) . 1_665 ?
W4B O14 K3A 98.3(14) . 1_655 ?
W4B O14 K3B 98.3(13) . 1_655 ?
W5 O14 W4A 154.2(13) 1_655 . ?
W5 O14 W4B 149.5(14) 1_655 . ?
W5 O14 K3A 97.7(13) 1_655 1_655 ?
W5 O14 K3A 102.3(14) 1_655 1_665 ?
W5 O14 K3B 107.3(14) 1_655 1_655 ?
K3A O14 K3A 66.8(6) 1_665 1_655 ?
K3B O14 K3A 26.0(10) 1_655 1_655 ?
K3B O14 K3A 41.8(10) 1_655 1_665 ?
W4A O15 K4A 90.9(10) . 2_666 ?
W4A O15 K4A 107.4(11) . 2_656 ?
W4A O15 K4B 88.9(10) . 2_666 ?
W4A O15 K4B 108.2(12) . 2_656 ?
W4B O15 W4A 15.5(7) . . ?
W4B O15 W6 147.6(14) . 1_655 ?
W4B O15 K4A 100.1(12) . 2_656 ?
W4B O15 K4A 100.8(12) . 2_666 ?
W4B O15 K4B 100.9(13) . 2_666 ?
W4B O15 K4B 103.6(12) . 2_656 ?
W6 O15 W4A 143.7(14) 1_655 . ?
W6 O15 K4A 103.4(11) 1_655 2_666 ?
W6 O15 K4A 108.9(11) 1_655 2_656 ?
W6 O15 K4B 98.8(11) 1_655 2_666 ?
W6 O15 K4B 107.6(12) 1_655 2_656 ?
K4A O15 K4A 67.6(6) 2_656 2_666 ?
K4A O15 K4B 78.5(9) 2_656 2_666 ?
K4A O15 K4B 11.0(7) 2_666 2_666 ?
K4B O15 K4A 56.9(9) 2_656 2_666 ?
K4B O15 K4A 10.9(9) 2_656 2_656 ?
K4B O15 K4B 67.8(8) 2_656 2_666 ?
W5 O16 W5 173(3) . 1_545 ?
W5 O16 K3A 85.9(19) . . ?
W5 O16 K3A 87.4(19) 1_545 . ?
W5 O16 K4A 93(2) . 2_656 ?
W5 O16 K4A 94(2) 1_545 2_656 ?
W5 O16 K4B 105(2) 1_545 2_656 ?
W5 O16 K4B 81.3(19) . 2_656 ?
K4A O16 K3A 178.7(18) 2_656 . ?
K4A O16 K4B 12.1(7) 2_656 2_656 ?
K4B O16 K3A 166.6(17) 2_656 . ?
W5 O17 K4A 95.9(11) . 2_656 ?
W5 O17 K4A 110.7(11) . 2_666 ?
W5 O17 K4B 108.0(11) . 2_666 ?
W5 O17 K4B 97.5(11) . 2_656 ?
W6 O17 W5 143.0(15) . . ?
W6 O17 K4A 106.3(11) . 2_666 ?
W6 O17 K4A 91.5(11) . 2_656 ?
W6 O17 K4B 97.9(12) . 2_656 ?
W6 O17 K4B 109.0(11) . 2_666 ?
K4A O17 K4A 73.9(8) 2_666 2_656 ?
K4A O17 K4B 8.3(8) 2_666 2_666 ?
K4A O17 K4B 60.8(10) 2_666 2_656 ?
K4A O17 K4B 81.8(9) 2_656 2_666 ?
K4B O17 K4A 13.4(7) 2_656 2_656 ?
K4B O17 K4B 68.6(8) 2_656 2_666 ?
W6 O18 K4A 103.9(12) . 2_656 ?
W6 O18 K4A 93.0(12) . 2_666 ?
W6 O18 K4B 93.4(12) . 2_666 ?
W6 O18 K4B 105.7(12) . 2_656 ?
W7 O18 W6 150.6(15) . . ?
W7 O18 K4A 101.0(12) . 2_666 ?
W7 O18 K4A 104.8(12) . 2_656 ?
W7 O18 K4B 98.0(12) . 2_666 ?
W7 O18 K4B 103.7(12) . 2_656 ?
K4A O18 K4A 74.6(8) 2_656 2_666 ?
K4A O18 K4B 5.7(7) 2_666 2_666 ?
K4A O18 K4B 80.1(10) 2_656 2_666 ?
K4B O18 K4A 15.6(9) 2_656 2_656 ?
K4B O18 K4A 59.3(10) 2_656 2_666 ?
K4B O18 K4B 64.7(8) 2_656 2_666 ?
W6 O19 W6 156.9(12) . 1_545 ?
W6 O19 K4A 102.7(14) 1_545 2_656 ?
W6 O19 K4A 99.3(15) . 2_656 ?
W6 O19 K4B 67.2(7) . 2_556 ?
W6 O19 K4B 90.6(9) 1_545 2_556 ?
W6 O19 K4B 115.1(10) 1_545 2_656 ?
W6 O19 K4B 86.9(11) . 2_656 ?
K4A O19 K4B 12.4(9) 2_656 2_656 ?
K4A O19 K4B 166.5(16) 2_656 2_556 ?
K4B O19 K4B 154.1(13) 2_656 2_556 ?
W6 O20 K4A 97.6(10) . 2_556 ?
W6 O20 K4A 110.5(10) . 2_566 ?
W6 O20 K4B 97.9(11) . 2_556 ?
W6 O20 K4B 107.9(11) . 2_566 ?
W8 O20 W6 148.2(14) . . ?
W8 O20 K4A 101.0(10) . 2_566 ?
W8 O20 K4A 98.7(10) . 2_556 ?
W8 O20 K4B 101.9(11) . 2_566 ?
W8 O20 K4B 102.4(11) . 2_556 ?
K4A O20 K4A 66.9(6) 2_566 2_556 ?
K4A O20 K4B 12.3(7) 2_566 2_566 ?
K4B O20 K4A 79.1(9) 2_566 2_556 ?
K4B O20 K4A 58.3(9) 2_556 2_566 ?
K4B O20 K4A 9.1(8) 2_556 2_556 ?
K4B O20 K4B 70.3(8) 2_556 2_566 ?
W7 O21 W7 152(3) . 1_545 ?
W7 O21 K4A 79.7(17) 1_545 2_656 ?
W7 O21 K4A 102(2) . . ?
W7 O21 K4A 73.4(19) . 2_656 ?
W7 O21 K4A 104(2) 1_545 . ?
W7 O21 K4B 89(2) . . ?
W7 O21 K4B 117(2) 1_545 . ?
W7 O21 K4B 90.0(18) 1_545 2_656 ?
W7 O21 K4B 63.6(18) . 2_656 ?
K4A O21 K4A 173.7(19) . 2_656 ?
K4A O21 K4B 13.3(9) . . ?
K4A O21 K4B 10.6(6) 2_656 2_656 ?
K4A O21 K4B 165.6(18) . 2_656 ?
K4B O21 K4A 161.0(18) . 2_656 ?
K4B O21 K4B 152.4(18) . 2_656 ?
O21 O21 W7 74.7(19) 2_656 . ?
O21 O21 W7 77.4(16) 2_656 1_545 ?
O21 O21 K4A 160(8) 2_656 . ?
O21 O21 K4A 15(6) 2_656 2_656 ?
O21 O21 K4B 22(5) 2_656 2_656 ?
O21 O21 K4B 152(6) 2_656 . ?
W7 O22 K4A 93.0(12) . . ?
W7 O22 K4A 103.5(13) . 1_565 ?
W7 O22 K4B 100.9(14) . . ?
W7 O22 K4B 107.5(13) . 1_565 ?
W8 O22 W7 148.7(12) . . ?
W8 O22 K4A 111.1(14) . . ?
W8 O22 K4A 102.6(13) . 1_565 ?
W8 O22 K4B 95.8(12) . 1_565 ?
W8 O22 K4B 106.9(15) . . ?
K4A O22 K4A 72.5(7) . 1_565 ?
K4A O22 K4B 81.8(8) . 1_565 ?
K4A O22 K4B 10.1(7) 1_565 1_565 ?
K4B O22 K4A 13.1(8) . . ?
K4B O22 K4A 60.6(9) . 1_565 ?
K4B O22 K4B 69.5(7) . 1_565 ?
W8 O23 W8 180.00(3) 1_545 . ?
W8 O23 K4A 93.1(15) . . ?
W8 O23 K4A 86.9(15) 1_545 2_556 ?
W8 O23 K4A 93.1(15) . 2_556 ?
W8 O23 K4A 86.9(15) 1_545 . ?
W8 O23 K4B 81.6(15) . . ?
W8 O23 K4B 81.6(15) . 2_556 ?
W8 O23 K4B 98.4(15) 1_545 . ?
W8 O23 K4B 98.4(15) 1_545 2_556 ?
K4A O23 K4A 174(3) 2_556 . ?
K4B O23 K4A 174(2) 2_556 . ?
K4B O23 K4A 174(2) . 2_556 ?
K4B O23 K4A 12.1(7) . . ?
K4B O23 K4A 12.1(7) 2_556 2_556 ?
K4B O23 K4B 163(3) 2_556 . ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.27544
2 0.24568
3 0.22563
4 0.25325
_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Cs4W11O35
_database_code_depnum_ccdc_archive 'CCDC 2211343'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_Cs4W11O35           
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form


_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs4 O35 W11'
_chemical_formula_weight         3113.99

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           3
_space_group_name_H-M_alt        'P 2'
_space_group_name_Hall           'P 2y'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'

_cell_length_a                   7.3357(5)
_cell_length_b                   3.8684(3)
_cell_length_c                   26.4516(18)
_cell_angle_alpha                90
_cell_angle_beta                 97.962(3)
_cell_angle_gamma                90
_cell_volume                     743.39(9)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    9105
_cell_measurement_theta_min      2.33
_cell_measurement_theta_max      33.22

_exptl_crystal_description       plate
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    6.956
_exptl_crystal_F_000             1314
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.010
_exptl_absorpt_coefficient_mu    47.304
_shelx_estimated_absorpt_T_min   0.201
_shelx_estimated_absorpt_T_max   0.649
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.4572
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1024 before and 0.0599 after correction. The Ratio of minimum to maximum transmission is 0.6125. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_diffrn_reflns_number            21365
_diffrn_reflns_av_unetI/netI     0.0547
_diffrn_reflns_av_R_equivalents  0.0625
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_l_min       -40
_diffrn_reflns_limit_l_max       40
_diffrn_reflns_theta_min         2.332
_diffrn_reflns_theta_max         33.223
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             5683
_reflns_number_gt                5319
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.777
_reflns_Friedel_fraction_max     1.000
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0738P)²+9.7065P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_chemical_absolute_configuration ?
_refine_ls_number_reflns         5683
_refine_ls_number_parameters     169
_refine_ls_number_restraints     3
_refine_ls_R_factor_all          0.0550
_refine_ls_R_factor_gt           0.0513
_refine_ls_wR_factor_ref         0.1289
_refine_ls_wR_factor_gt          0.1260
_refine_ls_goodness_of_fit_ref   1.044
_refine_ls_restrained_S_all      1.057
_refine_ls_shift/su_max          8.881
_refine_ls_shift/su_mean         0.422

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.000000 0.4866(16) 0.000000 0.0348(8) Uani 1 2 d S T P . .
W2 W 0.3137(5) 0.4670(9) 0.12146(7) 0.0231(8) Uani 1 1 d . . . . .
W3A W 0.8116(7) 0.4181(19) 0.12194(8) 0.0112(8) Uani 0.70(2) 1 d . . P . .
W3B W 0.8022(14) 0.560(4) 0.11944(17) 0.0065(18) Uani 0.30(2) 1 d D . P . .
W4A W 0.6219(4) 0.422(6) 0.24750(9) 0.0041(19) Uani 0.54(6) 1 d D . P . .
W4B W 0.6211(6) 0.542(8) 0.24668(18) 0.007(2) Uani 0.46(6) 1 d . . P . .
W5 W 0.9426(3) 0.5497(9) 0.37214(6) 0.0068(3) Uani 1 1 d . . . . .
W6 W 0.4293(3) 0.4319(10) 0.37105(5) 0.0099(3) Uani 1 1 d . . . . .
Cs1 Cs 0.500000 0.000000 0.000000 0.0109(7) Uani 0.816(6) 2 d S T P . .
Cs2 Cs 0.1168(6) -0.0242(19) 0.24685(7) 0.0251(7) Uani 0.943(3) 1 d . . P . .
Cs3 Cs 0.7315(17) 0.0058(17) 0.48963(12) 0.0587(17) Uani 0.648(3) 1 d . . P . .
O1 O 0.000000 0.05(3) 0.000000 0.059(10) Uiso 1 2 d S . P . .
O2 O 0.155(4) 0.483(5) -0.0502(11) 0.014(5) Uiso 1 1 d . . . . .
O3 O 0.211(5) 0.479(6) 0.0513(13) 0.022(7) Uiso 1 1 d . . . . .
O4 O 0.411(4) 0.485(5) 0.1875(13) 0.017(6) Uiso 1 1 d . . . . .
O5 O 0.545(6) 0.482(6) 0.0988(5) 0.016(3) Uiso 1 1 d . . . . .
O6 O 0.070(7) 0.473(7) 0.1382(5) 0.020(3) Uiso 1 1 d . . . . .
O7 O 0.320(4) -0.030(6) 0.1244(7) 0.008(3) Uiso 1 1 d . . . . .
O8 O 0.813(4) 0.003(6) 0.1113(11) 0.026(6) Uiso 1 1 d D . . . .
O9 O 0.771(4) 0.476(5) 0.1869(12) 0.015(6) Uiso 1 1 d . . . . .
O10 O 0.599(4) 0.007(9) 0.2394(6) 0.016(5) Uiso 1 1 d D . . . .
O11 O 0.829(3) 0.483(4) 0.2899(10) 0.007(4) Uiso 1 1 d . . . . .
O12 O 0.455(5) 0.481(6) 0.2897(14) 0.028(8) Uiso 1 1 d . . . . .
O13 O 1.021(5) 0.543(9) 0.4343(13) 0.038(7) Uiso 1 1 d . . . . .
O14 O 0.937(3) 0.020(4) 0.3676(6) 0.003(3) Uiso 1 1 d . . . . .
O15 O 0.691(6) 0.480(7) 0.3776(4) 0.014(3) Uiso 1 1 d . . . . .
O16 O 1.170(6) 0.486(5) 0.3453(5) 0.013(3) Uiso 1 1 d . . . . .
O17 O 0.415(3) 0.468(5) 0.4364(8) 0.009(4) Uiso 1 1 d . . . . .
O18 O 0.428(4) -0.006(5) 0.3554(9) 0.024(5) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.69(10) . ?
W1 O2 1.86(3) 2 ?
W1 O2 1.86(3) . ?
W1 O3 1.91(3) 2 ?
W1 O3 1.91(3) . ?
W1 O1 2.18(10) 1_565 ?
W1 Cs1 4.123(3) 1_455 ?
W1 Cs1 4.123(3) . ?
W1 Cs1 4.171(3) 1_565 ?
W1 Cs1 4.171(3) 1_465 ?
W2 O4 1.79(3) . ?
W2 O5 1.88(4) . ?
W2 O6 1.90(5) . ?
W2 O3 1.90(3) . ?
W2 O7 1.93(2) . ?
W2 O7 1.95(2) 1_565 ?
W2 Cs1 4.083(3) . ?
W2 Cs1 4.202(3) 1_565 ?
W2 Cs2 4.245(5) . ?
W2 Cs2 4.276(5) 1_565 ?
W3A W3B 0.556(11) . ?
W3A O8 1.63(2) . ?
W3A O9 1.80(3) . ?
W3A O6 1.90(5) 1_655 ?
W3A O2 1.96(3) 2_655 ?
W3A O5 1.98(4) . ?
W3A O8 2.28(2) 1_565 ?
W3A Cs1 4.025(3) . ?
W3A Cs2 4.100(6) 1_655 ?
W3A Cs2 4.305(5) 1_665 ?
W3A Cs1 4.319(6) 1_565 ?
W3B O8 1.73(3) 1_565 ?
W3B O9 1.86(3) . ?
W3B O5 1.91(4) . ?
W3B O2 1.92(3) 2_655 ?
W3B O6 1.99(5) 1_655 ?
W3B O8 2.17(3) . ?
W3B Cs1 3.982(10) 1_565 ?
W3B Cs2 4.137(8) 1_665 ?
W3B Cs1 4.201(9) . ?
W3B Cs2 4.431(11) 1_655 ?
W4A W4B 0.465(9) . ?
W4A O10 1.63(4) . ?
W4A O11 1.78(2) . ?
W4A O12 1.78(4) . ?
W4A O4 2.07(3) . ?
W4A O9 2.07(3) . ?
W4A O10 2.28(4) 1_565 ?
W4A Cs2 4.022(13) 1_655 ?
W4A Cs2 4.086(11) . ?
W4A Cs2 4.217(13) 1_665 ?
W4A Cs2 4.278(14) 1_565 ?
W4B O11 1.79(2) . ?
W4B O12 1.79(4) . ?
W4B O10 1.81(4) 1_565 ?
W4B O4 2.05(3) . ?
W4B O10 2.08(4) . ?
W4B O9 2.07(3) . ?
W4B Cs2 4.004(15) 1_665 ?
W4B Cs2 4.063(15) 1_565 ?
W4B Cs2 4.244(18) 1_655 ?
W4B Cs2 4.300(18) . ?
W5 O13 1.67(3) . ?
W5 O14 1.822(17) 1_565 ?
W5 O15 1.89(4) . ?
W5 O16 1.92(4) . ?
W5 O14 2.054(17) . ?
W5 O11 2.23(3) . ?
W5 Cs3 4.062(7) 1_565 ?
W5 Cs2 4.063(4) 1_665 ?
W5 Cs3 4.221(8) . ?
W5 Cs2 4.326(5) 1_655 ?
W5 Cs3 4.447(6) 2_766 ?
W5 Cs3 4.592(7) 2_756 ?
W6 O17 1.75(2) . ?
W6 O18 1.75(2) . ?
W6 O15 1.91(4) . ?
W6 O16 1.94(4) 1_455 ?
W6 O12 2.19(4) . ?
W6 O18 2.21(2) 1_565 ?
W6 Cs3 3.943(6) . ?
W6 Cs2 4.132(4) . ?
W6 Cs3 4.214(7) 1_565 ?
W6 Cs2 4.288(5) 1_565 ?
W6 Cs3 4.347(6) 2_656 ?
W6 Cs3 4.594(7) 2_666 ?
Cs1 O5 3.192(17) . ?
Cs1 O5 3.192(17) 2_655 ?
Cs1 O3 3.25(3) . ?
Cs1 O3 3.25(3) 2_655 ?
Cs1 O2 3.28(3) 2_655 ?
Cs1 O2 3.28(3) . ?
Cs1 O5 3.274(17) 2_645 ?
Cs1 O5 3.274(17) 1_545 ?
Cs1 O3 3.35(3) 1_545 ?
Cs1 O3 3.35(3) 2_645 ?
Cs1 O2 3.36(3) 1_545 ?
Cs1 O2 3.36(3) 2_645 ?
Cs1 O8 3.47(3) . ?
Cs1 O8 3.47(3) 2_655 ?
Cs1 O1 3.673(5) . ?
Cs1 O1 3.673(5) 1_655 ?
Cs1 O7 3.714(19) 2_655 ?
Cs1 O7 3.714(19) . ?
Cs1 Cs1 3.8684(3) 1_565 ?
Cs1 Cs1 3.8684(3) 1_545 ?
Cs2 O11 3.17(2) 1_445 ?
Cs2 O11 3.20(2) 1_455 ?
Cs2 O16 3.200(16) 1_445 ?
Cs2 O12 3.22(3) 1_545 ?
Cs2 O12 3.24(3) . ?
Cs2 O16 3.248(17) 1_455 ?
Cs2 O6 3.435(19) . ?
Cs2 O9 3.40(3) 1_455 ?
Cs2 O9 3.40(3) 1_445 ?
Cs2 O18 3.41(2) . ?
Cs2 O4 3.42(3) 1_545 ?
Cs2 O4 3.46(3) . ?
Cs2 O6 3.45(2) 1_545 ?
Cs2 O10 3.58(3) . ?
Cs2 O14 3.624(18) 1_455 ?
Cs2 O7 3.75(2) . ?
Cs2 O10 3.77(3) 1_455 ?
Cs2 Cs2 3.8684(3) 1_545 ?
Cs2 Cs2 3.8684(3) 1_565 ?
Cs2 O8 3.95(3) 1_455 ?
Cs3 O17 2.96(2) 2_656 ?
Cs3 O13 3.09(4) 2_746 ?
Cs3 O17 3.11(2) . ?
Cs3 O17 3.14(2) 2_646 ?
Cs3 O13 3.26(3) 2_756 ?
Cs3 O13 3.27(4) 1_545 ?
Cs3 O17 3.29(2) 1_545 ?
Cs3 O13 3.44(4) . ?
Cs3 O15 3.462(17) . ?
Cs3 Cs3 3.51(2) 2_656 ?
Cs3 O15 3.571(18) 1_545 ?
Cs3 O14 3.748(18) . ?
Cs3 Cs3 3.8684(3) 1_565 ?
Cs3 Cs3 3.8684(3) 1_545 ?
Cs3 Cs3 3.90(2) 2_756 ?
Cs3 O18 3.92(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 89.5(6) . 2 ?
O1 W1 O2 89.5(6) . . ?
O2 W1 O2 179.1(13) 2 . ?
O1 W1 O3 89.1(7) . 2 ?
O2 W1 O3 89.6(6) 2 2 ?
O2 W1 O3 90.4(6) . 2 ?
O1 W1 O3 89.1(7) . . ?
O2 W1 O3 90.4(6) 2 . ?
O2 W1 O3 89.6(6) . . ?
O3 W1 O3 178.3(15) 2 . ?
O1 W1 O1 180.000(13) . 1_565 ?
O2 W1 O1 90.5(6) 2 1_565 ?
O2 W1 O1 90.5(6) . 1_565 ?
O3 W1 O1 90.9(7) 2 1_565 ?
O3 W1 O1 90.9(7) . 1_565 ?
O1 W1 Cs1 62.83(8) . 1_455 ?
O2 W1 Cs1 50.7(8) 2 1_455 ?
O2 W1 Cs1 128.7(8) . 1_455 ?
O3 W1 Cs1 50.2(9) 2 1_455 ?
O3 W1 Cs1 128.7(9) . 1_455 ?
O1 W1 Cs1 117.17(8) 1_565 1_455 ?
O1 W1 Cs1 62.83(8) . . ?
O2 W1 Cs1 128.7(8) 2 . ?
O2 W1 Cs1 50.7(8) . . ?
O3 W1 Cs1 128.7(9) 2 . ?
O3 W1 Cs1 50.2(9) . . ?
O1 W1 Cs1 117.17(8) 1_565 . ?
Cs1 W1 Cs1 125.66(15) 1_455 . ?
O1 W1 Cs1 118.43(8) . 1_565 ?
O2 W1 Cs1 128.8(8) 2 1_565 ?
O2 W1 Cs1 51.8(8) . 1_565 ?
O3 W1 Cs1 129.2(9) 2 1_565 ?
O3 W1 Cs1 51.8(9) . 1_565 ?
O1 W1 Cs1 61.57(8) 1_565 1_565 ?
Cs1 W1 Cs1 178.74(15) 1_455 1_565 ?
Cs1 W1 Cs1 55.602(5) . 1_565 ?
O1 W1 Cs1 118.43(8) . 1_465 ?
O2 W1 Cs1 51.8(8) 2 1_465 ?
O2 W1 Cs1 128.8(8) . 1_465 ?
O3 W1 Cs1 51.8(9) 2 1_465 ?
O3 W1 Cs1 129.2(9) . 1_465 ?
O1 W1 Cs1 61.57(8) 1_565 1_465 ?
Cs1 W1 Cs1 55.602(5) 1_455 1_465 ?
Cs1 W1 Cs1 178.74(15) . 1_465 ?
Cs1 W1 Cs1 123.14(15) 1_565 1_465 ?
O4 W2 O5 93.0(12) . . ?
O4 W2 O6 91.9(12) . . ?
O5 W2 O6 174.4(9) . . ?
O4 W2 O3 176.4(11) . . ?
O5 W2 O3 86.7(12) . . ?
O6 W2 O3 88.3(12) . . ?
O4 W2 O7 89.7(9) . . ?
O5 W2 O7 91.5(10) . . ?
O6 W2 O7 91.2(11) . . ?
O3 W2 O7 93.9(9) . . ?
O4 W2 O7 85.3(8) . 1_565 ?
O5 W2 O7 87.9(10) . 1_565 ?
O6 W2 O7 89.7(11) . 1_565 ?
O3 W2 O7 91.0(9) . 1_565 ?
O7 W2 O7 175.0(11) . 1_565 ?
O4 W2 Cs1 130.6(9) . . ?
O5 W2 Cs1 49.3(6) . . ?
O6 W2 Cs1 128.2(7) . . ?
O3 W2 Cs1 51.3(9) . . ?
O7 W2 Cs1 65.2(6) . . ?
O7 W2 Cs1 117.7(6) 1_565 . ?
O4 W2 Cs1 126.6(9) . 1_565 ?
O5 W2 Cs1 48.5(6) . 1_565 ?
O6 W2 Cs1 126.0(6) . 1_565 ?
O3 W2 Cs1 50.9(9) . 1_565 ?
O7 W2 Cs1 120.8(6) . 1_565 ?
O7 W2 Cs1 62.1(6) 1_565 1_565 ?
Cs1 W2 Cs1 55.64(3) . 1_565 ?
O4 W2 Cs2 52.4(9) . . ?
O5 W2 Cs2 133.1(6) . . ?
O6 W2 Cs2 52.4(6) . . ?
O3 W2 Cs2 129.9(10) . . ?
O7 W2 Cs2 62.0(6) . . ?
O7 W2 Cs2 115.1(6) 1_565 . ?
Cs1 W2 Cs2 127.15(11) . . ?
Cs1 W2 Cs2 177.17(11) 1_565 . ?
O4 W2 Cs2 50.2(9) . 1_565 ?
O5 W2 Cs2 130.5(6) . 1_565 ?
O6 W2 Cs2 51.9(7) . 1_565 ?
O3 W2 Cs2 127.9(9) . 1_565 ?
O7 W2 Cs2 115.9(6) . 1_565 ?
O7 W2 Cs2 61.2(6) 1_565 1_565 ?
Cs1 W2 Cs2 178.79(11) . 1_565 ?
Cs1 W2 Cs2 123.21(11) 1_565 1_565 ?
Cs2 W2 Cs2 53.99(5) . 1_565 ?
W3B W3A O8 162.8(11) . . ?
W3B W3A O9 87.6(9) . . ?
O8 W3A O9 107.1(12) . . ?
W3B W3A O6 91.2(16) . 1_655 ?
O8 W3A O6 96.8(14) . 1_655 ?
O9 W3A O6 93.4(11) . 1_655 ?
W3B W3A O2 77.9(8) . 2_655 ?
O8 W3A O2 87.3(12) . 2_655 ?
O9 W3A O2 165.4(10) . 2_655 ?
O6 W3A O2 87.1(11) 1_655 2_655 ?
W3B W3A O5 74.8(15) . . ?
O8 W3A O5 95.8(13) . . ?
O9 W3A O5 89.7(11) . . ?
O6 W3A O5 165.5(12) 1_655 . ?
O2 W3A O5 86.4(10) 2_655 . ?
W3B W3A O8 7.5(16) . 1_565 ?
O8 W3A O8 162.8(17) . 1_565 ?
O9 W3A O8 90.0(10) . 1_565 ?
O6 W3A O8 83.9(12) 1_655 1_565 ?
O2 W3A O8 75.6(9) 2_655 1_565 ?
O5 W3A O8 81.9(10) . 1_565 ?
W3B W3A Cs1 104.7(8) . . ?
O8 W3A Cs1 58.9(10) . . ?
O9 W3A Cs1 131.8(9) . . ?
O6 W3A Cs1 131.8(7) 1_655 . ?
O2 W3A Cs1 53.9(8) 2_655 . ?
O5 W3A Cs1 51.4(5) . . ?
O8 W3A Cs1 108.2(7) 1_565 . ?
W3B W3A Cs2 123.6(8) . 1_655 ?
O8 W3A Cs2 73.3(10) . 1_655 ?
O9 W3A Cs2 54.9(9) . 1_655 ?
O6 W3A Cs2 56.4(6) 1_655 1_655 ?
O2 W3A Cs2 134.8(8) 2_655 1_655 ?
O5 W3A Cs2 134.9(6) . 1_655 ?
O8 W3A Cs2 120.1(7) 1_565 1_655 ?
Cs1 W3A Cs2 131.6(2) . 1_655 ?
W3B W3A Cs2 68.9(8) . 1_665 ?
O8 W3A Cs2 127.6(10) . 1_665 ?
O9 W3A Cs2 48.8(9) . 1_665 ?
O6 W3A Cs2 51.1(7) 1_655 1_665 ?
O2 W3A Cs2 123.8(8) 2_655 1_665 ?
O5 W3A Cs2 124.0(6) . 1_665 ?
O8 W3A Cs2 65.6(7) 1_565 1_665 ?
Cs1 W3A Cs2 173.5(2) . 1_665 ?
Cs2 W3A Cs2 54.74(5) 1_655 1_665 ?
W3B W3A Cs1 49.6(8) . 1_565 ?
O8 W3A Cs1 113.6(10) . 1_565 ?
O9 W3A Cs1 120.6(8) . 1_565 ?
O6 W3A Cs1 121.3(7) 1_655 1_565 ?
O2 W3A Cs1 48.4(8) 2_655 1_565 ?
O5 W3A Cs1 46.1(6) . 1_565 ?
O8 W3A Cs1 53.3(7) 1_565 1_565 ?
Cs1 W3A Cs1 55.10(5) . 1_565 ?
Cs2 W3A Cs1 173.14(18) 1_655 1_565 ?
Cs2 W3A Cs1 118.50(18) 1_665 1_565 ?
W3A W3B O8 170(2) . 1_565 ?
W3A W3B O9 75.1(10) . . ?
O8 W3B O9 107.9(12) 1_565 . ?
W3A W3B O5 88.9(16) . . ?
O8 W3B O5 100.5(14) 1_565 . ?
O9 W3B O5 90.0(12) . . ?
W3A W3B O2 85.8(10) . 2_655 ?
O8 W3B O2 91.0(12) 1_565 2_655 ?
O9 W3B O2 160.8(13) . 2_655 ?
O5 W3B O2 89.4(11) . 2_655 ?
W3A W3B O6 72.6(15) . 1_655 ?
O8 W3B O6 97.8(15) 1_565 1_655 ?
O9 W3B O6 88.7(12) . 1_655 ?
O5 W3B O6 161.2(15) . 1_655 ?
O2 W3B O6 85.7(11) 2_655 1_655 ?
W3A W3B O8 12.8(9) . . ?
O8 W3B O8 165.6(18) 1_565 . ?
O9 W3B O8 86.1(11) . . ?
O5 W3B O8 82.2(12) . . ?
O2 W3B O8 74.8(10) 2_655 . ?
O6 W3B O8 78.9(13) 1_655 . ?
W3A W3B Cs1 124.3(9) . 1_565 ?
O8 W3B Cs1 60.5(10) 1_565 1_565 ?
O9 W3B Cs1 135.1(10) . 1_565 ?
O5 W3B Cs1 54.7(6) . 1_565 ?
O2 W3B Cs1 57.2(8) 2_655 1_565 ?
O6 W3B Cs1 133.9(7) 1_655 1_565 ?
O8 W3B Cs1 111.7(8) . 1_565 ?
W3A W3B Cs2 103.9(8) . 1_665 ?
O8 W3B Cs2 71.7(10) 1_565 1_665 ?
O9 W3B Cs2 54.1(9) . 1_665 ?
O5 W3B Cs2 135.2(7) . 1_665 ?
O2 W3B Cs2 133.5(10) 2_655 1_665 ?
O6 W3B Cs2 56.0(6) 1_655 1_665 ?
O8 W3B Cs2 116.3(9) . 1_665 ?
Cs1 W3B Cs2 131.8(4) 1_565 1_665 ?
W3A W3B Cs1 68.0(8) . . ?
O8 W3B Cs1 116.5(10) 1_565 . ?
O9 W3B Cs1 120.7(10) . . ?
O5 W3B Cs1 46.2(7) . . ?
O2 W3B Cs1 49.0(8) 2_655 . ?
O6 W3B Cs1 120.1(8) 1_655 . ?
O8 W3B Cs1 55.7(8) . . ?
Cs1 W3B Cs1 56.35(8) 1_565 . ?
Cs2 W3B Cs1 171.8(4) 1_665 . ?
W3A W3B Cs2 50.4(7) . 1_655 ?
O8 W3B Cs2 124.8(10) 1_565 1_655 ?
O9 W3B Cs2 45.6(9) . 1_655 ?
O5 W3B Cs2 121.7(7) . 1_655 ?
O2 W3B Cs2 120.5(9) 2_655 1_655 ?
O6 W3B Cs2 48.0(7) 1_655 1_655 ?
O8 W3B Cs2 63.0(8) . 1_655 ?
Cs1 W3B Cs2 174.6(4) 1_565 1_655 ?
Cs2 W3B Cs2 53.54(9) 1_665 1_655 ?
Cs1 W3B Cs2 118.3(4) . 1_655 ?
W4B W4A O10 168.6(10) . . ?
W4B W4A O11 84.3(12) . . ?
O10 W4A O11 106.1(13) . . ?
W4B W4A O12 84.0(15) . . ?
O10 W4A O12 98.2(14) . . ?
O11 W4A O12 100.8(8) . . ?
W4B W4A O4 81.0(9) . . ?
O10 W4A O4 87.9(11) . . ?
O11 W4A O4 162.0(14) . . ?
O12 W4A O4 87.8(14) . . ?
W4B W4A O9 82.5(8) . . ?
O10 W4A O9 93.0(12) . . ?
O11 W4A O9 88.7(11) . . ?
O12 W4A O9 162.6(16) . . ?
O4 W4A O9 79.3(5) . . ?
W4B W4A O10 4.1(9) . 1_565 ?
O10 W4A O10 164.8(13) . 1_565 ?
O11 W4A O10 88.3(11) . 1_565 ?
O12 W4A O10 83.3(13) . 1_565 ?
O4 W4A O10 77.0(10) . 1_565 ?
O9 W4A O10 82.4(10) . 1_565 ?
W4B W4A Cs2 115.7(6) . 1_655 ?
O10 W4A Cs2 69.6(11) . 1_655 ?
O11 W4A Cs2 50.6(8) . 1_655 ?
O12 W4A Cs2 139.1(11) . 1_655 ?
O4 W4A Cs2 128.7(9) . 1_655 ?
O9 W4A Cs2 57.7(8) . 1_655 ?
O10 W4A Cs2 118.7(8) 1_565 1_655 ?
W4B W4A Cs2 114.6(8) . . ?
O10 W4A Cs2 60.4(10) . . ?
O11 W4A Cs2 139.1(9) . . ?
O12 W4A Cs2 49.9(10) . . ?
O4 W4A Cs2 57.8(8) . . ?
O9 W4A Cs2 128.0(9) . . ?
O10 W4A Cs2 111.4(8) 1_565 . ?
Cs2 W4A Cs2 129.6(7) 1_655 . ?
W4B W4A Cs2 59.9(6) . 1_665 ?
O10 W4A Cs2 125.0(11) . 1_665 ?
O11 W4A Cs2 43.3(8) . 1_665 ?
O12 W4A Cs2 127.1(12) . 1_665 ?
O4 W4A Cs2 119.2(9) . 1_665 ?
O9 W4A Cs2 53.0(8) . 1_665 ?
O10 W4A Cs2 63.0(8) 1_565 1_665 ?
Cs2 W4A Cs2 55.95(7) 1_655 1_665 ?
Cs2 W4A Cs2 174.4(6) . 1_665 ?
W4B W4A Cs2 59.6(8) . 1_565 ?
O10 W4A Cs2 115.0(10) . 1_565 ?
O11 W4A Cs2 126.9(10) . 1_565 ?
O12 W4A Cs2 43.0(11) . 1_565 ?
O4 W4A Cs2 52.0(9) . 1_565 ?
O9 W4A Cs2 119.8(9) . 1_565 ?
O10 W4A Cs2 56.7(8) 1_565 1_565 ?
Cs2 W4A Cs2 175.3(6) 1_655 1_565 ?
Cs2 W4A Cs2 55.04(8) . 1_565 ?
Cs2 W4A Cs2 119.4(6) 1_665 1_565 ?
W4A W4B O11 80.8(14) . . ?
W4A W4B O12 81.1(17) . . ?
O11 W4B O12 99.8(8) . . ?
W4A W4B O10 174.9(11) . 1_565 ?
O11 W4B O10 104.3(14) . 1_565 ?
O12 W4B O10 98.1(14) . 1_565 ?
W4A W4B O4 86.1(10) . . ?
O11 W4B O4 163.3(17) . . ?
O12 W4B O4 88.2(14) . . ?
O10 W4B O4 88.9(13) 1_565 . ?
W4A W4B O10 8.9(8) . . ?
O11 W4B O10 88.9(14) . . ?
O12 W4B O10 83.0(14) . . ?
O10 W4B O10 166.3(13) 1_565 . ?
O4 W4B O10 77.5(11) . . ?
W4A W4B O9 84.6(9) . . ?
O11 W4B O9 88.5(11) . . ?
O12 W4B O9 162.0(19) . . ?
O10 W4B O9 95.2(13) 1_565 . ?
O4 W4B O9 80.0(5) . . ?
O10 W4B O9 81.2(11) . . ?
W4A W4B Cs2 114.4(7) . 1_665 ?
O11 W4B Cs2 50.1(8) . 1_665 ?
O12 W4B Cs2 138.6(12) . 1_665 ?
O10 W4B Cs2 69.6(10) 1_565 1_665 ?
O4 W4B Cs2 129.2(11) . 1_665 ?
O10 W4B Cs2 118.3(9) . 1_665 ?
O9 W4B Cs2 58.1(8) . 1_665 ?
W4A W4B Cs2 114.7(8) . 1_565 ?
O11 W4B Cs2 138.4(9) . 1_565 ?
O12 W4B Cs2 49.9(11) . 1_565 ?
O10 W4B Cs2 61.6(10) 1_565 1_565 ?
O4 W4B Cs2 57.2(9) . 1_565 ?
O10 W4B Cs2 110.7(9) . 1_565 ?
O9 W4B Cs2 129.4(10) . 1_565 ?
Cs2 W4B Cs2 130.8(9) 1_665 1_565 ?
W4A W4B Cs2 58.6(6) . 1_655 ?
O11 W4B Cs2 43.9(8) . 1_655 ?
O12 W4B Cs2 126.0(14) . 1_655 ?
O10 W4B Cs2 125.1(10) 1_565 1_655 ?
O4 W4B Cs2 119.8(10) . 1_655 ?
O10 W4B Cs2 62.7(9) . 1_655 ?
O9 W4B Cs2 52.3(8) . 1_655 ?
Cs2 W4B Cs2 55.84(8) 1_665 1_655 ?
Cs2 W4B Cs2 173.3(8) 1_565 1_655 ?
W4A W4B Cs2 59.8(8) . . ?
O11 W4B Cs2 126.3(13) . . ?
O12 W4B Cs2 43.4(11) . . ?
O10 W4B Cs2 116.3(10) 1_565 . ?
O4 W4B Cs2 52.5(9) . . ?
O10 W4B Cs2 55.9(9) . . ?
O9 W4B Cs2 119.2(10) . . ?
Cs2 W4B Cs2 174.1(8) 1_665 . ?
Cs2 W4B Cs2 55.02(9) 1_565 . ?
Cs2 W4B Cs2 118.3(8) 1_655 . ?
O13 W5 O14 94.7(13) . 1_565 ?
O13 W5 O15 97.4(12) . . ?
O14 W5 O15 97.8(10) 1_565 . ?
O13 W5 O16 99.4(13) . . ?
O14 W5 O16 96.6(9) 1_565 . ?
O15 W5 O16 156.8(9) . . ?
O13 W5 O14 92.4(13) . . ?
O14 W5 O14 172.8(10) 1_565 . ?
O15 W5 O14 81.5(10) . . ?
O16 W5 O14 82.0(9) . . ?
O13 W5 O11 172.3(13) . . ?
O14 W5 O11 92.8(7) 1_565 . ?
O15 W5 O11 79.8(7) . . ?
O16 W5 O11 81.4(9) . . ?
O14 W5 O11 80.1(6) . . ?
O13 W5 Cs3 50.8(12) . 1_565 ?
O14 W5 Cs3 67.0(6) 1_565 1_565 ?
O15 W5 Cs3 61.5(6) . 1_565 ?
O16 W5 Cs3 141.5(7) . 1_565 ?
O14 W5 Cs3 118.2(5) . 1_565 ?
O11 W5 Cs3 131.7(6) . 1_565 ?
O13 W5 Cs2 135.0(12) . 1_665 ?
O14 W5 Cs2 63.1(6) 1_565 1_665 ?
O15 W5 Cs2 122.8(5) . 1_665 ?
O16 W5 Cs2 50.3(5) . 1_665 ?
O14 W5 Cs2 111.3(5) . 1_665 ?
O11 W5 Cs2 50.9(6) . 1_665 ?
Cs3 W5 Cs2 130.10(14) 1_565 1_665 ?
O13 W5 Cs3 51.5(12) . . ?
O14 W5 Cs3 122.6(6) 1_565 . ?
O15 W5 Cs3 53.9(5) . . ?
O16 W5 Cs3 129.5(6) . . ?
O14 W5 Cs3 62.6(5) . . ?
O11 W5 Cs3 122.3(6) . . ?
Cs3 W5 Cs3 55.64(10) 1_565 . ?
Cs2 W5 Cs3 172.63(13) 1_665 . ?
O13 W5 Cs2 130.5(11) . 1_655 ?
O14 W5 Cs2 117.9(6) 1_565 1_655 ?
O15 W5 Cs2 112.4(6) . 1_655 ?
O16 W5 Cs2 44.4(7) . 1_655 ?
O14 W5 Cs2 56.5(5) . 1_655 ?
O11 W5 Cs2 45.9(6) . 1_655 ?
Cs3 W5 Cs2 173.33(17) 1_565 1_655 ?
Cs2 W5 Cs2 54.81(4) 1_665 1_655 ?
Cs3 W5 Cs2 119.06(13) . 1_655 ?
O13 W5 Cs3 28.6(13) . 2_766 ?
O14 W5 Cs3 70.3(6) 1_565 2_766 ?
O15 W5 Cs3 114.4(5) . 2_766 ?
O16 W5 Cs3 87.7(6) . 2_766 ?
O14 W5 Cs3 116.6(5) . 2_766 ?
O11 W5 Cs3 158.7(5) . 2_766 ?
Cs3 W5 Cs3 54.4(3) 1_565 2_766 ?
Cs2 W5 Cs3 108.40(14) 1_665 2_766 ?
Cs3 W5 Cs3 78.62(18) . 2_766 ?
Cs2 W5 Cs3 130.63(18) 1_655 2_766 ?
O13 W5 Cs3 30.2(12) . 2_756 ?
O14 W5 Cs3 120.9(6) 1_565 2_756 ?
O15 W5 Cs3 106.2(5) . 2_756 ?
O16 W5 Cs3 81.5(5) . 2_756 ?
O14 W5 Cs3 66.0(5) . 2_756 ?
O11 W5 Cs3 143.7(5) . 2_756 ?
Cs3 W5 Cs3 78.55(18) 1_565 2_756 ?
Cs2 W5 Cs3 130.35(17) 1_665 2_756 ?
Cs3 W5 Cs3 52.3(3) . 2_756 ?
Cs2 W5 Cs3 101.44(13) 1_655 2_756 ?
Cs3 W5 Cs3 50.64(7) 2_766 2_756 ?
O17 W6 O18 108.3(10) . . ?
O17 W6 O15 95.7(8) . . ?
O18 W6 O15 95.0(12) . . ?
O17 W6 O16 98.4(9) . 1_455 ?
O18 W6 O16 92.9(11) . 1_455 ?
O15 W6 O16 160.8(9) . 1_455 ?
O17 W6 O12 170.3(9) . . ?
O18 W6 O12 81.3(10) . . ?
O15 W6 O12 81.9(10) . . ?
O16 W6 O12 82.0(11) 1_455 . ?
O17 W6 O18 96.2(9) . 1_565 ?
O18 W6 O18 155.5(13) . 1_565 ?
O15 W6 O18 84.2(10) . 1_565 ?
O16 W6 O18 81.4(10) 1_455 1_565 ?
O12 W6 O18 74.3(9) . 1_565 ?
O17 W6 Cs3 49.7(7) . . ?
O18 W6 Cs3 76.5(8) . . ?
O15 W6 Cs3 61.4(5) . . ?
O16 W6 Cs3 137.7(6) 1_455 . ?
O12 W6 Cs3 134.5(8) . . ?
O18 W6 Cs3 123.2(6) 1_565 . ?
O17 W6 Cs2 135.7(7) . . ?
O18 W6 Cs2 54.0(8) . . ?
O15 W6 Cs2 123.6(5) . . ?
O16 W6 Cs2 50.1(5) 1_455 . ?
O12 W6 Cs2 51.1(8) . . ?
O18 W6 Cs2 106.5(6) 1_565 . ?
Cs3 W6 Cs2 130.00(15) . . ?
O17 W6 Cs3 47.3(7) . 1_565 ?
O18 W6 Cs3 132.3(8) . 1_565 ?
O15 W6 Cs3 57.5(6) . 1_565 ?
O16 W6 Cs3 126.4(6) 1_455 1_565 ?
O12 W6 Cs3 125.2(8) . 1_565 ?
O18 W6 Cs3 67.0(6) 1_565 1_565 ?
Cs3 W6 Cs3 56.51(9) . 1_565 ?
Cs2 W6 Cs3 173.48(13) . 1_565 ?
O17 W6 Cs2 128.1(7) . 1_565 ?
O18 W6 Cs2 108.1(8) . 1_565 ?
O15 W6 Cs2 116.5(5) . 1_565 ?
O16 W6 Cs2 44.3(6) 1_455 1_565 ?
O12 W6 Cs2 46.9(8) . 1_565 ?
O18 W6 Cs2 52.2(6) 1_565 1_565 ?
Cs3 W6 Cs2 175.32(15) . 1_565 ?
Cs2 W6 Cs2 54.66(4) . 1_565 ?
Cs3 W6 Cs2 118.83(12) 1_565 1_565 ?
O17 W6 Cs3 29.9(6) . 2_656 ?
O18 W6 Cs3 80.8(8) . 2_656 ?
O15 W6 Cs3 110.3(4) . 2_656 ?
O16 W6 Cs3 88.3(6) 1_455 2_656 ?
O12 W6 Cs3 159.2(7) . 2_656 ?
O18 W6 Cs3 122.5(6) 1_565 2_656 ?
Cs3 W6 Cs3 49.9(3) . 2_656 ?
Cs2 W6 Cs3 109.05(13) . 2_656 ?
Cs3 W6 Cs3 75.24(17) 1_565 2_656 ?
Cs2 W6 Cs3 131.04(17) 1_565 2_656 ?
O17 W6 Cs3 27.4(6) . 2_666 ?
O18 W6 Cs3 131.9(8) . 2_666 ?
O15 W6 Cs3 104.2(5) . 2_666 ?
O16 W6 Cs3 83.2(5) 1_455 2_666 ?
O12 W6 Cs3 144.3(7) . 2_666 ?
O18 W6 Cs3 71.4(6) 1_565 2_666 ?
Cs3 W6 Cs3 75.07(18) . 2_666 ?
Cs2 W6 Cs3 131.94(16) . 2_666 ?
Cs3 W6 Cs3 46.8(3) 1_565 2_666 ?
Cs2 W6 Cs3 102.02(13) 1_565 2_666 ?
Cs3 W6 Cs3 51.19(7) 2_656 2_666 ?
O5 Cs1 O5 108.5(7) . 2_655 ?
O5 Cs1 O3 47.5(9) . . ?
O5 Cs1 O3 90.5(8) 2_655 . ?
O5 Cs1 O3 90.5(8) . 2_655 ?
O5 Cs1 O3 47.5(9) 2_655 2_655 ?
O3 Cs1 O3 110.5(10) . 2_655 ?
O5 Cs1 O2 49.3(9) . 2_655 ?
O5 Cs1 O2 89.2(8) 2_655 2_655 ?
O3 Cs1 O2 91.0(5) . 2_655 ?
O3 Cs1 O2 48.1(4) 2_655 2_655 ?
O5 Cs1 O2 89.2(8) . . ?
O5 Cs1 O2 49.3(9) 2_655 . ?
O3 Cs1 O2 48.1(4) . . ?
O3 Cs1 O2 91.0(5) 2_655 . ?
O2 Cs1 O2 110.5(8) 2_655 . ?
O5 Cs1 O5 178.1(6) . 2_645 ?
O5 Cs1 O5 73.5(3) 2_655 2_645 ?
O3 Cs1 O5 133.0(9) . 2_645 ?
O3 Cs1 O5 90.9(8) 2_655 2_645 ?
O2 Cs1 O5 131.3(9) 2_655 2_645 ?
O2 Cs1 O5 92.1(7) . 2_645 ?
O5 Cs1 O5 73.5(3) . 1_545 ?
O5 Cs1 O5 178.1(6) 2_655 1_545 ?
O3 Cs1 O5 90.9(8) . 1_545 ?
O3 Cs1 O5 133.0(9) 2_655 1_545 ?
O2 Cs1 O5 92.1(7) 2_655 1_545 ?
O2 Cs1 O5 131.3(9) . 1_545 ?
O5 Cs1 O5 104.6(7) 2_645 1_545 ?
O5 Cs1 O3 91.1(8) . 1_545 ?
O5 Cs1 O3 133.2(9) 2_655 1_545 ?
O3 Cs1 O3 71.8(7) . 1_545 ?
O3 Cs1 O3 177.7(7) 2_655 1_545 ?
O2 Cs1 O3 132.6(3) 2_655 1_545 ?
O2 Cs1 O3 90.6(4) . 1_545 ?
O5 Cs1 O3 87.4(8) 2_645 1_545 ?
O5 Cs1 O3 46.2(9) 1_545 1_545 ?
O5 Cs1 O3 133.2(9) . 2_645 ?
O5 Cs1 O3 91.1(8) 2_655 2_645 ?
O3 Cs1 O3 177.7(7) . 2_645 ?
O3 Cs1 O3 71.8(7) 2_655 2_645 ?
O2 Cs1 O3 90.6(4) 2_655 2_645 ?
O2 Cs1 O3 132.6(3) . 2_645 ?
O5 Cs1 O3 46.2(9) 2_645 2_645 ?
O5 Cs1 O3 87.4(8) 1_545 2_645 ?
O3 Cs1 O3 105.9(10) 1_545 2_645 ?
O5 Cs1 O2 131.3(9) . 1_545 ?
O5 Cs1 O2 92.1(7) 2_655 1_545 ?
O3 Cs1 O2 90.3(4) . 1_545 ?
O3 Cs1 O2 132.5(4) 2_655 1_545 ?
O2 Cs1 O2 178.1(6) 2_655 1_545 ?
O2 Cs1 O2 71.4(6) . 1_545 ?
O5 Cs1 O2 48.0(9) 2_645 1_545 ?
O5 Cs1 O2 86.5(7) 1_545 1_545 ?
O3 Cs1 O2 46.8(4) 1_545 1_545 ?
O3 Cs1 O2 88.1(4) 2_645 1_545 ?
O5 Cs1 O2 92.1(7) . 2_645 ?
O5 Cs1 O2 131.3(9) 2_655 2_645 ?
O3 Cs1 O2 132.5(4) . 2_645 ?
O3 Cs1 O2 90.3(4) 2_655 2_645 ?
O2 Cs1 O2 71.4(6) 2_655 2_645 ?
O2 Cs1 O2 178.1(6) . 2_645 ?
O5 Cs1 O2 86.5(7) 2_645 2_645 ?
O5 Cs1 O2 48.0(9) 1_545 2_645 ?
O3 Cs1 O2 88.1(4) 1_545 2_645 ?
O3 Cs1 O2 46.8(4) 2_645 2_645 ?
O2 Cs1 O2 106.8(8) 1_545 2_645 ?
O5 Cs1 O8 47.3(7) . . ?
O5 Cs1 O8 132.4(7) 2_655 . ?
O3 Cs1 O8 92.1(8) . . ?
O3 Cs1 O8 87.7(8) 2_655 . ?
O2 Cs1 O8 43.2(6) 2_655 . ?
O2 Cs1 O8 136.5(6) . . ?
O5 Cs1 O8 131.4(7) 2_645 . ?
O5 Cs1 O8 48.9(7) 1_545 . ?
O3 Cs1 O8 92.3(7) 1_545 . ?
O3 Cs1 O8 87.9(7) 2_645 . ?
O2 Cs1 O8 135.4(6) 1_545 . ?
O2 Cs1 O8 44.9(6) 2_645 . ?
O5 Cs1 O8 132.4(7) . 2_655 ?
O5 Cs1 O8 47.3(7) 2_655 2_655 ?
O3 Cs1 O8 87.7(8) . 2_655 ?
O3 Cs1 O8 92.1(8) 2_655 2_655 ?
O2 Cs1 O8 136.5(6) 2_655 2_655 ?
O2 Cs1 O8 43.2(6) . 2_655 ?
O5 Cs1 O8 48.9(7) 2_645 2_655 ?
O5 Cs1 O8 131.4(7) 1_545 2_655 ?
O3 Cs1 O8 87.9(7) 1_545 2_655 ?
O3 Cs1 O8 92.3(7) 2_645 2_655 ?
O2 Cs1 O8 44.9(6) 1_545 2_655 ?
O2 Cs1 O8 135.4(6) 2_645 2_655 ?
O8 Cs1 O8 179.6(7) . 2_655 ?
O5 Cs1 O1 87.7(12) . . ?
O5 Cs1 O1 88.8(12) 2_655 . ?
O3 Cs1 O1 42.4(14) . . ?
O3 Cs1 O1 132.8(14) 2_655 . ?
O2 Cs1 O1 133.3(14) 2_655 . ?
O2 Cs1 O1 41.8(14) . . ?
O5 Cs1 O1 92.3(12) 2_645 . ?
O5 Cs1 O1 91.3(12) 1_545 . ?
O3 Cs1 O1 48.9(14) 1_545 . ?
O3 Cs1 O1 136.1(14) 2_645 . ?
O2 Cs1 O1 48.1(14) 1_545 . ?
O2 Cs1 O1 136.9(14) 2_645 . ?
O8 Cs1 O1 122.9(5) . . ?
O8 Cs1 O1 57.1(5) 2_655 . ?
O5 Cs1 O1 88.8(12) . 1_655 ?
O5 Cs1 O1 87.7(12) 2_655 1_655 ?
O3 Cs1 O1 132.8(14) . 1_655 ?
O3 Cs1 O1 42.4(14) 2_655 1_655 ?
O2 Cs1 O1 41.8(14) 2_655 1_655 ?
O2 Cs1 O1 133.3(14) . 1_655 ?
O5 Cs1 O1 91.3(12) 2_645 1_655 ?
O5 Cs1 O1 92.3(12) 1_545 1_655 ?
O3 Cs1 O1 136.1(14) 1_545 1_655 ?
O3 Cs1 O1 48.9(14) 2_645 1_655 ?
O2 Cs1 O1 136.9(14) 1_545 1_655 ?
O2 Cs1 O1 48.1(14) 2_645 1_655 ?
O8 Cs1 O1 57.1(5) . 1_655 ?
O8 Cs1 O1 122.9(5) 2_655 1_655 ?
O1 Cs1 O1 174(3) . 1_655 ?
O5 Cs1 O7 137.3(7) . 2_655 ?
O5 Cs1 O7 45.8(7) 2_655 2_655 ?
O3 Cs1 O7 136.1(7) . 2_655 ?
O3 Cs1 O7 46.8(7) 2_655 2_655 ?
O2 Cs1 O7 91.6(6) 2_655 2_655 ?
O2 Cs1 O7 90.5(6) . 2_655 ?
O5 Cs1 O7 44.1(6) 2_645 2_655 ?
O5 Cs1 O7 132.8(6) 1_545 2_655 ?
O3 Cs1 O7 131.6(6) 1_545 2_655 ?
O3 Cs1 O7 45.4(7) 2_645 2_655 ?
O2 Cs1 O7 88.4(6) 1_545 2_655 ?
O2 Cs1 O7 89.4(6) 2_645 2_655 ?
O8 Cs1 O7 118.4(5) . 2_655 ?
O8 Cs1 O7 61.6(5) 2_655 2_655 ?
O1 Cs1 O7 118.7(4) . 2_655 ?
O1 Cs1 O7 61.6(4) 1_655 2_655 ?
O5 Cs1 O7 45.8(7) . . ?
O5 Cs1 O7 137.3(7) 2_655 . ?
O3 Cs1 O7 46.8(7) . . ?
O3 Cs1 O7 136.1(7) 2_655 . ?
O2 Cs1 O7 90.5(6) 2_655 . ?
O2 Cs1 O7 91.6(6) . . ?
O5 Cs1 O7 132.8(6) 2_645 . ?
O5 Cs1 O7 44.1(6) 1_545 . ?
O3 Cs1 O7 45.4(7) 1_545 . ?
O3 Cs1 O7 131.6(6) 2_645 . ?
O2 Cs1 O7 89.4(6) 1_545 . ?
O2 Cs1 O7 88.4(6) 2_645 . ?
O8 Cs1 O7 61.6(5) . . ?
O8 Cs1 O7 118.4(5) 2_655 . ?
O1 Cs1 O7 61.6(4) . . ?
O1 Cs1 O7 118.7(4) 1_655 . ?
O7 Cs1 O7 176.4(7) 2_655 . ?
O5 Cs1 Cs1 54.2(4) . 1_565 ?
O5 Cs1 Cs1 54.2(4) 2_655 1_565 ?
O3 Cs1 Cs1 55.2(5) . 1_565 ?
O3 Cs1 Cs1 55.2(5) 2_655 1_565 ?
O2 Cs1 Cs1 55.3(4) 2_655 1_565 ?
O2 Cs1 Cs1 55.3(4) . 1_565 ?
O5 Cs1 Cs1 127.7(3) 2_645 1_565 ?
O5 Cs1 Cs1 127.7(3) 1_545 1_565 ?
O3 Cs1 Cs1 127.0(5) 1_545 1_565 ?
O3 Cs1 Cs1 127.0(5) 2_645 1_565 ?
O2 Cs1 Cs1 126.6(4) 1_545 1_565 ?
O2 Cs1 Cs1 126.6(4) 2_645 1_565 ?
O8 Cs1 Cs1 89.8(4) . 1_565 ?
O8 Cs1 Cs1 89.8(4) 2_655 1_565 ?
O1 Cs1 Cs1 87.0(16) . 1_565 ?
O1 Cs1 Cs1 87.0(16) 1_655 1_565 ?
O7 Cs1 Cs1 91.8(3) 2_655 1_565 ?
O7 Cs1 Cs1 91.8(3) . 1_565 ?
O5 Cs1 Cs1 125.8(4) . 1_545 ?
O5 Cs1 Cs1 125.8(4) 2_655 1_545 ?
O3 Cs1 Cs1 124.8(5) . 1_545 ?
O3 Cs1 Cs1 124.8(5) 2_655 1_545 ?
O2 Cs1 Cs1 124.7(4) 2_655 1_545 ?
O2 Cs1 Cs1 124.7(4) . 1_545 ?
O5 Cs1 Cs1 52.3(3) 2_645 1_545 ?
O5 Cs1 Cs1 52.3(3) 1_545 1_545 ?
O3 Cs1 Cs1 53.0(5) 1_545 1_545 ?
O3 Cs1 Cs1 53.0(5) 2_645 1_545 ?
O2 Cs1 Cs1 53.4(4) 1_545 1_545 ?
O2 Cs1 Cs1 53.4(4) 2_645 1_545 ?
O8 Cs1 Cs1 90.2(4) . 1_545 ?
O8 Cs1 Cs1 90.2(4) 2_655 1_545 ?
O1 Cs1 Cs1 93.0(16) . 1_545 ?
O1 Cs1 Cs1 93.0(16) 1_655 1_545 ?
O7 Cs1 Cs1 88.2(3) 2_655 1_545 ?
O7 Cs1 Cs1 88.2(3) . 1_545 ?
Cs1 Cs1 Cs1 180.0 1_565 1_545 ?
O11 Cs2 O11 74.7(5) 1_445 1_455 ?
O11 Cs2 O16 50.5(8) 1_445 1_445 ?
O11 Cs2 O16 94.9(7) 1_455 1_445 ?
O11 Cs2 O12 92.0(5) 1_445 1_545 ?
O11 Cs2 O12 138.9(4) 1_455 1_545 ?
O16 Cs2 O12 50.2(10) 1_445 1_545 ?
O11 Cs2 O12 138.8(4) 1_445 . ?
O11 Cs2 O12 90.9(5) 1_455 . ?
O16 Cs2 O12 94.1(8) 1_445 . ?
O12 Cs2 O12 73.6(7) 1_545 . ?
O11 Cs2 O16 95.1(7) 1_445 1_455 ?
O11 Cs2 O16 49.8(8) 1_455 1_455 ?
O16 Cs2 O16 73.7(3) 1_445 1_455 ?
O12 Cs2 O16 94.5(8) 1_545 1_455 ?
O12 Cs2 O16 49.6(10) . 1_455 ?
O11 Cs2 O6 130.1(9) 1_445 . ?
O11 Cs2 O6 87.7(8) 1_455 . ?
O16 Cs2 O6 177.3(7) 1_445 . ?
O12 Cs2 O6 127.7(10) 1_545 . ?
O12 Cs2 O6 86.4(9) . . ?
O16 Cs2 O6 108.5(6) 1_455 . ?
O11 Cs2 O9 91.1(6) 1_445 1_455 ?
O11 Cs2 O9 48.1(7) 1_455 1_455 ?
O16 Cs2 O9 135.6(9) 1_445 1_455 ?
O12 Cs2 O9 172.9(8) 1_545 1_455 ?
O12 Cs2 O9 107.8(7) . 1_455 ?
O16 Cs2 O9 91.6(8) 1_455 1_455 ?
O6 Cs2 O9 46.4(10) . 1_455 ?
O11 Cs2 O9 48.4(7) 1_445 1_445 ?
O11 Cs2 O9 91.7(6) 1_455 1_445 ?
O16 Cs2 O9 92.4(8) 1_445 1_445 ?
O12 Cs2 O9 108.4(7) 1_545 1_445 ?
O12 Cs2 O9 172.8(8) . 1_445 ?
O16 Cs2 O9 135.9(9) 1_455 1_445 ?
O6 Cs2 O9 87.0(8) . 1_445 ?
O9 Cs2 O9 69.3(6) 1_455 1_445 ?
O11 Cs2 O18 96.4(6) 1_445 . ?
O11 Cs2 O18 94.9(6) 1_455 . ?
O16 Cs2 O18 48.4(7) 1_445 . ?
O12 Cs2 O18 47.2(7) 1_545 . ?
O12 Cs2 O18 45.7(7) . . ?
O16 Cs2 O18 47.3(7) 1_455 . ?
O6 Cs2 O18 132.0(8) . . ?
O9 Cs2 O18 138.6(6) 1_455 . ?
O9 Cs2 O18 140.6(6) 1_445 . ?
O11 Cs2 O4 109.0(6) 1_445 1_545 ?
O11 Cs2 O4 173.2(7) 1_455 1_545 ?
O16 Cs2 O4 91.8(8) 1_445 1_545 ?
O12 Cs2 O4 47.5(8) 1_545 1_545 ?
O12 Cs2 O4 89.6(7) . 1_545 ?
O16 Cs2 O4 133.9(9) 1_455 1_545 ?
O6 Cs2 O4 85.6(8) . 1_545 ?
O9 Cs2 O4 125.4(3) 1_455 1_545 ?
O9 Cs2 O4 87.0(4) 1_445 1_545 ?
O18 Cs2 O4 90.3(7) . 1_545 ?
O11 Cs2 O4 174.1(7) 1_445 . ?
O11 Cs2 O4 107.2(6) 1_455 . ?
O16 Cs2 O4 133.9(9) 1_445 . ?
O12 Cs2 O4 89.9(7) 1_545 . ?
O12 Cs2 O4 47.0(8) . . ?
O16 Cs2 O4 90.3(8) 1_455 . ?
O6 Cs2 O4 45.3(10) . . ?
O9 Cs2 O4 86.3(4) 1_455 . ?
O9 Cs2 O4 125.7(3) 1_445 . ?
O18 Cs2 O4 89.0(7) . . ?
O4 Cs2 O4 68.5(6) 1_545 . ?
O11 Cs2 O6 88.1(8) 1_445 1_545 ?
O11 Cs2 O6 130.4(9) 1_455 1_545 ?
O16 Cs2 O6 109.3(6) 1_445 1_545 ?
O12 Cs2 O6 86.6(9) 1_545 1_545 ?
O12 Cs2 O6 127.9(10) . 1_545 ?
O16 Cs2 O6 176.6(7) 1_455 1_545 ?
O6 Cs2 O6 68.4(3) . 1_545 ?
O9 Cs2 O6 87.2(8) 1_455 1_545 ?
O9 Cs2 O6 46.3(10) 1_445 1_545 ?
O18 Cs2 O6 133.6(8) . 1_545 ?
O4 Cs2 O6 45.5(10) 1_545 1_545 ?
O4 Cs2 O6 86.5(8) . 1_545 ?
O11 Cs2 O10 138.9(7) 1_445 . ?
O11 Cs2 O10 134.8(7) 1_455 . ?
O16 Cs2 O10 93.2(9) 1_445 . ?
O12 Cs2 O10 46.9(8) 1_545 . ?
O12 Cs2 O10 44.1(8) . . ?
O16 Cs2 O10 90.8(9) 1_455 . ?
O6 Cs2 O10 85.4(9) . . ?
O9 Cs2 O10 129.4(7) 1_455 . ?
O9 Cs2 O10 132.3(7) 1_445 . ?
O18 Cs2 O10 59.5(5) . . ?
O4 Cs2 O10 45.5(7) 1_545 . ?
O4 Cs2 O10 43.1(7) . . ?
O6 Cs2 O10 87.6(9) 1_545 . ?
O11 Cs2 O14 50.9(5) 1_445 1_455 ?
O11 Cs2 O14 47.2(5) 1_455 1_455 ?
O16 Cs2 O14 47.8(6) 1_445 1_455 ?
O12 Cs2 O14 94.2(7) 1_545 1_455 ?
O12 Cs2 O14 91.0(7) . 1_455 ?
O16 Cs2 O14 44.1(6) 1_455 1_455 ?
O6 Cs2 O14 134.8(7) . 1_455 ?
O9 Cs2 O14 92.7(6) 1_455 1_455 ?
O9 Cs2 O14 95.7(6) 1_445 1_455 ?
O18 Cs2 O14 62.6(4) . 1_455 ?
O4 Cs2 O14 139.6(6) 1_545 1_455 ?
O4 Cs2 O14 134.4(6) . 1_455 ?
O6 Cs2 O14 139.0(7) 1_545 1_455 ?
O10 Cs2 O14 122.0(4) . 1_455 ?
O11 Cs2 O7 132.1(6) 1_445 . ?
O11 Cs2 O7 132.2(6) 1_455 . ?
O16 Cs2 O7 132.9(7) 1_445 . ?
O12 Cs2 O7 85.5(8) 1_545 . ?
O12 Cs2 O7 85.9(8) . . ?
O16 Cs2 O7 132.8(7) 1_455 . ?
O6 Cs2 O7 44.5(8) . . ?
O9 Cs2 O7 87.7(6) 1_455 . ?
O9 Cs2 O7 87.3(6) 1_445 . ?
O18 Cs2 O7 115.3(5) . . ?
O4 Cs2 O7 41.1(6) 1_545 . ?
O4 Cs2 O7 42.5(6) . . ?
O6 Cs2 O7 44.1(7) 1_545 . ?
O10 Cs2 O7 55.8(5) . . ?
O14 Cs2 O7 176.9(5) 1_455 . ?
O11 Cs2 O10 47.4(6) 1_445 1_455 ?
O11 Cs2 O10 45.0(6) 1_455 1_455 ?
O16 Cs2 O10 94.0(9) 1_445 1_455 ?
O12 Cs2 O10 139.4(8) 1_545 1_455 ?
O12 Cs2 O10 135.7(8) . 1_455 ?
O16 Cs2 O10 91.7(8) 1_455 1_455 ?
O6 Cs2 O10 87.5(9) . 1_455 ?
O9 Cs2 O10 43.8(6) 1_455 1_455 ?
O9 Cs2 O10 46.8(7) 1_445 1_455 ?
O18 Cs2 O10 126.5(5) . 1_455 ?
O4 Cs2 O10 133.5(7) 1_545 1_455 ?
O4 Cs2 O10 130.2(7) . 1_455 ?
O6 Cs2 O10 89.5(9) 1_545 1_455 ?
O10 Cs2 O10 172.9(8) . 1_455 ?
O14 Cs2 O10 63.8(4) 1_455 1_455 ?
O7 Cs2 O10 118.2(4) . 1_455 ?
O11 Cs2 Cs2 53.1(4) 1_445 1_545 ?
O11 Cs2 Cs2 127.8(4) 1_455 1_545 ?
O16 Cs2 Cs2 53.7(3) 1_445 1_545 ?
O12 Cs2 Cs2 53.5(5) 1_545 1_545 ?
O12 Cs2 Cs2 127.1(5) . 1_545 ?
O16 Cs2 Cs2 127.4(3) 1_455 1_545 ?
O6 Cs2 Cs2 124.1(4) . 1_545 ?
O9 Cs2 Cs2 124.7(4) 1_455 1_545 ?
O9 Cs2 Cs2 55.3(4) 1_445 1_545 ?
O18 Cs2 Cs2 91.2(4) . 1_545 ?
O4 Cs2 Cs2 56.2(4) 1_545 1_545 ?
O4 Cs2 Cs2 124.7(4) . 1_545 ?
O6 Cs2 Cs2 55.7(4) 1_545 1_545 ?
O10 Cs2 Cs2 91.9(6) . 1_545 ?
O14 Cs2 Cs2 92.7(3) 1_455 1_545 ?
O7 Cs2 Cs2 89.6(4) . 1_545 ?
O10 Cs2 Cs2 91.8(6) 1_455 1_545 ?
O11 Cs2 Cs2 126.9(4) 1_445 1_565 ?
O11 Cs2 Cs2 52.2(4) 1_455 1_565 ?
O16 Cs2 Cs2 126.3(3) 1_445 1_565 ?
O12 Cs2 Cs2 126.5(5) 1_545 1_565 ?
O12 Cs2 Cs2 52.9(5) . 1_565 ?
O16 Cs2 Cs2 52.6(3) 1_455 1_565 ?
O6 Cs2 Cs2 55.9(4) . 1_565 ?
O9 Cs2 Cs2 55.3(4) 1_455 1_565 ?
O9 Cs2 Cs2 124.7(4) 1_445 1_565 ?
O18 Cs2 Cs2 88.8(4) . 1_565 ?
O4 Cs2 Cs2 123.8(4) 1_545 1_565 ?
O4 Cs2 Cs2 55.3(4) . 1_565 ?
O6 Cs2 Cs2 124.3(4) 1_545 1_565 ?
O10 Cs2 Cs2 88.1(6) . 1_565 ?
O14 Cs2 Cs2 87.3(3) 1_455 1_565 ?
O7 Cs2 Cs2 90.4(4) . 1_565 ?
O10 Cs2 Cs2 88.2(6) 1_455 1_565 ?
Cs2 Cs2 Cs2 180.0 1_545 1_565 ?
O11 Cs2 O8 91.3(6) 1_445 1_455 ?
O11 Cs2 O8 89.5(6) 1_455 1_455 ?
O16 Cs2 O8 138.1(7) 1_445 1_455 ?
O12 Cs2 O8 130.3(8) 1_545 1_455 ?
O12 Cs2 O8 127.6(7) . 1_455 ?
O16 Cs2 O8 134.5(7) 1_455 1_455 ?
O6 Cs2 O8 41.2(7) . 1_455 ?
O9 Cs2 O8 43.3(6) 1_455 1_455 ?
O9 Cs2 O8 45.7(6) 1_445 1_455 ?
O18 Cs2 O8 171.9(6) . 1_455 ?
O4 Cs2 O8 84.8(7) 1_545 1_455 ?
O4 Cs2 O8 83.2(7) . 1_455 ?
O6 Cs2 O8 44.0(7) 1_545 1_455 ?
O10 Cs2 O8 112.8(5) . 1_455 ?
O14 Cs2 O8 124.8(5) 1_455 1_455 ?
O7 Cs2 O8 57.1(5) . 1_455 ?
O10 Cs2 O8 61.0(5) 1_455 1_455 ?
Cs2 Cs2 O8 91.5(3) 1_545 1_455 ?
Cs2 Cs2 O8 88.5(3) 1_565 1_455 ?
O17 Cs3 O13 98.9(5) 2_656 2_746 ?
O17 Cs3 O17 68.6(7) 2_656 . ?
O13 Cs3 O17 164.4(8) 2_746 . ?
O17 Cs3 O17 78.6(5) 2_656 2_646 ?
O13 Cs3 O17 55.3(5) 2_746 2_646 ?
O17 Cs3 O17 111.4(5) . 2_646 ?
O17 Cs3 O13 55.2(5) 2_656 2_756 ?
O13 Cs3 O13 75.0(7) 2_746 2_756 ?
O17 Cs3 O13 103.3(8) . 2_756 ?
O17 Cs3 O13 104.2(5) 2_646 2_756 ?
O17 Cs3 O13 160.5(8) 2_656 1_545 ?
O13 Cs3 O13 67.3(12) 2_746 1_545 ?
O17 Cs3 O13 127.1(5) . 1_545 ?
O17 Cs3 O13 102.4(8) 2_646 1_545 ?
O13 Cs3 O13 106.5(6) 2_756 1_545 ?
O17 Cs3 O17 111.5(5) 2_656 1_545 ?
O13 Cs3 O17 103.2(8) 2_746 1_545 ?
O17 Cs3 O17 74.4(5) . 1_545 ?
O17 Cs3 O17 64.3(7) 2_646 1_545 ?
O13 Cs3 O17 165.2(8) 2_756 1_545 ?
O13 Cs3 O17 85.8(6) 1_545 1_545 ?
O17 Cs3 O13 102.6(8) 2_656 . ?
O13 Cs3 O13 106.6(6) 2_746 . ?
O17 Cs3 O13 85.8(5) . . ?
O17 Cs3 O13 161.5(7) 2_646 . ?
O13 Cs3 O13 63.5(11) 2_756 . ?
O13 Cs3 O13 70.3(7) 1_545 . ?
O17 Cs3 O13 129.9(4) 1_545 . ?
O17 Cs3 O15 104.4(6) 2_656 . ?
O13 Cs3 O15 146.9(10) 2_746 . ?
O17 Cs3 O15 48.5(8) . . ?
O17 Cs3 O15 152.5(9) 2_646 . ?
O13 Cs3 O15 99.5(8) 2_756 . ?
O13 Cs3 O15 83.8(8) 1_545 . ?
O17 Cs3 O15 89.8(7) 1_545 . ?
O13 Cs3 O15 45.6(8) . . ?
O17 Cs3 Cs3 56.7(4) 2_656 2_656 ?
O13 Cs3 Cs3 113.1(6) 2_746 2_656 ?
O17 Cs3 Cs3 52.6(5) . 2_656 ?
O17 Cs3 Cs3 58.8(4) 2_646 2_656 ?
O13 Cs3 Cs3 111.8(6) 2_756 2_656 ?
O13 Cs3 Cs3 140.4(7) 1_545 2_656 ?
O17 Cs3 Cs3 54.9(4) 1_545 2_656 ?
O13 Cs3 Cs3 137.2(6) . 2_656 ?
O15 Cs3 Cs3 99.4(7) . 2_656 ?
O17 Cs3 O15 153.7(9) 2_656 1_545 ?
O13 Cs3 O15 100.6(8) 2_746 1_545 ?
O17 Cs3 O15 88.9(6) . 1_545 ?
O17 Cs3 O15 98.2(6) 2_646 1_545 ?
O13 Cs3 O15 148.1(10) 2_756 1_545 ?
O13 Cs3 O15 45.8(9) 1_545 1_545 ?
O17 Cs3 O15 46.5(7) 1_545 1_545 ?
O13 Cs3 O15 88.7(8) . 1_545 ?
O15 Cs3 O15 66.7(2) . 1_545 ?
Cs3 Cs3 O15 99.1(7) 2_656 1_545 ?
O17 Cs3 O14 141.9(5) 2_656 . ?
O13 Cs3 O14 107.4(7) 2_746 . ?
O17 Cs3 O14 88.1(5) . . ?
O17 Cs3 O14 139.3(5) 2_646 . ?
O13 Cs3 O14 105.4(7) 2_756 . ?
O13 Cs3 O14 42.2(7) 1_545 . ?
O17 Cs3 O14 89.2(5) 1_545 . ?
O13 Cs3 O14 43.9(6) . . ?
O15 Cs3 O14 41.6(6) . . ?
Cs3 Cs3 O14 130.4(4) 2_656 . ?
O15 Cs3 O14 44.9(6) 1_545 . ?
O17 Cs3 Cs3 52.8(4) 2_656 1_565 ?
O13 Cs3 Cs3 125.5(7) 2_746 1_565 ?
O17 Cs3 Cs3 54.9(4) . 1_565 ?
O17 Cs3 Cs3 131.4(4) 2_646 1_565 ?
O13 Cs3 Cs3 50.5(6) 2_756 1_565 ?
O13 Cs3 Cs3 123.2(7) 1_545 1_565 ?
O17 Cs3 Cs3 129.2(4) 1_545 1_565 ?
O13 Cs3 Cs3 52.9(6) . 1_565 ?
O15 Cs3 Cs3 58.0(4) . 1_565 ?
Cs3 Cs3 Cs3 90.000(2) 2_656 1_565 ?
O15 Cs3 Cs3 124.7(4) 1_545 1_565 ?
O14 Cs3 Cs3 89.2(3) . 1_565 ?
O17 Cs3 Cs3 127.2(4) 2_656 1_545 ?
O13 Cs3 Cs3 54.5(7) 2_746 1_545 ?
O17 Cs3 Cs3 125.1(4) . 1_545 ?
O17 Cs3 Cs3 48.6(4) 2_646 1_545 ?
O13 Cs3 Cs3 129.5(6) 2_756 1_545 ?
O13 Cs3 Cs3 56.8(7) 1_545 1_545 ?
O17 Cs3 Cs3 50.8(4) 1_545 1_545 ?
O13 Cs3 Cs3 127.1(6) . 1_545 ?
O15 Cs3 Cs3 122.0(4) . 1_545 ?
Cs3 Cs3 Cs3 90.000(4) 2_656 1_545 ?
O15 Cs3 Cs3 55.3(4) 1_545 1_545 ?
O14 Cs3 Cs3 90.8(3) . 1_545 ?
Cs3 Cs3 Cs3 180.0 1_565 1_545 ?
O17 Cs3 Cs3 111.0(4) 2_656 2_756 ?
O13 Cs3 Cs3 54.4(6) 2_746 2_756 ?
O17 Cs3 Cs3 137.7(5) . 2_756 ?
O17 Cs3 Cs3 109.7(4) 2_646 2_756 ?
O13 Cs3 Cs3 56.5(6) 2_756 2_756 ?
O13 Cs3 Cs3 50.0(7) 1_545 2_756 ?
O17 Cs3 Cs3 134.5(4) 1_545 2_756 ?
O13 Cs3 Cs3 52.3(6) . 2_756 ?
O15 Cs3 Cs3 94.9(8) . 2_756 ?
Cs3 Cs3 Cs3 163.10(19) 2_656 2_756 ?
O15 Cs3 Cs3 94.8(7) 1_545 2_756 ?
O14 Cs3 Cs3 66.5(4) . 2_756 ?
Cs3 Cs3 Cs3 90.000(2) 1_565 2_756 ?
Cs3 Cs3 Cs3 90.000(2) 1_545 2_756 ?
O17 Cs3 O18 113.2(6) 2_656 . ?
O13 Cs3 O18 142.3(7) 2_746 . ?
O17 Cs3 O18 45.8(5) . . ?
O17 Cs3 O18 110.9(6) 2_646 . ?
O13 Cs3 O18 139.8(7) 2_756 . ?
O13 Cs3 O18 84.9(7) 1_545 . ?
O17 Cs3 O18 47.6(5) 1_545 . ?
O13 Cs3 O18 85.9(7) . . ?
O15 Cs3 O18 42.3(6) . . ?
Cs3 Cs3 O18 72.7(5) 2_656 . ?
O15 Cs3 O18 43.1(6) 1_545 . ?
O14 Cs3 O18 57.7(4) . . ?
Cs3 Cs3 O18 90.7(3) 1_565 . ?
Cs3 Cs3 O18 89.3(3) 1_545 . ?
Cs3 Cs3 O18 124.2(5) 2_756 . ?
O17 Cs3 W6 93.3(4) 2_656 . ?
O13 Cs3 W6 167.3(7) 2_746 . ?
O17 Cs3 W6 25.4(4) . . ?
O17 Cs3 W6 124.7(5) 2_646 . ?
O13 Cs3 W6 115.3(7) 2_756 . ?
O13 Cs3 W6 101.6(6) 1_545 . ?
O17 Cs3 W6 68.7(4) 1_545 . ?
O13 Cs3 W6 73.8(6) . . ?
O15 Cs3 W6 29.0(7) . . ?
Cs3 Cs3 W6 71.0(2) 2_656 . ?
O15 Cs3 W6 66.8(4) 1_545 . ?
O14 Cs3 W6 63.8(3) . . ?
Cs3 Cs3 W6 65.28(11) 1_565 . ?
Cs3 Cs3 W6 114.72(11) 1_545 . ?
Cs3 Cs3 W6 123.9(2) 2_756 . ?
O18 Cs3 W6 25.6(3) . . ?
O17 Cs3 W5 168.4(4) 2_656 1_545 ?
O13 Cs3 W5 89.7(7) 2_746 1_545 ?
O17 Cs3 W5 104.1(4) . 1_545 ?
O17 Cs3 W5 112.8(4) 2_646 1_545 ?
O13 Cs3 W5 120.7(7) 2_756 1_545 ?
O13 Cs3 W5 23.2(6) 1_545 1_545 ?
O17 Cs3 W5 73.7(4) 1_545 1_545 ?
O13 Cs3 W5 67.3(6) . 1_545 ?
O15 Cs3 W5 64.7(5) . 1_545 ?
Cs3 Cs3 W5 126.8(2) 2_656 1_545 ?
O15 Cs3 W5 27.7(7) 1_545 1_545 ?
O14 Cs3 W5 26.6(3) . 1_545 ?
Cs3 Cs3 W5 115.74(10) 1_565 1_545 ?
Cs3 Cs3 W5 64.26(11) 1_545 1_545 ?
Cs3 Cs3 W5 67.9(2) 2_756 1_545 ?
O18 Cs3 W5 62.0(4) . 1_545 ?
W6 Cs3 W5 78.75(6) . 1_545 ?
O17 Cs3 W6 127.5(5) 2_656 1_545 ?
O13 Cs3 W6 112.4(7) 2_746 1_545 ?
O17 Cs3 W6 71.5(4) . 1_545 ?
O17 Cs3 W6 85.7(4) 2_646 1_545 ?
O13 Cs3 W6 170.0(7) 2_756 1_545 ?
O13 Cs3 W6 71.7(6) 1_545 1_545 ?
O17 Cs3 W6 23.1(4) 1_545 1_545 ?
O13 Cs3 W6 107.1(6) . 1_545 ?
O15 Cs3 W6 70.6(5) . 1_545 ?
Cs3 Cs3 W6 72.3(2) 2_656 1_545 ?
O15 Cs3 W6 26.9(7) 1_545 1_545 ?
O14 Cs3 W6 66.4(3) . 1_545 ?
Cs3 Cs3 W6 121.79(8) 1_565 1_545 ?
Cs3 Cs3 W6 58.21(8) 1_545 1_545 ?
Cs3 Cs3 W6 121.4(2) 2_756 1_545 ?
O18 Cs3 W6 31.3(3) . 1_545 ?
W6 Cs3 W6 56.51(9) . 1_545 ?
W5 Cs3 W6 54.46(6) 1_545 1_545 ?
O17 Cs3 W5 112.9(4) 2_656 . ?
O13 Cs3 W5 121.8(7) 2_746 . ?
O17 Cs3 W5 73.0(4) . . ?
O17 Cs3 W5 168.4(4) 2_646 . ?
O13 Cs3 W5 84.7(6) 2_756 . ?
O13 Cs3 W5 67.5(6) 1_545 . ?
O17 Cs3 W5 108.0(4) 1_545 . ?
O13 Cs3 W5 22.3(6) . . ?
O15 Cs3 W5 26.2(7) . . ?
Cs3 Cs3 W5 125.2(2) 2_656 . ?
O15 Cs3 W5 70.7(5) 1_545 . ?
O14 Cs3 W5 29.1(3) . . ?
Cs3 Cs3 W5 60.10(9) 1_565 . ?
Cs3 Cs3 W5 119.90(9) 1_545 . ?
Cs3 Cs3 W5 68.7(2) 2_756 . ?
O18 Cs3 W5 63.8(4) . . ?
W6 Cs3 W5 55.19(6) . . ?
W5 Cs3 W5 55.64(10) 1_545 . ?
W6 Cs3 W5 85.61(6) 1_545 . ?
W1 O1 W1 180.0 . 1_545 ?
W1 O1 Cs1 93.0(16) . 1_455 ?
W1 O1 Cs1 87.0(16) 1_545 1_455 ?
W1 O1 Cs1 93.0(16) . . ?
W1 O1 Cs1 87.0(16) 1_545 . ?
Cs1 O1 Cs1 174(3) 1_455 . ?
W1 O2 W3B 151.0(17) . 2_655 ?
W1 O2 W3A 149.5(17) . 2_655 ?
W3B O2 W3A 16.4(4) 2_655 2_655 ?
W1 O2 Cs1 103.2(11) . . ?
W3B O2 Cs1 104.7(11) 2_655 . ?
W3A O2 Cs1 97.2(10) 2_655 . ?
W1 O2 Cs1 102.3(10) . 1_565 ?
W3B O2 Cs1 94.0(10) 2_655 1_565 ?
W3A O2 Cs1 105.6(11) 2_655 1_565 ?
Cs1 O2 Cs1 71.4(6) . 1_565 ?
W2 O3 W1 150(2) . . ?
W2 O3 Cs1 101.5(12) . . ?
W1 O3 Cs1 102.9(12) . . ?
W2 O3 Cs1 102.9(12) . 1_565 ?
W1 O3 Cs1 101.5(12) . 1_565 ?
Cs1 O3 Cs1 71.8(7) . 1_565 ?
W2 O4 W4B 154.7(19) . . ?
W2 O4 W4A 153.7(18) . . ?
W4B O4 W4A 13.0(3) . . ?
W2 O4 Cs2 106.0(12) . 1_565 ?
W4B O4 Cs2 92.5(11) . 1_565 ?
W4A O4 Cs2 99.5(12) . 1_565 ?
W2 O4 Cs2 103.3(11) . . ?
W4B O4 Cs2 99.5(12) . . ?
W4A O4 Cs2 91.8(10) . . ?
Cs2 O4 Cs2 68.5(6) 1_565 . ?
W2 O5 W3B 144.4(8) . . ?
W2 O5 W3A 142.6(8) . . ?
W3B O5 W3A 16.3(5) . . ?
W2 O5 Cs1 104.2(11) . . ?
W3B O5 Cs1 108.2(13) . . ?
W3A O5 Cs1 99.6(11) . . ?
W2 O5 Cs1 106.1(12) . 1_565 ?
W3B O5 Cs1 96.8(11) . 1_565 ?
W3A O5 Cs1 108.1(12) . 1_565 ?
Cs1 O5 Cs1 73.5(3) . 1_565 ?
W3A O6 W2 152.6(9) 1_455 . ?
W3A O6 W3B 16.2(5) 1_455 1_455 ?
W2 O6 W3B 150.8(9) . 1_455 ?
W3A O6 Cs2 96.2(12) 1_455 . ?
W2 O6 Cs2 101.6(12) . . ?
W3B O6 Cs2 106.5(14) 1_455 . ?
W3A O6 Cs2 103.5(14) 1_455 1_565 ?
W2 O6 Cs2 102.4(12) . 1_565 ?
W3B O6 Cs2 95.4(12) 1_455 1_565 ?
Cs2 O6 Cs2 68.4(3) . 1_565 ?
W2 O7 W2 175.0(12) . 1_545 ?
W2 O7 Cs1 86.7(7) . . ?
W2 O7 Cs1 90.3(7) 1_545 . ?
W2 O7 Cs2 91.0(7) . . ?
W2 O7 Cs2 91.8(7) 1_545 . ?
Cs1 O7 Cs2 176.6(7) . . ?
W3B O8 W3A 162.2(19) 1_545 . ?
W3B O8 W3A 2.4(5) 1_545 1_545 ?
W3A O8 W3A 162.8(17) . 1_545 ?
W3B O8 W3B 165.6(18) 1_545 . ?
W3A O8 W3B 4.3(3) . . ?
W3A O8 W3B 166.6(15) 1_545 . ?
W3B O8 Cs1 93.8(11) 1_545 . ?
W3A O8 Cs1 97.4(11) . . ?
W3A O8 Cs1 95.0(8) 1_545 . ?
W3B O8 Cs1 93.3(9) . . ?
W3B O8 Cs2 83.7(10) 1_545 1_655 ?
W3A O8 Cs2 83.5(10) . 1_655 ?
W3A O8 Cs2 82.7(8) 1_545 1_655 ?
W3B O8 Cs2 87.7(8) . 1_655 ?
Cs1 O8 Cs2 172.8(10) . 1_655 ?
W3A O9 W3B 17.4(4) . . ?
W3A O9 W4B 157.4(17) . . ?
W3B O9 W4B 149.5(17) . . ?
W3A O9 W4A 154.3(17) . . ?
W3B O9 W4A 155.1(17) . . ?
W4B O9 W4A 12.9(3) . . ?
W3A O9 Cs2 99.5(11) . 1_655 ?
W3B O9 Cs2 111.5(12) . 1_655 ?
W4B O9 Cs2 99.0(11) . 1_655 ?
W4A O9 Cs2 91.3(10) . 1_655 ?
W3A O9 Cs2 107.8(12) . 1_665 ?
W3B O9 Cs2 99.6(11) . 1_665 ?
W4B O9 Cs2 90.8(10) . 1_665 ?
W4A O9 Cs2 97.8(11) . 1_665 ?
Cs2 O9 Cs2 69.3(6) 1_655 1_665 ?
W4A O10 W4B 163.8(14) . 1_545 ?
W4A O10 W4B 2.5(2) . . ?
W4B O10 W4B 166.3(13) 1_545 . ?
W4A O10 W4A 164.8(13) . 1_545 ?
W4B O10 W4A 1.0(2) 1_545 1_545 ?
W4B O10 W4A 167.3(11) . 1_545 ?
W4A O10 Cs2 96.3(12) . . ?
W4B O10 Cs2 91.9(11) 1_545 . ?
W4B O10 Cs2 95.3(10) . . ?
W4A O10 Cs2 91.2(10) 1_545 . ?
W4A O10 Cs2 86.6(11) . 1_655 ?
W4B O10 Cs2 83.7(10) 1_545 1_655 ?
W4B O10 Cs2 87.9(10) . 1_655 ?
W4A O10 Cs2 84.5(9) 1_545 1_655 ?
Cs2 O10 Cs2 172.9(8) . 1_655 ?
W4A O11 W4B 15.0(3) . . ?
W4A O11 W5 143.2(13) . . ?
W4B O11 W5 141.0(13) . . ?
W4A O11 Cs2 114.1(11) . 1_665 ?
W4B O11 Cs2 104.2(11) . 1_665 ?
W5 O11 Cs2 96.0(7) . 1_665 ?
W4A O11 Cs2 104.0(10) . 1_655 ?
W4B O11 Cs2 113.3(11) . 1_655 ?
W5 O11 Cs2 104.0(8) . 1_655 ?
Cs2 O11 Cs2 74.7(5) 1_665 1_655 ?
W4A O12 W4B 15.0(4) . . ?
W4A O12 W6 139.9(18) . . ?
W4B O12 W6 142.5(19) . . ?
W4A O12 Cs2 114.7(15) . 1_565 ?
W4B O12 Cs2 104.8(14) . 1_565 ?
W6 O12 Cs2 103.3(11) . 1_565 ?
W4A O12 Cs2 105.2(14) . . ?
W4B O12 Cs2 114.3(15) . . ?
W6 O12 Cs2 97.2(11) . . ?
Cs2 O12 Cs2 73.6(7) 1_565 . ?
W5 O13 Cs3 136.5(18) . 2_766 ?
W5 O13 Cs3 134.9(17) . 2_756 ?
Cs3 O13 Cs3 75.0(7) 2_766 2_756 ?
W5 O13 Cs3 106.0(14) . 1_565 ?
Cs3 O13 Cs3 75.6(9) 2_766 1_565 ?
Cs3 O13 Cs3 114.4(10) 2_756 1_565 ?
W5 O13 Cs3 106.3(15) . . ?
Cs3 O13 Cs3 114.5(10) 2_766 . ?
Cs3 O13 Cs3 71.2(8) 2_756 . ?
Cs3 O13 Cs3 70.3(7) 1_565 . ?
W5 O14 W5 172.8(10) 1_545 . ?
W5 O14 Cs2 90.2(6) 1_545 1_655 ?
W5 O14 Cs2 95.3(6) . 1_655 ?
W5 O14 Cs3 86.4(6) 1_545 . ?
W5 O14 Cs3 88.3(6) . . ?
Cs2 O14 Cs3 175.8(6) 1_655 . ?
W5 O15 W6 170.1(8) . . ?
W5 O15 Cs3 99.9(10) . . ?
W6 O15 Cs3 89.6(9) . . ?
W5 O15 Cs3 90.7(9) . 1_565 ?
W6 O15 Cs3 95.6(10) . 1_565 ?
Cs3 O15 Cs3 66.7(2) . 1_565 ?
W5 O16 W6 138.1(7) . 1_655 ?
W5 O16 Cs2 102.2(11) . 1_665 ?
W6 O16 Cs2 110.6(13) 1_655 1_665 ?
W5 O16 Cs2 111.2(13) . 1_655 ?
W6 O16 Cs2 102.6(11) 1_655 1_655 ?
Cs2 O16 Cs2 73.7(3) 1_665 1_655 ?
W6 O17 Cs3 132.9(9) . 2_656 ?
W6 O17 Cs3 104.9(8) . . ?
Cs3 O17 Cs3 70.7(6) 2_656 . ?
W6 O17 Cs3 137.7(9) . 2_666 ?
Cs3 O17 Cs3 78.6(5) 2_656 2_666 ?
Cs3 O17 Cs3 113.4(7) . 2_666 ?
W6 O17 Cs3 109.7(9) . 1_565 ?
Cs3 O17 Cs3 113.5(7) 2_656 1_565 ?
Cs3 O17 Cs3 74.4(5) . 1_565 ?
Cs3 O17 Cs3 66.2(5) 2_666 1_565 ?
W6 O18 W6 155.5(13) . 1_545 ?
W6 O18 Cs2 101.5(9) . . ?
W6 O18 Cs2 97.0(7) 1_545 . ?
W6 O18 Cs3 77.9(8) . . ?
W6 O18 Cs3 81.7(6) 1_545 . ?
Cs2 O18 Cs3 172.6(9) . . ?

_refine_diff_density_max         6.028
_refine_diff_density_min         -9.635
_refine_diff_density_rms         0.688


_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Tl4W11O35
_database_code_depnum_ccdc_archive 'CCDC 2211346'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_Tl4W11O35           
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form

_audit_creation_date             2021-11-04
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
_shelx_SHELXL_version_number     2017/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'O35 Tl4 W11'
_chemical_formula_sum            'O35 Tl4 W11'
_chemical_formula_weight         3399.83
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tl Tl -2.8358 9.6688 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           3
_space_group_name_H-M_alt        'P 1 2 1'
_space_group_name_Hall           'P 2y'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'

_cell_length_a                   7.3114(8)
_cell_length_b                   3.8154(4)
_cell_length_c                   25.877(3)
_cell_angle_alpha                90
_cell_angle_beta                 98.109(3)
_cell_angle_gamma                90
_cell_volume                     714.65(13)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    9826
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      33.33
_cell_measurement_theta_min      2.38
_shelx_estimated_absorpt_T_max   0.349
_shelx_estimated_absorpt_T_min   0.082
_exptl_absorpt_coefficient_mu    66.626
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.3225
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1388 before and 0.0639 after correction. The Ratio of minimum to maximum transmission is 0.4320. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    7.900
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             1418
_exptl_crystal_size_max          0.075
_exptl_crystal_size_mid          0.054
_exptl_crystal_size_min          0.02
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0616
_diffrn_reflns_av_unetI/netI     0.0519
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       39
_diffrn_reflns_limit_l_min       -39
_diffrn_reflns_number            18889
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.335
_diffrn_reflns_theta_min         2.385
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_reflns_Friedel_coverage         0.775
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.998
_reflns_number_gt                5390
_reflns_number_total             5465
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         9.229
_refine_diff_density_min         -8.440
_refine_diff_density_rms         1.003
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.080
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     157
_refine_ls_number_reflns         5465
_refine_ls_number_restraints     3
_refine_ls_R_factor_all          0.0534
_refine_ls_R_factor_gt           0.0527
_refine_ls_restrained_S_all      1.083
_refine_ls_shift/su_max          0.263
_refine_ls_shift/su_mean         0.011
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0778P)²+41.4341P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1368
_refine_ls_wR_factor_ref         0.1378
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.25781
 0.25283 0.26478 0.22458
2. Restrained distances
 W1A-O1
 1.7 with sigma of 0.03
 W3-O8
 1.75 with sigma of 0.02
3. Others
 0.5*[Sof(Tl1)]+1*[Sof(Tl2)]+1*[Sof(Tl3)]=2 with esd of 0
 Sof(W1A)=0.5*(1-FVAR(2))
 Sof(W1B)=0.5*FVAR(2)
 Fixed Sof: O1(0.5)
 Fixed Y: Tl1(0)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1A W 0.000000 0.599(2) 0.000000 -0.0004(7) Uani 0.87(2) 2 d DS T P . .
W1B W 0.000000 0.446(12) 0.000000 0.013(6) Uani 0.13(2) 2 d S T P . .
W2 W 0.3184(3) 0.4755(16) 0.12301(7) 0.0161(5) Uani 1 1 d . . . . .
W3 W 0.8148(3) 0.4536(15) 0.12326(5) 0.0092(4) Uani 1 1 d D . . . .
W4 W 0.6278(3) 0.5709(14) 0.25006(3) 0.0089(4) Uani 1 1 d . . . . .
W5 W 0.9459(2) 0.5792(15) 0.37590(6) 0.0058(2) Uani 1 1 d . . . . .
W6 W 0.4348(3) 0.4716(15) 0.37640(7) 0.0073(3) Uani 1 1 d . . . . .
Tl1 Tl 0.500000 0.000000 0.000000 0.0597(14) Uani 0.884(6) 2 d S T P . .
Tl2 Tl 0.1297(7) 0.0387(17) 0.25698(8) 0.0448(6) Uani 0.882(3) 1 d . . P . .
Tl3 Tl 0.7413(12) 0.0232(14) 0.49272(9) 0.0509(11) Uani 0.676(3) 1 d . . P . .
O1 O 0.070(5) 1.006(9) -0.005(2) 0.008(9) Uiso 0.5 1 d D . P . .
O2 O 0.153(3) 0.503(5) -0.0508(8) 0.003(3) Uiso 1 1 d . . . . .
O3 O 0.206(4) 0.636(10) 0.0540(11) 0.025(6) Uiso 1 1 d . . . . .
O4 O 0.343(4) 0.021(9) 0.1279(10) 0.015(6) Uiso 1 1 d . . . . .
O5 O 0.417(4) 0.617(10) 0.1896(12) 0.022(5) Uiso 1 1 d . . . . .
O6 O 0.550(5) 0.517(6) 0.0989(7) 0.015(4) Uiso 1 1 d . . . . .
O7 O 0.074(5) 0.523(7) 0.1421(7) 0.017(4) Uiso 1 1 d . . . . .
O8 O 0.800(4) 0.037(5) 0.1074(11) 0.020(6) Uiso 1 1 d D . . . .
O9 O 0.775(3) 0.507(6) 0.1912(10) 0.011(5) Uiso 1 1 d . . . . .
O10 O 0.463(3) 0.514(5) 0.2932(8) 0.005(4) Uiso 1 1 d . . . . .
O11 O 0.553(4) 1.014(10) 0.2408(11) 0.025(6) Uiso 1 1 d . . . . .
O12 O 0.833(4) 0.622(10) 0.2980(11) 0.023(5) Uiso 1 1 d . . . . .
O13 O 1.028(4) 0.629(10) 0.4398(12) 0.024(5) Uiso 1 1 d . . . . .
O14 O 0.974(6) 1.046(14) 0.3827(16) 0.043(11) Uiso 1 1 d . . . . .
O15 O 1.171(5) 0.539(6) 0.3481(6) 0.012(3) Uiso 1 1 d . . . . .
O16 O 0.690(4) 0.531(6) 0.3843(6) 0.011(3) Uiso 1 1 d . . . . .
O17 O 0.414(4) 0.520(7) 0.4423(11) 0.017(5) Uiso 1 1 d . . . . .
O18 O 0.419(2) 0.017(4) 0.3559(8) 0.002(3) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1A W1B 0.58(4) . ?
W1A W1B 3.23(4) 1_565 ?
W1A Tl1 3.964(3) 1_465 ?
W1A Tl1 3.964(3) 1_565 ?
W1A O1 1.65(3) 2 ?
W1A O1 1.65(3) . ?
W1A O1 2.32(3) 2_545 ?
W1A O1 2.32(3) 1_545 ?
W1A O2 1.88(2) . ?
W1A O2 1.88(2) 2 ?
W1A O3 1.91(3) . ?
W1A O3 1.91(3) 2 ?
W1B Tl1 4.033(19) . ?
W1B Tl1 4.033(19) 1_455 ?
W1B O1 2.20(5) . ?
W1B O1 1.76(5) 1_545 ?
W1B O1 1.76(5) 2_545 ?
W1B O1 2.20(5) 2 ?
W1B O2 1.85(2) 2 ?
W1B O2 1.85(2) . ?
W1B O3 2.04(3) 2 ?
W1B O3 2.04(3) . ?
W2 Tl1 4.134(3) 1_565 ?
W2 Tl1 4.047(4) . ?
W2 Tl2 4.248(4) . ?
W2 Tl2 4.460(4) 1_565 ?
W2 O3 1.96(3) . ?
W2 O4 2.09(4) 1_565 ?
W2 O4 1.74(4) . ?
W2 O5 1.85(3) . ?
W2 O6 1.89(3) . ?
W2 O7 1.93(4) . ?
W3 Tl1 4.213(3) 1_565 ?
W3 Tl1 4.049(3) . ?
W3 Tl2 4.187(4) 1_655 ?
W3 Tl2 4.473(4) 1_665 ?
W3 O2 1.93(2) 2_655 ?
W3 O6 1.97(3) . ?
W3 O7 1.91(4) 1_655 ?
W3 O8 1.643(19) . ?
W3 O8 2.26(2) 1_565 ?
W3 O9 1.83(3) . ?
W4 Tl2 4.196(6) . ?
W4 Tl2 4.062(6) 1_665 ?
W4 Tl2 4.082(6) 1_565 ?
W4 Tl2 4.175(6) 1_655 ?
W4 O5 2.04(3) . ?
W4 O9 2.00(3) . ?
W4 O10 1.77(2) . ?
W4 O11 1.79(4) . ?
W4 O11 2.20(4) 1_545 ?
W4 O12 1.82(3) . ?
W5 Tl2 4.086(4) 1_655 ?
W5 Tl2 3.939(4) 1_665 ?
W5 Tl3 4.370(5) 2_756 ?
W5 Tl3 4.179(5) 2_766 ?
W5 Tl3 3.940(5) 1_565 ?
W5 Tl3 4.141(5) . ?
W5 O12 2.08(3) . ?
W5 O13 1.69(3) . ?
W5 O14 1.80(5) . ?
W5 O14 2.05(5) 1_545 ?
W5 O15 1.89(3) . ?
W5 O16 1.92(3) . ?
W6 Tl2 4.155(4) 1_565 ?
W6 Tl2 3.913(4) . ?
W6 Tl3 3.887(5) . ?
W6 Tl3 4.158(5) 2_656 ?
W6 Tl3 4.334(5) 2_666 ?
W6 Tl3 4.075(5) 1_565 ?
W6 O10 2.20(2) . ?
W6 O15 1.98(3) 1_455 ?
W6 O16 1.86(3) . ?
W6 O17 1.74(3) . ?
W6 O18 2.147(16) 1_565 ?
W6 O18 1.813(16) . ?
Tl1 Tl1 3.8154(4) 1_565 ?
Tl1 Tl1 3.8154(4) 1_545 ?
Tl1 O1 3.13(3) 1_545 ?
Tl1 O1 3.13(3) 2_645 ?
Tl1 O2 3.30(2) 2_655 ?
Tl1 O2 3.29(2) 1_545 ?
Tl1 O2 3.29(2) 2_645 ?
Tl1 O2 3.30(2) . ?
Tl1 O3 3.06(3) 1_545 ?
Tl1 O3 3.06(3) 2_645 ?
Tl1 O3 3.65(3) 2_655 ?
Tl1 O3 3.65(3) . ?
Tl1 O4 3.65(3) 2_655 ?
Tl1 O4 3.65(3) . ?
Tl1 O6 3.13(2) 1_545 ?
Tl1 O6 3.21(2) 2_655 ?
Tl1 O6 3.21(2) . ?
Tl1 O6 3.13(2) 2_645 ?
Tl1 O8 3.29(3) 2_655 ?
Tl1 O8 3.29(3) . ?
Tl2 Tl2 3.8154(4) 1_545 ?
Tl2 Tl2 3.8154(4) 1_565 ?
Tl2 O4 3.88(3) . ?
Tl2 O5 3.66(3) . ?
Tl2 O5 3.33(3) 1_545 ?
Tl2 O7 3.54(2) 1_545 ?
Tl2 O7 3.48(2) . ?
Tl2 O9 3.40(2) 1_455 ?
Tl2 O9 3.54(2) 1_445 ?
Tl2 O10 3.07(2) . ?
Tl2 O10 3.19(2) 1_545 ?
Tl2 O11 3.18(3) 1_545 ?
Tl2 O12 3.00(3) 1_445 ?
Tl2 O12 3.38(3) 1_455 ?
Tl2 O14 3.60(4) 1_445 ?
Tl2 O15 3.01(2) 1_455 ?
Tl2 O15 3.01(2) 1_445 ?
Tl2 O18 3.083(19) . ?
Tl3 Tl3 3.601(18) 2_656 ?
Tl3 Tl3 3.748(18) 2_756 ?
Tl3 Tl3 3.8154(4) 1_565 ?
Tl3 Tl3 3.8154(4) 1_545 ?
Tl3 O13 3.23(3) 2_756 ?
Tl3 O13 3.06(3) 1_545 ?
Tl3 O13 2.70(3) 2_746 ?
Tl3 O13 3.53(3) . ?
Tl3 O14 3.58(4) 2_746 ?
Tl3 O14 3.52(4) 1_545 ?
Tl3 O16 3.353(19) 1_545 ?
Tl3 O16 3.388(18) . ?
Tl3 O17 3.19(3) . ?
Tl3 O17 3.20(3) 1_545 ?
Tl3 O17 2.87(3) 2_656 ?
Tl3 O17 2.89(3) 2_646 ?
Tl3 O18 3.97(2) . ?
O1 O1 1.08(7) 2 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W1B W1A W1B 180.000(17) . 1_565 ?
W1B W1A Tl1 112.73(9) . 1_465 ?
W1B W1A Tl1 67.27(10) 1_565 1_465 ?
W1B W1A Tl1 67.27(10) 1_565 1_565 ?
W1B W1A Tl1 112.73(11) . 1_565 ?
W1B W1A O1 13.4(8) . 2_545 ?
W1B W1A O1 160.9(13) . . ?
W1B W1A O1 13.4(8) . 1_545 ?
W1B W1A O1 160.9(13) . 2 ?
W1B W1A O2 78.8(6) . . ?
W1B W1A O2 78.8(6) . 2 ?
W1B W1A O3 94.3(12) . . ?
W1B W1A O3 94.3(12) . 2 ?
Tl1 W1A Tl1 134.5(2) 1_565 1_465 ?
O1 W1A W1B 166.6(8) 1_545 1_565 ?
O1 W1A W1B 166.6(8) 2_545 1_565 ?
O1 W1A W1B 19.1(13) 2 1_565 ?
O1 W1A W1B 19.1(13) . 1_565 ?
O1 W1A Tl1 86.0(13) 2 1_565 ?
O1 W1A Tl1 86.0(13) . 1_465 ?
O1 W1A Tl1 125.8(8) 1_545 1_465 ?
O1 W1A Tl1 125.8(8) 2_545 1_565 ?
O1 W1A Tl1 99.6(8) 2_545 1_465 ?
O1 W1A Tl1 99.6(8) 1_545 1_565 ?
O1 W1A Tl1 48.7(13) 2 1_465 ?
O1 W1A Tl1 48.7(13) . 1_565 ?
O1 W1A O1 174.3(7) . 2_545 ?
O1 W1A O1 147(2) 2 2_545 ?
O1 W1A O1 26.9(17) 2_545 1_545 ?
O1 W1A O1 174.3(7) 2 1_545 ?
O1 W1A O1 147(2) . 1_545 ?
O1 W1A O1 38(3) 2 . ?
O1 W1A O2 117.1(18) 2 . ?
O1 W1A O2 84.9(17) . . ?
O1 W1A O2 117.1(18) . 2 ?
O1 W1A O2 84.9(17) 2 2 ?
O1 W1A O3 95(2) . 2 ?
O1 W1A O3 76(2) 2 2 ?
O1 W1A O3 76(2) . . ?
O1 W1A O3 95(2) 2 . ?
O2 W1A W1B 101.2(6) 2 1_565 ?
O2 W1A W1B 101.2(6) . 1_565 ?
O2 W1A Tl1 135.7(6) 2 1_565 ?
O2 W1A Tl1 55.6(6) 2 1_465 ?
O2 W1A Tl1 55.6(6) . 1_565 ?
O2 W1A Tl1 135.7(6) . 1_465 ?
O2 W1A O1 90.2(13) 2 1_545 ?
O2 W1A O1 90.2(13) . 2_545 ?
O2 W1A O1 67.5(13) 2 2_545 ?
O2 W1A O1 67.5(13) . 1_545 ?
O2 W1A O2 157.6(12) 2 . ?
O2 W1A O3 89.4(8) . 2 ?
O2 W1A O3 92.3(8) . . ?
O2 W1A O3 89.4(8) 2 . ?
O2 W1A O3 92.3(8) 2 2 ?
O3 W1A W1B 85.7(12) 2 1_565 ?
O3 W1A W1B 85.7(12) . 1_565 ?
O3 W1A Tl1 127.1(10) . 1_465 ?
O3 W1A Tl1 48.6(9) . 1_565 ?
O3 W1A Tl1 127.1(10) 2 1_565 ?
O3 W1A Tl1 48.6(9) 2 1_465 ?
O3 W1A O1 101.1(17) . 2_545 ?
O3 W1A O1 101.1(16) 2 1_545 ?
O3 W1A O1 87.4(16) 2 2_545 ?
O3 W1A O1 87.4(16) . 1_545 ?
O3 W1A O3 171(2) . 2 ?
W1A W1B W1A 180.0 . 1_545 ?
W1A W1B Tl1 115.0(6) . 1_455 ?
W1A W1B Tl1 65.0(6) 1_545 1_455 ?
W1A W1B Tl1 115.0(6) . . ?
W1A W1B Tl1 65.0(6) 1_545 . ?
W1A W1B O1 162.2(12) . 2_545 ?
W1A W1B O1 14.2(10) . . ?
W1A W1B O1 14.2(10) . 2 ?
W1A W1B O1 162.2(12) . 1_545 ?
W1A W1B O2 83.3(15) . . ?
W1A W1B O2 83.3(15) . 2 ?
W1A W1B O3 69.1(16) . 2 ?
W1A W1B O3 69.1(16) . . ?
Tl1 W1B Tl1 130.1(11) 1_455 . ?
O1 W1B W1A 165.8(10) 2 1_545 ?
O1 W1B W1A 17.8(12) 2_545 1_545 ?
O1 W1B W1A 17.8(12) 1_545 1_545 ?
O1 W1B W1A 165.8(10) . 1_545 ?
O1 W1B Tl1 128.7(12) . 1_455 ?
O1 W1B Tl1 128.7(12) 2 . ?
O1 W1B Tl1 47.7(11) 2_545 1_455 ?
O1 W1B Tl1 82.5(14) 2_545 . ?
O1 W1B Tl1 101.1(10) 2 1_455 ?
O1 W1B Tl1 47.7(11) 1_545 . ?
O1 W1B Tl1 101.1(10) . . ?
O1 W1B Tl1 82.5(14) 1_545 1_455 ?
O1 W1B O1 148(2) 2_545 2 ?
O1 W1B O1 36(2) 2_545 1_545 ?
O1 W1B O1 176.3(9) 2_545 . ?
O1 W1B O1 176.3(9) 1_545 2 ?
O1 W1B O1 28(2) . 2 ?
O1 W1B O1 148(2) 1_545 . ?
O1 W1B O2 112(2) 2_545 . ?
O1 W1B O2 81.6(19) 2_545 2 ?
O1 W1B O2 81.6(19) 1_545 . ?
O1 W1B O2 112(2) 1_545 2 ?
O1 W1B O3 119(2) 1_545 2 ?
O1 W1B O3 101(2) 2_545 2 ?
O1 W1B O3 119(2) 2_545 . ?
O1 W1B O3 101(2) 1_545 . ?
O2 W1B W1A 96.7(15) 2 1_545 ?
O2 W1B W1A 96.7(15) . 1_545 ?
O2 W1B Tl1 54.0(8) . . ?
O2 W1B Tl1 133.4(10) . 1_455 ?
O2 W1B Tl1 54.0(8) 2 1_455 ?
O2 W1B Tl1 133.4(10) 2 . ?
O2 W1B O1 71.4(17) 2 2 ?
O2 W1B O1 95(2) . 2 ?
O2 W1B O1 95(2) 2 . ?
O2 W1B O1 71.4(17) . . ?
O2 W1B O2 167(3) 2 . ?
O2 W1B O3 89.0(10) . . ?
O2 W1B O3 89.0(10) 2 2 ?
O2 W1B O3 86.2(10) . 2 ?
O2 W1B O3 86.2(10) 2 . ?
O3 W1B W1A 110.9(16) . 1_545 ?
O3 W1B W1A 110.9(16) 2 1_545 ?
O3 W1B Tl1 64.4(10) 2 1_455 ?
O3 W1B Tl1 64.4(10) . . ?
O3 W1B Tl1 137.1(9) . 1_455 ?
O3 W1B Tl1 137.1(9) 2 . ?
O3 W1B O1 77(2) . 2 ?
O3 W1B O1 77(2) 2 . ?
O3 W1B O1 62.5(19) . . ?
O3 W1B O1 62.5(19) 2 2 ?
O3 W1B O3 138(3) . 2 ?
Tl1 W2 Tl1 55.58(3) . 1_565 ?
Tl1 W2 Tl2 174.09(11) 1_565 . ?
Tl1 W2 Tl2 130.27(11) . . ?
Tl1 W2 Tl2 177.69(11) . 1_565 ?
Tl1 W2 Tl2 122.23(10) 1_565 1_565 ?
Tl2 W2 Tl2 51.90(4) . 1_565 ?
O3 W2 Tl1 64.2(10) . . ?
O3 W2 Tl1 44.3(9) . 1_565 ?
O3 W2 Tl2 115.0(10) . 1_565 ?
O3 W2 Tl2 136.5(9) . . ?
O3 W2 O4 76.4(13) . 1_565 ?
O4 W2 Tl1 117.3(8) 1_565 . ?
O4 W2 Tl1 62.0(8) 1_565 1_565 ?
O4 W2 Tl1 64.5(9) . . ?
O4 W2 Tl1 119.7(9) . 1_565 ?
O4 W2 Tl2 117.5(9) . 1_565 ?
O4 W2 Tl2 60.4(8) 1_565 1_565 ?
O4 W2 Tl2 66.0(9) . . ?
O4 W2 Tl2 112.1(8) 1_565 . ?
O4 W2 O3 113.8(14) . . ?
O4 W2 O4 167.7(17) . 1_565 ?
O4 W2 O5 101.5(15) . . ?
O4 W2 O6 91.2(13) . . ?
O4 W2 O7 99.5(13) . . ?
O5 W2 Tl1 137.2(9) . . ?
O5 W2 Tl1 116.7(11) . 1_565 ?
O5 W2 Tl2 59.0(10) . . ?
O5 W2 Tl2 42.2(9) . 1_565 ?
O5 W2 O3 144.7(18) . . ?
O5 W2 O4 68.5(14) . 1_565 ?
O5 W2 O6 91.8(11) . . ?
O5 W2 O7 89.3(10) . . ?
O6 W2 Tl1 46.0(7) . 1_565 ?
O6 W2 Tl1 50.9(6) . . ?
O6 W2 Tl2 135.3(7) . . ?
O6 W2 Tl2 127.2(7) . 1_565 ?
O6 W2 O3 87.3(11) . . ?
O6 W2 O4 82.1(11) . 1_565 ?
O6 W2 O7 168.8(10) . . ?
O7 W2 Tl1 131.5(7) . . ?
O7 W2 Tl1 124.1(7) . 1_565 ?
O7 W2 Tl2 49.9(7) . 1_565 ?
O7 W2 Tl2 53.8(6) . . ?
O7 W2 O3 85.3(10) . . ?
O7 W2 O4 88.0(11) . 1_565 ?
Tl1 W3 Tl1 54.97(2) . 1_565 ?
Tl1 W3 Tl2 132.42(11) . 1_655 ?
Tl1 W3 Tl2 120.35(10) 1_565 1_665 ?
Tl1 W3 Tl2 174.87(10) . 1_665 ?
Tl2 W3 Tl1 172.22(10) 1_655 1_565 ?
Tl2 W3 Tl2 52.15(4) 1_655 1_665 ?
O2 W3 Tl1 53.9(6) 2_655 . ?
O2 W3 Tl1 49.1(6) 2_655 1_565 ?
O2 W3 Tl2 135.3(6) 2_655 1_655 ?
O2 W3 Tl2 125.6(6) 2_655 1_665 ?
O2 W3 O6 85.8(8) 2_655 . ?
O2 W3 O8 74.8(9) 2_655 1_565 ?
O6 W3 Tl1 51.3(6) . . ?
O6 W3 Tl1 44.6(7) . 1_565 ?
O6 W3 Tl2 124.2(6) . 1_665 ?
O6 W3 Tl2 135.5(6) . 1_655 ?
O6 W3 O8 78.6(10) . 1_565 ?
O7 W3 Tl1 122.8(7) 1_655 1_565 ?
O7 W3 Tl1 134.0(7) 1_655 . ?
O7 W3 Tl2 49.3(7) 1_655 1_665 ?
O7 W3 Tl2 55.3(6) 1_655 1_655 ?
O7 W3 O2 89.0(8) 1_655 2_655 ?
O7 W3 O6 164.4(10) 1_655 . ?
O7 W3 O8 85.9(10) 1_655 1_565 ?
O8 W3 Tl1 105.7(7) 1_565 . ?
O8 W3 Tl1 51.7(10) . . ?
O8 W3 Tl1 50.9(7) 1_565 1_565 ?
O8 W3 Tl1 106.3(10) . 1_565 ?
O8 W3 Tl2 81.3(10) . 1_655 ?
O8 W3 Tl2 121.9(7) 1_565 1_655 ?
O8 W3 Tl2 69.8(7) 1_565 1_665 ?
O8 W3 Tl2 133.2(10) . 1_665 ?
O8 W3 O2 82.2(12) . 2_655 ?
O8 W3 O6 90.8(12) . . ?
O8 W3 O7 103.0(12) . 1_655 ?
O8 W3 O8 155.2(17) . 1_565 ?
O8 W3 O9 109.5(13) . . ?
O9 W3 Tl1 121.8(7) . 1_565 ?
O9 W3 Tl1 130.8(8) . . ?
O9 W3 Tl2 48.5(8) . 1_665 ?
O9 W3 Tl2 52.6(7) . 1_655 ?
O9 W3 O2 167.9(10) . 2_655 ?
O9 W3 O6 90.6(10) . . ?
O9 W3 O7 91.5(10) . 1_655 ?
O9 W3 O8 93.1(10) . 1_565 ?
Tl2 W4 Tl2 54.87(8) 1_565 . ?
Tl2 W4 Tl2 174.30(9) 1_665 . ?
Tl2 W4 Tl2 121.72(11) 1_655 . ?
Tl2 W4 Tl2 174.15(9) 1_565 1_655 ?
Tl2 W4 Tl2 55.17(8) 1_665 1_655 ?
Tl2 W4 Tl2 127.72(12) 1_665 1_565 ?
O5 W4 Tl2 125.0(9) . 1_665 ?
O5 W4 Tl2 60.6(9) . . ?
O5 W4 Tl2 129.6(9) . 1_655 ?
O5 W4 Tl2 54.2(9) . 1_565 ?
O5 W4 O11 81.4(14) . 1_545 ?
O9 W4 Tl2 122.5(7) . . ?
O9 W4 Tl2 131.7(7) . 1_565 ?
O9 W4 Tl2 53.8(7) . 1_655 ?
O9 W4 Tl2 60.5(7) . 1_665 ?
O9 W4 O5 81.6(8) . . ?
O9 W4 O11 87.3(10) . 1_545 ?
O10 W4 Tl2 40.5(7) . . ?
O10 W4 Tl2 136.0(7) . 1_665 ?
O10 W4 Tl2 48.2(6) . 1_565 ?
O10 W4 Tl2 126.0(6) . 1_655 ?
O10 W4 O5 89.2(10) . . ?
O10 W4 O9 162.5(9) . . ?
O10 W4 O11 76.6(10) . 1_545 ?
O10 W4 O11 88.6(11) . . ?
O10 W4 O12 98.9(9) . . ?
O11 W4 Tl2 129.8(8) 1_545 1_665 ?
O11 W4 Tl2 48.1(8) 1_545 . ?
O11 W4 Tl2 102.2(10) . . ?
O11 W4 Tl2 81.3(10) . 1_665 ?
O11 W4 Tl2 48.1(10) . 1_565 ?
O11 W4 Tl2 135.9(10) . 1_655 ?
O11 W4 Tl2 102.5(8) 1_545 1_565 ?
O11 W4 Tl2 74.9(8) 1_545 1_655 ?
O11 W4 O5 68.3(14) . . ?
O11 W4 O9 101.6(12) . . ?
O11 W4 O11 146.5(16) . 1_545 ?
O11 W4 O12 101.4(16) . . ?
O12 W4 Tl2 125.3(10) . 1_565 ?
O12 W4 Tl2 52.2(11) . 1_655 ?
O12 W4 Tl2 131.4(10) . . ?
O12 W4 Tl2 43.0(10) . 1_665 ?
O12 W4 O5 166.9(16) . . ?
O12 W4 O9 93.0(11) . . ?
O12 W4 O11 110.4(14) . 1_545 ?
Tl2 W5 Tl2 56.74(5) 1_665 1_655 ?
Tl2 W5 Tl3 128.05(10) 1_665 1_565 ?
Tl2 W5 Tl3 128.69(12) 1_665 2_756 ?
Tl2 W5 Tl3 128.09(13) 1_655 2_766 ?
Tl2 W5 Tl3 118.83(9) 1_655 . ?
Tl2 W5 Tl3 98.59(9) 1_655 2_756 ?
Tl2 W5 Tl3 104.32(9) 1_665 2_766 ?
Tl2 W5 Tl3 175.12(9) 1_665 . ?
Tl3 W5 Tl2 174.69(13) 1_565 1_655 ?
Tl3 W5 Tl3 54.9(2) 1_565 2_766 ?
Tl3 W5 Tl3 52.2(2) . 2_756 ?
Tl3 W5 Tl3 80.00(14) . 2_766 ?
Tl3 W5 Tl3 79.95(14) 1_565 2_756 ?
Tl3 W5 Tl3 52.96(6) 2_766 2_756 ?
Tl3 W5 Tl3 56.28(7) 1_565 . ?
O12 W5 Tl2 48.6(9) . 1_665 ?
O12 W5 Tl2 55.7(9) . 1_655 ?
O12 W5 Tl3 127.9(9) . . ?
O12 W5 Tl3 124.7(9) . 1_565 ?
O12 W5 Tl3 152.6(10) . 2_756 ?
O12 W5 Tl3 148.8(10) . 2_766 ?
O13 W5 Tl2 133.2(11) . 1_655 ?
O13 W5 Tl2 126.9(11) . 1_665 ?
O13 W5 Tl3 47.3(11) . 1_565 ?
O13 W5 Tl3 38.5(12) . 2_756 ?
O13 W5 Tl3 57.3(12) . . ?
O13 W5 Tl3 22.9(12) . 2_766 ?
O13 W5 O12 168.7(17) . . ?
O13 W5 O14 76.8(18) . . ?
O13 W5 O14 90.6(17) . 1_545 ?
O13 W5 O15 99.9(12) . . ?
O13 W5 O16 96.9(11) . . ?
O14 W5 Tl2 61.6(11) 1_545 1_655 ?
O14 W5 Tl2 117.9(11) 1_545 1_665 ?
O14 W5 Tl2 121.9(13) . 1_655 ?
O14 W5 Tl2 65.7(13) . 1_665 ?
O14 W5 Tl3 63.2(13) . 1_565 ?
O14 W5 Tl3 107.2(12) 1_545 2_766 ?
O14 W5 Tl3 54.3(11) 1_545 2_756 ?
O14 W5 Tl3 118.9(13) . . ?
O14 W5 Tl3 113.9(11) 1_545 1_565 ?
O14 W5 Tl3 58.1(11) 1_545 . ?
O14 W5 Tl3 58.5(13) . 2_766 ?
O14 W5 Tl3 111.4(13) . 2_756 ?
O14 W5 O12 100.6(15) 1_545 . ?
O14 W5 O12 92.3(17) . . ?
O14 W5 O14 165(2) . 1_545 ?
O14 W5 O15 91.4(15) . . ?
O14 W5 O16 100.5(15) . . ?
O15 W5 Tl2 43.7(7) . 1_655 ?
O15 W5 Tl2 47.8(6) . 1_665 ?
O15 W5 Tl3 82.5(6) . 2_756 ?
O15 W5 Tl3 86.4(7) . 2_766 ?
O15 W5 Tl3 140.5(7) . 1_565 ?
O15 W5 Tl3 131.2(7) . . ?
O15 W5 O12 83.4(9) . . ?
O15 W5 O14 82.6(14) . 1_545 ?
O15 W5 O16 161.3(9) . . ?
O16 W5 Tl2 125.1(5) . 1_665 ?
O16 W5 Tl2 117.7(6) . 1_655 ?
O16 W5 Tl3 112.1(5) . 2_766 ?
O16 W5 Tl3 106.1(6) . 2_756 ?
O16 W5 Tl3 58.3(6) . 1_565 ?
O16 W5 Tl3 54.0(6) . . ?
O16 W5 O12 81.8(9) . . ?
O16 W5 O14 89.0(14) . 1_545 ?
Tl2 W6 Tl2 56.35(5) . 1_565 ?
Tl2 W6 Tl3 128.66(13) 1_565 2_656 ?
Tl2 W6 Tl3 98.09(10) 1_565 2_666 ?
Tl2 W6 Tl3 128.53(13) . 2_666 ?
Tl2 W6 Tl3 105.19(10) . 2_656 ?
Tl2 W6 Tl3 173.82(10) . 1_565 ?
Tl3 W6 Tl2 128.91(11) . . ?
Tl3 W6 Tl2 174.67(12) . 1_565 ?
Tl3 W6 Tl2 117.52(9) 1_565 1_565 ?
Tl3 W6 Tl3 57.21(7) . 1_565 ?
Tl3 W6 Tl3 53.35(6) 2_656 2_666 ?
Tl3 W6 Tl3 79.17(14) 1_565 2_656 ?
Tl3 W6 Tl3 50.6(2) 1_565 2_666 ?
Tl3 W6 Tl3 79.11(14) . 2_666 ?
Tl3 W6 Tl3 53.1(2) . 2_656 ?
O10 W6 Tl2 49.2(5) . 1_565 ?
O10 W6 Tl2 51.6(5) . . ?
O10 W6 Tl3 124.6(5) . 1_565 ?
O10 W6 Tl3 131.9(5) . . ?
O10 W6 Tl3 144.0(5) . 2_666 ?
O10 W6 Tl3 155.6(5) . 2_656 ?
O15 W6 Tl2 49.1(6) 1_455 . ?
O15 W6 Tl2 42.7(7) 1_455 1_565 ?
O15 W6 Tl3 127.7(6) 1_455 1_565 ?
O15 W6 Tl3 81.1(6) 1_455 2_666 ?
O15 W6 Tl3 140.2(7) 1_455 . ?
O15 W6 Tl3 87.6(6) 1_455 2_656 ?
O15 W6 O10 81.3(8) 1_455 . ?
O15 W6 O18 76.6(9) 1_455 1_565 ?
O16 W6 Tl2 126.1(6) . . ?
O16 W6 Tl2 116.2(6) . 1_565 ?
O16 W6 Tl3 112.5(5) . 2_656 ?
O16 W6 Tl3 60.6(6) . . ?
O16 W6 Tl3 105.0(6) . 2_666 ?
O16 W6 Tl3 54.4(6) . 1_565 ?
O16 W6 O10 82.4(7) . . ?
O16 W6 O15 158.9(9) . 1_455 ?
O16 W6 O18 85.8(8) . 1_565 ?
O17 W6 Tl2 134.3(9) . . ?
O17 W6 Tl2 124.0(9) . 1_565 ?
O17 W6 Tl3 48.6(9) . 1_565 ?
O17 W6 Tl3 26.7(9) . 2_666 ?
O17 W6 Tl3 33.6(9) . 2_656 ?
O17 W6 Tl3 53.9(9) . . ?
O17 W6 O10 169.6(10) . . ?
O17 W6 O15 97.6(11) . 1_455 ?
O17 W6 O16 96.1(11) . . ?
O17 W6 O18 112.2(10) . . ?
O17 W6 O18 97.4(10) . 1_565 ?
O18 W6 Tl2 105.9(6) . 1_565 ?
O18 W6 Tl2 46.1(5) 1_565 1_565 ?
O18 W6 Tl2 50.1(6) . . ?
O18 W6 Tl2 102.1(5) 1_565 . ?
O18 W6 Tl3 128.6(5) 1_565 . ?
O18 W6 Tl3 80.3(6) . 2_656 ?
O18 W6 Tl3 135.7(6) . 1_565 ?
O18 W6 Tl3 73.2(5) 1_565 2_666 ?
O18 W6 Tl3 71.8(5) 1_565 1_565 ?
O18 W6 Tl3 79.2(6) . . ?
O18 W6 Tl3 126.1(5) 1_565 2_656 ?
O18 W6 Tl3 132.9(6) . 2_666 ?
O18 W6 O10 72.2(7) 1_565 . ?
O18 W6 O10 78.1(8) . . ?
O18 W6 O15 89.8(9) . 1_455 ?
O18 W6 O16 99.8(9) . . ?
O18 W6 O18 148.8(11) . 1_565 ?
Tl1 Tl1 Tl1 180.0 1_565 1_545 ?
O1 Tl1 Tl1 89.6(6) 2_645 1_565 ?
O1 Tl1 Tl1 90.4(6) 1_545 1_545 ?
O1 Tl1 Tl1 89.6(6) 1_545 1_565 ?
O1 Tl1 Tl1 90.4(6) 2_645 1_545 ?
O1 Tl1 O1 179.1(12) 2_645 1_545 ?
O1 Tl1 O2 43.5(8) 2_645 2_645 ?
O1 Tl1 O2 136.2(8) 1_545 2_655 ?
O1 Tl1 O2 136.2(8) 2_645 . ?
O1 Tl1 O2 43.0(8) 1_545 . ?
O1 Tl1 O2 43.5(8) 1_545 1_545 ?
O1 Tl1 O2 43.0(8) 2_645 2_655 ?
O1 Tl1 O2 137.2(8) 1_545 2_645 ?
O1 Tl1 O2 137.2(8) 2_645 1_545 ?
O1 Tl1 O3 50.7(9) 2_645 2_655 ?
O1 Tl1 O3 128.5(9) 2_645 . ?
O1 Tl1 O3 128.5(9) 1_545 2_655 ?
O1 Tl1 O3 50.7(9) 1_545 . ?
O1 Tl1 O4 114.0(11) 1_545 2_655 ?
O1 Tl1 O4 65.9(11) 1_545 . ?
O1 Tl1 O4 114.0(11) 2_645 . ?
O1 Tl1 O4 65.9(11) 2_645 2_655 ?
O1 Tl1 O6 91.5(11) 2_645 2_655 ?
O1 Tl1 O6 91.5(11) 1_545 . ?
O1 Tl1 O6 88.0(11) 1_545 2_655 ?
O1 Tl1 O6 88.0(11) 2_645 . ?
O1 Tl1 O8 54.6(12) 2_645 . ?
O1 Tl1 O8 54.6(12) 1_545 2_655 ?
O1 Tl1 O8 125.4(12) 1_545 . ?
O1 Tl1 O8 125.4(12) 2_645 2_655 ?
O2 Tl1 Tl1 125.5(3) 2_655 1_545 ?
O2 Tl1 Tl1 54.5(3) . 1_565 ?
O2 Tl1 Tl1 54.5(3) 2_655 1_565 ?
O2 Tl1 Tl1 54.8(3) 2_645 1_545 ?
O2 Tl1 Tl1 54.8(3) 1_545 1_545 ?
O2 Tl1 Tl1 125.2(3) 2_645 1_565 ?
O2 Tl1 Tl1 125.2(3) 1_545 1_565 ?
O2 Tl1 Tl1 125.5(3) . 1_545 ?
O2 Tl1 O2 109.0(7) 2_655 . ?
O2 Tl1 O2 70.7(4) 1_545 . ?
O2 Tl1 O2 70.7(4) 2_645 2_655 ?
O2 Tl1 O2 179.7(6) 1_545 2_655 ?
O2 Tl1 O2 109.6(7) 1_545 2_645 ?
O2 Tl1 O2 179.7(6) 2_645 . ?
O2 Tl1 O3 85.5(6) 2_655 . ?
O2 Tl1 O3 85.5(6) . 2_655 ?
O2 Tl1 O3 133.9(5) 2_645 . ?
O2 Tl1 O3 133.9(5) 1_545 2_655 ?
O2 Tl1 O3 94.2(5) 1_545 . ?
O2 Tl1 O3 94.2(5) 2_645 2_655 ?
O2 Tl1 O3 45.9(5) 2_655 2_655 ?
O2 Tl1 O3 45.9(5) . . ?
O2 Tl1 O4 92.9(6) 2_645 2_655 ?
O2 Tl1 O4 88.5(6) 2_645 . ?
O2 Tl1 O4 88.5(6) 1_545 2_655 ?
O2 Tl1 O4 91.4(6) 2_655 2_655 ?
O2 Tl1 O4 87.1(6) 2_655 . ?
O2 Tl1 O4 87.1(6) . 2_655 ?
O2 Tl1 O4 92.9(6) 1_545 . ?
O2 Tl1 O4 91.4(6) . . ?
O2 Tl1 O8 41.9(5) 2_655 . ?
O2 Tl1 O8 134.0(5) 2_655 2_655 ?
O2 Tl1 O8 134.0(5) . . ?
O2 Tl1 O8 45.8(5) 1_545 2_655 ?
O2 Tl1 O8 138.3(6) 2_645 2_655 ?
O2 Tl1 O8 41.9(5) . 2_655 ?
O2 Tl1 O8 45.8(5) 2_645 . ?
O2 Tl1 O8 138.3(6) 1_545 . ?
O3 Tl1 Tl1 117.0(7) 1_545 1_565 ?
O3 Tl1 Tl1 131.7(6) 2_655 1_545 ?
O3 Tl1 Tl1 63.0(7) 2_645 1_545 ?
O3 Tl1 Tl1 117.0(7) 2_645 1_565 ?
O3 Tl1 Tl1 63.0(7) 1_545 1_545 ?
O3 Tl1 Tl1 131.7(6) . 1_545 ?
O3 Tl1 Tl1 48.3(6) 2_655 1_565 ?
O3 Tl1 Tl1 48.3(6) . 1_565 ?
O3 Tl1 O1 41.7(10) 2_645 2_645 ?
O3 Tl1 O1 138.9(10) 2_645 1_545 ?
O3 Tl1 O1 41.7(10) 1_545 1_545 ?
O3 Tl1 O1 138.9(10) 1_545 2_645 ?
O3 Tl1 O2 129.2(6) 1_545 2_655 ?
O3 Tl1 O2 84.0(6) 1_545 . ?
O3 Tl1 O2 96.2(7) 2_645 1_545 ?
O3 Tl1 O2 50.8(6) 1_545 1_545 ?
O3 Tl1 O2 129.2(6) 2_645 . ?
O3 Tl1 O2 84.0(6) 2_645 2_655 ?
O3 Tl1 O2 50.8(6) 2_645 2_645 ?
O3 Tl1 O2 96.2(7) 1_545 2_645 ?
O3 Tl1 O3 96.6(11) 2_655 . ?
O3 Tl1 O3 165.3(11) 2_645 . ?
O3 Tl1 O3 68.7(6) 1_545 . ?
O3 Tl1 O3 165.3(11) 1_545 2_655 ?
O3 Tl1 O3 68.7(6) 2_645 2_655 ?
O3 Tl1 O3 126.0(14) 1_545 2_645 ?
O3 Tl1 O4 50.3(7) . . ?
O3 Tl1 O4 139.0(8) 1_545 2_655 ?
O3 Tl1 O4 42.7(8) 2_645 2_655 ?
O3 Tl1 O4 139.0(8) 2_645 . ?
O3 Tl1 O4 42.7(8) 1_545 . ?
O3 Tl1 O4 50.3(7) 2_655 2_655 ?
O3 Tl1 O4 127.6(7) . 2_655 ?
O3 Tl1 O4 127.6(7) 2_655 . ?
O3 Tl1 O6 50.8(9) 1_545 1_545 ?
O3 Tl1 O6 129.4(9) 2_645 . ?
O3 Tl1 O6 50.8(9) 2_645 2_645 ?
O3 Tl1 O6 95.7(9) 2_645 1_545 ?
O3 Tl1 O6 95.7(9) 1_545 2_645 ?
O3 Tl1 O6 129.4(9) 1_545 2_655 ?
O3 Tl1 O6 85.5(8) 2_645 2_655 ?
O3 Tl1 O6 85.5(9) 1_545 . ?
O3 Tl1 O8 88.7(7) 2_645 . ?
O3 Tl1 O8 88.7(7) 1_545 2_655 ?
O3 Tl1 O8 93.5(7) 1_545 . ?
O3 Tl1 O8 93.5(7) 2_645 2_655 ?
O4 Tl1 Tl1 91.3(6) 2_655 1_545 ?
O4 Tl1 Tl1 88.7(6) 2_655 1_565 ?
O4 Tl1 Tl1 91.3(6) . 1_545 ?
O4 Tl1 Tl1 88.7(6) . 1_565 ?
O4 Tl1 O4 177.5(11) 2_655 . ?
O6 Tl1 Tl1 126.0(4) 2_645 1_565 ?
O6 Tl1 Tl1 54.0(4) 1_545 1_545 ?
O6 Tl1 Tl1 127.9(4) . 1_545 ?
O6 Tl1 Tl1 52.1(4) 2_655 1_565 ?
O6 Tl1 Tl1 127.9(4) 2_655 1_545 ?
O6 Tl1 Tl1 52.1(4) . 1_565 ?
O6 Tl1 Tl1 54.0(4) 2_645 1_545 ?
O6 Tl1 Tl1 126.0(4) 1_545 1_565 ?
O6 Tl1 O1 88.5(11) 2_645 1_545 ?
O6 Tl1 O1 88.5(11) 1_545 2_645 ?
O6 Tl1 O1 92.1(11) 2_645 2_645 ?
O6 Tl1 O1 92.1(11) 1_545 1_545 ?
O6 Tl1 O2 48.8(7) 1_545 2_645 ?
O6 Tl1 O2 131.3(7) 1_545 . ?
O6 Tl1 O2 131.3(7) 2_645 2_655 ?
O6 Tl1 O2 91.3(6) 2_645 . ?
O6 Tl1 O2 48.1(7) 2_655 . ?
O6 Tl1 O2 48.1(7) . 2_655 ?
O6 Tl1 O2 131.8(7) . 1_545 ?
O6 Tl1 O2 92.4(6) 2_655 1_545 ?
O6 Tl1 O2 87.4(6) . . ?
O6 Tl1 O2 48.8(7) 2_645 1_545 ?
O6 Tl1 O2 91.3(6) 1_545 2_655 ?
O6 Tl1 O2 88.9(7) 1_545 1_545 ?
O6 Tl1 O2 88.9(7) 2_645 2_645 ?
O6 Tl1 O2 87.4(6) 2_655 2_655 ?
O6 Tl1 O2 92.4(6) . 2_645 ?
O6 Tl1 O2 131.8(7) 2_655 2_645 ?
O6 Tl1 O3 83.7(7) 2_655 . ?
O6 Tl1 O3 134.2(8) 1_545 2_655 ?
O6 Tl1 O3 83.7(7) . 2_655 ?
O6 Tl1 O3 45.0(8) . . ?
O6 Tl1 O3 45.0(8) 2_655 2_655 ?
O6 Tl1 O3 134.2(8) 2_645 . ?
O6 Tl1 O3 94.9(7) 1_545 . ?
O6 Tl1 O3 94.9(7) 2_645 2_655 ?
O6 Tl1 O4 137.6(7) 1_545 2_655 ?
O6 Tl1 O4 44.6(8) 2_645 2_655 ?
O6 Tl1 O4 43.9(8) . . ?
O6 Tl1 O4 44.6(8) 1_545 . ?
O6 Tl1 O4 133.9(7) 2_655 . ?
O6 Tl1 O4 43.9(8) 2_655 2_655 ?
O6 Tl1 O4 133.9(7) . 2_655 ?
O6 Tl1 O4 137.6(7) 2_645 . ?
O6 Tl1 O6 73.9(4) 2_645 2_655 ?
O6 Tl1 O6 178.1(7) 2_645 . ?
O6 Tl1 O6 178.1(7) 1_545 2_655 ?
O6 Tl1 O6 108.0(8) 2_645 1_545 ?
O6 Tl1 O6 73.9(4) 1_545 . ?
O6 Tl1 O6 104.2(8) 2_655 . ?
O6 Tl1 O8 46.7(7) 2_655 2_655 ?
O6 Tl1 O8 46.7(7) . . ?
O6 Tl1 O8 134.5(7) 2_645 . ?
O6 Tl1 O8 129.3(7) 2_655 . ?
O6 Tl1 O8 49.4(7) 1_545 . ?
O6 Tl1 O8 129.3(7) . 2_655 ?
O6 Tl1 O8 49.4(7) 2_645 2_655 ?
O6 Tl1 O8 134.5(7) 1_545 2_655 ?
O8 Tl1 Tl1 87.6(4) . 1_565 ?
O8 Tl1 Tl1 87.6(4) 2_655 1_565 ?
O8 Tl1 Tl1 92.4(4) 2_655 1_545 ?
O8 Tl1 Tl1 92.4(4) . 1_545 ?
O8 Tl1 O3 90.4(6) . . ?
O8 Tl1 O3 90.4(6) 2_655 2_655 ?
O8 Tl1 O3 86.3(6) . 2_655 ?
O8 Tl1 O3 86.3(6) 2_655 . ?
O8 Tl1 O4 59.5(7) . . ?
O8 Tl1 O4 120.4(7) 2_655 . ?
O8 Tl1 O4 120.4(7) . 2_655 ?
O8 Tl1 O4 59.5(7) 2_655 2_655 ?
O8 Tl1 O8 175.1(7) . 2_655 ?
W6 Tl2 W5 77.89(4) . 1_445 ?
Tl2 Tl2 W5 63.57(6) 1_545 1_445 ?
Tl2 Tl2 W5 116.43(6) 1_565 1_445 ?
Tl2 Tl2 W6 114.97(6) 1_545 . ?
Tl2 Tl2 W6 65.03(6) 1_565 . ?
Tl2 Tl2 Tl2 180.0 1_565 1_545 ?
Tl2 Tl2 O4 89.0(5) 1_545 . ?
Tl2 Tl2 O4 91.0(5) 1_565 . ?
O4 Tl2 W5 152.6(5) . 1_445 ?
O4 Tl2 W6 115.7(5) . . ?
O5 Tl2 W5 157.5(5) . 1_445 ?
O5 Tl2 W5 120.3(6) 1_545 1_445 ?
O5 Tl2 W6 79.6(5) . . ?
O5 Tl2 W6 106.6(5) 1_545 . ?
O5 Tl2 Tl2 52.9(6) . 1_565 ?
O5 Tl2 Tl2 127.1(6) . 1_545 ?
O5 Tl2 Tl2 118.9(7) 1_545 1_565 ?
O5 Tl2 Tl2 61.1(6) 1_545 1_545 ?
O5 Tl2 O4 43.3(8) . . ?
O5 Tl2 O4 35.0(8) 1_545 . ?
O5 Tl2 O5 66.0(5) 1_545 . ?
O5 Tl2 O7 45.4(8) 1_545 1_545 ?
O5 Tl2 O7 79.4(8) 1_545 . ?
O5 Tl2 O9 119.0(5) 1_545 1_455 ?
O5 Tl2 O9 86.9(6) 1_545 1_445 ?
O5 Tl2 O12 164.3(8) 1_545 1_455 ?
O5 Tl2 O14 141.4(10) 1_545 1_445 ?
O7 Tl2 W5 113.4(5) 1_545 1_445 ?
O7 Tl2 W5 153.3(7) . 1_445 ?
O7 Tl2 W6 115.8(5) . . ?
O7 Tl2 W6 152.0(7) 1_545 . ?
O7 Tl2 Tl2 57.8(4) . 1_565 ?
O7 Tl2 Tl2 122.1(4) . 1_545 ?
O7 Tl2 Tl2 56.3(4) 1_545 1_545 ?
O7 Tl2 Tl2 123.7(4) 1_545 1_565 ?
O7 Tl2 O4 44.4(8) . . ?
O7 Tl2 O4 44.0(8) 1_545 . ?
O7 Tl2 O5 43.7(8) . . ?
O7 Tl2 O5 86.6(7) 1_545 . ?
O7 Tl2 O7 65.9(3) . 1_545 ?
O7 Tl2 O9 84.5(7) . 1_445 ?
O7 Tl2 O14 138.7(10) 1_545 1_445 ?
O7 Tl2 O14 139.1(10) . 1_445 ?
O9 Tl2 W5 107.7(4) 1_455 1_445 ?
O9 Tl2 W5 79.2(4) 1_445 1_445 ?
O9 Tl2 W6 157.0(4) 1_445 . ?
O9 Tl2 W6 118.9(4) 1_455 . ?
O9 Tl2 Tl2 125.0(4) 1_445 1_565 ?
O9 Tl2 Tl2 58.3(4) 1_455 1_565 ?
O9 Tl2 Tl2 55.0(4) 1_445 1_545 ?
O9 Tl2 Tl2 121.7(4) 1_455 1_545 ?
O9 Tl2 O4 86.1(6) 1_445 . ?
O9 Tl2 O4 87.1(6) 1_455 . ?
O9 Tl2 O5 123.3(5) 1_445 . ?
O9 Tl2 O5 83.9(6) 1_455 . ?
O9 Tl2 O7 83.2(7) 1_455 1_545 ?
O9 Tl2 O7 44.5(8) 1_445 1_545 ?
O9 Tl2 O7 45.9(8) 1_455 . ?
O9 Tl2 O9 66.7(5) 1_455 1_445 ?
O9 Tl2 O14 97.8(9) 1_445 1_445 ?
O9 Tl2 O14 97.6(9) 1_455 1_445 ?
O10 Tl2 W5 79.7(4) 1_545 1_445 ?
O10 Tl2 W5 111.6(4) . 1_445 ?
O10 Tl2 W6 72.9(4) 1_545 . ?
O10 Tl2 W6 34.1(4) . . ?
O10 Tl2 Tl2 126.1(4) . 1_545 ?
O10 Tl2 Tl2 53.9(4) . 1_565 ?
O10 Tl2 Tl2 51.1(4) 1_545 1_545 ?
O10 Tl2 Tl2 128.9(4) 1_545 1_565 ?
O10 Tl2 O4 82.8(6) . . ?
O10 Tl2 O4 81.9(6) 1_545 . ?
O10 Tl2 O5 93.0(6) 1_545 . ?
O10 Tl2 O5 46.0(6) . . ?
O10 Tl2 O5 48.6(7) 1_545 1_545 ?
O10 Tl2 O5 85.0(7) . 1_545 ?
O10 Tl2 O7 86.5(7) . . ?
O10 Tl2 O7 83.7(7) 1_545 1_545 ?
O10 Tl2 O7 125.2(8) . 1_545 ?
O10 Tl2 O7 125.3(8) 1_545 . ?
O10 Tl2 O9 111.0(6) . 1_455 ?
O10 Tl2 O9 105.0(6) 1_545 1_445 ?
O10 Tl2 O9 166.7(6) 1_545 1_455 ?
O10 Tl2 O9 168.8(6) . 1_445 ?
O10 Tl2 O10 75.0(5) . 1_545 ?
O10 Tl2 O11 46.7(7) . 1_545 ?
O10 Tl2 O12 91.8(6) . 1_455 ?
O10 Tl2 O12 144.9(5) 1_545 1_455 ?
O10 Tl2 O14 93.3(8) . 1_445 ?
O10 Tl2 O14 93.8(8) 1_545 1_445 ?
O10 Tl2 O18 48.8(5) . . ?
O11 Tl2 W5 122.3(6) 1_545 1_445 ?
O11 Tl2 W6 70.1(6) 1_545 . ?
O11 Tl2 Tl2 91.7(7) 1_545 1_565 ?
O11 Tl2 Tl2 88.3(7) 1_545 1_545 ?
O11 Tl2 O4 51.0(7) 1_545 . ?
O11 Tl2 O5 38.7(8) 1_545 1_545 ?
O11 Tl2 O5 47.1(8) 1_545 . ?
O11 Tl2 O7 84.4(9) 1_545 . ?
O11 Tl2 O7 82.7(9) 1_545 1_545 ?
O11 Tl2 O9 125.5(7) 1_545 1_445 ?
O11 Tl2 O9 129.5(8) 1_545 1_455 ?
O11 Tl2 O10 45.9(8) 1_545 1_545 ?
O11 Tl2 O12 137.7(9) 1_545 1_455 ?
O11 Tl2 O14 123.9(9) 1_545 1_445 ?
O12 Tl2 W5 75.1(6) 1_455 1_445 ?
O12 Tl2 W5 31.2(5) 1_445 1_445 ?
O12 Tl2 W6 78.1(5) 1_455 . ?
O12 Tl2 W6 107.7(6) 1_445 . ?
O12 Tl2 Tl2 48.8(6) 1_455 1_565 ?
O12 Tl2 Tl2 122.0(7) 1_445 1_565 ?
O12 Tl2 Tl2 58.0(7) 1_445 1_545 ?
O12 Tl2 Tl2 131.2(6) 1_455 1_545 ?
O12 Tl2 O4 133.9(8) 1_445 . ?
O12 Tl2 O4 129.4(7) 1_455 . ?
O12 Tl2 O5 118.1(10) 1_445 1_545 ?
O12 Tl2 O5 100.9(8) 1_455 . ?
O12 Tl2 O5 168.9(7) 1_445 . ?
O12 Tl2 O7 128.8(8) 1_455 1_545 ?
O12 Tl2 O7 85.1(8) 1_455 . ?
O12 Tl2 O7 90.0(9) 1_445 1_545 ?
O12 Tl2 O7 125.5(9) 1_445 . ?
O12 Tl2 O9 94.0(7) 1_455 1_445 ?
O12 Tl2 O9 48.2(6) 1_455 1_455 ?
O12 Tl2 O9 85.2(7) 1_445 1_455 ?
O12 Tl2 O9 49.3(7) 1_445 1_445 ?
O12 Tl2 O10 97.1(7) 1_445 1_545 ?
O12 Tl2 O10 141.8(6) 1_445 . ?
O12 Tl2 O11 142.8(10) 1_445 1_545 ?
O12 Tl2 O12 73.1(6) 1_445 1_455 ?
O12 Tl2 O14 54.0(9) 1_455 1_445 ?
O12 Tl2 O14 49.2(10) 1_445 1_445 ?
O12 Tl2 O15 52.1(8) 1_445 1_445 ?
O12 Tl2 O15 93.2(9) 1_445 1_455 ?
O12 Tl2 O18 98.0(6) 1_445 . ?
O14 Tl2 W5 27.1(9) 1_445 1_445 ?
O14 Tl2 W6 60.0(7) 1_445 . ?
O14 Tl2 Tl2 90.4(9) 1_445 1_545 ?
O14 Tl2 Tl2 89.6(9) 1_445 1_565 ?
O14 Tl2 O4 174.8(8) 1_445 . ?
O14 Tl2 O5 134.7(10) 1_445 . ?
O15 Tl2 W5 71.2(5) 1_455 1_445 ?
O15 Tl2 W5 27.7(6) 1_445 1_445 ?
O15 Tl2 W6 70.5(5) 1_445 . ?
O15 Tl2 W6 29.8(6) 1_455 . ?
O15 Tl2 Tl2 50.7(4) 1_445 1_545 ?
O15 Tl2 Tl2 50.7(4) 1_455 1_565 ?
O15 Tl2 Tl2 129.3(4) 1_445 1_565 ?
O15 Tl2 Tl2 129.3(4) 1_455 1_545 ?
O15 Tl2 O4 130.9(7) 1_445 . ?
O15 Tl2 O4 132.5(8) 1_455 . ?
O15 Tl2 O5 89.4(8) 1_455 . ?
O15 Tl2 O5 95.9(8) 1_445 1_545 ?
O15 Tl2 O5 139.0(8) 1_445 . ?
O15 Tl2 O5 135.6(9) 1_455 1_545 ?
O15 Tl2 O7 174.5(6) 1_455 1_545 ?
O15 Tl2 O7 172.9(6) 1_445 . ?
O15 Tl2 O7 108.6(6) 1_455 . ?
O15 Tl2 O7 107.0(6) 1_445 1_545 ?
O15 Tl2 O9 136.5(8) 1_455 1_445 ?
O15 Tl2 O9 89.9(7) 1_445 1_445 ?
O15 Tl2 O9 135.1(8) 1_445 1_455 ?
O15 Tl2 O9 92.5(7) 1_455 1_455 ?
O15 Tl2 O10 100.4(7) 1_455 1_545 ?
O15 Tl2 O10 98.5(7) 1_445 . ?
O15 Tl2 O10 53.2(8) 1_455 . ?
O15 Tl2 O10 52.1(7) 1_445 1_545 ?
O15 Tl2 O11 97.4(9) 1_455 1_545 ?
O15 Tl2 O11 95.3(9) 1_445 1_545 ?
O15 Tl2 O12 99.7(8) 1_445 1_455 ?
O15 Tl2 O12 48.4(8) 1_455 1_455 ?
O15 Tl2 O14 45.3(10) 1_455 1_445 ?
O15 Tl2 O14 46.1(10) 1_445 1_445 ?
O15 Tl2 O15 78.5(4) 1_445 1_455 ?
O15 Tl2 O18 49.7(6) 1_445 . ?
O15 Tl2 O18 52.2(6) 1_455 . ?
O18 Tl2 W5 67.0(3) . 1_445 ?
O18 Tl2 W6 26.8(3) . . ?
O18 Tl2 Tl2 88.5(3) . 1_545 ?
O18 Tl2 Tl2 91.5(3) . 1_565 ?
O18 Tl2 O4 113.7(5) . . ?
O18 Tl2 O5 90.7(6) . 1_545 ?
O18 Tl2 O5 92.2(6) . . ?
O18 Tl2 O7 131.8(7) . 1_545 ?
O18 Tl2 O7 135.1(7) . . ?
O18 Tl2 O9 139.1(5) . 1_445 ?
O18 Tl2 O9 144.6(5) . 1_455 ?
O18 Tl2 O10 48.2(5) . 1_545 ?
O18 Tl2 O11 62.7(6) . 1_545 ?
O18 Tl2 O12 98.8(6) . 1_455 ?
O18 Tl2 O14 61.1(8) . 1_445 ?
W5 Tl3 W6 55.95(5) 1_545 1_545 ?
W5 Tl3 O18 63.5(3) 1_545 . ?
W6 Tl3 W5 80.50(5) . 1_545 ?
W6 Tl3 W6 57.21(7) . 1_545 ?
W6 Tl3 O18 26.7(2) . . ?
Tl3 Tl3 W5 115.47(7) 1_565 1_545 ?
Tl3 Tl3 W5 64.53(7) 1_545 1_545 ?
Tl3 Tl3 W5 124.33(16) 2_656 1_545 ?
Tl3 Tl3 W5 65.80(15) 2_756 1_545 ?
Tl3 Tl3 W6 58.91(7) 1_545 1_545 ?
Tl3 Tl3 W6 121.09(6) 1_565 1_545 ?
Tl3 Tl3 W6 122.78(16) 2_756 . ?
Tl3 Tl3 W6 116.12(8) 1_545 . ?
Tl3 Tl3 W6 68.43(14) 2_656 1_545 ?
Tl3 Tl3 W6 121.09(15) 2_756 1_545 ?
Tl3 Tl3 W6 63.88(8) 1_565 . ?
Tl3 Tl3 W6 67.33(15) 2_656 . ?
Tl3 Tl3 Tl3 90.000(3) 2_756 1_565 ?
Tl3 Tl3 Tl3 90.000(2) 2_656 1_565 ?
Tl3 Tl3 Tl3 90.000(1) 2_756 1_545 ?
Tl3 Tl3 Tl3 168.34(14) 2_656 2_756 ?
Tl3 Tl3 Tl3 90.000(4) 2_656 1_545 ?
Tl3 Tl3 Tl3 180.0(5) 1_565 1_545 ?
Tl3 Tl3 O18 68.0(3) 2_656 . ?
Tl3 Tl3 O18 89.7(2) 1_545 . ?
Tl3 Tl3 O18 123.6(3) 2_756 . ?
Tl3 Tl3 O18 90.3(2) 1_565 . ?
O13 Tl3 W5 24.0(6) 1_545 1_545 ?
O13 Tl3 W5 89.3(7) 2_746 1_545 ?
O13 Tl3 W5 119.9(6) 2_756 1_545 ?
O13 Tl3 W5 70.9(6) . 1_545 ?
O13 Tl3 W6 75.9(6) 1_545 1_545 ?
O13 Tl3 W6 73.8(5) . . ?
O13 Tl3 W6 169.5(7) 2_746 . ?
O13 Tl3 W6 163.9(6) 2_756 1_545 ?
O13 Tl3 W6 103.1(6) 1_545 . ?
O13 Tl3 W6 110.3(5) . 1_545 ?
O13 Tl3 W6 114.7(8) 2_746 1_545 ?
O13 Tl3 W6 107.7(6) 2_756 . ?
O13 Tl3 Tl3 123.8(8) 2_746 1_565 ?
O13 Tl3 Tl3 135.8(6) 2_756 1_545 ?
O13 Tl3 Tl3 60.2(6) 2_756 2_756 ?
O13 Tl3 Tl3 119.4(7) 1_545 1_565 ?
O13 Tl3 Tl3 53.7(7) 2_746 2_756 ?
O13 Tl3 Tl3 44.2(6) 2_756 1_565 ?
O13 Tl3 Tl3 117.5(6) 2_746 2_656 ?
O13 Tl3 Tl3 49.0(6) . 1_565 ?
O13 Tl3 Tl3 131.0(6) . 1_545 ?
O13 Tl3 Tl3 142.3(7) 1_545 2_656 ?
O13 Tl3 Tl3 45.4(6) 1_545 2_756 ?
O13 Tl3 Tl3 112.8(5) 2_756 2_656 ?
O13 Tl3 Tl3 52.5(5) . 2_756 ?
O13 Tl3 Tl3 56.2(8) 2_746 1_545 ?
O13 Tl3 Tl3 133.3(5) . 2_656 ?
O13 Tl3 Tl3 60.6(7) 1_545 1_545 ?
O13 Tl3 O13 104.8(5) 1_545 2_756 ?
O13 Tl3 O13 56.4(10) 2_756 . ?
O13 Tl3 O13 70.4(6) 1_545 . ?
O13 Tl3 O13 67.2(11) 2_746 1_545 ?
O13 Tl3 O13 79.6(8) 2_746 2_756 ?
O13 Tl3 O13 105.4(5) 2_746 . ?
O13 Tl3 O14 102.0(10) 2_746 1_545 ?
O13 Tl3 O14 45.8(10) 2_756 2_746 ?
O13 Tl3 O14 93.8(10) 1_545 2_746 ?
O13 Tl3 O14 98.4(10) 2_756 1_545 ?
O13 Tl3 O14 91.8(9) . 2_746 ?
O13 Tl3 O14 37.1(11) 2_746 2_746 ?
O13 Tl3 O14 37.7(10) 1_545 1_545 ?
O13 Tl3 O16 147.5(8) 2_756 1_545 ?
O13 Tl3 O16 49.7(8) 1_545 1_545 ?
O13 Tl3 O16 91.6(7) 2_756 . ?
O13 Tl3 O16 147.1(9) 2_746 . ?
O13 Tl3 O16 85.0(8) 1_545 . ?
O13 Tl3 O16 102.5(9) 2_746 1_545 ?
O13 Tl3 O17 163.4(9) 2_746 . ?
O13 Tl3 O17 104.5(7) 2_746 2_656 ?
O13 Tl3 O17 60.9(7) 2_746 2_646 ?
O13 Tl3 O17 129.3(6) 1_545 . ?
O13 Tl3 O17 107.0(9) 2_746 1_545 ?
O13 Tl3 O17 92.6(7) 1_545 1_545 ?
O13 Tl3 O18 144.1(8) 2_746 . ?
O13 Tl3 O18 88.2(5) . . ?
O13 Tl3 O18 133.4(7) 2_756 . ?
O13 Tl3 O18 87.5(6) 1_545 . ?
O14 Tl3 W5 27.2(9) 1_545 1_545 ?
O14 Tl3 W5 117.7(8) 2_746 1_545 ?
O14 Tl3 W6 150.0(9) 2_746 1_545 ?
O14 Tl3 W6 72.1(8) 1_545 1_545 ?
O14 Tl3 W6 152.2(9) 2_746 . ?
O14 Tl3 W6 69.8(7) 1_545 . ?
O14 Tl3 Tl3 132.6(7) 1_545 2_656 ?
O14 Tl3 Tl3 91.4(9) 2_746 1_545 ?
O14 Tl3 Tl3 88.6(9) 2_746 1_565 ?
O14 Tl3 Tl3 111.1(7) 2_746 2_656 ?
O14 Tl3 Tl3 88.6(9) 1_545 1_565 ?
O14 Tl3 Tl3 59.0(7) 1_545 2_756 ?
O14 Tl3 Tl3 91.4(9) 1_545 1_545 ?
O14 Tl3 Tl3 57.3(7) 2_746 2_756 ?
O14 Tl3 O13 44.5(10) 1_545 . ?
O14 Tl3 O14 116.2(7) 1_545 2_746 ?
O14 Tl3 O18 178.6(9) 2_746 . ?
O14 Tl3 O18 64.6(7) 1_545 . ?
O16 Tl3 W5 29.2(5) 1_545 1_545 ?
O16 Tl3 W5 67.7(4) . 1_545 ?
O16 Tl3 W6 67.3(4) 1_545 . ?
O16 Tl3 W6 72.4(4) . 1_545 ?
O16 Tl3 W6 26.8(5) 1_545 1_545 ?
O16 Tl3 W6 28.6(5) . . ?
O16 Tl3 Tl3 55.1(4) . 1_565 ?
O16 Tl3 Tl3 95.2(6) . 2_656 ?
O16 Tl3 Tl3 56.0(3) 1_545 1_545 ?
O16 Tl3 Tl3 124.9(4) . 1_545 ?
O16 Tl3 Tl3 94.4(6) . 2_756 ?
O16 Tl3 Tl3 124.0(3) 1_545 1_565 ?
O16 Tl3 Tl3 94.4(6) 1_545 2_756 ?
O16 Tl3 Tl3 95.2(6) 1_545 2_656 ?
O16 Tl3 O13 46.1(7) . . ?
O16 Tl3 O13 92.6(7) 1_545 . ?
O16 Tl3 O14 49.2(9) 1_545 1_545 ?
O16 Tl3 O14 135.6(9) . 2_746 ?
O16 Tl3 O14 138.5(10) 1_545 2_746 ?
O16 Tl3 O14 47.6(9) . 1_545 ?
O16 Tl3 O16 68.9(3) 1_545 . ?
O16 Tl3 O18 42.9(5) 1_545 . ?
O16 Tl3 O18 44.0(5) . . ?
O17 Tl3 W5 163.2(6) 2_656 1_545 ?
O17 Tl3 W5 106.7(5) . 1_545 ?
O17 Tl3 W5 76.9(5) 1_545 1_545 ?
O17 Tl3 W5 112.6(6) 2_646 1_545 ?
O17 Tl3 W6 26.2(5) . . ?
O17 Tl3 W6 24.1(5) 1_545 1_545 ?
O17 Tl3 W6 123.5(6) 2_656 1_545 ?
O17 Tl3 W6 68.4(5) 1_545 . ?
O17 Tl3 W6 86.0(6) 2_656 . ?
O17 Tl3 W6 72.6(5) . 1_545 ?
O17 Tl3 W6 82.4(6) 2_646 1_545 ?
O17 Tl3 W6 120.9(6) 2_646 . ?
O17 Tl3 Tl3 126.8(5) 1_545 1_565 ?
O17 Tl3 Tl3 114.6(6) 2_656 2_756 ?
O17 Tl3 Tl3 48.3(5) 2_646 1_545 ?
O17 Tl3 Tl3 131.3(5) 2_656 1_545 ?
O17 Tl3 Tl3 114.5(6) 2_646 2_756 ?
O17 Tl3 Tl3 57.9(5) 2_646 2_656 ?
O17 Tl3 Tl3 137.0(5) . 2_756 ?
O17 Tl3 Tl3 49.8(5) 1_545 2_656 ?
O17 Tl3 Tl3 136.7(5) 1_545 2_756 ?
O17 Tl3 Tl3 126.5(5) . 1_545 ?
O17 Tl3 Tl3 57.7(6) 2_656 2_656 ?
O17 Tl3 Tl3 48.7(6) 2_656 1_565 ?
O17 Tl3 Tl3 49.6(5) . 2_656 ?
O17 Tl3 Tl3 53.5(5) . 1_565 ?
O17 Tl3 Tl3 53.2(5) 1_545 1_545 ?
O17 Tl3 Tl3 131.7(5) 2_646 1_565 ?
O17 Tl3 O13 162.6(7) 1_545 2_756 ?
O17 Tl3 O13 95.7(8) . 2_756 ?
O17 Tl3 O13 159.9(8) 2_656 1_545 ?
O17 Tl3 O13 84.6(6) . . ?
O17 Tl3 O13 112.2(6) 2_646 2_756 ?
O17 Tl3 O13 106.6(9) 2_646 1_545 ?
O17 Tl3 O13 165.0(8) 2_646 . ?
O17 Tl3 O13 133.4(5) 1_545 . ?
O17 Tl3 O13 55.1(6) 2_656 2_756 ?
O17 Tl3 O13 95.7(8) 2_656 . ?
O17 Tl3 O14 133.5(9) 1_545 2_746 ?
O17 Tl3 O14 131.4(10) . 2_746 ?
O17 Tl3 O14 73.6(9) 2_646 2_746 ?
O17 Tl3 O14 71.6(10) 2_656 2_746 ?
O17 Tl3 O14 94.3(9) . 1_545 ?
O17 Tl3 O14 96.0(9) 1_545 1_545 ?
O17 Tl3 O14 137.2(11) 2_656 1_545 ?
O17 Tl3 O14 139.7(10) 2_646 1_545 ?
O17 Tl3 O16 95.8(7) 2_656 . ?
O17 Tl3 O16 48.2(7) 1_545 1_545 ?
O17 Tl3 O16 148.5(8) 2_656 1_545 ?
O17 Tl3 O16 96.2(7) 2_646 1_545 ?
O17 Tl3 O16 90.1(7) . 1_545 ?
O17 Tl3 O16 48.0(7) . . ?
O17 Tl3 O16 90.9(7) 1_545 . ?
O17 Tl3 O16 148.9(8) 2_646 . ?
O17 Tl3 O17 107.5(5) 2_656 1_545 ?
O17 Tl3 O17 83.0(8) 2_656 2_646 ?
O17 Tl3 O17 107.5(5) 2_646 . ?
O17 Tl3 O17 60.4(10) 2_646 1_545 ?
O17 Tl3 O17 73.3(6) . 1_545 ?
O17 Tl3 O17 60.7(10) 2_656 . ?
O17 Tl3 O18 46.9(6) 1_545 . ?
O17 Tl3 O18 47.2(6) . . ?
O17 Tl3 O18 106.5(6) 2_646 . ?
O17 Tl3 O18 107.0(6) 2_656 . ?
O18 Tl3 W6 30.9(2) . 1_545 ?
W1A O1 W1A 147(2) . 1_565 ?
W1A O1 W1B 143(2) . 1_565 ?
W1A O1 W1B 5.0(4) . . ?
W1A O1 Tl1 103.4(10) 1_565 1_565 ?
W1A O1 Tl1 108.0(16) . 1_565 ?
W1B O1 W1A 152.4(18) . 1_565 ?
W1B O1 W1A 4.4(5) 1_565 1_565 ?
W1B O1 W1B 148(2) 1_565 . ?
W1B O1 Tl1 103.2(13) . 1_565 ?
W1B O1 Tl1 107.7(13) 1_565 1_565 ?
O1 O1 W1A 76.6(8) 2 1_565 ?
O1 O1 W1A 70.9(13) 2 . ?
O1 O1 W1B 75.8(10) 2 . ?
O1 O1 W1B 72.2(12) 2 1_565 ?
O1 O1 Tl1 165(7) 2 1_565 ?
W1A O2 W3 149.8(11) . 2_655 ?
W1A O2 Tl1 109.6(8) . . ?
W1A O2 Tl1 96.3(7) . 1_565 ?
W1B O2 W1A 17.9(12) . . ?
W1B O2 W3 147.6(12) . 2_655 ?
W1B O2 Tl1 99.0(11) . . ?
W1B O2 Tl1 107.0(11) . 1_565 ?
W3 O2 Tl1 104.5(7) 2_655 1_565 ?
W3 O2 Tl1 97.9(7) 2_655 . ?
Tl1 O2 Tl1 70.7(4) 1_565 . ?
W1A O3 W1B 16.5(11) . . ?
W1A O3 W2 146.2(19) . . ?
W1A O3 Tl1 103.4(12) . 1_565 ?
W1A O3 Tl1 96.6(12) . . ?
W1B O3 Tl1 110.3(12) . 1_565 ?
W1B O3 Tl1 85.3(13) . . ?
W2 O3 W1B 134(2) . . ?
W2 O3 Tl1 109.1(12) . 1_565 ?
W2 O3 Tl1 86.9(11) . . ?
Tl1 O3 Tl1 68.7(6) 1_565 . ?
W2 O4 W2 167.7(17) . 1_545 ?
W2 O4 Tl1 87.6(9) 1_545 . ?
W2 O4 Tl1 89.9(11) . . ?
W2 O4 Tl2 91.6(10) 1_545 . ?
W2 O4 Tl2 89.7(10) . . ?
Tl1 O4 Tl2 174.7(9) . . ?
W2 O5 W4 147.2(19) . . ?
W2 O5 Tl2 95.3(12) . . ?
W2 O5 Tl2 115.8(12) . 1_565 ?
W4 O5 Tl2 96.0(11) . 1_565 ?
W4 O5 Tl2 90.2(11) . . ?
Tl2 O5 Tl2 66.0(5) 1_565 . ?
W2 O6 W3 140.4(10) . . ?
W2 O6 Tl1 101.9(11) . . ?
W2 O6 Tl1 108.3(12) . 1_565 ?
W3 O6 Tl1 100.1(10) . . ?
W3 O6 Tl1 109.3(12) . 1_565 ?
Tl1 O6 Tl1 73.9(4) 1_565 . ?
W2 O7 Tl2 99.7(11) . . ?
W2 O7 Tl2 105.5(11) . 1_565 ?
W3 O7 W2 147.6(11) 1_455 . ?
W3 O7 Tl2 106.5(12) 1_455 1_565 ?
W3 O7 Tl2 97.9(10) 1_455 . ?
Tl2 O7 Tl2 65.9(3) . 1_565 ?
W3 O8 W3 155.2(17) . 1_545 ?
W3 O8 Tl1 96.9(8) 1_545 . ?
W3 O8 Tl1 105.3(11) . . ?
W3 O9 W4 156.9(14) . . ?
W3 O9 Tl2 102.0(9) . 1_655 ?
W3 O9 Tl2 108.6(10) . 1_665 ?
W4 O9 Tl2 90.0(8) . 1_665 ?
W4 O9 Tl2 97.9(9) . 1_655 ?
Tl2 O9 Tl2 66.7(4) 1_655 1_665 ?
W4 O10 W6 142.5(11) . . ?
W4 O10 Tl2 107.4(8) . 1_565 ?
W4 O10 Tl2 117.5(9) . . ?
W6 O10 Tl2 99.3(7) . 1_565 ?
W6 O10 Tl2 94.3(7) . . ?
Tl2 O10 Tl2 75.0(5) . 1_565 ?
W4 O11 W4 146.5(16) . 1_565 ?
W4 O11 Tl2 101.0(12) 1_565 1_565 ?
W4 O11 Tl2 107.2(14) . 1_565 ?
W4 O12 W5 146.2(16) . . ?
W4 O12 Tl2 102.7(13) . 1_655 ?
W4 O12 Tl2 112.6(13) . 1_665 ?
W5 O12 Tl2 93.9(11) . 1_655 ?
W5 O12 Tl2 100.2(11) . 1_665 ?
Tl2 O12 Tl2 73.1(6) 1_665 1_655 ?
W5 O13 Tl3 108.7(13) . 1_565 ?
W5 O13 Tl3 99.0(13) . . ?
W5 O13 Tl3 122.4(17) . 2_756 ?
W5 O13 Tl3 143.0(18) . 2_766 ?
Tl3 O13 Tl3 67.3(7) 2_756 . ?
Tl3 O13 Tl3 117.6(10) 2_766 . ?
Tl3 O13 Tl3 80.9(9) 2_766 1_565 ?
Tl3 O13 Tl3 79.6(8) 2_766 2_756 ?
Tl3 O13 Tl3 116.6(9) 1_565 2_756 ?
Tl3 O13 Tl3 70.4(6) 1_565 . ?
W5 O14 W5 165(2) . 1_565 ?
W5 O14 Tl2 88.3(14) 1_565 1_665 ?
W5 O14 Tl2 87.1(14) . 1_665 ?
W5 O14 Tl3 89.6(16) . 1_565 ?
W5 O14 Tl3 92.3(14) 1_565 1_565 ?
W5 O14 Tl3 96.2(17) . 2_766 ?
W5 O14 Tl3 98.0(15) 1_565 2_766 ?
Tl3 O14 Tl2 126.6(12) 2_766 1_665 ?
Tl3 O14 Tl2 169.5(14) 1_565 1_665 ?
Tl3 O14 Tl3 63.7(7) 1_565 2_766 ?
W5 O15 W6 136.3(9) . 1_655 ?
W5 O15 Tl2 104.5(11) . 1_665 ?
W5 O15 Tl2 110.6(12) . 1_655 ?
W6 O15 Tl2 101.1(10) 1_655 1_655 ?
W6 O15 Tl2 110.9(12) 1_655 1_665 ?
Tl2 O15 Tl2 78.5(4) 1_665 1_655 ?
W5 O16 Tl3 92.5(8) . 1_565 ?
W5 O16 Tl3 98.7(9) . . ?
W6 O16 W5 167.3(10) . . ?
W6 O16 Tl3 98.8(9) . 1_565 ?
W6 O16 Tl3 90.8(8) . . ?
Tl3 O16 Tl3 68.9(3) 1_565 . ?
W6 O17 Tl3 137.5(13) . 2_666 ?
W6 O17 Tl3 107.3(11) . 1_565 ?
W6 O17 Tl3 99.9(11) . . ?
W6 O17 Tl3 126.8(12) . 2_656 ?
Tl3 O17 Tl3 72.7(7) 2_656 . ?
Tl3 O17 Tl3 72.4(6) 2_666 1_565 ?
Tl3 O17 Tl3 119.4(9) 2_656 1_565 ?
Tl3 O17 Tl3 119.4(9) 2_666 . ?
Tl3 O17 Tl3 83.0(8) 2_656 2_666 ?
Tl3 O17 Tl3 73.3(6) . 1_565 ?
W6 O18 W6 148.8(11) . 1_545 ?
W6 O18 Tl2 103.0(7) . . ?
W6 O18 Tl2 103.8(6) 1_545 . ?
W6 O18 Tl3 74.2(6) . . ?
W6 O18 Tl3 77.3(5) 1_545 . ?
Tl2 O18 Tl3 172.9(6) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.25781
2 0.25283
3 0.26478
4 0.22458

_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Rb4W11O35
_database_code_depnum_ccdc_archive 'CCDC 2211345'
loop_
_audit_author_name
_audit_author_address
'Sergey F. Solodovnikov'
;Nikolaev Institute of Inorganic Chemistry Siberian Branch of Russian Academy of Sciences
Russia
;
_audit_update_record             
;
2022-10-06 deposited with the CCDC.	2023-01-31 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_SHFSU01_Rb4W11O35           
;
PROBLEM: The absolute value of parameter shift to su ratio > 0.20
RESPONSE: The precession images of  studied Hexagonal Tungsten Bronze-like crystals showed that along with weak Bragg reflections corresponding to supercells with doubling one or two shortest lattice parameters, there are elongated diffuse scattering peaks. Cooling crystals down to 80 K led to increasing the intensity of these diffusion peaks, but did not resolve them into separate Bragg reflections. To avoid the negative effect of diffusion superstructure reflections on the structural data, we processed raw data frames and solved the structures within their subcells.
;
# Added during the CSD deposition process: Thursday 06 October 2022 08:28 AM
# end Validation Reply Form

_audit_creation_date             2022-07-13
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
_shelx_SHELXL_version_number     2017/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'O35 Rb4 W11'
_chemical_formula_sum            'O35 Rb4 W11'
_chemical_formula_weight         2924.23
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           3
_space_group_name_H-M_alt        'P 1 2 1'
_space_group_name_Hall           'P 2y'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'

_cell_length_a                   3.8369(3)
_cell_length_b                   7.3201(5)
_cell_length_c                   25.6712(16)
_cell_angle_alpha                90
_cell_angle_beta                 90.006(3)
_cell_angle_gamma                90
_cell_volume                     721.01(9)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    9992
_cell_measurement_temperature    259(2)
_cell_measurement_theta_max      33.25
_cell_measurement_theta_min      2.38
_shelx_estimated_absorpt_T_max   0.632
_shelx_estimated_absorpt_T_min   0.126
_exptl_absorpt_coefficient_mu    50.504
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.4302
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1053 before and 0.0517 after correction. The Ratio of minimum to maximum transmission is 0.5763. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    6.735
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             1242
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.01
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0581
_diffrn_reflns_av_unetI/netI     0.0448
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       39
_diffrn_reflns_limit_l_min       -39
_diffrn_reflns_number            20842
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.278
_diffrn_reflns_theta_min         2.380
_diffrn_ambient_temperature      259(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Incoatec IuS3.0 microfocus X-ray tube'
_diffrn_radiation_monochromator  'Incoatec HELIOS multilayer mirrors'
_diffrn_measurement_device_type  'Bruker D8 Venture diffractometer'
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_detector_type            'Bruker PHOTON III area detector'
_diffrn_detector                 PIXEL
_diffrn_detector_area_resol_mean 7.41
_reflns_Friedel_coverage         0.878
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.997
_reflns_number_gt                5431
_reflns_number_total             5524
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         6.422
_refine_diff_density_min         -10.940
_refine_diff_density_rms         0.931
_refine_ls_abs_structure_details 
;
 Twinning involves inversion, so Flack parameter cannot be determined
;
_refine_ls_abs_structure_Flack   ?
_refine_ls_extinction_coef       0.00059(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_goodness_of_fit_ref   1.211
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     178
_refine_ls_number_reflns         5524
_refine_ls_number_restraints     5
_refine_ls_R_factor_all          0.0622
_refine_ls_R_factor_gt           0.0613
_refine_ls_restrained_S_all      1.222
_refine_ls_shift/su_max          0.367
_refine_ls_shift/su_mean         0.047
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0525P)²+76.4989P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1720
_refine_ls_wR_factor_ref         0.1727
_refine_special_details          
;
 Refined as a 4-component inversion twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.22807
 0.25879 0.25679 0.25635
2. Restrained distances
 W1-O1 = W2-O4 = W6A-O17
 1.7 with sigma of 0.015
3. Others
 1*[Sof(Rb1)]+0.5*[Sof(Rb2A)]+0.5*[Sof(Rb2B)]+0.5*[Sof(Rb3)]+0.5*[Sof(Rb4A)]+
 0.5*[Sof(Rb4B)]=2 with esd of 0
 Sof(W6B)=1-FVAR(1)
 Sof(W6A)=FVAR(1)
 Fixed Sof: W1(0.5)
 Fixed Y: W1(0)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.6006(8) 0.000000 0.00044(19) 0.0061(4) Uani 0.5 1 d D . P . .
W2 W 0.4443(13) 0.7466(10) 0.12298(12) 0.0280(7) Uani 1 1 d D . . . .
W3 W 0.5352(6) 0.2519(10) 0.12213(11) 0.0176(8) Uani 1 1 d . . . . .
W4 W 0.5477(5) 0.5000(9) 0.24916(5) 0.0149(4) Uani 1 1 d . . . . .
W5 W 0.5083(8) 0.2439(8) 0.37424(11) 0.0079(3) Uani 1 1 d . . . . .
W6A W 0.5953(19) 0.7624(14) 0.3755(3) 0.0176(16) Uani 0.463(14) 1 d D . P . .
W6B W 0.4087(17) 0.7494(9) 0.37267(15) 0.0077(11) Uani 0.537(14) 1 d . . P . .
Rb1 Rb 0.009(2) 0.0072(19) 0.2505(2) 0.0418(16) Uani 0.895(5) 1 d . . P . .
Rb2A Rb 0.000000 0.5182(15) 0.000000 0.024(3) Uani 0.629(9) 2 d S T P . .
Rb2B Rb 0.500000 0.518(3) 0.000000 0.002(6) Uani 0.159(9) 2 d S T P . .
Rb3 Rb 0.000000 0.0653(13) 0.500000 0.0265(16) Uani 0.871(9) 2 d DS T P . .
Rb4A Rb 0.000000 0.521(4) 0.500000 0.039(6) Uani 0.443(9) 2 d S T P . .
Rb4B Rb 0.500000 0.523(3) 0.500000 0.09(4) Uani 0.108(9) 2 d S T P . .
O1 O 1.000000 0.068(6) 0.000000 0.026(10) Uiso 1 2 d DS . P . .
O2 O 0.519(11) -0.176(5) 0.0495(15) 0.023(7) Uiso 1 1 d . . . . .
O3 O 0.589(10) 0.181(4) -0.0522(13) 0.016(5) Uiso 1 1 d . . . . .
O4 O 0.015(6) 0.782(6) 0.1128(18) 0.042(11) Uiso 1 1 d D . . . .
O5 O 0.419(9) 0.680(4) 0.1920(13) 0.015(5) Uiso 1 1 d . . . . .
O6 O 0.459(8) 0.996(7) 0.1414(9) 0.019(4) Uiso 1 1 d . . . . .
O7 O 0.477(9) 0.499(8) 0.0999(9) 0.023(5) Uiso 1 1 d . . . . .
O8 O 0.977(8) 0.267(4) 0.1304(11) 0.012(5) Uiso 1 1 d . . . . .
O9 O 0.516(9) 0.320(5) 0.1882(13) 0.019(6) Uiso 1 1 d . . . . .
O10 O 0.994(8) 0.555(3) 0.2484(10) 0.009(4) Uiso 1 1 d . . . . .
O11 O 0.510(8) 0.307(4) 0.2915(12) 0.016(5) Uiso 1 1 d . . . . .
O12 O 0.582(10) 0.682(4) 0.2962(13) 0.017(6) Uiso 1 1 d . . . . .
O13 O 0.559(8) 0.194(5) 0.4349(12) 0.020(6) Uiso 1 1 d . . . . .
O14 O 0.516(8) 0.495(6) 0.3813(8) 0.018(4) Uiso 1 1 d . . . . .
O15 O 0.027(7) 0.253(5) 0.3626(10) 0.015(5) Uiso 1 1 d . . . . .
O16 O 0.536(6) -0.002(5) 0.3481(7) 0.010(3) Uiso 1 1 d . . . . .
O17 O 1.007(4) 0.793(3) 0.3778(7) -0.001(3) Uiso 1 1 d D . . . .
O18 O 0.486(11) 0.800(5) 0.4399(14) 0.026(8) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 W1 0.772(6) 2_655 ?
W1 W1 3.065(6) 2_755 ?
W1 W2 3.675(5) 2_645 ?
W1 W3 3.637(5) . ?
W1 W3 3.684(7) 2_655 ?
W1 Rb2B 3.55(2) 1_545 ?
W1 O1 2.358(10) 1_455 ?
W1 O1 1.612(13) . ?
W1 O2 1.83(4) . ?
W1 O2 1.87(4) 2_655 ?
W1 O3 2.01(3) 2_655 ?
W1 O3 1.89(3) . ?
W2 W3 3.715(3) 1_565 ?
W2 W3 3.638(3) . ?
W2 W4 3.730(4) . ?
W2 Rb2B 3.580(12) . ?
W2 O2 1.99(4) 1_565 ?
W2 O4 2.22(3) 1_655 ?
W2 O4 1.686(19) . ?
W2 O5 1.84(3) . ?
W2 O6 1.89(5) . ?
W2 O7 1.91(5) . ?
W3 W4 3.733(3) . ?
W3 Rb2B 3.693(13) . ?
W3 O3 1.93(3) 2_655 ?
W3 O6 1.96(5) 1_545 ?
W3 O7 1.91(5) . ?
W3 O8 2.15(3) 1_455 ?
W3 O8 1.71(3) . ?
W3 O9 1.77(3) . ?
W4 W4 3.8369(3) 1_655 ?
W4 W5 3.721(4) . ?
W4 W6A 3.774(7) . ?
W4 W6B 3.698(5) . ?
W4 O5 2.03(3) . ?
W4 O9 2.05(3) . ?
W4 O10 2.16(3) 1_455 ?
W4 O10 1.76(3) . ?
W4 O11 1.79(3) . ?
W4 O12 1.80(3) . ?
W5 W6A 3.541(8) 1_545 ?
W5 W6A 3.810(8) . ?
W5 W6B 3.721(5) . ?
W5 W6B 3.640(5) 1_545 ?
W5 Rb4B 3.821(12) . ?
W5 O11 2.17(3) . ?
W5 O13 1.61(3) . ?
W5 O14 1.85(4) . ?
W5 O15 2.01(3) 1_655 ?
W5 O15 1.87(3) . ?
W5 O16 1.93(4) . ?
W6A W6B 3.123(7) 1_655 ?
W6A W6B 0.726(7) . ?
W6A Rb4B 3.662(12) . ?
W6A O12 2.12(3) . ?
W6A O14 1.99(4) . ?
W6A O16 1.88(4) 1_565 ?
W6A O17 2.270(17) 1_455 ?
W6A O17 1.596(17) . ?
W6A O18 1.73(4) . ?
W6B Rb4B 3.681(11) . ?
W6B O12 2.13(3) . ?
W6B O14 1.92(4) . ?
W6B O16 1.99(4) 1_565 ?
W6B O17 1.580(18) 1_455 ?
W6B O17 2.321(18) . ?
W6B O18 1.79(4) . ?
Rb1 Rb1 3.8369(3) 1_455 ?
Rb1 Rb1 3.8369(3) 1_655 ?
Rb1 O4 3.90(5) 1_545 ?
Rb1 O5 3.24(3) 1_545 ?
Rb1 O5 3.62(3) 1_445 ?
Rb1 O6 3.29(3) 1_545 ?
Rb1 O6 3.51(3) 1_445 ?
Rb1 O8 3.62(3) 1_455 ?
Rb1 O9 3.37(4) 1_455 ?
Rb1 O9 3.40(4) . ?
Rb1 O10 3.31(3) 1_445 ?
Rb1 O11 3.10(3) 1_455 ?
Rb1 O11 3.10(3) . ?
Rb1 O12 3.12(3) 1_445 ?
Rb1 O12 3.45(4) 1_545 ?
Rb1 O15 3.39(3) . ?
Rb1 O16 3.09(2) 1_455 ?
Rb1 O16 3.22(2) . ?
Rb1 O17 3.62(2) 1_445 ?
Rb2A Rb2A 3.8369(3) 1_655 ?
Rb2A Rb2B 1.91845(17) 1_455 ?
Rb2A Rb2B 1.91845(18) . ?
Rb2A O1 3.29(4) 1_455 ?
Rb2A O2 3.26(4) 1_565 ?
Rb2A O2 3.17(4) 2_665 ?
Rb2A O2 3.17(4) 1_465 ?
Rb2A O2 3.26(4) 2_565 ?
Rb2A O3 3.60(4) . ?
Rb2A O3 3.22(4) 1_455 ?
Rb2A O3 3.22(4) 2_655 ?
Rb2A O3 3.60(4) 2 ?
Rb2A O4 3.48(5) . ?
Rb2A O4 3.48(5) 2 ?
Rb2A O7 3.26(3) 2_655 ?
Rb2A O7 3.15(3) 2 ?
Rb2A O7 3.15(3) . ?
Rb2A O7 3.26(3) 1_455 ?
Rb2A O8 3.82(3) 2_655 ?
Rb2A O8 3.82(3) 1_455 ?
Rb2B Rb2B 3.8369(3) 1_655 ?
Rb2B Rb2B 3.8369(3) 1_455 ?
Rb2B O2 2.58(4) 2_665 ?
Rb2B O2 2.58(4) 1_565 ?
Rb2B O3 2.83(4) . ?
Rb2B O3 2.83(4) 2_655 ?
Rb2B O4 3.95(5) . ?
Rb2B O4 3.95(5) 2_655 ?
Rb2B O7 2.57(2) . ?
Rb2B O7 2.57(2) 2_655 ?
Rb3 Rb3 3.8369(3) 1_455 ?
Rb3 Rb3 3.8369(3) 1_655 ?
Rb3 Rb4A 3.34(3) . ?
Rb3 Rb4A 3.98(3) 1_545 ?
Rb3 Rb4B 3.86(2) . ?
Rb3 Rb4B 3.86(2) 1_455 ?
Rb3 O13 2.88(4) . ?
Rb3 O13 2.88(4) 2_556 ?
Rb3 O13 2.559(13) 1_455 ?
Rb3 O13 2.559(13) 2_656 ?
Rb3 O15 3.79(3) . ?
Rb3 O15 3.79(3) 2_556 ?
Rb3 O17 3.72(2) 1_445 ?
Rb3 O17 3.72(2) 2_646 ?
Rb3 O18 3.10(4) 1_545 ?
Rb3 O18 3.17(4) 2_646 ?
Rb3 O18 3.10(4) 2_546 ?
Rb3 O18 3.17(4) 1_445 ?
Rb4A Rb4A 3.8369(4) 1_655 ?
Rb4A Rb4A 3.8369(4) 1_455 ?
Rb4A Rb4B 1.9185(4) 1_455 ?
Rb4A Rb4B 1.9185(4) . ?
Rb4A O13 3.62(4) . ?
Rb4A O13 3.38(4) 1_455 ?
Rb4A O13 3.62(4) 2_556 ?
Rb4A O13 3.38(4) 2_656 ?
Rb4A O14 3.64(2) 2_556 ?
Rb4A O14 3.64(2) . ?
Rb4A O14 3.57(3) 2_656 ?
Rb4A O14 3.57(3) 1_455 ?
Rb4A O17 3.71(2) 2_656 ?
Rb4A O17 3.71(2) 1_455 ?
Rb4A O18 3.17(4) . ?
Rb4A O18 3.23(4) 1_455 ?
Rb4A O18 3.17(4) 2_556 ?
Rb4A O18 3.23(4) 2_656 ?
Rb4B Rb4B 3.8369(4) 1_655 ?
Rb4B Rb4B 3.8369(3) 1_455 ?
Rb4B O13 2.94(4) . ?
Rb4B O13 2.94(4) 2_656 ?
Rb4B O14 3.06(2) 2_656 ?
Rb4B O14 3.06(2) . ?
Rb4B O18 2.55(4) 2_656 ?
Rb4B O18 2.55(4) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W1 W1 W1 177.9(9) 2_655 2_755 ?
W1 W1 W2 92.32(19) 2_755 2_645 ?
W1 W1 W2 85.9(6) 2_655 2_645 ?
W1 W1 W3 94.32(17) 2_755 . ?
W1 W1 W3 97.77(18) 2_755 2_655 ?
W1 W1 W3 80.4(6) 2_655 2_655 ?
W1 W1 W3 87.5(6) 2_655 . ?
W1 W1 Rb2B 96.24(6) 2_755 1_545 ?
W1 W1 Rb2B 83.76(6) 2_655 1_545 ?
W1 W1 O1 161.9(15) 2_655 . ?
W1 W1 O1 12.3(10) 2_655 1_455 ?
W1 W1 O2 81.3(14) 2_655 . ?
W1 W1 O2 74.7(13) 2_655 2_655 ?
W1 W1 O3 87.5(12) 2_655 . ?
W1 W1 O3 70.0(12) 2_655 2_655 ?
W3 W1 W2 60.64(9) 2_655 2_645 ?
W3 W1 W2 173.35(11) . 2_645 ?
W3 W1 W3 118.0(2) . 2_655 ?
Rb2B W1 W2 59.37(10) 1_545 2_645 ?
Rb2B W1 W3 118.66(15) 1_545 2_655 ?
Rb2B W1 W3 119.95(17) 1_545 . ?
O1 W1 W1 167.8(10) 1_455 2_755 ?
O1 W1 W1 18.0(15) . 2_755 ?
O1 W1 W2 93.3(5) 1_455 2_645 ?
O1 W1 W2 101.2(7) . 2_645 ?
O1 W1 W3 75.6(5) 1_455 2_655 ?
O1 W1 W3 88.5(8) . 2_655 ?
O1 W1 W3 80.2(5) 1_455 . ?
O1 W1 W3 85.1(8) . . ?
O1 W1 Rb2B 114.3(15) . 1_545 ?
O1 W1 Rb2B 96.0(10) 1_455 1_545 ?
O1 W1 O1 150(2) . 1_455 ?
O1 W1 O2 116.1(16) . 2_655 ?
O1 W1 O2 112.7(16) . . ?
O1 W1 O3 98.3(15) . 2_655 ?
O1 W1 O3 78.5(15) . . ?
O2 W1 W1 103.9(13) 2_655 2_755 ?
O2 W1 W1 100.2(13) . 2_755 ?
O2 W1 W2 18.6(12) 2_655 2_645 ?
O2 W1 W2 103.3(12) . 2_645 ?
O2 W1 W3 75.7(11) . . ?
O2 W1 W3 156.4(12) . 2_655 ?
O2 W1 W3 74.0(11) 2_655 2_655 ?
O2 W1 W3 156.8(12) 2_655 . ?
O2 W1 Rb2B 44.6(11) 2_655 1_545 ?
O2 W1 Rb2B 44.3(11) . 1_545 ?
O2 W1 O1 89.1(15) . 1_455 ?
O2 W1 O1 84.4(14) 2_655 1_455 ?
O2 W1 O2 87(2) . 2_655 ?
O2 W1 O3 144.6(15) 2_655 2_655 ?
O2 W1 O3 89.3(11) 2_655 . ?
O2 W1 O3 87.0(11) . 2_655 ?
O2 W1 O3 168.8(17) . . ?
O3 W1 W1 91.0(11) . 2_755 ?
O3 W1 W1 111.5(10) 2_655 2_755 ?
O3 W1 W2 152.1(10) 2_655 2_645 ?
O3 W1 W2 74.8(10) . 2_645 ?
O3 W1 W3 104.8(10) . . ?
O3 W1 W3 15.6(10) . 2_655 ?
O3 W1 W3 22.2(10) 2_655 . ?
O3 W1 W3 100.5(10) 2_655 2_655 ?
O3 W1 Rb2B 133.8(10) . 1_545 ?
O3 W1 Rb2B 128.1(10) 2_655 1_545 ?
O3 W1 O1 80.0(13) . 1_455 ?
O3 W1 O1 60.7(12) 2_655 1_455 ?
O3 W1 O3 90.1(19) . 2_655 ?
W1 W2 W1 12.02(9) 2_665 1_565 ?
W1 W2 W3 58.73(11) 1_565 1_565 ?
W1 W2 W3 59.80(12) 2_665 1_565 ?
W1 W2 W4 176.37(16) 2_665 . ?
W1 W2 W4 164.50(18) 1_565 . ?
W3 W2 W1 118.57(16) . 1_565 ?
W3 W2 W1 120.11(16) . 2_665 ?
W3 W2 W3 169.09(15) . 1_565 ?
W3 W2 W4 60.86(10) . . ?
W3 W2 W4 118.50(14) 1_565 . ?
Rb2B W2 W1 58.6(3) . 2_665 ?
Rb2B W2 W1 58.3(3) . 1_565 ?
Rb2B W2 W3 117.1(3) . 1_565 ?
Rb2B W2 W3 61.5(4) . . ?
Rb2B W2 W4 122.2(4) . . ?
O2 W2 W1 17.4(11) 1_565 2_665 ?
O2 W2 W1 13.6(10) 1_565 1_565 ?
O2 W2 W3 105.4(10) 1_565 . ?
O2 W2 W3 72.3(10) 1_565 1_565 ?
O2 W2 W4 161.1(11) 1_565 . ?
O2 W2 Rb2B 44.7(11) 1_565 . ?
O2 W2 O4 73.3(17) 1_565 1_655 ?
O4 W2 W1 83.4(12) 1_655 2_665 ?
O4 W2 W1 75.1(16) . 2_665 ?
O4 W2 W1 71.4(12) 1_655 1_565 ?
O4 W2 W1 87.1(16) . 1_565 ?
O4 W2 W3 86.4(16) . 1_565 ?
O4 W2 W3 91.2(12) 1_655 . ?
O4 W2 W3 77.9(12) 1_655 1_565 ?
O4 W2 W3 104.2(16) . . ?
O4 W2 W4 108.3(16) . . ?
O4 W2 W4 93.1(12) 1_655 . ?
O4 W2 Rb2B 83.8(12) 1_655 . ?
O4 W2 Rb2B 89.6(16) . . ?
O4 W2 O2 87(2) . 1_565 ?
O4 W2 O4 158(3) . 1_655 ?
O4 W2 O5 98(2) . . ?
O4 W2 O6 85.3(19) . . ?
O4 W2 O7 99(2) . . ?
O5 W2 W1 163.8(10) . 1_565 ?
O5 W2 W1 164.0(10) . 2_665 ?
O5 W2 W3 106.0(10) . 1_565 ?
O5 W2 W3 75.3(10) . . ?
O5 W2 W4 16.5(10) . . ?
O5 W2 Rb2B 136.7(10) . . ?
O5 W2 O2 174.6(18) . 1_565 ?
O5 W2 O4 101.4(16) . 1_655 ?
O5 W2 O6 91.0(13) . . ?
O5 W2 O7 92.9(13) . . ?
O6 W2 W1 73.9(8) . 1_565 ?
O6 W2 W1 74.2(8) . 2_665 ?
O6 W2 W3 164.2(8) . . ?
O6 W2 W3 15.3(8) . 1_565 ?
O6 W2 W4 104.4(8) . . ?
O6 W2 Rb2B 132.2(9) . . ?
O6 W2 O2 87.5(13) . 1_565 ?
O6 W2 O4 83.6(15) . 1_655 ?
O6 W2 O7 173.4(15) . . ?
O7 W2 W1 101.6(9) . 1_565 ?
O7 W2 W1 102.3(9) . 2_665 ?
O7 W2 W3 159.4(10) . 1_565 ?
O7 W2 W3 17.8(9) . . ?
O7 W2 W4 78.7(9) . . ?
O7 W2 Rb2B 43.8(9) . . ?
O7 W2 O2 88.1(14) . 1_565 ?
O7 W2 O4 90.5(16) . 1_655 ?
W1 W3 W1 12.09(10) . 2_655 ?
W1 W3 W2 60.44(13) . 1_545 ?
W1 W3 W2 59.56(12) 2_655 1_545 ?
W1 W3 W2 121.10(17) . . ?
W1 W3 W4 175.09(10) . . ?
W1 W3 W4 172.50(9) 2_655 . ?
W1 W3 Rb2B 62.6(3) . . ?
W1 W3 Rb2B 62.2(3) 2_655 . ?
W2 W3 W1 119.33(17) . 2_655 ?
W2 W3 W2 169.09(15) . 1_545 ?
W2 W3 W4 118.71(13) 1_545 . ?
W2 W3 W4 60.78(9) . . ?
W2 W3 Rb2B 58.5(3) . . ?
Rb2B W3 W2 121.8(3) . 1_545 ?
Rb2B W3 W4 119.1(3) . . ?
O3 W3 W1 15.3(10) 2_655 2_655 ?
O3 W3 W1 23.3(10) 2_655 . ?
O3 W3 W2 73.5(10) 2_655 1_545 ?
O3 W3 W2 104.4(10) 2_655 . ?
O3 W3 W4 161.2(10) 2_655 . ?
O3 W3 Rb2B 48.8(10) 2_655 . ?
O3 W3 O6 86.7(12) 2_655 1_545 ?
O3 W3 O8 81.9(13) 2_655 1_455 ?
O6 W3 W1 73.5(7) 1_545 2_655 ?
O6 W3 W1 75.1(8) 1_545 . ?
O6 W3 W2 14.7(8) 1_545 1_545 ?
O6 W3 W2 159.3(9) 1_545 . ?
O6 W3 W4 104.3(8) 1_545 . ?
O6 W3 Rb2B 135.5(8) 1_545 . ?
O6 W3 O8 82.7(12) 1_545 1_455 ?
O7 W3 W1 103.4(9) . . ?
O7 W3 W1 101.6(9) . 2_655 ?
O7 W3 W2 17.8(9) . . ?
O7 W3 W2 159.0(10) . 1_545 ?
O7 W3 W4 78.6(9) . . ?
O7 W3 Rb2B 40.8(9) . . ?
O7 W3 O3 86.9(13) . 2_655 ?
O7 W3 O6 164.4(15) . 1_545 ?
O7 W3 O8 82.3(13) . 1_455 ?
O8 W3 W1 88.2(8) 1_455 2_655 ?
O8 W3 W1 94.0(10) . . ?
O8 W3 W1 106.1(10) . 2_655 ?
O8 W3 W1 100.3(8) 1_455 . ?
O8 W3 W2 98.9(10) . 1_545 ?
O8 W3 W2 91.8(10) . . ?
O8 W3 W2 81.6(8) 1_455 . ?
O8 W3 W2 87.5(8) 1_455 1_545 ?
O8 W3 W4 81.3(10) . . ?
O8 W3 W4 84.4(8) 1_455 . ?
O8 W3 Rb2B 96.2(10) . . ?
O8 W3 Rb2B 91.2(8) 1_455 . ?
O8 W3 O3 112.2(15) . 2_655 ?
O8 W3 O6 100.2(13) . 1_545 ?
O8 W3 O7 95.3(15) . . ?
O8 W3 O8 165.6(17) . 1_455 ?
O8 W3 O9 84.5(15) . . ?
O9 W3 W1 162.5(11) . 2_655 ?
O9 W3 W1 165.7(11) . . ?
O9 W3 W2 73.2(11) . . ?
O9 W3 W2 105.6(11) . 1_545 ?
O9 W3 W4 13.2(11) . . ?
O9 W3 Rb2B 131.7(11) . . ?
O9 W3 O3 163.3(17) . 2_655 ?
O9 W3 O6 91.1(13) . 1_545 ?
O9 W3 O7 91.0(13) . . ?
O9 W3 O8 81.4(14) . 1_455 ?
W2 W4 W3 58.36(5) . . ?
W2 W4 W4 96.10(9) . 1_655 ?
W2 W4 W6A 120.35(19) . . ?
W3 W4 W4 90.73(4) . 1_655 ?
W3 W4 W6A 177.46(14) . . ?
W5 W4 W2 171.49(10) . . ?
W5 W4 W3 120.55(10) . . ?
W5 W4 W4 92.34(6) . 1_655 ?
W5 W4 W6A 61.10(11) . . ?
W6A W4 W4 87.23(11) . 1_655 ?
W6B W4 W2 119.36(13) . . ?
W6B W4 W3 170.93(11) . . ?
W6B W4 W4 98.30(10) . 1_655 ?
W6B W4 W5 60.20(7) . . ?
W6B W4 W6A 11.09(10) . . ?
O5 W4 W2 14.9(9) . . ?
O5 W4 W3 71.4(9) . . ?
O5 W4 W4 104.1(10) . 1_655 ?
O5 W4 W5 159.9(10) . . ?
O5 W4 W6A 107.6(9) . . ?
O5 W4 W6B 105.3(9) . . ?
O5 W4 O9 81.5(9) . . ?
O5 W4 O10 68.5(12) . 1_455 ?
O9 W4 W2 69.1(9) . . ?
O9 W4 W3 11.4(9) . . ?
O9 W4 W4 93.4(10) . 1_655 ?
O9 W4 W5 109.4(9) . . ?
O9 W4 W6A 170.5(9) . . ?
O9 W4 W6B 164.5(10) . . ?
O9 W4 O10 93.2(12) . 1_455 ?
O10 W4 W2 78.3(7) 1_455 . ?
O10 W4 W2 89.0(9) . . ?
O10 W4 W3 94.0(7) 1_455 . ?
O10 W4 W3 96.6(9) . . ?
O10 W4 W4 13.3(8) . 1_655 ?
O10 W4 W4 169.2(7) 1_455 1_655 ?
O10 W4 W5 99.5(9) . . ?
O10 W4 W5 93.5(7) 1_455 . ?
O10 W4 W6A 87.7(7) 1_455 . ?
O10 W4 W6A 81.1(9) . . ?
O10 W4 W6B 92.1(9) . . ?
O10 W4 W6B 76.9(7) 1_455 . ?
O10 W4 O5 94.6(13) . . ?
O10 W4 O9 101.4(13) . . ?
O10 W4 O10 155.9(14) . 1_455 ?
O10 W4 O11 105.5(14) . . ?
O10 W4 O12 76.4(15) . . ?
O11 W4 W2 154.4(10) . . ?
O11 W4 W3 98.4(10) . . ?
O11 W4 W4 94.7(11) . 1_655 ?
O11 W4 W5 22.2(10) . . ?
O11 W4 W6A 83.3(10) . . ?
O11 W4 W6B 81.8(10) . . ?
O11 W4 O5 158.5(15) . . ?
O11 W4 O9 87.2(14) . . ?
O11 W4 O10 94.2(12) . 1_455 ?
O11 W4 O12 100.5(11) . . ?
O12 W4 W2 103.5(10) . . ?
O12 W4 W3 161.0(10) . . ?
O12 W4 W4 85.8(12) . 1_655 ?
O12 W4 W5 78.3(10) . . ?
O12 W4 W6A 17.2(10) . . ?
O12 W4 W6B 21.8(11) . . ?
O12 W4 O5 91.3(14) . . ?
O12 W4 O9 172.4(15) . . ?
O12 W4 O10 86.6(14) . 1_455 ?
W4 W5 W6A 60.14(12) . . ?
W4 W5 W6B 59.58(8) . . ?
W4 W5 Rb4B 117.4(3) . . ?
W6A W5 W4 120.38(17) 1_545 . ?
W6A W5 W6A 169.5(3) 1_545 . ?
W6A W5 W6B 179.5(2) 1_545 . ?
W6A W5 W6B 11.50(11) 1_545 1_545 ?
W6A W5 Rb4B 121.7(3) 1_545 . ?
W6A W5 Rb4B 57.3(3) . . ?
W6B W5 W4 119.71(12) 1_545 . ?
W6B W5 W6A 178.99(19) 1_545 . ?
W6B W5 W6A 10.98(11) . . ?
W6B W5 W6B 168.01(19) 1_545 . ?
W6B W5 Rb4B 58.4(3) . . ?
W6B W5 Rb4B 122.7(3) 1_545 . ?
O11 W5 W4 18.1(8) . . ?
O11 W5 W6A 102.8(8) . 1_545 ?
O11 W5 W6A 78.2(8) . . ?
O11 W5 W6B 101.6(8) . 1_545 ?
O11 W5 W6B 77.2(8) . . ?
O11 W5 Rb4B 135.4(8) . . ?
O13 W5 W4 160.6(13) . . ?
O13 W5 W6A 101.9(13) . . ?
O13 W5 W6A 75.8(12) . 1_545 ?
O13 W5 W6B 78.4(13) . 1_545 ?
O13 W5 W6B 104.3(12) . . ?
O13 W5 Rb4B 46.0(13) . . ?
O13 W5 O11 172.9(14) . . ?
O13 W5 O14 97.4(14) . . ?
O13 W5 O15 106.4(14) . . ?
O13 W5 O15 91.8(14) . 1_655 ?
O13 W5 O16 96.9(14) . . ?
O14 W5 W4 65.3(7) . . ?
O14 W5 W6A 171.1(9) . 1_545 ?
O14 W5 W6A 6.5(8) . . ?
O14 W5 W6B 9.3(9) . . ?
O14 W5 W6B 172.9(9) . 1_545 ?
O14 W5 Rb4B 52.1(7) . . ?
O14 W5 O11 83.3(10) . . ?
O14 W5 O15 88.0(14) . 1_655 ?
O14 W5 O15 89.9(15) . . ?
O14 W5 O16 164.6(10) . . ?
O15 W5 W4 79.3(8) 1_655 . ?
O15 W5 W4 83.4(9) . . ?
O15 W5 W6A 97.4(11) . 1_545 ?
O15 W5 W6A 86.6(10) 1_655 1_545 ?
O15 W5 W6A 83.2(10) 1_655 . ?
O15 W5 W6A 93.0(11) . . ?
O15 W5 W6B 82.1(11) . . ?
O15 W5 W6B 86.0(11) . 1_545 ?
O15 W5 W6B 93.9(10) 1_655 . ?
O15 W5 W6B 97.7(10) 1_655 1_545 ?
O15 W5 Rb4B 96.7(8) 1_655 . ?
O15 W5 Rb4B 96.2(9) . . ?
O15 W5 O11 81.1(12) 1_655 . ?
O15 W5 O11 80.7(12) . . ?
O15 W5 O15 161.8(16) . 1_655 ?
O15 W5 O16 91.8(13) . . ?
O16 W5 W4 99.6(7) . . ?
O16 W5 W6A 21.1(6) . 1_545 ?
O16 W5 W6A 158.4(7) . . ?
O16 W5 W6B 158.8(7) . . ?
O16 W5 W6B 21.8(7) . 1_545 ?
O16 W5 Rb4B 142.7(7) . . ?
O16 W5 O11 81.8(11) . . ?
O16 W5 O15 85.6(12) . 1_655 ?
W4 W6A W5 58.76(15) . . ?
W5 W6A W4 119.6(2) 1_565 . ?
W5 W6A W5 169.5(2) 1_565 . ?
W5 W6A Rb4B 118.3(4) 1_565 . ?
W6B W6A W4 78.4(7) . . ?
W6B W6A W4 90.7(2) 1_655 . ?
W6B W6A W5 93.3(3) 1_655 . ?
W6B W6A W5 92.1(9) . 1_565 ?
W6B W6A W5 77.5(9) . . ?
W6B W6A W5 97.1(2) 1_655 1_565 ?
W6B W6A W6B 168.3(10) . 1_655 ?
W6B W6A Rb4B 85.8(7) . . ?
W6B W6A Rb4B 96.1(2) 1_655 . ?
W6B W6A O12 81.0(12) . . ?
W6B W6A O14 74.3(13) . . ?
W6B W6A O16 87.9(12) . 1_565 ?
W6B W6A O17 15.1(8) . 1_455 ?
W6B W6A O17 176.2(11) . . ?
W6B W6A O18 83.1(15) . . ?
Rb4B W6A W4 120.1(4) . . ?
Rb4B W6A W5 61.5(3) . . ?
O12 W6A W4 14.5(9) . . ?
O12 W6A W5 73.3(9) . . ?
O12 W6A W5 105.4(9) . 1_565 ?
O12 W6A W6B 89.5(10) . 1_655 ?
O12 W6A Rb4B 134.6(10) . . ?
O12 W6A O17 91.7(11) . 1_455 ?
O14 W6A W4 63.6(7) . . ?
O14 W6A W5 6.1(8) . . ?
O14 W6A W5 165.3(10) . 1_565 ?
O14 W6A W6B 97.1(10) . 1_655 ?
O14 W6A Rb4B 56.5(7) . . ?
O14 W6A O12 78.1(11) . . ?
O14 W6A O17 86.8(11) . 1_455 ?
O16 W6A W4 98.0(7) 1_565 . ?
O16 W6A W5 154.3(8) 1_565 . ?
O16 W6A W5 21.6(7) 1_565 1_565 ?
O16 W6A W6B 98.0(8) 1_565 1_655 ?
O16 W6A Rb4B 139.0(8) 1_565 . ?
O16 W6A O12 83.8(11) 1_565 . ?
O16 W6A O14 156.2(11) 1_565 . ?
O16 W6A O17 78.4(9) 1_565 1_455 ?
O17 W6A W4 98.7(7) . . ?
O17 W6A W4 91.4(5) 1_455 . ?
O17 W6A W5 78.9(6) 1_455 1_565 ?
O17 W6A W5 90.7(5) 1_455 . ?
O17 W6A W5 103.2(8) . . ?
O17 W6A W5 87.3(8) . 1_565 ?
O17 W6A W6B 176.0(6) 1_455 1_655 ?
O17 W6A W6B 10.5(7) . 1_655 ?
O17 W6A Rb4B 97.7(7) . . ?
O17 W6A Rb4B 85.7(5) 1_455 . ?
O17 W6A O12 95.6(13) . . ?
O17 W6A O14 106.7(13) . . ?
O17 W6A O16 90.2(11) . 1_565 ?
O17 W6A O17 165.7(13) . 1_455 ?
O17 W6A O18 100.5(16) . . ?
O18 W6A W4 153.2(13) . . ?
O18 W6A W5 98.5(13) . . ?
O18 W6A W5 80.0(13) . 1_565 ?
O18 W6A W6B 105.6(14) . 1_655 ?
O18 W6A Rb4B 38.6(13) . . ?
O18 W6A O12 163.3(18) . . ?
O18 W6A O14 92.9(14) . . ?
O18 W6A O16 100.5(15) . 1_565 ?
O18 W6A O17 73.7(15) . 1_455 ?
W4 W6B W5 60.22(10) . . ?
W5 W6B W4 119.04(14) 1_565 . ?
W5 W6B W5 168.01(19) 1_565 . ?
W5 W6B Rb4B 115.3(3) 1_565 . ?
W6A W6B W4 100.3(2) 1_455 . ?
W6A W6B W4 90.5(7) . . ?
W6A W6B W5 91.6(9) . . ?
W6A W6B W5 76.4(9) . 1_565 ?
W6A W6B W5 97.6(2) 1_455 . ?
W6A W6B W5 94.3(2) 1_455 1_565 ?
W6A W6B W6A 168.3(10) . 1_455 ?
W6A W6B Rb4B 95.0(2) 1_455 . ?
W6A W6B Rb4B 82.8(8) . . ?
W6A W6B O12 79.3(12) . . ?
W6A W6B O14 84.4(13) . . ?
W6A W6B O16 70.7(11) . 1_565 ?
W6A W6B O17 158.0(12) . 1_455 ?
W6A W6B O17 2.6(8) . . ?
W6A W6B O18 73.2(15) . . ?
Rb4B W6B W4 121.7(3) . . ?
Rb4B W6B W5 62.2(3) . . ?
O12 W6B W4 18.2(9) . . ?
O12 W6B W5 102.1(9) . 1_565 ?
O12 W6B W5 75.3(9) . . ?
O12 W6B W6A 110.0(10) . 1_455 ?
O12 W6B Rb4B 133.1(9) . . ?
O12 W6B O17 77.0(11) . . ?
O14 W6B W4 65.7(7) . . ?
O14 W6B W5 8.9(9) . . ?
O14 W6B W5 160.1(10) . 1_565 ?
O14 W6B W6A 104.0(10) . 1_455 ?
O14 W6B Rb4B 56.0(7) . . ?
O14 W6B O12 79.2(11) . . ?
O14 W6B O16 150.6(12) . 1_565 ?
O14 W6B O17 85.1(11) . . ?
O16 W6B W4 98.3(6) 1_565 . ?
O16 W6B W5 152.7(7) 1_565 . ?
O16 W6B W5 21.1(7) 1_565 1_565 ?
O16 W6B W6A 103.1(8) 1_565 1_455 ?
O16 W6B Rb4B 132.1(7) 1_565 . ?
O16 W6B O12 81.0(11) 1_565 . ?
O16 W6B O17 69.4(9) 1_565 . ?
O17 W6B W4 108.2(7) 1_455 . ?
O17 W6B W4 88.5(5) . . ?
O17 W6B W5 84.2(7) 1_455 1_565 ?
O17 W6B W5 107.5(7) 1_455 . ?
O17 W6B W5 76.0(5) . 1_565 ?
O17 W6B W5 92.0(5) . . ?
O17 W6B W6A 169.3(6) . 1_455 ?
O17 W6B W6A 10.6(7) 1_455 1_455 ?
O17 W6B Rb4B 96.3(7) 1_455 . ?
O17 W6B Rb4B 85.3(5) . . ?
O17 W6B O12 115.4(12) 1_455 . ?
O17 W6B O14 113.4(13) 1_455 . ?
O17 W6B O16 94.6(10) 1_455 1_565 ?
O17 W6B O17 158.8(12) 1_455 . ?
O17 W6B O18 92.3(15) 1_455 . ?
O18 W6B W4 154.9(13) . . ?
O18 W6B W5 76.4(12) . 1_565 ?
O18 W6B W5 100.4(12) . . ?
O18 W6B W6A 97.9(14) . 1_455 ?
O18 W6B Rb4B 38.9(13) . . ?
O18 W6B O12 152.1(18) . . ?
O18 W6B O14 93.2(14) . . ?
O18 W6B O16 94.3(14) . 1_565 ?
O18 W6B O17 75.7(14) . . ?
Rb1 Rb1 W6B 67.25(13) 1_655 1_545 ?
Rb1 Rb1 W6B 112.75(13) 1_455 1_545 ?
Rb1 Rb1 Rb1 179.997(15) 1_655 1_455 ?
Rb1 Rb1 O4 90.4(4) 1_455 1_545 ?
Rb1 Rb1 O4 89.6(4) 1_655 1_545 ?
O4 Rb1 W6B 120.8(7) 1_545 1_545 ?
O5 Rb1 W6B 80.0(6) 1_545 1_545 ?
O5 Rb1 W6B 104.7(6) 1_445 1_545 ?
O5 Rb1 Rb1 128.7(6) 1_445 1_655 ?
O5 Rb1 Rb1 51.3(6) 1_445 1_455 ?
O5 Rb1 Rb1 60.9(6) 1_545 1_655 ?
O5 Rb1 Rb1 119.1(6) 1_545 1_455 ?
O5 Rb1 O4 49.4(8) 1_445 1_545 ?
O5 Rb1 O4 42.6(7) 1_545 1_545 ?
O5 Rb1 O5 67.8(6) 1_545 1_445 ?
O5 Rb1 O6 84.6(9) 1_545 1_445 ?
O5 Rb1 O6 48.1(10) 1_545 1_545 ?
O5 Rb1 O8 90.6(8) 1_545 1_455 ?
O5 Rb1 O9 90.1(7) 1_545 . ?
O5 Rb1 O9 123.8(6) 1_545 1_455 ?
O5 Rb1 O10 42.3(8) 1_545 1_445 ?
O5 Rb1 O12 48.4(8) 1_545 1_545 ?
O5 Rb1 O15 140.8(8) 1_545 . ?
O5 Rb1 O17 95.7(7) 1_545 1_445 ?
O5 Rb1 O17 95.0(6) 1_445 1_445 ?
O6 Rb1 W6B 117.3(7) 1_545 1_545 ?
O6 Rb1 W6B 148.5(8) 1_445 1_545 ?
O6 Rb1 Rb1 127.0(5) 1_445 1_655 ?
O6 Rb1 Rb1 53.0(5) 1_445 1_455 ?
O6 Rb1 Rb1 58.3(5) 1_545 1_655 ?
O6 Rb1 Rb1 121.7(5) 1_545 1_455 ?
O6 Rb1 O4 43.2(7) 1_445 1_545 ?
O6 Rb1 O4 38.3(9) 1_545 1_545 ?
O6 Rb1 O5 87.7(9) 1_545 1_445 ?
O6 Rb1 O5 43.8(9) 1_445 1_445 ?
O6 Rb1 O6 68.6(5) 1_545 1_445 ?
O6 Rb1 O8 46.6(8) 1_445 1_455 ?
O6 Rb1 O8 46.1(9) 1_545 1_455 ?
O6 Rb1 O9 46.9(10) 1_545 . ?
O6 Rb1 O9 84.7(9) 1_545 1_455 ?
O6 Rb1 O10 88.4(10) 1_545 1_445 ?
O6 Rb1 O12 86.4(9) 1_545 1_545 ?
O6 Rb1 O15 136.3(9) 1_545 . ?
O6 Rb1 O17 135.2(7) 1_445 1_445 ?
O6 Rb1 O17 139.3(9) 1_545 1_445 ?
O8 Rb1 W6B 159.1(5) 1_455 1_545 ?
O8 Rb1 Rb1 88.1(5) 1_455 1_455 ?
O8 Rb1 Rb1 91.9(5) 1_455 1_655 ?
O8 Rb1 O4 56.7(9) 1_455 1_545 ?
O8 Rb1 O5 88.5(7) 1_455 1_445 ?
O8 Rb1 O17 173.6(7) 1_455 1_445 ?
O9 Rb1 W6B 156.1(7) 1_455 1_545 ?
O9 Rb1 W6B 118.0(6) . 1_545 ?
O9 Rb1 Rb1 124.1(6) 1_455 1_655 ?
O9 Rb1 Rb1 55.9(6) 1_455 1_455 ?
O9 Rb1 Rb1 55.1(6) . 1_655 ?
O9 Rb1 Rb1 124.9(6) . 1_455 ?
O9 Rb1 O4 82.0(8) 1_455 1_545 ?
O9 Rb1 O4 81.6(9) . 1_545 ?
O9 Rb1 O5 84.4(7) 1_455 1_445 ?
O9 Rb1 O5 127.5(6) . 1_445 ?
O9 Rb1 O6 45.5(10) 1_455 1_445 ?
O9 Rb1 O6 89.1(9) . 1_445 ?
O9 Rb1 O8 42.9(8) . 1_455 ?
O9 Rb1 O8 38.9(8) 1_455 1_455 ?
O9 Rb1 O9 69.0(7) 1_455 . ?
O9 Rb1 O12 105.0(9) . 1_545 ?
O9 Rb1 O12 171.1(9) 1_455 1_545 ?
O9 Rb1 O17 135.6(7) . 1_445 ?
O9 Rb1 O17 136.0(8) 1_455 1_445 ?
O10 Rb1 W6B 62.9(6) 1_445 1_545 ?
O10 Rb1 Rb1 89.0(6) 1_445 1_455 ?
O10 Rb1 Rb1 91.0(6) 1_445 1_655 ?
O10 Rb1 O4 64.1(8) 1_445 1_545 ?
O10 Rb1 O5 47.2(7) 1_445 1_445 ?
O10 Rb1 O6 87.4(10) 1_445 1_445 ?
O10 Rb1 O8 120.7(7) 1_445 1_455 ?
O10 Rb1 O9 131.4(8) 1_445 1_455 ?
O10 Rb1 O9 132.4(9) 1_445 . ?
O10 Rb1 O12 47.6(8) 1_445 1_545 ?
O10 Rb1 O15 122.9(8) 1_445 . ?
O10 Rb1 O17 65.3(6) 1_445 1_445 ?
O11 Rb1 W6B 107.9(6) 1_455 1_545 ?
O11 Rb1 W6B 80.1(6) . 1_545 ?
O11 Rb1 Rb1 128.3(6) . 1_455 ?
O11 Rb1 Rb1 128.2(6) 1_455 1_655 ?
O11 Rb1 Rb1 51.7(6) . 1_655 ?
O11 Rb1 Rb1 51.8(6) 1_455 1_455 ?
O11 Rb1 O4 127.7(8) 1_455 1_545 ?
O11 Rb1 O4 127.0(9) . 1_545 ?
O11 Rb1 O5 112.3(9) . 1_545 ?
O11 Rb1 O5 169.5(9) 1_455 1_545 ?
O11 Rb1 O5 102.9(8) 1_455 1_445 ?
O11 Rb1 O5 175.0(9) . 1_445 ?
O11 Rb1 O6 85.2(9) 1_455 1_445 ?
O11 Rb1 O6 88.9(9) . 1_545 ?
O11 Rb1 O6 131.3(10) . 1_445 ?
O11 Rb1 O6 129.1(11) 1_455 1_545 ?
O11 Rb1 O8 84.1(8) 1_455 1_455 ?
O11 Rb1 O8 86.5(8) . 1_455 ?
O11 Rb1 O9 48.2(9) 1_455 1_455 ?
O11 Rb1 O9 91.6(9) . 1_455 ?
O11 Rb1 O9 92.1(9) 1_455 . ?
O11 Rb1 O9 47.8(8) . . ?
O11 Rb1 O10 134.7(8) 1_455 1_445 ?
O11 Rb1 O10 136.3(9) . 1_445 ?
O11 Rb1 O11 76.5(7) 1_455 . ?
O11 Rb1 O12 88.7(7) . 1_545 ?
O11 Rb1 O12 95.2(7) 1_455 1_445 ?
O11 Rb1 O12 140.2(6) 1_455 1_545 ?
O11 Rb1 O12 137.5(7) . 1_445 ?
O11 Rb1 O15 47.5(8) . . ?
O11 Rb1 O15 49.4(8) 1_455 . ?
O11 Rb1 O16 98.0(8) 1_455 . ?
O11 Rb1 O16 50.3(9) . . ?
O11 Rb1 O17 90.0(7) . 1_445 ?
O11 Rb1 O17 89.9(7) 1_455 1_445 ?
O12 Rb1 W6B 62.8(7) 1_445 1_545 ?
O12 Rb1 W6B 32.5(6) 1_545 1_545 ?
O12 Rb1 Rb1 121.6(7) 1_445 1_655 ?
O12 Rb1 Rb1 129.7(6) 1_545 1_455 ?
O12 Rb1 Rb1 50.3(6) 1_545 1_655 ?
O12 Rb1 Rb1 58.4(7) 1_445 1_455 ?
O12 Rb1 O4 91.2(9) 1_445 1_545 ?
O12 Rb1 O4 90.7(8) 1_545 1_545 ?
O12 Rb1 O5 94.7(8) 1_545 1_445 ?
O12 Rb1 O5 47.4(8) 1_445 1_445 ?
O12 Rb1 O5 82.1(10) 1_445 1_545 ?
O12 Rb1 O6 88.2(9) 1_445 1_445 ?
O12 Rb1 O6 125.2(11) 1_445 1_545 ?
O12 Rb1 O6 129.8(10) 1_545 1_445 ?
O12 Rb1 O8 134.7(8) 1_445 1_455 ?
O12 Rb1 O8 132.3(8) 1_545 1_455 ?
O12 Rb1 O9 172.0(10) 1_445 . ?
O12 Rb1 O9 113.8(9) 1_445 1_455 ?
O12 Rb1 O10 39.9(8) 1_445 1_445 ?
O12 Rb1 O12 71.3(7) 1_445 1_545 ?
O12 Rb1 O15 95.6(8) 1_445 . ?
O12 Rb1 O16 91.2(9) 1_445 . ?
O12 Rb1 O17 52.8(7) 1_545 1_445 ?
O12 Rb1 O17 47.9(7) 1_445 1_445 ?
O15 Rb1 W6B 64.8(6) . 1_545 ?
O15 Rb1 Rb1 91.2(5) . 1_455 ?
O15 Rb1 Rb1 88.8(5) . 1_655 ?
O15 Rb1 O4 172.8(10) . 1_545 ?
O15 Rb1 O5 135.6(7) . 1_445 ?
O15 Rb1 O6 134.5(9) . 1_445 ?
O15 Rb1 O8 116.4(7) . 1_455 ?
O15 Rb1 O9 91.7(8) . . ?
O15 Rb1 O9 93.1(8) . 1_455 ?
O15 Rb1 O12 93.7(8) . 1_545 ?
O15 Rb1 O17 57.6(7) . 1_445 ?
O16 Rb1 W6B 29.8(6) . 1_545 ?
O16 Rb1 W6B 64.9(5) 1_455 1_545 ?
O16 Rb1 Rb1 51.1(4) . 1_655 ?
O16 Rb1 Rb1 125.9(4) 1_455 1_655 ?
O16 Rb1 Rb1 128.9(4) . 1_455 ?
O16 Rb1 Rb1 54.1(4) 1_455 1_455 ?
O16 Rb1 O4 136.8(8) 1_455 1_545 ?
O16 Rb1 O4 133.8(7) . 1_545 ?
O16 Rb1 O5 130.1(10) 1_455 1_545 ?
O16 Rb1 O5 134.5(9) . 1_445 ?
O16 Rb1 O5 87.4(8) 1_455 1_445 ?
O16 Rb1 O5 92.2(9) . 1_545 ?
O16 Rb1 O6 175.0(9) 1_455 1_545 ?
O16 Rb1 O6 176.8(11) . 1_445 ?
O16 Rb1 O6 109.4(7) . 1_545 ?
O16 Rb1 O6 107.1(6) 1_455 1_445 ?
O16 Rb1 O8 132.9(8) 1_455 1_455 ?
O16 Rb1 O8 133.9(8) . 1_455 ?
O16 Rb1 O9 91.1(8) . . ?
O16 Rb1 O9 94.0(9) 1_455 1_455 ?
O16 Rb1 O9 136.9(10) 1_455 . ?
O16 Rb1 O9 137.3(9) . 1_455 ?
O16 Rb1 O10 90.1(9) . 1_445 ?
O16 Rb1 O10 88.9(9) 1_455 1_445 ?
O16 Rb1 O11 96.0(9) 1_455 . ?
O16 Rb1 O11 51.5(9) 1_455 1_455 ?
O16 Rb1 O12 94.8(8) 1_455 1_545 ?
O16 Rb1 O12 47.2(8) . 1_545 ?
O16 Rb1 O12 51.1(9) 1_455 1_445 ?
O16 Rb1 O15 48.6(7) . . ?
O16 Rb1 O15 48.5(8) 1_455 . ?
O16 Rb1 O16 74.8(4) 1_455 . ?
O16 Rb1 O17 42.2(6) 1_455 1_445 ?
O16 Rb1 O17 44.8(6) . 1_445 ?
O17 Rb1 W6B 23.5(3) 1_445 1_545 ?
O17 Rb1 Rb1 90.1(3) 1_445 1_655 ?
O17 Rb1 Rb1 89.9(3) 1_445 1_455 ?
O17 Rb1 O4 129.4(8) 1_445 1_545 ?
Rb2B Rb2A Rb2A 179.9(8) 1_455 1_655 ?
Rb2B Rb2A Rb2A 0.1(8) . 1_655 ?
Rb2B Rb2A Rb2B 179.8(17) 1_455 . ?
Rb2B Rb2A O1 89.9(8) 1_455 1_455 ?
Rb2B Rb2A O1 89.9(8) . 1_455 ?
Rb2B Rb2A O2 54.4(10) . 2_665 ?
Rb2B Rb2A O2 125.7(11) 1_455 2_665 ?
Rb2B Rb2A O2 52.4(10) 1_455 2_565 ?
Rb2B Rb2A O2 125.7(11) . 1_465 ?
Rb2B Rb2A O2 54.4(10) 1_455 1_465 ?
Rb2B Rb2A O2 127.8(10) 1_455 1_565 ?
Rb2B Rb2A O2 52.4(10) . 1_565 ?
Rb2B Rb2A O2 127.8(10) . 2_565 ?
Rb2B Rb2A O3 119.2(10) 1_455 2_655 ?
Rb2B Rb2A O3 51.1(9) . . ?
Rb2B Rb2A O3 128.8(10) . 2 ?
Rb2B Rb2A O3 60.6(9) . 2_655 ?
Rb2B Rb2A O3 51.1(9) 1_455 2 ?
Rb2B Rb2A O3 60.6(9) 1_455 1_455 ?
Rb2B Rb2A O3 128.8(10) 1_455 . ?
Rb2B Rb2A O3 119.2(10) . 1_455 ?
Rb2B Rb2A O4 91.0(6) 1_455 . ?
Rb2B Rb2A O4 91.0(6) . 2 ?
Rb2B Rb2A O4 89.1(6) 1_455 2 ?
Rb2B Rb2A O4 89.1(6) . . ?
Rb2B Rb2A O7 52.0(6) . 2_655 ?
Rb2B Rb2A O7 125.5(6) . 2 ?
Rb2B Rb2A O7 54.5(6) . . ?
Rb2B Rb2A O7 128.0(6) 1_455 2_655 ?
Rb2B Rb2A O7 52.0(6) 1_455 1_455 ?
Rb2B Rb2A O7 128.0(6) . 1_455 ?
Rb2B Rb2A O7 54.5(6) 1_455 2 ?
Rb2B Rb2A O7 125.5(6) 1_455 . ?
Rb2B Rb2A O8 91.3(6) 1_455 2_655 ?
Rb2B Rb2A O8 91.3(6) . 1_455 ?
Rb2B Rb2A O8 88.6(6) 1_455 1_455 ?
Rb2B Rb2A O8 88.6(6) . 2_655 ?
O1 Rb2A Rb2A 90.000(1) 1_455 1_655 ?
O1 Rb2A O3 46.8(6) 1_455 2 ?
O1 Rb2A O3 46.8(6) 1_455 . ?
O1 Rb2A O4 123.7(8) 1_455 . ?
O1 Rb2A O4 123.7(8) 1_455 2 ?
O1 Rb2A O8 61.2(4) 1_455 2_655 ?
O1 Rb2A O8 61.2(4) 1_455 1_455 ?
O2 Rb2A Rb2A 54.4(7) 2_665 1_655 ?
O2 Rb2A Rb2A 125.6(7) 1_465 1_655 ?
O2 Rb2A Rb2A 127.7(7) 2_565 1_655 ?
O2 Rb2A Rb2A 52.3(7) 1_565 1_655 ?
O2 Rb2A O1 135.0(7) 2_665 1_455 ?
O2 Rb2A O1 133.5(7) 1_565 1_455 ?
O2 Rb2A O1 135.0(7) 1_465 1_455 ?
O2 Rb2A O1 133.5(7) 2_565 1_455 ?
O2 Rb2A O2 90.0(14) 2_665 1_465 ?
O2 Rb2A O2 73.3(8) 1_465 1_565 ?
O2 Rb2A O2 73.3(8) 2_665 2_565 ?
O2 Rb2A O2 46.6(13) 2_665 1_565 ?
O2 Rb2A O2 46.6(13) 1_465 2_565 ?
O2 Rb2A O2 93.0(14) 1_565 2_565 ?
O2 Rb2A O3 135.2(6) 2_565 . ?
O2 Rb2A O3 103.4(8) 2_565 2 ?
O2 Rb2A O3 88.2(8) 2_665 . ?
O2 Rb2A O3 135.2(6) 1_565 2 ?
O2 Rb2A O3 131.3(7) 2_665 1_455 ?
O2 Rb2A O3 115.1(9) 2_665 2_655 ?
O2 Rb2A O3 176.7(10) 1_465 . ?
O2 Rb2A O3 131.3(7) 1_465 2_655 ?
O2 Rb2A O3 103.4(8) 1_565 . ?
O2 Rb2A O3 115.1(9) 1_465 1_455 ?
O2 Rb2A O3 88.2(8) 1_465 2 ?
O2 Rb2A O3 176.7(10) 2_665 2 ?
O2 Rb2A O4 44.3(8) 1_465 . ?
O2 Rb2A O4 86.0(10) 1_465 2 ?
O2 Rb2A O4 44.2(9) 2_565 2 ?
O2 Rb2A O4 44.2(9) 1_565 . ?
O2 Rb2A O4 87.3(9) 1_565 2 ?
O2 Rb2A O4 86.0(10) 2_665 . ?
O2 Rb2A O4 44.3(8) 2_665 2 ?
O2 Rb2A O4 87.3(9) 2_565 . ?
O2 Rb2A O7 87.7(10) 2_565 1_455 ?
O2 Rb2A O7 134.8(12) 1_465 2_655 ?
O2 Rb2A O7 95.7(10) 1_565 1_455 ?
O2 Rb2A O7 87.7(10) 1_565 2_655 ?
O2 Rb2A O7 134.8(12) 2_665 1_455 ?
O2 Rb2A O7 95.7(10) 2_565 2_655 ?
O2 Rb2A O7 49.9(12) 2_665 2_655 ?
O2 Rb2A O7 49.9(11) 1_465 1_455 ?
O2 Rb2A O8 88.6(8) 2_665 2_655 ?
O2 Rb2A O8 88.6(8) 1_465 1_455 ?
O2 Rb2A O8 131.2(8) 2_565 1_455 ?
O2 Rb2A O8 134.8(8) 1_465 2_655 ?
O2 Rb2A O8 90.2(8) 1_565 1_455 ?
O2 Rb2A O8 131.2(8) 1_565 2_655 ?
O2 Rb2A O8 90.2(8) 2_565 2_655 ?
O2 Rb2A O8 134.8(8) 2_665 1_455 ?
O3 Rb2A Rb2A 128.9(6) 2 1_655 ?
O3 Rb2A Rb2A 60.7(6) 2_655 1_655 ?
O3 Rb2A Rb2A 51.1(6) . 1_655 ?
O3 Rb2A Rb2A 119.3(6) 1_455 1_655 ?
O3 Rb2A O1 40.0(6) 2_655 1_455 ?
O3 Rb2A O1 40.0(6) 1_455 1_455 ?
O3 Rb2A O2 171.6(10) 2_655 2_565 ?
O3 Rb2A O2 171.6(10) 1_455 1_565 ?
O3 Rb2A O2 93.8(7) 1_455 2_565 ?
O3 Rb2A O2 93.8(7) 2_655 1_565 ?
O3 Rb2A O3 47.4(11) 2_655 . ?
O3 Rb2A O3 68.2(7) 1_455 . ?
O3 Rb2A O3 80.0(12) 1_455 2_655 ?
O3 Rb2A O3 47.4(11) 1_455 2 ?
O3 Rb2A O3 68.2(7) 2_655 2 ?
O3 Rb2A O3 93.6(11) . 2 ?
O3 Rb2A O4 94.1(9) 1_455 2 ?
O3 Rb2A O4 141.2(9) 1_455 . ?
O3 Rb2A O4 141.2(9) 2_655 2 ?
O3 Rb2A O4 94.1(9) 2_655 . ?
O3 Rb2A O7 89.6(11) 1_455 1_455 ?
O3 Rb2A O7 86.6(10) 2_655 1_455 ?
O3 Rb2A O7 86.6(10) 1_455 2_655 ?
O3 Rb2A O7 89.6(11) 2_655 2_655 ?
O3 Rb2A O8 48.0(7) 2 1_455 ?
O3 Rb2A O8 89.1(8) 1_455 1_455 ?
O3 Rb2A O8 89.1(8) 2_655 2_655 ?
O3 Rb2A O8 90.6(7) . 1_455 ?
O3 Rb2A O8 43.7(8) 1_455 2_655 ?
O3 Rb2A O8 48.0(7) . 2_655 ?
O3 Rb2A O8 90.6(7) 2 2_655 ?
O3 Rb2A O8 43.7(8) 2_655 1_455 ?
O4 Rb2A Rb2A 89.0(4) . 1_655 ?
O4 Rb2A Rb2A 91.0(4) 2 1_655 ?
O4 Rb2A O3 94.7(9) . 2 ?
O4 Rb2A O3 94.7(9) 2 . ?
O4 Rb2A O3 132.7(7) 2 2 ?
O4 Rb2A O3 132.7(7) . . ?
O4 Rb2A O4 112.6(15) . 2 ?
O4 Rb2A O8 174.6(8) . 2_655 ?
O4 Rb2A O8 62.6(9) 2 2_655 ?
O4 Rb2A O8 62.6(9) . 1_455 ?
O4 Rb2A O8 174.6(8) 2 1_455 ?
O7 Rb2A Rb2A 54.5(6) . 1_655 ?
O7 Rb2A Rb2A 125.5(6) 2 1_655 ?
O7 Rb2A Rb2A 52.0(6) 2_655 1_655 ?
O7 Rb2A Rb2A 128.0(6) 1_455 1_655 ?
O7 Rb2A O1 87.5(10) 1_455 1_455 ?
O7 Rb2A O1 87.5(10) 2 1_455 ?
O7 Rb2A O1 87.5(10) 2_655 1_455 ?
O7 Rb2A O1 87.5(10) . 1_455 ?
O7 Rb2A O2 92.5(11) 2 2_665 ?
O7 Rb2A O2 134.7(12) . 2_565 ?
O7 Rb2A O2 50.1(12) . 1_565 ?
O7 Rb2A O2 91.1(11) 2 1_465 ?
O7 Rb2A O2 92.5(11) . 1_465 ?
O7 Rb2A O2 134.7(12) 2 1_565 ?
O7 Rb2A O2 91.1(11) . 2_665 ?
O7 Rb2A O2 50.1(12) 2 2_565 ?
O7 Rb2A O3 130.5(11) 1_455 . ?
O7 Rb2A O3 91.8(10) . 2 ?
O7 Rb2A O3 44.9(10) 2_655 . ?
O7 Rb2A O3 130.5(11) 2_655 2 ?
O7 Rb2A O3 126.1(12) 2 2_655 ?
O7 Rb2A O3 49.0(11) . 2_655 ?
O7 Rb2A O3 126.1(12) . 1_455 ?
O7 Rb2A O3 44.9(10) 1_455 2 ?
O7 Rb2A O3 49.0(11) 2 1_455 ?
O7 Rb2A O3 91.8(10) 2 . ?
O7 Rb2A O3 84.7(10) 2 2 ?
O7 Rb2A O3 84.7(10) . . ?
O7 Rb2A O4 48.6(10) 2 2 ?
O7 Rb2A O4 48.6(10) . . ?
O7 Rb2A O4 131.9(10) 2_655 . ?
O7 Rb2A O4 135.3(10) 2 . ?
O7 Rb2A O4 51.7(10) 1_455 . ?
O7 Rb2A O4 51.7(10) 2_655 2 ?
O7 Rb2A O4 131.9(10) 1_455 2 ?
O7 Rb2A O4 135.3(10) . 2 ?
O7 Rb2A O7 73.5(5) 2 2_655 ?
O7 Rb2A O7 106.3(5) 2 1_455 ?
O7 Rb2A O7 175(2) 2_655 1_455 ?
O7 Rb2A O7 106.3(5) . 2_655 ?
O7 Rb2A O7 175(2) 2 . ?
O7 Rb2A O7 73.5(5) . 1_455 ?
O7 Rb2A O8 43.6(9) 1_455 1_455 ?
O7 Rb2A O8 43.9(9) 2 2_655 ?
O7 Rb2A O8 133.1(9) 2_655 1_455 ?
O7 Rb2A O8 43.9(9) . 1_455 ?
O7 Rb2A O8 133.1(9) 1_455 2_655 ?
O7 Rb2A O8 132.6(10) . 2_655 ?
O7 Rb2A O8 43.6(9) 2_655 2_655 ?
O7 Rb2A O8 132.6(9) 2 1_455 ?
O8 Rb2A Rb2A 88.7(4) 2_655 1_655 ?
O8 Rb2A Rb2A 91.3(4) 1_455 1_655 ?
O8 Rb2A O8 122.4(9) 2_655 1_455 ?
W1 Rb2B W1 179.57(8) 2_665 . ?
W1 Rb2B W1 167.94(9) 1_565 . ?
W1 Rb2B W1 167.94(9) 2_665 2_655 ?
W1 Rb2B W1 11.64(13) 2_655 . ?
W1 Rb2B W1 179.57(8) 1_565 2_655 ?
W1 Rb2B W1 12.49(12) 1_565 2_665 ?
W1 Rb2B W2 62.0(3) 1_565 2_655 ?
W1 Rb2B W2 62.5(4) 1_565 . ?
W1 Rb2B W2 62.5(4) 2_665 2_655 ?
W1 Rb2B W2 62.0(3) 2_665 . ?
W1 Rb2B W3 122.0(3) 1_565 2_655 ?
W1 Rb2B W3 121.1(3) 1_565 . ?
W1 Rb2B W3 121.1(3) 2_665 2_655 ?
W1 Rb2B W3 122.0(3) 2_665 . ?
W1 Rb2B Rb2B 83.76(6) 1_565 1_655 ?
W1 Rb2B Rb2B 96.24(6) 1_565 1_455 ?
W1 Rb2B Rb2B 95.82(6) . 1_455 ?
W1 Rb2B Rb2B 96.24(6) 2_665 1_655 ?
W1 Rb2B Rb2B 83.76(6) 2_665 1_455 ?
W1 Rb2B Rb2B 95.82(6) 2_655 1_655 ?
W1 Rb2B Rb2B 84.18(6) . 1_655 ?
W1 Rb2B Rb2B 84.18(6) 2_655 1_455 ?
W1 Rb2B O4 116.2(7) . 2_655 ?
W1 Rb2B O4 116.2(7) 2_655 . ?
W1 Rb2B O4 57.6(8) 1_565 2_655 ?
W1 Rb2B O4 64.0(8) 2_665 2_655 ?
W1 Rb2B O4 122.2(8) . . ?
W1 Rb2B O4 64.0(8) 1_565 . ?
W1 Rb2B O4 57.6(7) 2_665 . ?
W1 Rb2B O4 122.2(8) 2_655 2_655 ?
W2 Rb2B W1 118.0(3) . . ?
W2 Rb2B W1 118.0(3) 2_655 2_655 ?
W2 Rb2B W1 117.5(3) 2_655 . ?
W2 Rb2B W1 117.5(3) . 2_655 ?
W2 Rb2B W2 124.2(7) 2_655 . ?
W2 Rb2B W3 60.01(5) 2_655 2_655 ?
W2 Rb2B W3 60.01(5) . . ?
W2 Rb2B W3 173.3(4) . 2_655 ?
W2 Rb2B W3 173.3(4) 2_655 . ?
W2 Rb2B Rb2B 86.57(8) 2_655 1_655 ?
W2 Rb2B Rb2B 86.57(8) . 1_455 ?
W2 Rb2B Rb2B 93.43(8) . 1_655 ?
W2 Rb2B Rb2B 93.43(8) 2_655 1_455 ?
W2 Rb2B O4 116.5(9) . 2_655 ?
W2 Rb2B O4 25.3(4) 2_655 2_655 ?
W2 Rb2B O4 116.5(9) 2_655 . ?
W2 Rb2B O4 25.3(4) . . ?
W3 Rb2B W1 58.8(3) 2_655 . ?
W3 Rb2B W1 58.0(3) 2_655 2_655 ?
W3 Rb2B W1 58.0(3) . . ?
W3 Rb2B W1 58.8(3) . 2_655 ?
W3 Rb2B W3 116.4(6) 2_655 . ?
W3 Rb2B Rb2B 92.09(4) 2_655 1_655 ?
W3 Rb2B Rb2B 87.91(4) . 1_655 ?
W3 Rb2B Rb2B 87.91(4) 2_655 1_455 ?
W3 Rb2B Rb2B 92.09(4) . 1_455 ?
W3 Rb2B O4 149.7(4) 2_655 . ?
W3 Rb2B O4 149.7(4) . 2_655 ?
W3 Rb2B O4 69.7(6) . . ?
W3 Rb2B O4 69.7(6) 2_655 2_655 ?
Rb2A Rb2B W1 84.3(8) 1_655 . ?
Rb2A Rb2B W1 95.9(9) . . ?
Rb2A Rb2B W1 96.1(9) . 1_565 ?
Rb2A Rb2B W1 83.7(8) 1_655 1_565 ?
Rb2A Rb2B W1 84.3(8) . 2_655 ?
Rb2A Rb2B W1 83.7(8) . 2_665 ?
Rb2A Rb2B W1 96.1(9) 1_655 2_665 ?
Rb2A Rb2B W1 95.9(9) 1_655 2_655 ?
Rb2A Rb2B W2 93.4(4) . 2_655 ?
Rb2A Rb2B W2 86.5(4) . . ?
Rb2A Rb2B W2 86.5(4) 1_655 2_655 ?
Rb2A Rb2B W2 93.4(4) 1_655 . ?
Rb2A Rb2B W3 92.1(4) 1_655 2_655 ?
Rb2A Rb2B W3 92.1(4) . . ?
Rb2A Rb2B W3 88.0(4) 1_655 . ?
Rb2A Rb2B W3 88.0(4) . 2_655 ?
Rb2A Rb2B Rb2A 179.8(17) 1_655 . ?
Rb2A Rb2B Rb2B 179.9(8) 1_655 1_455 ?
Rb2A Rb2B Rb2B 0.1(8) 1_655 1_655 ?
Rb2A Rb2B Rb2B 179.9(8) . 1_655 ?
Rb2A Rb2B Rb2B 0.1(8) . 1_455 ?
Rb2A Rb2B O2 91.5(12) . 1_565 ?
Rb2A Rb2B O2 88.3(12) 1_655 1_565 ?
Rb2A Rb2B O2 88.3(12) . 2_665 ?
Rb2A Rb2B O2 91.5(12) 1_655 2_665 ?
Rb2A Rb2B O3 97.1(11) 1_655 2_655 ?
Rb2A Rb2B O3 83.1(10) 1_655 . ?
Rb2A Rb2B O3 97.1(11) . . ?
Rb2A Rb2B O3 83.1(10) . 2_655 ?
Rb2A Rb2B O4 118.1(7) . 2_655 ?
Rb2A Rb2B O4 61.8(5) . . ?
Rb2A Rb2B O4 61.8(5) 1_655 2_655 ?
Rb2A Rb2B O4 118.1(7) 1_655 . ?
Rb2A Rb2B O7 88.1(8) 1_655 2_655 ?
Rb2A Rb2B O7 92.0(8) 1_655 . ?
Rb2A Rb2B O7 92.0(8) . 2_655 ?
Rb2A Rb2B O7 88.1(8) . . ?
Rb2B Rb2B Rb2B 180.0 1_655 1_455 ?
Rb2B Rb2B O4 61.9(4) 1_655 2_655 ?
Rb2B Rb2B O4 118.1(4) 1_655 . ?
Rb2B Rb2B O4 118.1(4) 1_455 2_655 ?
Rb2B Rb2B O4 61.9(4) 1_455 . ?
O2 Rb2B W1 149.4(9) 2_665 2_655 ?
O2 Rb2B W1 30.7(9) 1_565 2_665 ?
O2 Rb2B W1 29.6(9) 2_665 2_665 ?
O2 Rb2B W1 149.4(9) 1_565 . ?
O2 Rb2B W1 150.4(9) 2_665 . ?
O2 Rb2B W1 150.4(9) 1_565 2_655 ?
O2 Rb2B W1 30.7(9) 2_665 1_565 ?
O2 Rb2B W1 29.6(9) 1_565 1_565 ?
O2 Rb2B W2 91.5(10) 1_565 2_655 ?
O2 Rb2B W2 32.9(8) 2_665 2_655 ?
O2 Rb2B W2 91.5(10) 2_665 . ?
O2 Rb2B W2 32.9(8) 1_565 . ?
O2 Rb2B W3 151.4(10) 2_665 . ?
O2 Rb2B W3 151.4(10) 1_565 2_655 ?
O2 Rb2B W3 92.3(8) 1_565 . ?
O2 Rb2B W3 92.3(8) 2_665 2_655 ?
O2 Rb2B Rb2B 91.6(9) 2_665 1_655 ?
O2 Rb2B Rb2B 88.4(9) 2_665 1_455 ?
O2 Rb2B Rb2B 88.4(9) 1_565 1_655 ?
O2 Rb2B Rb2B 91.6(9) 1_565 1_455 ?
O2 Rb2B O2 59.1(17) 1_565 2_665 ?
O2 Rb2B O3 171.4(12) 1_565 . ?
O2 Rb2B O3 171.4(11) 2_665 2_655 ?
O2 Rb2B O3 121.9(8) 2_665 . ?
O2 Rb2B O3 121.9(8) 1_565 2_655 ?
O2 Rb2B O4 85.5(12) 2_665 . ?
O2 Rb2B O4 39.3(11) 1_565 . ?
O2 Rb2B O4 85.5(12) 1_565 2_655 ?
O2 Rb2B O4 39.3(11) 2_665 2_655 ?
O3 Rb2B W1 31.1(7) . 2_655 ?
O3 Rb2B W1 148.8(7) 2_655 2_665 ?
O3 Rb2B W1 31.1(7) 2_655 . ?
O3 Rb2B W1 28.6(7) . . ?
O3 Rb2B W1 28.6(7) 2_655 2_655 ?
O3 Rb2B W1 148.8(7) . 1_565 ?
O3 Rb2B W1 151.5(7) 2_655 1_565 ?
O3 Rb2B W1 151.5(7) . 2_665 ?
O3 Rb2B W2 89.0(7) . 2_655 ?
O3 Rb2B W2 146.5(9) . . ?
O3 Rb2B W2 146.5(9) 2_655 2_655 ?
O3 Rb2B W2 89.0(7) 2_655 . ?
O3 Rb2B W3 30.9(7) . 2_655 ?
O3 Rb2B W3 30.9(7) 2_655 . ?
O3 Rb2B W3 86.5(9) 2_655 2_655 ?
O3 Rb2B W3 86.5(9) . . ?
O3 Rb2B Rb2B 83.0(7) . 1_655 ?
O3 Rb2B Rb2B 97.0(7) 2_655 1_655 ?
O3 Rb2B Rb2B 83.0(7) 2_655 1_455 ?
O3 Rb2B Rb2B 97.0(7) . 1_455 ?
O3 Rb2B O3 58.6(14) . 2_655 ?
O3 Rb2B O4 146.3(11) . . ?
O3 Rb2B O4 91.3(10) 2_655 . ?
O3 Rb2B O4 146.3(11) 2_655 2_655 ?
O3 Rb2B O4 91.3(10) . 2_655 ?
O4 Rb2B O4 121.3(15) . 2_655 ?
O7 Rb2B W1 87.0(13) . . ?
O7 Rb2B W1 93.1(13) 2_655 2_665 ?
O7 Rb2B W1 93.0(13) 2_655 1_565 ?
O7 Rb2B W1 86.9(13) 2_655 . ?
O7 Rb2B W1 87.0(13) 2_655 2_655 ?
O7 Rb2B W1 93.1(13) . 1_565 ?
O7 Rb2B W1 93.0(13) . 2_665 ?
O7 Rb2B W1 86.9(13) . 2_655 ?
O7 Rb2B W2 155.1(15) . 2_655 ?
O7 Rb2B W2 31.0(12) . . ?
O7 Rb2B W2 31.0(12) 2_655 2_655 ?
O7 Rb2B W2 155.1(15) 2_655 . ?
O7 Rb2B W3 29.1(12) . . ?
O7 Rb2B W3 144.9(15) 2_655 . ?
O7 Rb2B W3 29.1(12) 2_655 2_655 ?
O7 Rb2B W3 144.9(15) . 2_655 ?
O7 Rb2B Rb2B 92.0(8) . 1_655 ?
O7 Rb2B Rb2B 88.0(8) . 1_455 ?
O7 Rb2B Rb2B 92.0(8) 2_655 1_455 ?
O7 Rb2B Rb2B 88.0(8) 2_655 1_655 ?
O7 Rb2B O2 122.5(17) 2_655 1_565 ?
O7 Rb2B O2 63.6(15) . 1_565 ?
O7 Rb2B O2 63.6(15) 2_655 2_665 ?
O7 Rb2B O2 122.5(17) . 2_665 ?
O7 Rb2B O3 115.5(16) 2_655 2_655 ?
O7 Rb2B O3 58.4(14) . 2_655 ?
O7 Rb2B O3 58.4(14) 2_655 . ?
O7 Rb2B O3 115.5(16) . . ?
O7 Rb2B O4 43.8(12) 2_655 2_655 ?
O7 Rb2B O4 140.7(13) 2_655 . ?
O7 Rb2B O4 140.7(13) . 2_655 ?
O7 Rb2B O4 43.8(12) . . ?
O7 Rb2B O7 174(3) 2_655 . ?
W5 Rb3 W5 141.5(2) 2_656 1_455 ?
W5 Rb3 Rb4A 109.27(11) 1_455 1_545 ?
W5 Rb3 Rb4A 109.27(11) 2_656 1_545 ?
Rb3 Rb3 W5 61.56(5) 1_455 1_455 ?
Rb3 Rb3 W5 118.44(5) 1_655 1_455 ?
Rb3 Rb3 W5 118.44(5) 1_455 2_656 ?
Rb3 Rb3 W5 61.56(5) 1_655 2_656 ?
Rb3 Rb3 Rb3 180.0 1_655 1_455 ?
Rb3 Rb3 Rb4A 90.000(1) 1_655 1_545 ?
Rb3 Rb3 Rb4A 90.000(6) 1_455 1_545 ?
Rb3 Rb3 Rb4B 60.21(18) 1_655 . ?
Rb3 Rb3 Rb4B 119.79(18) 1_455 . ?
Rb3 Rb3 Rb4B 60.21(18) 1_455 1_455 ?
Rb3 Rb3 Rb4B 119.79(18) 1_655 1_455 ?
Rb4A Rb3 W5 70.73(11) . 1_455 ?
Rb4A Rb3 W5 70.73(11) . 2_656 ?
Rb4A Rb3 Rb3 90.000(3) . 1_455 ?
Rb4A Rb3 Rb3 90.000(4) . 1_655 ?
Rb4A Rb3 Rb4A 180.0 . 1_545 ?
Rb4A Rb3 Rb4B 29.79(17) . 1_455 ?
Rb4A Rb3 Rb4B 29.79(18) . . ?
Rb4A Rb3 O15 68.8(5) . . ?
Rb4A Rb3 O15 68.8(5) . 2_556 ?
Rb4A Rb3 O17 122.4(3) . 1_445 ?
Rb4A Rb3 O17 122.4(3) . 2_646 ?
Rb4B Rb3 W5 58.47(10) . 2_656 ?
Rb4B Rb3 W5 58.47(10) 1_455 1_455 ?
Rb4B Rb3 W5 87.15(17) . 1_455 ?
Rb4B Rb3 W5 87.15(17) 1_455 2_656 ?
Rb4B Rb3 Rb4A 150.21(18) . 1_545 ?
Rb4B Rb3 Rb4A 150.21(18) 1_455 1_545 ?
Rb4B Rb3 Rb4B 59.6(4) . 1_455 ?
O13 Rb3 W5 90.6(5) . 2_656 ?
O13 Rb3 W5 136.5(8) 1_455 2_656 ?
O13 Rb3 W5 136.5(8) 2_656 1_455 ?
O13 Rb3 W5 14.3(9) 2_656 2_656 ?
O13 Rb3 W5 76.9(3) 2_556 2_656 ?
O13 Rb3 W5 76.9(3) . 1_455 ?
O13 Rb3 W5 14.3(9) 1_455 1_455 ?
O13 Rb3 W5 90.6(5) 2_556 1_455 ?
O13 Rb3 Rb3 138.2(3) 2_556 1_655 ?
O13 Rb3 Rb3 41.8(3) . 1_655 ?
O13 Rb3 Rb3 41.8(3) 2_556 1_455 ?
O13 Rb3 Rb3 131.4(8) 2_656 1_455 ?
O13 Rb3 Rb3 138.2(3) . 1_455 ?
O13 Rb3 Rb3 48.6(8) 1_455 1_455 ?
O13 Rb3 Rb3 131.4(8) 1_455 1_655 ?
O13 Rb3 Rb3 48.6(8) 2_656 1_655 ?
O13 Rb3 Rb4A 68.4(8) 2_656 . ?
O13 Rb3 Rb4A 111.6(8) 1_455 1_545 ?
O13 Rb3 Rb4A 109.1(7) 2_556 1_545 ?
O13 Rb3 Rb4A 70.9(7) . . ?
O13 Rb3 Rb4A 109.1(7) . 1_545 ?
O13 Rb3 Rb4A 70.9(7) 2_556 . ?
O13 Rb3 Rb4A 111.6(8) 2_656 1_545 ?
O13 Rb3 Rb4A 68.4(8) 1_455 . ?
O13 Rb3 Rb4B 49.6(8) 2_656 . ?
O13 Rb3 Rb4B 90.5(8) 2_656 1_455 ?
O13 Rb3 Rb4B 94.9(6) . 1_455 ?
O13 Rb3 Rb4B 90.5(8) 1_455 . ?
O13 Rb3 Rb4B 49.6(8) 1_455 1_455 ?
O13 Rb3 Rb4B 49.1(7) . . ?
O13 Rb3 Rb4B 49.1(7) 2_556 1_455 ?
O13 Rb3 Rb4B 94.9(6) 2_556 . ?
O13 Rb3 O13 89.6(9) 2_656 2_556 ?
O13 Rb3 O13 76.5(12) 2_656 . ?
O13 Rb3 O13 141.7(14) . 2_556 ?
O13 Rb3 O13 89.6(9) 1_455 . ?
O13 Rb3 O13 136.7(16) 2_656 1_455 ?
O13 Rb3 O13 76.5(12) 1_455 2_556 ?
O13 Rb3 O15 43.6(9) 1_455 . ?
O13 Rb3 O15 116.3(8) . 2_556 ?
O13 Rb3 O15 117.2(10) 1_455 2_556 ?
O13 Rb3 O15 47.1(5) . . ?
O13 Rb3 O15 43.6(9) 2_656 2_556 ?
O13 Rb3 O15 47.1(5) 2_556 2_556 ?
O13 Rb3 O15 116.3(8) 2_556 . ?
O13 Rb3 O15 117.2(10) 2_656 . ?
O13 Rb3 O17 71.3(7) . 1_445 ?
O13 Rb3 O17 69.6(9) 2_656 2_646 ?
O13 Rb3 O17 69.6(9) 1_455 1_445 ?
O13 Rb3 O17 71.3(7) 2_556 2_646 ?
O13 Rb3 O17 138.1(9) 1_455 2_646 ?
O13 Rb3 O17 132.2(4) 2_556 1_445 ?
O13 Rb3 O17 132.2(4) . 2_646 ?
O13 Rb3 O17 138.1(9) 2_656 1_445 ?
O13 Rb3 O18 91.1(8) 2_556 1_445 ?
O13 Rb3 O18 112.4(8) 2_556 2_646 ?
O13 Rb3 O18 99.0(10) 1_455 2_546 ?
O13 Rb3 O18 59.7(8) 2_656 2_646 ?
O13 Rb3 O18 59.7(8) 1_455 1_445 ?
O13 Rb3 O18 99.0(10) 2_656 1_545 ?
O13 Rb3 O18 57.8(7) 2_556 2_546 ?
O13 Rb3 O18 107.7(9) 1_455 1_545 ?
O13 Rb3 O18 112.4(8) . 1_445 ?
O13 Rb3 O18 57.8(7) . 1_545 ?
O13 Rb3 O18 107.7(9) 2_656 2_546 ?
O13 Rb3 O18 160.4(12) 2_556 1_545 ?
O13 Rb3 O18 160.4(12) . 2_546 ?
O13 Rb3 O18 162.9(13) 1_455 2_646 ?
O13 Rb3 O18 91.1(8) . 2_646 ?
O13 Rb3 O18 162.9(13) 2_656 1_445 ?
O15 Rb3 W5 128.8(5) . 2_656 ?
O15 Rb3 W5 30.0(4) . 1_455 ?
O15 Rb3 W5 128.8(5) 2_556 1_455 ?
O15 Rb3 W5 30.0(4) 2_556 2_656 ?
O15 Rb3 Rb3 88.4(4) . 1_655 ?
O15 Rb3 Rb3 91.6(4) . 1_455 ?
O15 Rb3 Rb3 88.4(4) 2_556 1_455 ?
O15 Rb3 Rb3 91.6(4) 2_556 1_655 ?
O15 Rb3 Rb4A 111.2(5) 2_556 1_545 ?
O15 Rb3 Rb4A 111.2(5) . 1_545 ?
O15 Rb3 Rb4B 70.8(5) . . ?
O15 Rb3 Rb4B 70.8(5) 2_556 1_455 ?
O15 Rb3 Rb4B 72.5(5) 2_556 . ?
O15 Rb3 Rb4B 72.5(5) . 1_455 ?
O15 Rb3 O15 137.5(10) . 2_556 ?
O17 Rb3 W5 59.5(3) 1_445 1_455 ?
O17 Rb3 W5 149.5(3) 1_445 2_656 ?
O17 Rb3 W5 149.5(3) 2_646 1_455 ?
O17 Rb3 W5 59.5(3) 2_646 2_656 ?
O17 Rb3 Rb3 89.6(3) 2_646 1_455 ?
O17 Rb3 Rb3 90.4(3) 1_445 1_455 ?
O17 Rb3 Rb3 90.4(3) 2_646 1_655 ?
O17 Rb3 Rb3 89.6(3) 1_445 1_655 ?
O17 Rb3 Rb4A 57.6(3) 1_445 1_545 ?
O17 Rb3 Rb4A 57.6(3) 2_646 1_545 ?
O17 Rb3 Rb4B 118.0(3) 2_646 . ?
O17 Rb3 Rb4B 117.5(3) 2_646 1_455 ?
O17 Rb3 Rb4B 118.0(3) 1_445 1_455 ?
O17 Rb3 Rb4B 117.5(3) 1_445 . ?
O17 Rb3 O15 168.8(7) 2_646 . ?
O17 Rb3 O15 53.7(5) 2_646 2_556 ?
O17 Rb3 O15 168.8(7) 1_445 2_556 ?
O17 Rb3 O15 53.7(5) 1_445 . ?
O17 Rb3 O17 115.2(6) 1_445 2_646 ?
O18 Rb3 W5 60.6(7) 2_646 2_656 ?
O18 Rb3 W5 153.6(7) 1_445 2_656 ?
O18 Rb3 W5 95.0(7) 1_545 1_455 ?
O18 Rb3 W5 60.6(7) 1_445 1_455 ?
O18 Rb3 W5 95.0(7) 2_546 2_656 ?
O18 Rb3 W5 109.0(7) 2_546 1_455 ?
O18 Rb3 W5 109.0(7) 1_545 2_656 ?
O18 Rb3 W5 153.6(7) 2_646 1_455 ?
O18 Rb3 Rb3 127.0(7) 2_546 1_655 ?
O18 Rb3 Rb3 128.5(7) 2_646 1_455 ?
O18 Rb3 Rb3 51.5(7) 1_445 1_455 ?
O18 Rb3 Rb3 53.0(7) 2_546 1_455 ?
O18 Rb3 Rb3 51.5(7) 2_646 1_655 ?
O18 Rb3 Rb3 127.0(7) 1_545 1_455 ?
O18 Rb3 Rb3 53.0(7) 1_545 1_655 ?
O18 Rb3 Rb3 128.5(7) 1_445 1_655 ?
O18 Rb3 Rb4A 51.3(7) 2_546 1_545 ?
O18 Rb3 Rb4A 128.7(7) 1_545 . ?
O18 Rb3 Rb4A 128.7(7) 2_546 . ?
O18 Rb3 Rb4A 51.3(7) 1_545 1_545 ?
O18 Rb3 Rb4A 127.8(7) 1_445 . ?
O18 Rb3 Rb4A 52.2(7) 1_445 1_545 ?
O18 Rb3 Rb4A 52.2(7) 2_646 1_545 ?
O18 Rb3 Rb4A 127.8(7) 2_646 . ?
O18 Rb3 Rb4B 147.3(7) 1_545 1_455 ?
O18 Rb3 Rb4B 147.3(7) 2_546 . ?
O18 Rb3 Rb4B 104.1(7) 2_546 1_455 ?
O18 Rb3 Rb4B 147.2(7) 2_646 1_455 ?
O18 Rb3 Rb4B 147.2(7) 1_445 . ?
O18 Rb3 Rb4B 102.8(7) 2_646 . ?
O18 Rb3 Rb4B 104.1(7) 1_545 . ?
O18 Rb3 Rb4B 102.8(7) 1_445 1_455 ?
O18 Rb3 O15 75.3(9) 2_546 2_556 ?
O18 Rb3 O15 77.6(8) 2_646 2_556 ?
O18 Rb3 O15 131.2(8) 2_646 . ?
O18 Rb3 O15 131.2(8) 1_445 2_556 ?
O18 Rb3 O15 77.6(8) 1_445 . ?
O18 Rb3 O15 134.9(8) 2_546 . ?
O18 Rb3 O15 134.9(8) 1_545 2_556 ?
O18 Rb3 O15 75.3(9) 1_545 . ?
O18 Rb3 O17 40.6(8) 2_546 2_646 ?
O18 Rb3 O17 42.7(7) 1_445 1_445 ?
O18 Rb3 O17 95.1(8) 1_545 2_646 ?
O18 Rb3 O17 95.1(8) 2_546 1_445 ?
O18 Rb3 O17 40.6(8) 1_545 1_445 ?
O18 Rb3 O17 94.5(8) 2_646 1_445 ?
O18 Rb3 O17 94.5(8) 1_445 2_646 ?
O18 Rb3 O17 42.7(8) 2_646 2_646 ?
O18 Rb3 O18 75.5(8) 1_545 1_445 ?
O18 Rb3 O18 102.6(15) 2_546 1_545 ?
O18 Rb3 O18 59.0(13) 2_546 1_445 ?
O18 Rb3 O18 75.5(8) 2_546 2_646 ?
O18 Rb3 O18 104.4(14) 1_445 2_646 ?
O18 Rb3 O18 59.0(13) 1_545 2_646 ?
Rb3 Rb4A W6A 116.4(4) . 2_656 ?
Rb3 Rb4A Rb4A 90.000(6) . 1_455 ?
Rb3 Rb4A Rb4A 90.000(1) . 1_655 ?
Rb3 Rb4A O13 48.6(7) . 2_556 ?
Rb3 Rb4A O13 48.6(6) . . ?
Rb3 Rb4A O13 44.8(4) . 2_656 ?
Rb3 Rb4A O13 44.8(4) . 1_455 ?
Rb3 Rb4A O14 86.9(8) . 1_455 ?
Rb3 Rb4A O14 86.9(8) . 2_556 ?
Rb3 Rb4A O14 86.9(8) . 2_656 ?
Rb3 Rb4A O14 86.9(8) . . ?
Rb3 Rb4A O17 122.4(4) . 2_656 ?
Rb3 Rb4A O17 122.4(4) . 1_455 ?
Rb4A Rb4A W6A 66.95(12) 1_655 2_656 ?
Rb4A Rb4A W6A 113.05(12) 1_455 2_656 ?
Rb4A Rb4A Rb4A 180.0 1_655 1_455 ?
Rb4B Rb4A W6A 112.9(6) 1_455 2_656 ?
Rb4B Rb4A W6A 66.8(5) . 2_656 ?
Rb4B Rb4A Rb3 90.4(10) 1_455 . ?
Rb4B Rb4A Rb3 90.4(10) . . ?
Rb4B Rb4A Rb4A 179.6(10) 1_455 1_655 ?
Rb4B Rb4A Rb4A 0.4(10) . 1_655 ?
Rb4B Rb4A Rb4A 0.4(10) 1_455 1_455 ?
Rb4B Rb4A Rb4A 179.6(10) . 1_455 ?
Rb4B Rb4A Rb4B 179(2) . 1_455 ?
Rb4B Rb4A O13 126.6(11) 1_455 . ?
Rb4B Rb4A O13 60.2(9) . 2_656 ?
Rb4B Rb4A O13 54.0(8) . . ?
Rb4B Rb4A O13 60.2(9) 1_455 1_455 ?
Rb4B Rb4A O13 126.6(11) . 2_556 ?
Rb4B Rb4A O13 54.0(8) 1_455 2_556 ?
Rb4B Rb4A O13 120.4(11) . 1_455 ?
Rb4B Rb4A O13 120.4(11) 1_455 2_656 ?
Rb4B Rb4A O14 123.0(5) . 2_556 ?
Rb4B Rb4A O14 58.8(5) 1_455 1_455 ?
Rb4B Rb4A O14 123.0(5) 1_455 . ?
Rb4B Rb4A O14 121.3(5) 1_455 2_656 ?
Rb4B Rb4A O14 58.8(5) . 2_656 ?
Rb4B Rb4A O14 57.0(5) . . ?
Rb4B Rb4A O14 121.3(5) . 1_455 ?
Rb4B Rb4A O14 57.0(5) 1_455 2_556 ?
Rb4B Rb4A O17 89.4(6) . 1_455 ?
Rb4B Rb4A O17 90.2(6) . 2_656 ?
Rb4B Rb4A O17 90.2(6) 1_455 1_455 ?
Rb4B Rb4A O17 89.4(6) 1_455 2_656 ?
Rb4B Rb4A O18 53.6(10) 1_455 2_556 ?
Rb4B Rb4A O18 52.1(10) . 2_656 ?
Rb4B Rb4A O18 127.3(12) . 1_455 ?
Rb4B Rb4A O18 125.8(12) 1_455 . ?
Rb4B Rb4A O18 53.6(10) . . ?
Rb4B Rb4A O18 127.3(12) 1_455 2_656 ?
Rb4B Rb4A O18 125.8(13) . 2_556 ?
Rb4B Rb4A O18 52.1(10) 1_455 1_455 ?
O13 Rb4A W6A 115.7(4) . 2_656 ?
O13 Rb4A W6A 155.6(7) 1_455 2_656 ?
O13 Rb4A W6A 73.8(4) 2_656 2_656 ?
O13 Rb4A W6A 98.9(3) 2_556 2_656 ?
O13 Rb4A Rb4A 59.9(6) 2_656 1_655 ?
O13 Rb4A Rb4A 59.9(6) 1_455 1_455 ?
O13 Rb4A Rb4A 53.7(5) 2_556 1_455 ?
O13 Rb4A Rb4A 120.1(6) 1_455 1_655 ?
O13 Rb4A Rb4A 126.3(5) . 1_455 ?
O13 Rb4A Rb4A 53.7(5) . 1_655 ?
O13 Rb4A Rb4A 120.1(6) 2_656 1_455 ?
O13 Rb4A Rb4A 126.3(5) 2_556 1_655 ?
O13 Rb4A O13 66.4(8) 1_455 . ?
O13 Rb4A O13 57.5(10) 2_656 . ?
O13 Rb4A O13 97.2(13) . 2_556 ?
O13 Rb4A O13 89.6(9) 2_656 1_455 ?
O13 Rb4A O13 66.4(8) 2_656 2_556 ?
O13 Rb4A O13 57.5(10) 1_455 2_556 ?
O13 Rb4A O14 130.1(10) 1_455 2_656 ?
O13 Rb4A O14 132.3(10) . 2_556 ?
O13 Rb4A O14 43.8(8) 1_455 1_455 ?
O13 Rb4A O14 79.7(9) 1_455 . ?
O13 Rb4A O14 130.1(10) 2_656 1_455 ?
O13 Rb4A O14 96.0(9) 2_656 . ?
O13 Rb4A O14 43.8(8) 2_656 2_656 ?
O13 Rb4A O14 42.0(8) 2_556 2_556 ?
O13 Rb4A O14 96.0(9) 1_455 2_556 ?
O13 Rb4A O14 42.0(8) . . ?
O13 Rb4A O14 132.3(10) 2_556 . ?
O13 Rb4A O14 79.7(9) 2_656 2_556 ?
O13 Rb4A O17 142.6(7) 2_656 1_455 ?
O13 Rb4A O17 142.6(7) 1_455 2_656 ?
O13 Rb4A O17 88.0(5) 2_656 2_656 ?
O13 Rb4A O17 88.0(5) 1_455 1_455 ?
O13 Rb4A O17 138.4(4) . 2_656 ?
O13 Rb4A O17 87.7(5) . 1_455 ?
O13 Rb4A O17 138.4(4) 2_556 1_455 ?
O13 Rb4A O17 87.7(5) 2_556 2_656 ?
O14 Rb4A W6A 30.0(7) 2_656 2_656 ?
O14 Rb4A W6A 64.0(6) 2_556 2_656 ?
O14 Rb4A W6A 156.1(10) 1_455 2_656 ?
O14 Rb4A W6A 119.0(6) . 2_656 ?
O14 Rb4A Rb4A 58.7(5) 2_656 1_655 ?
O14 Rb4A Rb4A 57.0(5) 2_556 1_455 ?
O14 Rb4A Rb4A 123.0(5) 2_556 1_655 ?
O14 Rb4A Rb4A 121.3(5) 1_455 1_655 ?
O14 Rb4A Rb4A 57.0(5) . 1_655 ?
O14 Rb4A Rb4A 58.7(5) 1_455 1_455 ?
O14 Rb4A Rb4A 123.0(5) . 1_455 ?
O14 Rb4A Rb4A 121.3(5) 2_656 1_455 ?
O14 Rb4A O13 92.9(7) 2_656 . ?
O14 Rb4A O13 83.0(7) 1_455 . ?
O14 Rb4A O13 92.9(7) 1_455 2_556 ?
O14 Rb4A O13 83.0(7) 2_656 2_556 ?
O14 Rb4A O14 173.8(16) 1_455 2_656 ?
O14 Rb4A O14 173.9(15) . 2_556 ?
O14 Rb4A O14 64.3(4) 2_656 2_556 ?
O14 Rb4A O14 115.4(4) 2_656 . ?
O14 Rb4A O14 115.4(4) 1_455 2_556 ?
O14 Rb4A O14 64.3(4) 1_455 . ?
O14 Rb4A O17 47.0(7) 2_556 2_656 ?
O14 Rb4A O17 137.7(8) 2_556 1_455 ?
O14 Rb4A O17 47.0(7) . 1_455 ?
O14 Rb4A O17 138.2(8) 2_656 1_455 ?
O14 Rb4A O17 46.6(7) 2_656 2_656 ?
O14 Rb4A O17 137.7(8) . 2_656 ?
O14 Rb4A O17 46.6(7) 1_455 1_455 ?
O14 Rb4A O17 138.2(8) 1_455 2_656 ?
O17 Rb4A W6A 116.1(6) 1_455 2_656 ?
O17 Rb4A W6A 23.7(3) 2_656 2_656 ?
O17 Rb4A Rb4A 90.4(3) 2_656 1_655 ?
O17 Rb4A Rb4A 89.6(3) 1_455 1_655 ?
O17 Rb4A Rb4A 89.6(3) 2_656 1_455 ?
O17 Rb4A Rb4A 90.4(3) 1_455 1_455 ?
O17 Rb4A O17 115.3(8) 2_656 1_455 ?
O18 Rb4A W6A 63.4(8) 2_556 2_656 ?
O18 Rb4A W6A 82.8(8) . 2_656 ?
O18 Rb4A W6A 25.2(7) 2_656 2_656 ?
O18 Rb4A W6A 110.0(9) 1_455 2_656 ?
O18 Rb4A Rb3 130.1(8) 2_556 . ?
O18 Rb4A Rb3 129.2(7) 2_656 . ?
O18 Rb4A Rb3 129.2(8) 1_455 . ?
O18 Rb4A Rb3 130.1(8) . . ?
O18 Rb4A Rb4A 53.9(8) 2_556 1_455 ?
O18 Rb4A Rb4A 126.1(8) . 1_455 ?
O18 Rb4A Rb4A 53.9(8) . 1_655 ?
O18 Rb4A Rb4A 52.4(8) 2_656 1_655 ?
O18 Rb4A Rb4A 52.4(8) 1_455 1_455 ?
O18 Rb4A Rb4A 126.1(8) 2_556 1_655 ?
O18 Rb4A Rb4A 127.6(8) 2_656 1_455 ?
O18 Rb4A Rb4A 127.6(8) 1_455 1_655 ?
O18 Rb4A O13 113.8(9) . 2_656 ?
O18 Rb4A O13 106.1(8) 2_656 . ?
O18 Rb4A O13 84.6(6) 1_455 1_455 ?
O18 Rb4A O13 178.3(10) . 2_556 ?
O18 Rb4A O13 113.8(9) 2_556 1_455 ?
O18 Rb4A O13 81.5(7) 2_556 2_556 ?
O18 Rb4A O13 178.3(10) 2_556 . ?
O18 Rb4A O13 124.0(6) 2_656 2_556 ?
O18 Rb4A O13 120.8(7) . 1_455 ?
O18 Rb4A O13 106.1(8) 1_455 2_556 ?
O18 Rb4A O13 172.3(11) 2_656 1_455 ?
O18 Rb4A O13 120.8(7) 2_556 2_656 ?
O18 Rb4A O13 81.5(7) . . ?
O18 Rb4A O13 84.6(6) 2_656 2_656 ?
O18 Rb4A O13 172.3(11) 1_455 2_656 ?
O18 Rb4A O13 124.0(6) 1_455 . ?
O18 Rb4A O14 46.1(9) . . ?
O18 Rb4A O14 98.3(9) . 2_656 ?
O18 Rb4A O14 46.1(9) 2_556 2_556 ?
O18 Rb4A O14 139.7(11) 2_556 . ?
O18 Rb4A O14 46.4(9) 1_455 1_455 ?
O18 Rb4A O14 95.8(9) 2_656 . ?
O18 Rb4A O14 95.8(9) 1_455 2_556 ?
O18 Rb4A O14 88.1(9) 1_455 . ?
O18 Rb4A O14 85.7(9) 2_556 2_656 ?
O18 Rb4A O14 139.3(11) 1_455 2_656 ?
O18 Rb4A O14 139.7(11) . 2_556 ?
O18 Rb4A O14 85.7(9) . 1_455 ?
O18 Rb4A O14 88.1(9) 2_656 2_556 ?
O18 Rb4A O14 98.3(9) 2_556 1_455 ?
O18 Rb4A O14 139.3(11) 2_656 1_455 ?
O18 Rb4A O14 46.4(9) 2_656 2_656 ?
O18 Rb4A O17 94.0(9) 2_556 1_455 ?
O18 Rb4A O17 94.0(9) . 2_656 ?
O18 Rb4A O17 93.5(8) 1_455 2_656 ?
O18 Rb4A O17 93.5(8) 2_656 1_455 ?
O18 Rb4A O17 40.5(8) 2_556 2_656 ?
O18 Rb4A O17 42.5(8) 2_656 2_656 ?
O18 Rb4A O17 40.5(8) . 1_455 ?
O18 Rb4A O17 42.5(8) 1_455 1_455 ?
O18 Rb4A O18 99.7(15) . 2_556 ?
O18 Rb4A O18 73.7(9) 2_556 2_656 ?
O18 Rb4A O18 101.6(15) 2_656 1_455 ?
O18 Rb4A O18 57.7(13) . 2_656 ?
O18 Rb4A O18 73.7(9) . 1_455 ?
O18 Rb4A O18 57.7(12) 2_556 1_455 ?
W5 Rb4B W5 115.3(6) . 2_656 ?
W5 Rb4B Rb3 119.0(2) . 1_565 ?
W5 Rb4B Rb3 62.6(3) 2_656 1_655 ?
W5 Rb4B Rb3 119.0(2) 2_656 1_665 ?
W5 Rb4B Rb3 62.6(3) . . ?
W5 Rb4B Rb3 118.6(2) . 1_665 ?
W5 Rb4B Rb3 62.1(3) 2_656 . ?
W5 Rb4B Rb3 62.1(3) . 1_655 ?
W5 Rb4B Rb3 118.6(2) 2_656 1_565 ?
W5 Rb4B Rb4B 90.48(5) . 1_455 ?
W5 Rb4B Rb4B 89.52(5) . 1_655 ?
W5 Rb4B Rb4B 89.52(5) 2_656 1_455 ?
W5 Rb4B Rb4B 90.48(5) 2_656 1_655 ?
W6A Rb4B W5 173.6(4) 2_656 . ?
W6A Rb4B W5 173.6(4) . 2_656 ?
W6A Rb4B W5 61.17(11) 2_656 2_656 ?
W6A Rb4B W5 61.17(11) . . ?
W6A Rb4B W6A 122.9(6) 2_656 . ?
W6A Rb4B W6B 123.4(6) . 2_656 ?
W6A Rb4B W6B 11.34(11) . . ?
W6A Rb4B W6B 11.34(11) 2_656 2_656 ?
W6A Rb4B W6B 123.4(6) 2_656 . ?
W6A Rb4B Rb3 117.7(2) . . ?
W6A Rb4B Rb3 111.4(2) 2_656 . ?
W6A Rb4B Rb3 61.7(3) . 1_665 ?
W6A Rb4B Rb3 61.7(3) 2_656 1_565 ?
W6A Rb4B Rb3 67.2(3) 2_656 1_665 ?
W6A Rb4B Rb3 67.2(3) . 1_565 ?
W6A Rb4B Rb3 117.7(2) 2_656 1_655 ?
W6A Rb4B Rb3 111.4(2) . 1_655 ?
W6A Rb4B Rb4B 95.73(12) 2_656 1_655 ?
W6A Rb4B Rb4B 84.26(12) 2_656 1_455 ?
W6A Rb4B Rb4B 84.27(12) . 1_655 ?
W6A Rb4B Rb4B 95.73(12) . 1_455 ?
W6B Rb4B W5 59.43(8) . . ?
W6B Rb4B W5 59.42(8) 2_656 2_656 ?
W6B Rb4B W5 171.9(4) 2_656 . ?
W6B Rb4B W5 171.9(4) . 2_656 ?
W6B Rb4B W6B 126.5(6) . 2_656 ?
W6B Rb4B Rb3 63.5(3) 2_656 1_665 ?
W6B Rb4B Rb3 68.7(3) 2_656 1_565 ?
W6B Rb4B Rb3 116.0(2) 2_656 . ?
W6B Rb4B Rb3 63.5(3) . 1_565 ?
W6B Rb4B Rb3 110.1(2) 2_656 1_655 ?
W6B Rb4B Rb3 116.0(2) . 1_655 ?
W6B Rb4B Rb3 110.1(2) . . ?
W6B Rb4B Rb3 68.7(3) . 1_665 ?
W6B Rb4B Rb4B 84.54(10) 2_656 1_655 ?
W6B Rb4B Rb4B 95.46(10) . 1_655 ?
W6B Rb4B Rb4B 84.54(10) . 1_455 ?
W6B Rb4B Rb4B 95.46(10) 2_656 1_455 ?
Rb3 Rb4B Rb3 176.0(3) 1_655 1_565 ?
Rb3 Rb4B Rb3 124.41(4) . 1_565 ?
Rb3 Rb4B Rb3 51.6(3) 1_665 1_565 ?
Rb3 Rb4B Rb3 176.0(3) . 1_665 ?
Rb3 Rb4B Rb3 124.41(4) 1_655 1_665 ?
Rb3 Rb4B Rb3 59.6(3) . 1_655 ?
Rb4A Rb4B W5 90.3(5) . . ?
Rb4A Rb4B W5 89.3(5) . 2_656 ?
Rb4A Rb4B W5 90.3(5) 1_655 2_656 ?
Rb4A Rb4B W5 89.3(5) 1_655 . ?
Rb4A Rb4B W6A 84.4(5) . 2_656 ?
Rb4A Rb4B W6A 84.4(5) 1_655 . ?
Rb4A Rb4B W6A 95.9(5) . . ?
Rb4A Rb4B W6A 95.9(5) 1_655 2_656 ?
Rb4A Rb4B W6B 95.6(5) . 2_656 ?
Rb4A Rb4B W6B 84.7(5) . . ?
Rb4A Rb4B W6B 84.7(5) 1_655 2_656 ?
Rb4A Rb4B W6B 95.6(5) 1_655 . ?
Rb4A Rb4B Rb3 59.8(9) 1_655 1_655 ?
Rb4A Rb4B Rb3 59.8(9) . . ?
Rb4A Rb4B Rb3 116.2(11) 1_655 1_565 ?
Rb4A Rb4B Rb3 119.4(11) . 1_655 ?
Rb4A Rb4B Rb3 64.6(9) . 1_565 ?
Rb4A Rb4B Rb3 119.4(11) 1_655 . ?
Rb4A Rb4B Rb3 64.6(9) 1_655 1_665 ?
Rb4A Rb4B Rb3 116.2(11) . 1_665 ?
Rb4A Rb4B Rb4A 179(2) . 1_655 ?
Rb4A Rb4B Rb4B 179.6(10) 1_655 1_455 ?
Rb4A Rb4B Rb4B 0.4(10) . 1_455 ?
Rb4A Rb4B Rb4B 179.6(10) . 1_655 ?
Rb4A Rb4B Rb4B 0.4(10) 1_655 1_655 ?
Rb4A Rb4B O13 85.3(10) . 2_656 ?
Rb4A Rb4B O13 85.3(10) 1_655 . ?
Rb4A Rb4B O13 94.1(10) 1_655 2_656 ?
Rb4A Rb4B O13 94.1(10) . . ?
Rb4A Rb4B O14 91.2(6) . . ?
Rb4A Rb4B O14 91.2(6) 1_655 2_656 ?
Rb4A Rb4B O14 88.8(6) . 2_656 ?
Rb4A Rb4B O14 88.8(6) 1_655 . ?
Rb4A Rb4B O18 91.5(12) . 2_656 ?
Rb4A Rb4B O18 91.5(13) 1_655 . ?
Rb4A Rb4B O18 89.1(12) . . ?
Rb4A Rb4B O18 89.1(12) 1_655 2_656 ?
Rb4B Rb4B Rb3 119.79(17) 1_655 . ?
Rb4B Rb4B Rb3 60.21(18) 1_655 1_655 ?
Rb4B Rb4B Rb3 60.21(18) 1_455 . ?
Rb4B Rb4B Rb3 115.80(13) 1_655 1_565 ?
Rb4B Rb4B Rb3 64.20(14) 1_455 1_565 ?
Rb4B Rb4B Rb3 115.80(13) 1_455 1_665 ?
Rb4B Rb4B Rb3 119.79(17) 1_455 1_655 ?
Rb4B Rb4B Rb3 64.20(14) 1_655 1_665 ?
Rb4B Rb4B Rb4B 180.0 1_655 1_455 ?
O13 Rb4B W5 92.5(7) 2_656 . ?
O13 Rb4B W5 92.5(7) . 2_656 ?
O13 Rb4B W5 23.2(4) 2_656 2_656 ?
O13 Rb4B W5 23.2(4) . . ?
O13 Rb4B W6A 83.6(6) 2_656 2_656 ?
O13 Rb4B W6A 83.6(6) . . ?
O13 Rb4B W6A 153.6(8) 2_656 . ?
O13 Rb4B W6A 153.6(8) . 2_656 ?
O13 Rb4B W6B 82.6(5) . . ?
O13 Rb4B W6B 82.6(5) 2_656 2_656 ?
O13 Rb4B W6B 150.0(6) 2_656 . ?
O13 Rb4B W6B 150.0(6) . 2_656 ?
O13 Rb4B Rb3 41.5(4) . 1_655 ?
O13 Rb4B Rb3 134.7(7) . 1_665 ?
O13 Rb4B Rb3 47.7(8) . . ?
O13 Rb4B Rb3 134.7(7) 2_656 1_565 ?
O13 Rb4B Rb3 41.5(4) 2_656 . ?
O13 Rb4B Rb3 140.4(3) 2_656 1_665 ?
O13 Rb4B Rb3 47.7(8) 2_656 1_655 ?
O13 Rb4B Rb3 140.4(3) . 1_565 ?
O13 Rb4B Rb4B 94.4(6) . 1_455 ?
O13 Rb4B Rb4B 94.4(6) 2_656 1_655 ?
O13 Rb4B Rb4B 85.6(6) . 1_655 ?
O13 Rb4B Rb4B 85.6(6) 2_656 1_455 ?
O13 Rb4B O13 70.0(12) . 2_656 ?
O13 Rb4B O14 51.4(9) 2_656 2_656 ?
O13 Rb4B O14 120.9(11) . 2_656 ?
O13 Rb4B O14 120.9(11) 2_656 . ?
O13 Rb4B O14 51.4(9) . . ?
O14 Rb4B W5 143.8(10) . 2_656 ?
O14 Rb4B W5 28.5(8) . . ?
O14 Rb4B W5 28.5(8) 2_656 2_656 ?
O14 Rb4B W5 143.8(10) 2_656 . ?
O14 Rb4B W6A 32.8(8) 2_656 2_656 ?
O14 Rb4B W6A 32.8(8) . . ?
O14 Rb4B W6A 154.8(10) . 2_656 ?
O14 Rb4B W6A 154.8(10) 2_656 . ?
O14 Rb4B W6B 156.1(10) . 2_656 ?
O14 Rb4B W6B 31.4(8) . . ?
O14 Rb4B W6B 156.1(10) 2_656 . ?
O14 Rb4B W6B 31.4(8) 2_656 2_656 ?
O14 Rb4B Rb3 87.2(8) 2_656 1_655 ?
O14 Rb4B Rb3 86.0(8) 2_656 . ?
O14 Rb4B Rb3 93.0(8) . 1_665 ?
O14 Rb4B Rb3 86.0(8) . 1_655 ?
O14 Rb4B Rb3 94.0(8) 2_656 1_665 ?
O14 Rb4B Rb3 87.2(8) . . ?
O14 Rb4B Rb3 94.0(8) . 1_565 ?
O14 Rb4B Rb3 93.0(8) 2_656 1_565 ?
O14 Rb4B Rb4B 91.2(6) . 1_455 ?
O14 Rb4B Rb4B 88.8(6) . 1_655 ?
O14 Rb4B Rb4B 88.8(6) 2_656 1_455 ?
O14 Rb4B Rb4B 91.2(6) 2_656 1_655 ?
O14 Rb4B O14 172.2(18) . 2_656 ?
O18 Rb4B W5 159.5(10) . 2_656 ?
O18 Rb4B W5 85.1(8) . . ?
O18 Rb4B W5 159.5(10) 2_656 . ?
O18 Rb4B W5 85.1(8) 2_656 2_656 ?
O18 Rb4B W6A 25.0(8) . . ?
O18 Rb4B W6A 98.3(10) 2_656 . ?
O18 Rb4B W6A 98.3(10) . 2_656 ?
O18 Rb4B W6A 25.0(8) 2_656 2_656 ?
O18 Rb4B W6B 100.4(10) . 2_656 ?
O18 Rb4B W6B 100.4(10) 2_656 . ?
O18 Rb4B W6B 26.2(8) . . ?
O18 Rb4B W6B 26.2(8) 2_656 2_656 ?
O18 Rb4B Rb3 44.9(9) 2_656 1_565 ?
O18 Rb4B Rb3 44.9(9) . 1_665 ?
O18 Rb4B Rb3 132.9(9) 2_656 1_655 ?
O18 Rb4B Rb3 132.9(9) . . ?
O18 Rb4B Rb3 134.5(9) 2_656 . ?
O18 Rb4B Rb3 134.5(9) . 1_655 ?
O18 Rb4B Rb3 43.5(9) . 1_565 ?
O18 Rb4B Rb3 43.5(9) 2_656 1_665 ?
O18 Rb4B Rb4B 91.2(9) . 1_655 ?
O18 Rb4B Rb4B 91.2(9) 2_656 1_455 ?
O18 Rb4B Rb4B 88.8(9) 2_656 1_655 ?
O18 Rb4B Rb4B 88.8(9) . 1_455 ?
O18 Rb4B O13 173.9(10) 2_656 . ?
O18 Rb4B O13 108.0(8) . . ?
O18 Rb4B O13 108.0(8) 2_656 2_656 ?
O18 Rb4B O13 173.9(10) . 2_656 ?
O18 Rb4B O14 56.7(11) 2_656 2_656 ?
O18 Rb4B O14 131.0(13) . 2_656 ?
O18 Rb4B O14 56.7(11) . . ?
O18 Rb4B O14 131.0(13) 2_656 . ?
O18 Rb4B O18 74.5(17) . 2_656 ?
W1 O1 W1 144(3) . 2_755 ?
W1 O1 W1 156(2) 2_655 1_655 ?
W1 O1 W1 150(2) 2_755 2_655 ?
W1 O1 W1 150(2) . 1_655 ?
W1 O1 W1 5.9(4) . 2_655 ?
W1 O1 W1 5.9(4) 2_755 1_655 ?
W1 O1 Rb2A 108.0(15) 2_755 1_655 ?
W1 O1 Rb2A 72.0(15) 2_755 1_645 ?
W1 O1 Rb2A 108.0(15) . 1_655 ?
W1 O1 Rb2A 102.2(10) 2_655 1_655 ?
W1 O1 Rb2A 77.8(10) 2_655 1_645 ?
W1 O1 Rb2A 102.2(10) 1_655 1_655 ?
W1 O1 Rb2A 72.0(15) . 1_645 ?
W1 O1 Rb2A 77.8(10) 1_655 1_645 ?
W1 O1 Rb2B 77.8(11) 2_755 1_655 ?
W1 O1 Rb2B 138.3(18) 2_755 . ?
W1 O1 Rb2B 132.4(14) 1_655 . ?
W1 O1 Rb2B 132.4(14) 2_655 1_655 ?
W1 O1 Rb2B 72.0(7) 2_655 . ?
W1 O1 Rb2B 72.0(7) 1_655 1_655 ?
W1 O1 Rb2B 138.3(18) . 1_655 ?
W1 O1 Rb2B 77.8(11) . . ?
Rb2A O1 Rb2A 180.0 1_655 1_645 ?
Rb2A O1 Rb2B 30.2(4) 1_655 1_655 ?
Rb2A O1 Rb2B 149.8(4) 1_645 1_655 ?
Rb2A O1 Rb2B 30.2(4) 1_655 . ?
Rb2A O1 Rb2B 149.8(4) 1_645 . ?
Rb2B O1 Rb2B 60.5(8) 1_655 . ?
W1 O2 W1 24.1(5) . 2_655 ?
W1 O2 W2 151(2) . 1_545 ?
W1 O2 W2 144(2) 2_655 1_545 ?
W1 O2 Rb2A 97.0(15) . 1_645 ?
W1 O2 Rb2A 108.7(16) . 1_545 ?
W1 O2 Rb2A 93.2(14) 2_655 1_545 ?
W1 O2 Rb2A 110.7(16) 2_655 1_645 ?
W1 O2 Rb2B 104.7(16) 2_655 1_545 ?
W1 O2 Rb2B 106.1(16) . 1_545 ?
W2 O2 Rb2A 105.2(14) 1_545 1_645 ?
W2 O2 Rb2A 94.9(13) 1_545 1_545 ?
W2 O2 Rb2B 102.4(14) 1_545 1_545 ?
Rb2A O2 Rb2A 73.3(8) 1_645 1_545 ?
Rb2B O2 Rb2A 37.2(5) 1_545 1_645 ?
Rb2B O2 Rb2A 36.1(5) 1_545 1_545 ?
W1 O3 W1 22.5(4) . 2_655 ?
W1 O3 W3 149(2) . 2_655 ?
W1 O3 Rb2A 103.2(13) . . ?
W1 O3 Rb2A 88.8(11) 2_655 . ?
W1 O3 Rb2A 114.0(13) 2_655 1_655 ?
W1 O3 Rb2A 103.2(13) . 1_655 ?
W1 O3 Rb2B 102.6(13) 2_655 . ?
W1 O3 Rb2B 106.0(14) . . ?
W3 O3 W1 134.5(19) 2_655 2_655 ?
W3 O3 Rb2A 107.7(13) 2_655 1_655 ?
W3 O3 Rb2A 90.4(12) 2_655 . ?
W3 O3 Rb2B 100.2(13) 2_655 . ?
Rb2A O3 Rb2A 68.2(7) 1_655 . ?
Rb2B O3 Rb2A 36.3(4) . 1_655 ?
Rb2B O3 Rb2A 31.9(4) . . ?
W2 O4 W2 158(3) . 1_455 ?
W2 O4 Rb1 86.3(13) 1_455 1_565 ?
W2 O4 Rb1 86.0(16) . 1_565 ?
W2 O4 Rb2A 91.0(13) 1_455 . ?
W2 O4 Rb2A 93.5(17) . . ?
W2 O4 Rb2B 65.1(14) . . ?
W2 O4 Rb2B 62.7(9) 1_455 1_455 ?
W2 O4 Rb2B 119.6(16) 1_455 . ?
W2 O4 Rb2B 121(2) . 1_455 ?
Rb1 O4 Rb2B 148.9(9) 1_565 1_455 ?
Rb2A O4 Rb1 171.2(15) . 1_565 ?
Rb2A O4 Rb2B 28.6(3) . 1_455 ?
Rb2A O4 Rb2B 29.1(4) . . ?
Rb2B O4 Rb1 151.0(6) . 1_565 ?
Rb2B O4 Rb2B 57.7(7) . 1_455 ?
W2 O5 W4 148.6(18) . . ?
W2 O5 Rb1 106.0(13) . 1_565 ?
W2 O5 Rb1 100.9(13) . 1_665 ?
W4 O5 Rb1 88.7(11) . 1_665 ?
W4 O5 Rb1 105.3(12) . 1_565 ?
Rb1 O5 Rb1 67.8(6) 1_565 1_665 ?
W2 O6 W3 150.0(14) . 1_565 ?
W2 O6 Rb1 103.8(14) . 1_665 ?
W2 O6 Rb1 102.7(14) . 1_565 ?
W3 O6 Rb1 95.2(12) 1_565 1_665 ?
W3 O6 Rb1 105.7(15) 1_565 1_565 ?
Rb1 O6 Rb1 68.6(5) 1_565 1_665 ?
W2 O7 W3 144.4(14) . . ?
W2 O7 Rb2A 104.2(17) . 1_655 ?
W2 O7 Rb2A 99.9(16) . . ?
W2 O7 Rb2B 105.2(19) . . ?
W3 O7 Rb2A 101.8(15) . 1_655 ?
W3 O7 Rb2A 110.7(18) . . ?
W3 O7 Rb2B 110.2(19) . . ?
Rb2A O7 Rb2A 73.5(5) . 1_655 ?
Rb2B O7 Rb2A 36.1(4) . 1_655 ?
Rb2B O7 Rb2A 37.4(4) . . ?
W3 O8 W3 165.6(17) . 1_655 ?
W3 O8 Rb1 96.1(11) . 1_655 ?
W3 O8 Rb1 91.4(9) 1_655 1_655 ?
W3 O8 Rb2A 86.8(10) . 1_655 ?
W3 O8 Rb2A 85.1(9) 1_655 1_655 ?
Rb1 O8 Rb2A 175.7(9) 1_655 1_655 ?
W3 O9 W4 155(2) . . ?
W3 O9 Rb1 103.9(14) . 1_655 ?
W3 O9 Rb1 106.6(14) . . ?
W4 O9 Rb1 96.2(12) . . ?
W4 O9 Rb1 92.4(11) . 1_655 ?
Rb1 O9 Rb1 69.0(7) 1_655 . ?
W4 O10 W4 155.9(14) . 1_655 ?
W4 O10 Rb1 77.5(8) . 1_655 ?
W4 O10 Rb1 78.4(7) 1_655 1_655 ?
W4 O10 Rb1 99.8(10) 1_655 1_665 ?
W4 O10 Rb1 104.3(12) . 1_665 ?
Rb1 O10 Rb1 177.6(10) 1_665 1_655 ?
W4 O11 W5 139.7(17) . . ?
W4 O11 Rb1 107.6(13) . 1_655 ?
W4 O11 Rb1 113.8(14) . . ?
W5 O11 Rb1 100.5(11) . 1_655 ?
W5 O11 Rb1 100.3(11) . . ?
Rb1 O11 Rb1 76.5(7) 1_655 . ?
W4 O12 W6A 148.3(18) . . ?
W4 O12 W6B 140.0(19) . . ?
W4 O12 Rb1 103.6(13) . 1_565 ?
W4 O12 Rb1 110.5(14) . 1_665 ?
W6A O12 W6B 19.6(4) . . ?
W6A O12 Rb1 97.8(12) . 1_665 ?
W6A O12 Rb1 98.6(12) . 1_565 ?
W6B O12 Rb1 109.4(12) . 1_665 ?
W6B O12 Rb1 87.3(11) . 1_565 ?
Rb1 O12 Rb1 71.3(7) 1_665 1_565 ?
W5 O13 Rb3 123.1(13) . . ?
W5 O13 Rb3 142.6(19) . 1_655 ?
W5 O13 Rb4A 112.3(16) . 1_655 ?
W5 O13 Rb4A 103.0(11) . . ?
W5 O13 Rb4B 110.8(14) . . ?
Rb3 O13 Rb3 89.6(9) 1_655 . ?
Rb3 O13 Rb4A 109.5(11) 1_655 . ?
Rb3 O13 Rb4A 66.8(7) 1_655 1_655 ?
Rb3 O13 Rb4A 60.5(8) . . ?
Rb3 O13 Rb4A 108.6(11) . 1_655 ?
Rb3 O13 Rb4B 83.2(10) . . ?
Rb3 O13 Rb4B 88.9(9) 1_655 . ?
Rb4A O13 Rb4A 66.4(8) 1_655 . ?
Rb4B O13 Rb4A 34.5(4) . 1_655 ?
Rb4B O13 Rb4A 31.9(4) . . ?
W5 O14 W6A 167.4(15) . . ?
W5 O14 W6B 161.8(17) . . ?
W5 O14 Rb4A 97.2(12) . . ?
W5 O14 Rb4A 98.4(12) . 1_655 ?
W5 O14 Rb4B 99.5(12) . . ?
W6A O14 Rb4A 95.3(11) . . ?
W6A O14 Rb4A 86.0(11) . 1_655 ?
W6A O14 Rb4B 90.6(11) . . ?
W6B O14 W6A 21.3(5) . . ?
W6B O14 Rb4A 85.8(10) . . ?
W6B O14 Rb4A 99.0(12) . 1_655 ?
W6B O14 Rb4B 92.6(12) . . ?
Rb4A O14 Rb4A 64.3(4) 1_655 . ?
Rb4B O14 Rb4A 32.5(3) . 1_655 ?
Rb4B O14 Rb4A 31.8(2) . . ?
W5 O15 W5 161.8(16) . 1_455 ?
W5 O15 Rb1 97.9(11) . . ?
W5 O15 Rb1 95.1(10) 1_455 . ?
W5 O15 Rb3 79.8(8) 1_455 . ?
W5 O15 Rb3 82.3(9) . . ?
W5 O15 Rb4A 82.0(8) 1_455 . ?
W5 O15 Rb4A 84.4(9) . . ?
Rb1 O15 Rb3 126.7(10) . . ?
Rb1 O15 Rb4A 176.1(10) . . ?
Rb3 O15 Rb4A 50.4(5) . . ?
W5 O16 W6B 137.0(11) . 1_545 ?
W5 O16 Rb1 107.2(12) . 1_655 ?
W5 O16 Rb1 102.5(11) . . ?
W6A O16 W5 137.3(10) 1_545 . ?
W6A O16 W6B 21.4(4) 1_545 1_545 ?
W6A O16 Rb1 104.7(12) 1_545 1_655 ?
W6A O16 Rb1 112.8(13) 1_545 . ?
W6B O16 Rb1 115.0(13) 1_545 1_655 ?
W6B O16 Rb1 96.4(10) 1_545 . ?
Rb1 O16 Rb1 74.8(4) 1_655 . ?
W6A O17 W6A 165.7(13) . 1_655 ?
W6A O17 W6B 1.2(3) . . ?
W6A O17 W6B 159.0(14) . 1_655 ?
W6A O17 Rb1 91.0(6) 1_655 1_665 ?
W6A O17 Rb1 91.7(8) . 1_665 ?
W6A O17 Rb3 95.7(8) . 1_665 ?
W6A O17 Rb3 94.7(6) 1_655 1_665 ?
W6A O17 Rb4A 87.0(7) . 1_655 ?
W6A O17 Rb4A 88.6(6) 1_655 1_655 ?
W6B O17 W6A 165.6(10) . 1_655 ?
W6B O17 W6A 6.9(4) 1_655 1_655 ?
W6B O17 W6B 158.8(12) 1_655 . ?
W6B O17 Rb1 90.6(6) . 1_665 ?
W6B O17 Rb1 90.6(8) 1_655 1_665 ?
W6B O17 Rb3 100.7(8) 1_655 1_665 ?
W6B O17 Rb3 96.6(6) . 1_665 ?
W6B O17 Rb4A 88.2(7) 1_655 1_655 ?
W6B O17 Rb4A 88.1(5) . 1_655 ?
Rb1 O17 Rb3 122.0(6) 1_665 1_665 ?
Rb1 O17 Rb4A 173.2(7) 1_665 1_655 ?
Rb4A O17 Rb3 64.8(4) 1_655 1_665 ?
W6A O18 W6B 23.7(5) . . ?
W6A O18 Rb3 136.2(19) . 1_565 ?
W6A O18 Rb3 114.5(18) . 1_665 ?
W6A O18 Rb4A 120.3(17) . . ?
W6A O18 Rb4A 102.0(16) . 1_655 ?
W6A O18 Rb4B 116.4(18) . . ?
W6B O18 Rb3 120.6(18) . 1_565 ?
W6B O18 Rb3 134.5(18) . 1_665 ?
W6B O18 Rb4A 103.7(16) . . ?
W6B O18 Rb4A 115.5(16) . 1_655 ?
W6B O18 Rb4B 114.9(17) . . ?
Rb3 O18 Rb3 75.5(8) 1_565 1_665 ?
Rb3 O18 Rb4A 78.8(10) 1_565 . ?
Rb3 O18 Rb4A 77.0(10) 1_665 1_655 ?
Rb3 O18 Rb4A 121.7(12) 1_565 1_655 ?
Rb3 O18 Rb4A 121.6(12) 1_665 . ?
Rb4A O18 Rb4A 73.7(9) . 1_655 ?
Rb4B O18 Rb3 100.4(12) . 1_665 ?
Rb4B O18 Rb3 102.1(12) . 1_565 ?
Rb4B O18 Rb4A 36.4(6) . 1_655 ?
Rb4B O18 Rb4A 37.3(6) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.22807
2 0.25879
3 0.25679
4 0.25635

_exptl_crystal_recrystallization_method 'From the Melt'
